On October 23rd, 2014, we updated our
By continuing to use LinkedIn’s SlideShare service, you agree to the revised terms, so please take a few minutes to review them.
viii CONTENTS Further Reading 95 Problems 95 4 Fluid Flow and Metal Evaporation in Welding 97 4.1 Fluid Flow in Arcs 97 4.2 Fluid Flow in Weld Pools 103 4.3 Metal Evaporation 114 4.4 Active Flux GTAW 116 References 117 Further Reading 119 Problems 120 5 Residual Stresses, Distortion, and Fatigue 122 5.1 Residual Stresses 122 5.2 Distortion 126 5.3 Fatigue 131 5.4 Case Studies 137 References 140 Further Reading 141 Problems 141II THE FUSION ZONE 143 6 Basic Solidiﬁcation Concepts 145 6.1 Solute Redistribution during Solidiﬁcation 145 6.2 Solidiﬁcation Modes and Constitutional Supercooling 155 6.3 Microsegregation and Banding 160 6.4 Effect of Cooling Rate 163 6.5 Solidiﬁcation Path 166 References 167 Further Reading 168 Problems 169 7 Weld Metal Solidiﬁcation I: Grain Structure 170 7.1 Epitaxial Growth at Fusion Boundary 170 7.2 Nonepitaxial Growth at Fusion Boundary 172 7.3 Competitive Growth in Bulk Fusion Zone 174 7.4 Effect of Welding Parameters on Grain Structure 174 7.5 Weld Metal Nucleation Mechanisms 178 7.6 Grain Structure Control 187
CONTENTS ix References 195 Further Reading 197 Problems 197 8 Weld Metal Solidiﬁcation II: Microstructure within Grains 199 8.1 Solidiﬁcation Modes 199 8.2 Dendrite and Cell Spacing 204 8.3 Effect of Welding Parameters 206 8.4 Reﬁning Microstructure within Grains 209 References 213 Further Reading 213 Problems 214 9 Post-Solidiﬁcation Phase Transformations 216 9.1 Ferrite-to-Austenite Transformation in Austenitic Stainless Steel Welds 216 9.2 Austenite-to-Ferrite Transformation in Low-Carbon, Low-Alloy Steel Welds 232 References 239 Further Reading 241 Problems 24110 Weld Metal Chemical Inhomogeneities 243 10.1 Microsegregation 243 10.2 Banding 249 10.3 Inclusions and Gas Porosity 250 10.4 Inhomogeneities Near Fusion Boundary 252 10.5 Macrosegregation in Bulk Weld Metal 255 References 260 Further Reading 261 Problems 26111 Weld Metal Solidiﬁcation Cracking 263 11.1 Characteristics, Cause, and Testing 263 11.2 Metallurgical Factors 268 11.3 Mechanical Factors 284 11.4 Reducing Solidiﬁcation Cracking 285 11.5 Case Study: Failure of a Large Exhaust Fan 295 References 296 Further Reading 299 Problems 299
x CONTENTSIII THE PARTIALLY MELTED ZONE 301 12 Formation of the Partially Melted Zone 303 12.1 Evidence of Liquation 303 12.2 Liquation Mechanisms 304 12.3 Directional Solidiﬁcation of Liquated Material 314 12.4 Grain Boundary Segregation 314 12.5 Grain Boundary Solidiﬁcation Modes 316 12.6 Partially Melted Zone in Cast Irons 318 References 318 Problems 319 13 Difﬁculties Associated with the Partially Melted Zone 321 13.1 Liquation Cracking 321 13.2 Loss of Strength and Ductility 328 13.3 Hydrogen Cracking 328 13.4 Remedies 330 References 336 Problems 338IV THE HEAT-AFFECTED ZONE 341 14 Work-Hardened Materials 343 14.1 Background 343 14.2 Recrystallization and Grain Growth in Welding 347 14.3 Effect of Welding Parameters and Process 349 References 351 Further Reading 352 Problems 352 15 Precipitation-Hardening Materials I: Aluminum Alloys 353 15.1 Background 353 15.2 Al–Cu–Mg and Al–Mg–Si Alloys 359 15.3 Al–Zn–Mg Alloys 367 15.4 Friction Stir Welding of Aluminum Alloys 370 References 371 Further Reading 372 Problems 372 16 Precipitation-Hardening Materials II: Nickel-Base Alloys 375 16.1 Background 375
CONTENTS xi 16.2 Reversion of Precipitate and Loss of Strength 379 16.3 Postweld Heat Treatment Cracking 384 References 390 Further Reading 392 Problems 39217 Transformation-Hardening Materials: Carbon and Alloy Steels 393 17.1 Phase Diagram and CCT Diagrams 393 17.2 Carbon Steels 396 17.3 Low-Alloy Steels 404 17.4 Hydrogen Cracking 410 17.5 Reheat Cracking 418 17.6 Lamellar Tearing 422 17.7 Case Studies 425 References 427 Further Reading 429 Problems 43018 Corrosion-Resistant Materials: Stainless Steels 431 18.1 Classiﬁcation of Stainless Steels 431 18.2 Austenitic Stainless Steels 433 18.3 Ferritic Stainless Steels 446 18.4 Martensitic Stainless Steels 449 18.5 Case Study: Failure of a Pipe 451 References 452 Further Reading 453 Problems 454Index 455
PREFACESince the publication of the ﬁrst edition of this book in 1987, there has beenmuch new progress made in welding metallurgy. The purpose for the secondedition is to update and improve the ﬁrst edition. Examples of improvementsinclude (1) much sharper photomicrographs and line drawings; (2) integrationof the phase diagram, thermal cycles, and kinetics with the microstructure toexplain microstructural development and defect formation in welds; and (3)additional exercise problems. Speciﬁc revisions are as follows. In Chapter 1 the illustrations for all welding processes have been re-drawn to show both the overall process and the welding area. In Chapter2 the heat source efﬁciency has been updated and the melting efﬁciencyadded. Chapter 3 has been revised extensively, with the dissolution ofatomic nitrogen, oxygen, and hydrogen in the molten metal considered andelectrochemical reactions added. Chapter 4 has also been revised extensively,with the arc added, and with ﬂow visualization, arc plasma dragging, andturbulence included in weld pool convection. Shot peening is added toChapter 5. Chapter 6 has been revised extensively, with solute redistribution andmicrosegregation expanded and the solidiﬁcation path added. Chapter 7 nowincludes nonepitaxial growth at the fusion boundary and formation of non-dendritic equiaxed grains. In Chapter 8 solidiﬁcation modes are explained withmore illustrations. Chapter 9 has been expanded signiﬁcantly to add ferriteformation mechanisms, new ferrite prediction methods, the effect of coolingrate, and factors affecting the austenite–ferrite transformation. Chapter 10now includes the effect of both solid-state diffusion and dendrite tip under-cooling on microsegregation. Chapter 11 has been revised extensively toinclude the effect of eutectic reactions, liquid distribution, and ductility ofthe solidifying metal on solidiﬁcation cracking and the calculation of fractionof liquid in multicomponent alloys. Chapter 12 has been rewritten completely to include six different liquationmechanisms in the partially melted zone (PMZ), the direction and modes ofgrain boundary (GB) solidiﬁcation, and the resultant GB segregation. Chapter13 has been revised extensively to include the mechanism of PMZ crackingand the effect of the weld-metal composition on cracking. Chapter 15 now includes the heat-affected zone (HAZ) in aluminum–lithium–copper welds and friction stir welds and Chapter 16 the HAZ ofInconel 718. Chapter 17 now includes the effect of multiple-pass welding on xiii
xiv PREFACEreheat cracking and Chapter 18 the grain boundary chromium depletion in asensitized austenitic stainless steel. The author thanks the National Science Foundation and NASA forsupporting his welding research, from which this book draws frequently.He also thanks the American Welding Society and ASM International for per-missions to use numerous copyrighted materials. Finally, he thanks C. Huang,G. Cao, C. Limmaneevichitr, H. D. Lu, K. W. Keehn, and T. Tantanawat for pro-viding technical material, requesting permissions, and proofreading. Sindo KouMadison, Wisconsin
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-4PART IIntroduction
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-41 Fusion Welding ProcessesFusion welding processes will be described in this chapter, including gaswelding, arc welding, and high-energy beam welding. The advantages and dis-advantages of each process will be discussed.1.1 OVERVIEW1.1.1 Fusion Welding ProcessesFusion welding is a joining process that uses fusion of the base metal to makethe weld. The three major types of fusion welding processes are as follows: 1. Gas welding: Oxyacetylene welding (OAW) 2. Arc welding: Shielded metal arc welding (SMAW) Gas–tungsten arc welding (GTAW) Plasma arc welding (PAW) Gas–metal arc welding (GMAW) Flux-cored arc welding (FCAW) Submerged arc welding (SAW) Electroslag welding (ESW) 3. High-energy beam welding: Electron beam welding (EBW) Laser beam welding (LBW) Since there is no arc involved in the electroslag welding process, it is notexactly an arc welding process. For convenience of discussion, it is groupedwith arc welding processes.1.1.2 Power Density of Heat SourceConsider directing a 1.5-kW hair drier very closely to a 304 stainless steel sheet1.6 mm (1/16 in.) thick. Obviously, the power spreads out over an area of roughly 3
4 FUSION WELDING PROCESSES50 mm (2 in.) diameter, and the sheet just heats up gradually but will not melt.With GTAW at 1.5 kW, however, the arc concentrates on a small area of about6 mm (1/4 in.) diameter and can easily produce a weld pool. This example clearlydemonstrates the importance of the power density of the heat source inwelding. The heat sources for the gas, arc, and high-energy beam welding processesare a gas ﬂame, an electric arc, and a high-energy beam, respectively. Thepower density increases from a gas ﬂame to an electric arc and a high-energybeam. As shown in Figure 1.1, as the power density of the heat sourceincreases, the heat input to the workpiece that is required for weldingdecreases. The portion of the workpiece material exposed to a gas ﬂame heatsup so slowly that, before any melting occurs, a large amount of heat is alreadyconducted away into the bulk of the workpiece. Excessive heating can causedamage to the workpiece, including weakening and distortion. On the con-trary, the same material exposed to a sharply focused electron or laser beamcan melt or even vaporize to form a deep keyhole instantaneously, and beforemuch heat is conducted away into the bulk of the workpiece, welding is com-pleted (1). Therefore, the advantages of increasing the power density of the heatsource are deeper weld penetration, higher welding speeds, and better weldquality with less damage to the workpiece, as indicated in Figure 1.1. Figure1.2 shows that the weld strength (of aluminum alloys) increases as the heatinput per unit length of the weld per unit thickness of the workpiece decreases(2). Figure 1.3a shows that angular distortion is much smaller in EBW than in Increasing damage to workpiece Heat input to workpiece gas welding arc welding Increasing penetration, welding speed, weld quality, high energy equipment cost beam welding Power density of heat sourceFigure 1.1 Variation of heat input to the workpiece with power density of the heatsource.
OVERVIEW 5 60 2219 Strength, ksi 50 5083 7039 40 30 6061 5 10 50 100 500 Heat input, kJ/in./in.Figure 1.2 Variation of weld strength with heat input per unit length of weld per unitthickness of workpiece. Reprinted from Mendez and Eagar (2). 8 Productivity, inch of weld/s 0.04 0.4 4 40 400 7 Distortion angle α degree 107 10 6 Laser Capital equipment, dollars Power density, W/m 2 electron beam t 4 105 105 W α GTA 2 Arc 103 103 EBW Flame 0 0 20 40 0.1 1 10 100 (a) Weld thickness t, mm (b) Productivity, cm/sFigure 1.3 Comparisons between welding processes: (a) angular distortion; (b) capitalequipment cost. Reprinted from Mendez and Eagar (2).GTAW (2). Unfortunately, as shown in Figure 1.3b, the costs of laser and elec-tron beam welding machines are very high (2).1.1.3 Welding Processes and MaterialsTable 1.1 summarizes the fusion welding processes recommended for carbonsteels, low-alloy steels, stainless steels, cast irons, nickel-base alloys, and
TABLE 1.1 Overview of Welding Processesa6 Material Thicknessb SMAW SAW GMAW FCAW GTAW PAW ESW OFW EBW LBW Carbon S ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ ✕ Low-alloy S ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ Stainless S ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ Cast iron I ✕ ✕ M ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ Nickel S ✕ ✕ ✕ ✕ ✕ ✕ ✕ and alloys I ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ Aluminum S ✕ ✕ ✕ ✕ ✕ ✕ and alloys I ✕ ✕ ✕ ✕ M ✕ ✕ ✕ T ✕ ✕ a Process code: SMAW, shielded metal arc welding; SAW, submerged arc welding; GMAW, gas–metal arc welding; FCAW, ﬂux-cored arc welding; GTAW, gas–tungsten arc welding; PAW, plasma arc welding; ESW, electroslag welding; OFW, oxyfuel gas welding; EBW, electron beam welding; LBW, laser beam welding. b Abbreviations: S, sheet, up to 3 mm (1/8 in.); I, intermediate, 3–6 mm (1/8–1/4 in.); M, medium, 6–19 mm (1/4–3/4 in.); T, thick, 19 mm (3/4 in.) and up; X, recommended. Source: Welding Handbook (3).
OXYACETYLENE WELDING 7 (a) butt joint t (b) lap joint join ed ge (e) corner joint (c) T-joint (d) Figure 1.4 Five basic types of weld joint designs.aluminum alloys (3). For one example, GMAW can be used for all the materi-als of almost all thickness ranges while GTAW is mostly for thinner workpieces.For another example, any arc welding process that requires the use of a ﬂux,such as SMAW, SAW, FCAW, and ESW, is not applicable to aluminum alloys.1.1.4 Types of Joints and Welding PositionsFigure 1.4 shows the basic weld joint designs in fusion welding: the butt, lap,T-, edge, and corner joints. Figure 1.5 shows the transverse cross section ofsome typical weld joint variations. The surface of the weld is called the face,the two junctions between the face and the workpiece surface are called thetoes, and the portion of the weld beyond the workpiece surface is called thereinforcement. Figure 1.6 shows four welding positions.1.2 OXYACETYLENE WELDING1.2.1 The ProcessGas welding is a welding process that melts and joins metals by heating themwith a ﬂame caused by the reaction between a fuel gas and oxygen. Oxy-acetylene welding (OAW), shown in Figure 1.7, is the most commonly usedgas welding process because of its high ﬂame temperature. A ﬂux may be usedto deoxidize and cleanse the weld metal. The ﬂux melts, solidiﬁes, and formsa slag skin on the resultant weld metal. Figure 1.8 shows three different typesof ﬂames in oxyacetylene welding: neutral, reducing, and oxidizing (4), whichare described next.1.2.2 Three Types of FlamesA. Neutral Flame This refers to the case where oxygen (O2) and acetylene(C2H2) are mixed in equal amounts and burned at the tip of the welding torch.A short inner cone and a longer outer envelope characterize a neutral ﬂame
8 FUSION WELDING PROCESSES Reinforcement Toe (a) Toe (d) Toe Butt joint; T-joint; square weld fillet weld (b) Reinforcement (e) Toe Toe Toe Root Butt joint; T-joint; single-V-groove weld single bevel weld (c) Toe Toe Lap joint; fillet weld Figure 1.5 Typical weld joint variations.(Figure 1.8a). The inner cone is the area where the primary combustion takesplace through the chemical reaction between O2 and C2H2, as shown in Figure1.9. The heat of this reaction accounts for about two-thirds of the total heatgenerated. The products of the primary combustion, CO and H2, react with O2from the surrounding air and form CO2 and H2O. This is the secondary com-bustion, which accounts for about one-third of the total heat generated. Thearea where this secondary combustion takes place is called the outer enve-lope. It is also called the protection envelope since CO and H2 here consumethe O2 entering from the surrounding air, thereby protecting the weld metalfrom oxidation. For most metals, a neutral ﬂame is used.B. Reducing Flame When excess acetylene is used, the resulting ﬂame iscalled a reducing ﬂame.The combustion of acetylene is incomplete.As a result,a greenish acetylene feather between the inert cone and the outer envelopecharacterizes a reducing ﬂame (Figure 1.8b). This ﬂame is reducing in natureand is desirable for welding aluminum alloys because aluminum oxidizeseasily. It is also good for welding high-carbon steels (also called carburizingﬂame in this case) because excess oxygen can oxidize carbon and form CO gasporosity in the weld metal.
OXYACETYLENE WELDING 9 (a) flat (b) horizontal (c) vertical (d) overhead Figure 1.6 Four welding positions. Flow meter Regulator Oxygen Welding direction Valve O2 Gas torch C2H2 Acetylene (a) Workpiece Oxygen/acetylene mixture Filler rod Protection envelope Primary combustion Metal droplet Slag Weld (b) metal Base metal Weld poolFigure 1.7 Oxyacetylene welding: (a) overall process; (b) welding area enlarged.
10 FUSION WELDING PROCESSES Neutral Flame inner cone (a) inner cone Reducing Flame (b) acetylene feather inner cone Oxidizing Flame (c)Figure 1.8 Three types of ﬂames in oxyacetylene welding. Modiﬁed from WeldingJournal (4). Courtesy of American Welding Society. Gas C2H2 + O2 Primary combustion in inner cone (2/3 total heat) : Torch 2C2H2 + 2O2 (from cylinder) 4CO + 2H2 inner Secondary combustion in outer 2800 - 3500 oC cone envelope (1/3 total heat) : Flame 2500 oC outer 4CO + 2O2 (from air) 4CO2 envelope 2H2 + O2 (from air) 2H2O 1000 oCFigure 1.9 Chemical reactions and temperature distribution in a neutral oxyacetyleneﬂame.C. Oxidizing Flame When excess oxygen is used, the ﬂame becomes oxi-dizing because of the presence of unconsumed oxygen. A short white innercone characterizes an oxidizing ﬂame (Figure 1.8c). This ﬂame is preferredwhen welding brass because copper oxide covers the weld pool and thus pre-vents zinc from evaporating from the weld pool.1.2.3 Advantages and DisadvantagesThe main advantage of the oxyacetylene welding process is that the equip-ment is simple, portable, and inexpensive. Therefore, it is convenient for main-tenance and repair applications. However, due to its limited power density, the
SHIELDED METAL ARC WELDING 11welding speed is very low and the total heat input per unit length of the weldis rather high, resulting in large heat-affected zones and severe distortion. Theoxyacetylene welding process is not recommended for welding reactive metalssuch as titanium and zirconium because of its limited protection power.1.3 SHIELDED METAL ARC WELDING1.3.1 The ProcessShielded metal arc welding (SMAW) is a process that melts and joins metalsby heating them with an arc established between a sticklike covered electrodeand the metals, as shown in Figure 1.10. It is often called stick welding.The electrode holder is connected through a welding cable to one terminalof the power source and the workpiece is connected through a second cableto the other terminal of the power source (Figure 1.10a). The core of the covered electrode, the core wire, conducts the electriccurrent to the arc and provides ﬁller metal for the joint. For electrical contact,the top 1.5 cm of the core wire is bare and held by the electrode holder. Theelectrode holder is essentially a metal clamp with an electrically insulatedoutside shell for the welder to hold safely. The heat of the arc causes both the core wire and the ﬂux covering at theelectrode tip to melt off as droplets (Figure 1.10b). The molten metal collectsin the weld pool and solidiﬁes into the weld metal. The lighter molten ﬂux, onthe other hand, ﬂoats on the pool surface and solidiﬁes into a slag layer at thetop of the weld metal.1.3.2 Functions of Electrode CoveringThe covering of the electrode contains various chemicals and even metalpowder in order to perform one or more of the functions described below.A. Protection It provides a gaseous shield to protect the molten metal fromair. For a cellulose-type electrode, the covering contains cellulose, (C6H10O5)x.A large volume of gas mixture of H2, CO, H2O, and CO2 is produced whencellulose in the electrode covering is heated and decomposes. For a limestone-(CaCO3Ϫ) type electrode, on the other hand, CO2 gas and CaO slag form whenthe limestone decomposes. The limestone-type electrode is a low-hydrogen-type electrode because it produces a gaseous shield low in hydrogen. It is oftenused for welding metals that are susceptible to hydrogen cracking, such ashigh-strength steels.B. Deoxidation It provides deoxidizers and ﬂuxing agents to deoxidize andcleanse the weld metal. The solid slag formed also protects the already solid-iﬁed but still hot weld metal from oxidation.
12 FUSION WELDING PROCESSES (a) Electrode Power holder Source Welding Cable 1 direction Stick electrode Cable 2 Workpiece Core wire (b) Flux covering Metal Gaseous shield droplet Flux Arc droplet Slag Weld metal Base metal Weld poolFigure 1.10 Shielded metal arc welding: (a) overall process; (b) welding area enlarged.C. Arc Stabilization It provides arc stabilizers to help maintain a stablearc. The arc is an ionic gas (a plasma) that conducts the electric current.Arc stabilizers are compounds that decompose readily into ions in the arc,such as potassium oxalate and lithium carbonate. They increase the electricalconductivity of the arc and help the arc conduct the electric current moresmoothly.D. Metal Addition It provides alloying elements and/or metal powder tothe weld pool. The former helps control the composition of the weld metalwhile the latter helps increase the deposition rate.1.3.3 Advantages and DisadvantagesThe welding equipment is relatively simple, portable, and inexpensive as com-pared to other arc welding processes. For this reason, SMAW is often used formaintenance, repair, and ﬁeld construction. However, the gas shield in SMAWis not clean enough for reactive metals such as aluminum and titanium. Thedeposition rate is limited by the fact that the electrode covering tends to over-heat and fall off when excessively high welding currents are used. The limitedlength of the electrode (about 35 cm) requires electrode changing, and thisfurther reduces the overall production rate.
GAS–TUNGSTEN ARC WELDING 131.4 GAS–TUNGSTEN ARC WELDING1.4.1 The ProcessGas–tungsten arc welding (GTAW) is a process that melts and joins metals byheating them with an arc established between a nonconsumable tungsten elec-trode and the metals, as shown in Figure 1.11. The torch holding the tungstenelectrode is connected to a shielding gas cylinder as well as one terminal ofthe power source, as shown in Figure 1.11a. The tungsten electrode is usuallyin contact with a water-cooled copper tube, called the contact tube, as shownin Figure 1.11b, which is connected to the welding cable (cable 1) from theterminal. This allows both the welding current from the power source toenter the electrode and the electrode to be cooled to prevent overheating. Theworkpiece is connected to the other terminal of the power source through adifferent cable (cable 2). The shielding gas goes through the torch body andis directed by a nozzle toward the weld pool to protect it from the air. Pro-tection from the air is much better in GTAW than in SMAW because an inertgas such as argon or helium is usually used as the shielding gas and becausethe shielding gas is directed toward the weld pool. For this reason, GTAW is Flow Regulator meter (a) Welding Shielding gas direction Torch cylinder Cable 1 Filler rod Cable 2 Power source Workpiece Tungsten electrode Shielding (b) gas Contact tube Filler Cable 1 rod Shielding gas Shielding gas nozzle Metal Arc droplet Weld metal Base metal Weld poolFigure 1.11 Gas–tungsten arc welding: (a) overall process; (b) welding area enlarged.
14 FUSION WELDING PROCESSESalso called tungsten–inert gas (TIG) welding. However, in special occasions anoninert gas (Chapter 3) can be added in a small quantity to the shielding gas.Therefore, GTAW seems a more appropriate name for this welding process.When a ﬁller rod is needed, for instance, for joining thicker materials, it canbe fed either manually or automatically into the arc.1.4.2 PolarityFigure 1.12 shows three different polarities in GTAW (5), which are describednext.A. Direct-Current Electrode Negative (DCEN) This, also called the straightpolarity, is the most common polarity in GTAW. The electrode is connected tothe negative terminal of the power supply. As shown in Figure 1.12a, electronsare emitted from the tungsten electrode and accelerated while travelingthrough the arc. A signiﬁcant amount of energy, called the work function, isrequired for an electron to be emitted from the electrode. When the electronenters the workpiece, an amount of energy equivalent to the work function isreleased. This is why in GTAW with DCEN more power (about two-thirds) islocated at the work end of the arc and less (about one-third) at the electrodeend. Consequently, a relatively narrow and deep weld is produced.B. Direct-Current Electrode Positive (DCEP) This is also called the reversepolarity. The electrode is connected to the positive terminal of the powersource. As shown in Figure 1.12b, the heating effect of electrons is now at thetungsten electrode rather than at the workpiece. Consequently, a shallow weldis produced. Furthermore, a large-diameter, water-cooled electrodes must beused in order to prevent the electrode tip from melting. The positive ions ofthe shielding gas bombard the workpiece, as shown in Figure 1.13, knockingoff oxide ﬁlms and producing a clean weld surface. Therefore, DCEP can be DC electrode DC electrode AC negative positive pool deep weld, shallow weld, intermediate no surface cleaning surface cleaning (a) (b) (c) Figure 1.12 Three different polarities in GTAW.
GAS–TUNGSTEN ARC WELDING 15 Cleaning action (electrode positive) bombarding heavy ion Ar+ knocked-off atoms M O oxide film on surface M O M O M Workpiece (negative) Figure 1.13 Surface cleaning action in GTAW with DC electrode positive.used for welding thin sheets of strong oxide-forming materials such as alu-minum and magnesium, where deep penetration is not required.C. Alternating Current (AC) Reasonably good penetration and oxidecleaning action can both be obtained, as illustrated in Figure 1.12c.This is oftenused for welding aluminum alloys.1.4.3 ElectrodesTungsten electrodes with 2% cerium or thorium have better electronemissivity, current-carrying capacity, and resistance to contamination thanpure tungsten electrodes (3). As a result, arc starting is easier and the arc ismore stable. The electron emissivity refers to the ability of the electrode tipto emit electrons. A lower electron emissivity implies a higher electrode tiptemperature required to emit electrons and hence a greater risk of melting thetip.1.4.4 Shielding GasesBoth argon and helium can be used. Table 1.2 lists the properties of someshielding gases (6). As shown, the ionization potentials for argon and heliumare 15.7 and 24.5 eV (electron volts), respectively. Since it is easier to ionizeargon than helium, arc initiation is easier and the voltage drop across the arcis lower with argon. Also, since argon is heavier than helium, it offers moreeffective shielding and greater resistance to cross draft than helium. WithDCEP or AC, argon also has a greater oxide cleaning action than helium.These advantages plus the lower cost of argon make it more attractive forGTAW than helium.
16 FUSION WELDING PROCESSESTABLE 1.2 Properties of Shielding Gases Used for Welding Molecular Speciﬁc Gravity Ionization Chemical Weight with Respect to Air Density PotentialGas Symbol (g/mol) at 1 atm and 0°C (g/L) (eV)Argon Ar 39.95 1.38 1.784 15.7Carbon dioxide CO2 44.01 1.53 1.978 14.4Helium He 4.00 0.1368 0.178 24.5Hydrogen H2 2.016 0.0695 0.090 13.5Nitrogen N2 28.01 0.967 1.25 14.5Oxygen O2 32.00 1.105 1.43 13.2Source: Reprinted from Lyttle (6). Because of the greater voltage drop across a helium arc than an argon arc,however, higher power inputs and greater sensitivity to variations in the arclength can be obtained with helium. The former allows the welding of thickersections and the use of higher welding speeds. The latter, on the other hand,allows a better control of the arc length during automatic GTAW.1.4.5 Advantages and DisadvantagesGas–tungsten arc welding is suitable for joining thin sections because of itslimited heat inputs. The feeding rate of the ﬁller metal is somewhat indepen-dent of the welding current, thus allowing a variation in the relative amountof the fusion of the base metal and the fusion of the ﬁller metal. Therefore,the control of dilution and energy input to the weld can be achieved withoutchanging the size of the weld. It can also be used to weld butt joints of thinsheets by fusion alone, that is, without the addition of ﬁller metals or autoge-nous welding. Since the GTAW process is a very clean welding process, it canbe used to weld reactive metals, such as titanium and zirconium, aluminum,and magnesium. However, the deposition rate in GTAW is low. Excessive welding currentscan cause melting of the tungsten electrode and results in brittle tungsteninclusions in the weld metal. However, by using preheated ﬁller metals, thedeposition rate can be improved. In the hot-wire GTAW process, the wire isfed into and in contact with the weld pool so that resistance heating can beobtained by passing an electric current through the wire.1.5 PLASMA ARC WELDING1.5.1 The ProcessPlasma arc welding (PAW) is an arc welding process that melts and joins metalsby heating them with a constricted arc established between a tungsten elec-
PLASMA ARC WELDING 17trode and the metals, as shown in Figure 1.14. It is similar to GTAW, but anoriﬁce gas as well as a shielding gas is used. As shown in Figure 1.15, the arc inPAW is constricted or collimated because of the converging action of the oriﬁcegas nozzle, and the arc expands only slightly with increasing arc length (5).Direct-current electrode negative is normally used, but a special variable-polarity PAW machine has been developed for welding aluminum, where thepresence of aluminum oxide ﬁlms prevents a keyhole from being established.1.5.2 Arc InitiationThe tungsten electrode sticks out of the shielding gas nozzle in GTAW (Figure1.11b) while it is recessed in the oriﬁce gas nozzle in PAW (Figure 1.14b). Con-sequently, arc initiation cannot be achieved by striking the electrode tip againstthe workpiece as in GTAW. The control console (Figure 1.14a) allows a pilotarc to be initiated, with the help of a high-frequency generator, between theelectrode tip and the water-cooled oriﬁce gas nozzle. The arc is then gradually Shielding gas (a) Control console Orifice gas Welding direction Power Source Torch Filler rod Cables Workpiece Orifice gas Tungsten Shielding (b) electrode gas Orifice gas nozzle Shielding gas (water cooled) nozzle Orifice Arc plasma Molten metal Weld metal Base metal KeyholeFigure 1.14 Plasma arc welding: (a) overall process; (b) welding area enlarged andshown with keyholing.
18 FUSION WELDING PROCESSES Plasma arc Gas tungsten arcFigure 1.15 Comparison between a gas–tungsten arc and a plasma arc. From WeldingHandbook (5). Courtesy of American Welding Society.transferred from between the electrode tip and the oriﬁce gas nozzle tobetween the electrode tip and the workpiece.1.5.3 KeyholingIn addition to the melt-in mode adopted in conventional arc welding processes(such as GTAW), the keyholing mode can also be used in PAW in certainranges of metal thickness (e.g., 2.5–6.4 mm). With proper combinations of theoriﬁce gas ﬂow, the travel speed, and the welding current, keyholing is possi-ble. Keyholing is a positive indication of full penetration and it allows theuse of signiﬁcantly higher welding speeds than GTAW. For example, it hasbeen reported (7) that PAW took one-ﬁfth to one-tenth as long to completea 2.5-m-long weld in 6.4-mm-thick 410 stainless steel as GTAW. Gas–tungstenarc welding requires multiple passes and is limited in welding speed. As shownin Figure 1.16, 304 stainless steel up to 13 mm (1/2 in.) thick can be welded in asingle pass (8). The wine-cup-shaped weld is common in keyholing PAW.1.5.4 Advantages and DisadvantagesPlasma arc welding has several advantages over GTAW. With a collimated arc,PAW is less sensitive to unintentional arc length variations during manualwelding and thus requires less operator skill than GTAW. The short arc lengthin GTAW can cause a welder to unintentionally touch the weld pool with theelectrode tip and contaminate the weld metal with tungsten. However, PAWdoes not have this problem since the electrode is recessed in the nozzle. Asalready mentioned, the keyhole is a positive indication of full penetration, andit allows higher welding speeds to be used in PAW. However, the PAW torch is more complicated. It requires proper electrodetip conﬁguration and positioning, selection of correct oriﬁce size for the appli-cation, and setting of both oriﬁce and shielding gas ﬂow rates. Because of the
GAS–METAL ARC WELDING 19Figure 1.16 A plasma arc weld made in 13-mm-thick 304 stainless steel with keyhol-ing. From Lesnewich (8).need for a control console, the equipment cost is higher in PAW than in GTAW.The equipment for variable-polarity PAW is much more expensive than thatfor GTAW.1.6 GAS–METAL ARC WELDING1.6.1 The ProcessGas–metal arc welding (GMAW) is a process that melts and joins metals byheating them with an arc established between a continuously fed ﬁller wireelectrode and the metals, as shown in Figure 1.17. Shielding of the arc and themolten weld pool is often obtained by using inert gases such as argon andhelium, and this is why GMAW is also called the metal–inert gas (MIG)welding process. Since noninert gases, particularly CO2, are also used, GMAWseems a more appropriate name. This is the most widely used arc weldingprocess for aluminum alloys. Figure 1.18 shows gas–metal arc welds of 5083aluminum, one made with Ar shielding and the other with 75% He–25% Arshielding (9). Unlike in GTAW, DCEP is used in GMAW. A stable arc, smoothmetal transfer with low spatter loss and good weld penetration can beobtained. With DCEN or AC, however, metal transfer is erratic.1.6.2 Shielding GasesArgon, helium, and their mixtures are used for nonferrous metals as well asstainless and alloy steels. The arc energy is less uniformly dispersed in an Ararc than in a He arc because of the lower thermal conductivity of Ar. Conse-quently, the Ar arc plasma has a very high energy core and an outer mantleof lesser thermal energy. This helps produce a stable, axial transfer of metal
20 FUSION WELDING PROCESSES Flow meter Regulator (a) Wire Wire drive reel & control Welding Wire direction Gun electrode Workpiece Power Shielding Cable 1 Source gas cylinder Cable 2 Wire electrode Shielding gas Contact tube (b) Cable 1 Shielding Shielding gas gas nozzle Metal Arc droplet Weld metal Base metal Weld poolFigure 1.17 Gas–metal arc welding: (a) overall process; (b) welding area enlarged.Figure 1.18 Gas–metal arc welds in 6.4-mm-thick 5083 aluminum made with argon(left) and 75% He–25% Ar (right). Reprinted from Gibbs (9). Courtesy of AmericanWelding Society.droplets through an Ar arc plasma. The resultant weld transverse cross sectionis often characterized by a papillary- (nipple-) type penetration pattern (10)such as that shown in Figure 1.18 (left). With pure He shielding, on the otherhand, a broad, parabolic-type penetration is often observed. With ferrous metals, however, He shielding may produce spatter and Arshielding may cause undercutting at the fusion lines. Adding O2 (about 3%)or CO2 (about 9%) to Ar reduces the problems. Carbon and low-alloy steelsare often welded with CO2 as the shielding gas, the advantages being higher
GAS–METAL ARC WELDING 21welding speed, greater penetration, and lower cost. Since CO2 shielding pro-duces a high level of spatter, a relatively low voltage is used to maintain a shortburied arc to minimize spatter; that is, the electrode tip is actually below theworkpiece surface (10).1.6.3 Modes of Metal TransferThe molten metal at the electrode tip can be transferred to the weld pool bythree basic transfer modes: globular, spray, and short-circuiting.A. Globular Transfer Discrete metal drops close to or larger than theelectrode diameter travel across the arc gap under the inﬂuence of gravity.Figure 1.19a shows globular transfer during GMAW of steel at 180 A andwith Ar–2% O2 shielding (11). Globular transfer often is not smooth andproduces spatter. At relatively low welding current globular transferoccurs regardless of the type of the shielding gas. With CO2 and He, however,it occurs at all usable welding currents. As already mentioned, a shortburied arc is used in CO2-shielded GMAW of carbon and low-alloy steels tominimize spatter.Figure 1.19 Metal transfer during GMAW of steel with Ar–2% O2 shielding: (a)globular transfer at 180 A and 29 V shown at every 3 ¥ 10-3 s; (b) spray transfer at320 A and 29 V shown at every 2.5 ¥ 10-4 s. Reprinted from Jones et al. (11). Courtesyof American Welding Society.
22 FUSION WELDING PROCESSESB. Spray Transfer Above a critical current level, small discrete metal dropstravel across the arc gap under the inﬂuence of the electromagnetic force atmuch higher frequency and speed than in the globular mode. Figure 1.19bshows spray transfer during GMAW of steel at 320 A and with Ar–2% O2shielding (11). Metal transfer is much more stable and spatter free. The criti-cal current level depends on the material and size of the electrode and thecomposition of the shielding gas. In the case of Figure 1.19, the critical currentwas found to be between 280 and 320 A (11).C. Short-Circuiting Transfer The molten metal at the electrode tip is trans-ferred from the electrode to the weld pool when it touches the pool surface,that is, when short circuiting occurs. Short-circuiting transfer encompasses thelowest range of welding currents and electrode diameters. It produces a smalland fast-freezing weld pool that is desirable for welding thin sections, out-of-position welding (such as overhead-position welding), and bridging large rootopenings.1.6.4 Advantages and DisadvantagesLike GTAW, GMAW can be very clean when using an inert shielding gas. Themain advantage of GMAW over GTAW is the much higher deposition rate,which allows thicker workpieces to be welded at higher welding speeds. Thedual-torch and twin-wire processes further increase the deposition rate ofGMAW (12). The skill to maintain a very short and yet stable arc in GTAWis not required. However, GMAW guns can be bulky and difﬁcult-to-reachsmall areas or corners.1.7 FLUX-CORE ARC WELDING1.7.1 The ProcessFlux-core arc welding (FCAW) is similar to GMAW, as shown in Figure 1.20a.However, as shown in Figure 1.20b, the wire electrode is ﬂux cored rather thansolid; that is, the electrode is a metal tube with ﬂux wrapped inside. The func-tions of the ﬂux are similar to those of the electrode covering in SMAW, includ-ing protecting the molten metal from air. The use of additional shielding gasis optional.1.8 SUBMERGED ARC WELDING1.8.1 The ProcessSubmerged arc welding (SAW) is a process that melts and joins metals byheating them with an arc established between a consumable wire electrode
SUBMERGED ARC WELDING 23 Regulator Flow meter (a) Wire Wire drive reel & control Welding Wire direction Gun electrode Power Shielding Workpiece Source gas Cable 1 cylinder Cable 2 Wire electrode Shielding gas Contact tube (b) Cable 1 Shielding gas Metal droplet nozzle Flux droplet Arc Slag Shielding gas (optional) Weld metal Base metal Weld pool Figure 1.20 Flux-core arc welding: (a) overall process; (b) welding area enlarged.and the metals, with the arc being shielded by a molten slag and granular ﬂux,as shown in Figure 1.21. This process differs from the arc welding processesdiscussed so far in that the arc is submerged and thus invisible. The ﬂux is sup-plied from a hopper (Figure 1.21a), which travels with the torch. No shieldinggas is needed because the molten metal is separated from the air by the moltenslag and granular ﬂux (Figure 1.21b). Direct-current electrode positive is mostoften used. However, at very high welding currents (e.g., above 900 A) AC ispreferred in order to minimize arc blow. Arc blow is caused by the electro-magnetic (Lorentz) force as a result of the interaction between the electriccurrent itself and the magnetic ﬁeld it induces.1.8.2 Advantages and DisadvantagesThe protecting and reﬁning action of the slag helps produce clean welds inSAW. Since the arc is submerged, spatter and heat losses to the surroundingair are eliminated even at high welding currents. Both alloying elements andmetal powders can be added to the granular ﬂux to control the weld metalcomposition and increase the deposition rate, respectively. Using two or moreelectrodes in tandem further increases the deposition rate. Because of its high
24 FUSION WELDING PROCESSES Flux hopper Wire reel (a) Wire electrode Wire drive & control Welding Cables direction Power Source Workpiece Granular flux Droplet Wire electrode Arc Molten slag (b) Solidified slag Base metal Weld metal Metal poolFigure 1.21 Submerged arc welding: (a) overall process; (b) welding area enlarged.deposition rate, workpieces much thicker than that in GTAW and GMAW canbe welded by SAW. However, the relatively large volumes of molten slag andmetal pool often limit SAW to ﬂat-position welding and circumferentialwelding (of pipes). The relatively high heat input can reduce the weld qualityand increase distortions.1.9 ELECTROSLAG WELDING1.9.1 The ProcessElectroslag welding (ESW) is a process that melts and joins metals by heatingthem with a pool of molten slag held between the metals and continuouslyfeeding a ﬁller wire electrode into it, as shown in Figure 1.22. The weld poolis covered with molten slag and moves upward as welding progresses. A pairof water-cooled copper shoes, one in the front of the workpiece and onebehind it, keeps the weld pool and the molten slag from breaking out. Similarto SAW, the molten slag in ESW protects the weld metal from air and reﬁnesit. Strictly speaking, however, ESW is not an arc welding process, because thearc exists only during the initiation period of the process, that is, when the arc
ELECTROSLAG WELDING 25 Wire reel Wire feed motor & control Workpiece Cable Water- cooled Power (a) Source copper shoes Cable Bottom support Wire electrode Consumable guide tube Base metal (b) Molten slag Weld pool Weld metal Figure 1.22 Electroslag welding: (a) overall process; (b) welding area enlarged.heats up the ﬂux and melts it. The arc is then extinguished, and the resistanceheating generated by the electric current passing through the slag keeps itmolten. In order to make heating more uniform, the electrode is often oscil-lated, especially when welding thicker sections. Figure 1.23 is the transversecross section of an electroslag weld in a steel 7 cm thick (13). Typical examplesof the application of ESW include the welding of ship hulls, storage tanks, andbridges.1.9.2 Advantages and DisadvantagesElectroslag welding can have extremely high deposition rates, but only onesingle pass is required no matter how thick the workpiece is. Unlike SAW orother arc welding processes, there is no angular distortion in ESW because the
26 FUSION WELDING PROCESSESFigure 1.23 Transverse cross section of electroslag weld in 70-mm-thick steel.Reprinted from Eichhorn et al. (13). Courtesy of American Welding Society. Deposition Rate, Lb/hr 0 40 80 120 160 200 6010 6012 SMAW Welding Process (100% Duty Cycle) 7018 7024 cold GTAW/PAW wire fine wire spray GMAW CO2 shielded FCAW iron powder SAW with iron powder added 1 electrode 2 electrodes 3 electrodes ESW 4 electrodes 5 electrodes 0 20 40 60 80 Deposition Rate, Kg/hr Figure 1.24 Deposition rate in arc welding processes. Modiﬁed from Cary (14).weld is symmetrical with respect to its axis. However, the heat input is veryhigh and the weld quality can be rather poor, including low toughness causedby the coarse grains in the fusion zone and the heat-affected zone. Electroslagwelding is restricted to vertical position welding because of the very largepools of the molten metal and slag. Figure 1.24 summarizes the deposition rates of the arc welding processesdiscussed so far (14). As shown, the deposition rate increases in the order of
ELECTRON BEAM WELDING 27GTAW, SMAW, GMAW and FCAW, SAW, and ESW. The deposition rate canbe much increased by adding iron powder in SAW or using more than onewire in SAW, ESW, and GMAW (not shown).1.10 ELECTRON BEAM WELDING1.10.1 The ProcessElectron beam welding (EBW) is a process that melts and joins metals byheating them with an electron beam. As shown in Figure 1.25a, the cathode ofthe electron beam gun is a negatively charged ﬁlament (15). When heated upto its thermionic emission temperature, this ﬁlament emits electrons. Theseelectrons are accelerated by the electric ﬁeld between a negatively chargedbias electrode (located slightly below the cathode) and the anode. They passthrough the hole in the anode and are focused by an electromagnetic coil toa point at the workpiece surface. The beam currents and the acceleratingvoltages employed for typical EBW vary over the ranges of 50–1000 mA and30–175 kV, respectively. An electron beam of very high intensity can vaporizethe metal and form a vapor hole during welding, that is, a keyhole, as depictedin Figure 1.25b. Figure 1.26 shows that the beam diameter decreases with decreasingambient pressure (1). Electrons are scattered when they hit air molecules, andthe lower the ambient pressure, the less they are scattered. This is the mainreason for EBW in a vacuum chamber. The electron beam can be focused to diameters in the range of 0.3–0.8 mmand the resulting power density can be as high as 1010 W/m2 (1). The very high bias high electrode voltage cathode electron anode beam focusing weld coil weldingn weld pool bead directio vacuum chamber electron moten beam metal to cross- keyhole section pump specimen of weld (a) (b)Figure 1.25 Electron beam welding: (a) process; (b) keyhole. Modiﬁed from Arata(15).
28 FUSION WELDING PROCESSES 750 torr 500 torr 250 torr 50 torr 5 torrFigure 1.26 Dispersion of electron beam at various ambient pressures (1). Reprintedfrom Welding Handbook (1). Courtesy of American Welding Society. gas tungsten arc weld electron beam 13 mm weld (0.5 in) (a) (b)Figure 1.27 Welds in 13-mm-thick 2219 aluminum: (a) electron beam weld; (b)gas–tungsten arc weld. From Farrell (16).power density makes it possible to vaporize the material and produce a deep-penetrating keyhole and hence weld. Figure 1.27 shows a single-pass electronbeam weld and a dual-pass gas–tungsten arc weld in a 13-mm-thick (0.5-in.)2219 aluminum, the former being much narrower (16). The energy requiredper unit length of the weld is much lower in the electron beam weld (1.5 kJ/cm,or 3.8 kJ/in.) than in the gas–tungsten arc weld (22.7 kJ/cm, or 57.6 kJ/in.). Electron beam welding is not intended for incompletely degassed materi-als such as rimmed steels. Under high welding speeds gas bubbles that do nothave enough time to leave deep weld pools result in weld porosity. Materialscontaining high-vapor-pressure constituents, such as Mg alloys and Pb-containing alloys, are not recommended for EBW because evaporation ofthese elements tends to foul the pumps or contaminate the vacuum system.1.10.2 Advantages and DisadvantagesWith a very high power density in EBW, full-penetration keyholing is possi-ble even in thick workpieces. Joints that require multiple-pass arc welding can
LASER BEAM WELDING 29 SB49 A387 Missed joint (a) 48356 47421 (b)Figure 1.28 Missed joints in electron beam welds in 150-mm-thick steels: (a)2.25Cr–1Mo steel with a transverse ﬂux density of 3.5 G parallel to joint plane; (b) SB(C–Mn) steel and A387 (2.25Cr–1Mo) steel. Reprinted from Blakeley and Sanderson(17). Courtesy of American Welding Society.be welded in a single pass at a high welding speed. Consequently, the totalheat input per unit length of the weld is much lower than that in arc welding,resulting in a very narrow heat-affected zone and little distortion. Reactiveand refractory metals can be welded in vacuum where there is no air to causecontamination. Some dissimilar metals can also be welded because the veryrapid cooling in EBW can prevent the formation of coarse, brittle intermetal-lic compounds. When welding parts varying greatly in mass and size, the abilityof the electron beam to precisely locate the weld and form a favorably shapedfusion zone helps prevent excessive melting of the smaller part. However, the equipment cost for EBW is very high. The requirement ofhigh vacuum (10-3–10-6 torr) and x-ray shielding is inconvenient and time con-suming. For this reason, medium-vacuum (10-3–25 torr) EBW and nonvacuum(1 atm) EBW have also been developed. The ﬁne beam size requires preciseﬁt-up of the joint and alignment of the joint with the gun. As shown in Figure1.28, residual and dissimilar metal magnetism can cause beam deﬂection andresult in missed joints (17).1.11 LASER BEAM WELDING1.11.1 The ProcessLaser beam welding (LBW) is a process that melts and joins metals by heatingthem with a laser beam. The laser beam can be produced either by a solid-
30 FUSION WELDING PROCESSESstate laser or a gas laser. In either case, the laser beam can be focused anddirected by optical means to achieve high power densities. In a solid-statelaser, a single crystal is doped with small concentrations of transition elementsor rare earth elements. For instance, in a YAG laser the crystal of yttrium–aluminum–garnet (YAG) is doped with neodymium. The electrons of thedopant element can be selectively excited to higher energy levels upon expo-sure to high-intensity ﬂash lamps, as shown in Figure 1.29a. Lasing occurs whenthese excited electrons return to their normal energy state, as shown in Figure1.29b. The power level of solid-state lasers has improved signiﬁcantly, and con-tinuous YAG lasers of 3 or even 5 kW have been developed. In a CO2 laser, a gas mixture of CO2, N2, and He is continuously excitedby electrodes connected to the power supply and lases continuously. Higher Reflecting mirror Power source Crystal High (a) intensity flash lamp Cooling system Patially reflecting mirror Focusing lens Pool Weld Travel direction Workpiece energy absorbed energy emitted from flash lamp as heat excited outer intermediate electron energy ground levels inner electrons nucleus (b) energy normal emitted as electron light (photon) orbitsFigure 1.29 Laser beam welding with solid-state laser: (a) process; (b) energy absorp-tion and emission during laser action. Modiﬁed from Welding Handbook (1).
LASER BEAM WELDING 31 laser beam weldingn weld pool weld directio bead molten metal cross- keyhole section of weld 2 mm (a) (b)Figure 1.30 Laser beam welding with CO2 laser: (a) process; (b) weld in 13-mm-thickA633 steel. (b) Courtesy of E.A. Metzbower.power can be achieved by a CO2 laser than a solid-state laser, for instance,15 kW. Figure 1.30a shows LBW in the keyholing mode. Figure 1.30b shows aweld in a 13-mm-thick A633 steel made with a 15-kW CO2 laser at 20 mm/s(18). Besides solid-state and gas lasers, semiconductor-based diode lasers havealso been developed. Diode lasers of 2.5 kW power and 1 mm focus diameterhave been demonstrated (19). While keyholing is not yet possible, conduction-mode (surface melting) welding has produced full-penetration welds with adepth–width ratio of 3 : 1 or better in 3-mm-thick sheets.1.11.2 ReﬂectivityThe very high reﬂectivity of a laser beam by the metal surface is a well-knownproblem in LBW. As much as about 95% of the CO2 beam power can bereﬂected by a polished metal surface. Reﬂectivity is slightly lower with a YAGlaser beam. Surface modiﬁcations such as roughening, oxidizing, and coatingcan reduce reﬂectivity signiﬁcantly (20). Once keyholing is established, absorp-tion is high because the beam is trapped inside the hole by internal reﬂection.1.11.3 Shielding GasA plasma (an ionic gas) is produced during LBW, especially at high powerlevels, due to ionization by the laser beam. The plasma can absorb and scatterthe laser beam and reduce the depth of penetration signiﬁcantly. It is there-fore necessary to remove or suppress the plasma (21). The shielding gas forprotecting the molten metal can be directed sideways to blow and deﬂect theplasma away from the beam path. Helium is often preferred to argon as theshielding gas for high-power LBW because of greater penetration depth (22).
32 FUSION WELDING PROCESSESSince the ionization energy of helium (24.5 eV) is higher than that of argon(15.7 eV), helium is less likely to be ionized and become part of the plasmathan argon. However, helium is lighter than air and is thus less effective in dis-placing air from the beam path. Helium–10% Ar shielding has been foundto improve penetration over pure He at high-speed welding where a lightshielding gas may not have enough time to displace air from the beam path(23).1.11.4 Lasers in Arc WeldingAs shown in Figure 1.31, laser-assisted gas metal arc welding (LAGMAW) hasdemonstrated signiﬁcantly greater penetration than conventional GMAW(24). In addition to direct heating, the laser beam acts to focus the arc byheating its path through the arc. This increases ionization and hence the con-ductivity of the arc along the beam path and helps focus the arc energy alongthe path. It has been suggested that combining the arc power with a 5-kW CO2laser, LAGMAW has the potential to achieve weld penetration in mild steelequivalent to that of a 20–25-kW laser (24). Albright et al. (25) have shownthat a lower power CO (not CO2) laser of 7 W and 1 mm diameter can initi-ate, guide, and focus an Ar–1% CO gas–tungsten arc.1.11.5 Advantages and DisadvantagesLike EBW, LBW can produce deep and narrow welds at high welding speeds,with a narrow heat-affected zone and little distortion of the workpiece. It can 12 10 Penetration (mm) 8 6 4 LAGMAW 2 GMAW 0 300 400 500 600 700 Welding current (A)Figure 1.31 Weld penetration in GMAW and laser-assisted GMAW using CO2 laserat 5.7 kW. Reprinted from Hyatt et al. (24). Courtesy of American Welding Society.
REFERENCES 33be used for welding dissimilar metals or parts varying greatly in mass and size.Unlike EBW, however, vacuum and x-ray shielding are not required in LBW.However, the very high reﬂectivity of a laser beam by the metal surface is amajor drawback, as already mentioned. Like EBW, the equipment cost is veryhigh, and precise joint ﬁt-up and alignment are required.REFERENCES 1. Welding Handbook, Vol. 3, 7th ed., American Welding Society, Miami, FL, 1980, pp. 170–238. 2. Mendez, P. F., and Eagar, T. W., Advanced Materials and Processes, 159: 39, 2001. 3. Welding Handbook, Vol. 1, 7th ed., American Welding Society, Miami, FL, 1976, pp. 2–32. 4. Welding Workbook, Data Sheet 212a, Weld. J., 77: 65, 1998. 5. Welding Handbook, Vol. 2, 7th ed., American Welding Society, Miami, FL, 1978, pp. 78–112, 296–330. 6. Lyttle, K. A., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993, p. 64. 7. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979, pp. 2–1 to 3– 40. 8. Lesnewich, A., in Weldability of Steels, 3rd ed., Eds. R. D. Stout and W. D. Doty, Welding Research Council, New York, 1978, p. 5. 9. Gibbs, F. E., Weld. J., 59: 23, 1980.10. Fact Sheet—Choosing Shielding for GMA Welding, Weld. J., 79: 18, 2000.11. Jones, L. A., Eagar, T. W., and Lang, J. H., Weld. J., 77: 135s, 1998.12. Blackman, S. A., and Dorling, D. V., Weld. J., 79: 39, 2000.13. Eichhorn, F., Remmel, J., and Wubbels, B., Weld. J., 63: 37, 1984.14. Cary, H. B., Modern Welding Technology, Prentice-Hall, Englewood Cliffs, NJ, 1979.15. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Appli- cation to Heat Processing, Okada Memorial Japan Society, 1985.16. Farrell, W. J., The Use of Electron Beam to Fabricate Structural Members, Creative Manufacturing Seminars, ASTME Paper SP 63-208, 1962–1963.17. Blakeley, P. J., and Sanderson, A., Weld. J., 63: 42, 1984.18. Metzbower, E. A., private communication, Naval Research Laboratory, Washington, DC.19. Bliedtner, J., Heyse, Th., Jahn, D., Michel, G., Muller, H., and Wolff, D., Weld. J., 80: 47, 2001.20. Xie, J., and Kar, A., Weld. J., 78: 343s, 1999.21. Mazumder, J., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993, p. 874.22. Rockstroh, T., and Mazumder, J., J. Appl. Phys., 61: 917, 1987.
34 FUSION WELDING PROCESSES23. Seaman, F., Role of Shielding Gas in Laser Welding, Technical Paper MR77-982, Society of Manufacturing Engineers, Dearborn, MI, 1977.24. Hyatt, C. V., Magee, K. H., Porter, J. F., Merchant, V. E., and Matthews, J. R., Weld. J., 80: 163s, 2001.25. Albright, C. E., Eastman, J., and Lempert, W., Weld. J., 80: 55, 2001.26. Ushio, M., Matsuda, F., and Sadek, A. A., in “ International Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, March 1993, p. 408.FURTHER READING1. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Applica- tion to Heat Processing, Okada Memorial Society for the Promotion of Welding, Japan, 1985.2. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979.3. Welding Handbook, Vols. 1–3, 7th ed., American Welding Society, Miami, FL, 1980.4. Duley, W. W., Laser Welding, Wiley, New York, 1999.5. ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993.PROBLEMS1.1 It has been suggested that compared to SMAW, the cooling rate is higher in GMAW and it is, therefore, more likely for heat-affected zone cracking to occur in hardenable steels. What is the main reason for the cooling rate to be higher in GMAW than SMAW?1.2 The diameter of the electrodes to be used in SMAW depends on factors such as the workpiece thickness, the welding position, and the joint design. Large electrodes, with their corresponding high currents, tend to produce large weld pools. When welding in the overhead or vertical position, do you prefer using larger or smaller electrodes?1.3 In arc welding, the magnetic ﬁeld induced by the welding current passing through the electrode and the workpiece can interact with the arc and cause “arc blow.” Severe arc blow can cause excessive weld spatter and incomplete fusion. When arc blow is a problem in SMAW, do you expect to minimize it by using DC or AC for welding?1.4 In the hot-wire GTAW process, shown in Figure P1.4, the tip of the ﬁller metal wire is dipped in the weld pool and the wire itself is resistance heated by means of a second power source between the contact tube of the wire and the workpiece. In the case of steels, the deposition rate can
PROBLEMS 35 Filler wire Tungsten electrode Wire feeder Contact tube Contact tube Cable 1 Shielding gas nozzle 2nd Cable 3 Arc Shielding gas power source Cable 4 Weld metal Base metal Weld pool Figure P1.4 be more than doubled this way. Do you prefer using an AC or a DC power source for heating the wire? Do you expect to apply this process to aluminum and copper alloys?1.5 In GTAW the welding cable is connected to the tungsten electrode through a water-cooled copper contact tube, as shown in Figure 1.11. Why is the tube positioned near the lower end of the electrode instead of the top?1.6 Measurements of the axial temperature distribution along the GTAW electrode have shown that the temperature drops sharply from the electrode tip toward the contact tube. Why? For instance, with a 2.4-mm-diameter W–ThO2 electrode at 150 A, the temperature drops from about 3600 K at the tip to about 2000 K at 5 mm above the tip. Under the same condition but with a W–CeO2 electrode, the tempera- ture drops from about 2700 K at the tip to about 1800 K at 5 mm above the tip (26). Which electrode can carry more current before melting and why?1.7 Experimental results show that in EBW the penetration depth of the weld decreases as the welding speed increases. Explain why. Under the same power and welding speed, do you expect a much greater penetra- tion depth in aluminum or steel and why?1.8 How does the working distance in EBW affect the depth–width ratio of the resultant weld?1.9 Consider EBW in the presence of a gas environment. Under the same power and welding speed, rank and explain the weld penetration for Ar, He, and air. The speciﬁc gravities of Ar, He, and air with respect to air are 1.38, 0.137, and 1, respectively, at 1 atm, 0°C.
36 FUSION WELDING PROCESSES weld transverse cross-section 1 mm 1 mm Figure P1.10 steel 15 cm weld steel transverse cross-section 15 cm Figure P1.111.10 Which arc welding process could have been used for joining the edge weld of thin-gauge steel shown in Figure P1.10 and why?1.11 Two 15-cm-thick steel plates were joined together in a single pass, as shown in Figure P1.11. Which welding process could have been used and why?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-42 Heat Flow in WeldingHeat ﬂow during welding, as will be shown throughout Parts II–IV of thisbook, can strongly affect phase transformations during welding and thus theresultant microstructure and properties of the weld. It is also responsible forweld residual stresses and distortion, as will be discussed in Chapter 5.2.1 HEAT SOURCE2.1.1 Heat Source EfﬁciencyA. Deﬁnition The heat source efﬁciency h is deﬁned as Qt weld Q h= = (2.1) Qnominalt weld Qnominalwhere Q is the rate of heat transfer from the heat source to the workpiece,Qnominal the nominal power of the heat source, and tweld the welding time. Aportion of the power provided by the heat source is transferred to the work-piece and the remaining portion is lost to the surroundings. Consequently,h < 1. If the heat source efﬁciency h is known, the heat transfer rate to theworkpiece, Q, can be easily determined from Equation (2.1). In arc welding with a constant voltage E and a constant current I, the arcefﬁciency can be expressed as Qt weld Q h= = (2.2) EIt weld EIEquation (2.2) can also be applied to electron beam welding, where h is theheat source efﬁciency. In laser beam welding, Qnominal in Equation (2.1) is thepower of the laser beam, for instance, 2500 W. It should be noted that in the welding community the term heat input oftenrefers to Qnominal, or EI in the case of arc welding, and the term heat input perunit length of weld often refers to the ratio Qnominal/V, or EI/V, where V is thewelding speed.B. Measurements The heat source efﬁciency can be measured with acalorimeter. The heat transferred from the heat source to the workpiece is in 37
38 HEAT FLOW IN WELDING GTAW Pipe torch Arc Water in Water out Thermocouple Insulation Thermocouple (a) Temperature, oF 50 Shaded area 120 Temperature, oC ∞ =∫ [ ]dt 40 0 Tout- Tin 100 Tout 30 80 Tin 20 100 120 Time, seconds (b)Figure 2.1 Measurement of arc efﬁciency in GTAW: (a) calorimeter; (b) rise in coolingwater temperature as a function of time. Modiﬁed from Kou et al. (1, 2).turn transferred from the workpiece to the calorimeter, which can be deter-mined as described below. Kou et al. (1, 2) used simple tubular calorimeters to determine the arcefﬁciency in GTAW of aluminum, as shown in Figure 2.1a. The calorimetercan be a round cross section if the workpiece is a pipe or a rectangularcross section if the workpiece is a sheet. The temperature rise in the cool-ing water (Tout - Tin) can be measured using thermocouples or thermistors.Heat transfer from the workpiece to the calorimeter is as follows (1–3): • • Qt weld = Ú0 WC (Tout - Tin ) dt ª WC Ú0 (Tout - Tin )dt (2.3)where W is the mass ﬂow rate of water, C the speciﬁc heat of water, Tout theoutlet water temperature, Tin the inlet water temperature, and t time. The inte-gral corresponds to the shaded area in Figure 2.1b. The arc efﬁciency h can bedetermined from Equations (2.2) and (2.3). Giedt et al. (4) used the Seebeck envelop calorimeter shown in Figure 2.2ato measure the arc efﬁciency in GTAW. The name Seebeck came fromthe Seebeck thermoelectric effect of a thermocouple, namely, a voltage isproduced between two thermocouple junctions of different temperatures.The torch can be quickly withdrawn after welding, and the calorimeter lidcan be closed to minimize heat losses to the surrounding air. As shown inFigure 2.2b, heat transfer from the workpiece to the calorimeter can bedetermined by measuring the temperature difference DT and hence gradient
HEAT SOURCE 39(a) Cooling water flow Gradient layer Thermocouple junctions for sensing temperature difference Direction of heat flow Temperature Temperature ∆T profile L (b) Distance Figure 2.2 Measurement of arc efﬁciency in GTAW: (a) calorimeter; (b) layer of tem- perature gradient. Reprinted from Giedt et al. (4). Courtesy of American Welding Society. across a “gradient layer” of material of known thermal conductivity k and thickness L: • DT Qt weld = AÚ0 k dt (2.4) L
40 HEAT FLOW IN WELDINGwhere A is the area for heat ﬂow and DT/L the temperature gradient. The arcefﬁciency h can be determined from Equations (2.4) and (2.2). This type ofcalorimeter was later used to determine the arc efﬁciencies in PAW, GMAW,and SAW (5–8). Figure 2.3 shows the results of arc efﬁciency measurements in GTAW andPAW (2, 5, 7, 9), and Figure 2.4 shows similar results in GMAW and SAW (7,10). These results were obtained using the two types of calorimeters describedabove except for the results of Lu and Kou for GMAW (10, 11), which aredescribed in what follows. In GMAW the arc, metal droplets, and cathode heating all contribute to theefﬁciency of the heat source. It has been observed in GMAW of aluminumand steel with Ar shielding that current ﬂow or electron emission occurs not 1.0 GTAW 0.8 Arc Efficiency 0.6 PAW Fuerschbach et al. (1991) 0.4 GTAW: Dupont et al. (1995) Kou and Lu (1985) 0.2 Fuerschbach et al. (1991) PAW: Dupont et al. (1995) Evans et al. (1998) 0.0 0 10 20 30 Travel Speed, mm/s Figure 2.3 Arc efﬁciencies in GTAW and PAW. 1.0 SAW 0.8 Arc Efficiency GMAW 0.6 Lu and Kou (1989) 0.4 GMAW: Lu and Kou (1989) DuPont et al. (1995) 0.2 SAW: DuPont et al. (1995) 75 125 175 225 275 325 375 425 Current, A Figure 2.4 Arc efﬁciencies in GMAW and SAW.
HEAT SOURCE 41uniformly over the workpiece surface but over localized areas on the work-piece surface called cathode spots (12, 13). The localized heating, calledcathode heating, causes the surface oxide to dissociate and leaves a clean metalsurface (12). Cathode heating is attributed to ﬁeld-type emission of electrons.Unlike thermionic emission at the tungsten electrode in DC electrode-negative GTAW, ﬁeld emission electrons do not cool the cathode (6). Lu and Kou (10, 11) used a combination of three calorimeters to estimatethe amounts of heat transfer from the arc, ﬁller metal droplets, and cathodeheating to the workpiece in GMAW of aluminum. Figure 2.5a shows the mea-surement of heat transfer from droplets (11). The arc is established betweena GMAW torch and a GTA torch and the droplets collect in the calorimeterbelow. From the water temperature rise and the masses and speciﬁc heats ofthe water and the copper basin, the heat transfer from droplets can be deter- Filler wire GMAW GTAW torch torch Droplets Radiation baffle Cu basin Thermistor Water Insulation (a) Filler wire GMAW torch (b) Weld O-ring Workpiece Water out Water in DT DT DT: differential Insulation thermistor Filler wire GMAW torch (c) GTAW Weld torch O-ring Workpiece Water out Water in DT DT InsulationFigure 2.5 Calorimeter for measuring heat inputs in GMAW: (a) metal droplets; (b)total heat input; (c) combined heat inputs from arc and metal droplets. Reprinted fromLu and Kou (10, 11). Courtesy of American Welding Society.
42 HEAT FLOW IN WELDING GMAW Total 80 Total Power inputs, % GMAW Power inputs, kW 6 1.6 mm (1/16 in) 4043 filler metal 1.6 mm (1/16 in) Arc + 60 4043 filler metal droplets Arc 4 40 Droplets Droplets 2 20 Cathode 0 0 0 2 4 6 8 0 2 4 6 8 Current x voltage, kW (a) Current x voltage, kW (b)Figure 2.6 Power inputs during GMAW of aluminum: (a) measured results; (b) break-down of total power input. Reprinted from Lu and Kou (10). Courtesy of AmericanWelding Society.mined. Figure 2.5b shows the measurement of the total heat transfer to theworkpiece. Figure 2.5c shows the measurement of the combined heat transferfrom the arc and the droplets, with cathode heating shifted to the tungstenelectrode of a nearby GTAW torch (10). The results are shown in Figure 2.6a.By subtracting the combined heat transfer from the arc and droplets from thetotal heat transfer to the workpiece, heat transfer from cathode heating wasdetermined. Figure 2.6b shows the breakdown of the total heat transfer to theworkpiece into those from the arc, droplets, and cathode heating. Within therange of the power studied, the overall efﬁciency was about 80%, with about45% from the arc, 25% from droplets, and 10% from cathode heating. The heat source efﬁciency can be very low in LBW because of the highreﬂectivity of metal surfaces to a laser beam, for instance, 98% for CO2 laseron polished aluminum. The reﬂectivity can be found by determining the ratioof the reﬂected beam power to the incident beam power. Xie and Kar (14)show that roughening the surface with sandpapers and oxidizing the surfaceby brief exposure to high temperatures can reduce the reﬂectivity signiﬁcantly.C. Heat Source Efﬁciencies in Various Welding Processes Figure 2.7 sum-marizes the heat source efﬁciencies measured in several welding processes. Afew comments are made as follows: LBW: The heat source efﬁciency is very low because of the high reﬂectiv- ity of metal surfaces but can be signiﬁcantly improved by surface modi- ﬁcations, such as roughening, oxidizing, or coating. PAW: The heat source efﬁciency is much higher than LBW because reﬂec- tivity is not a problem. GTAW: Unlike in PAW there are no heat losses from the arc plasma to the water-cooled constricting torch nozzle. With DCEN, the imparting elec- trons are a major source of heat transfer to the workpiece. They release the work function as heat and their kinetic energy is also converted into
HEAT SOURCE 43 1.0 Heat Source Efficiency 0.8 0.6 modifications 0.4 dcen surface 0.2 0 LBW PAW GTAW SMAW GMAW SAW EBW Figure 2.7 Heat source efﬁciencies in several welding processes. Afiller AbaseFigure 2.8 Transverse cross section of weld showing areas representing contributionsfrom base metal and ﬁller metal. heat at the workpiece. In AC GTAW, however, electrons bombard the workpiece only during the electrode-negative half cycle, and the arc efﬁ- ciency is thus lower. In GTAW with DCEP, the arc efﬁciency is even lower because the electrons bombard the electrode rather than the workpiece. GMAW, SMAW: Unlike in GTAW, heat transfer to the electrode can be transferred back to the workpiece through metal droplets, thus improv- ing the arc efﬁciency. SAW: Unlike in GMAW or SMAW, the arc is covered with a thermally insu- lating blanket of molten slag and granular ﬂux, thus reducing heat losses to the surroundings and improving the arc efﬁciency. EBW: The keyhole in EBW acts like a “black body” trapping the energy from the electron beam. As a result, the efﬁciency of the electron beam is very high.2.1.2 Melting EfﬁciencyThe ability of the heat source to melt the base metal (as well as the ﬁller metal)is of practical interest to the welder. Figure 2.8 shows the cross-sectional area
44 HEAT FLOW IN WELDINGrepresenting the portion of the weld metal contributed by the base metal, Abase,and that contributed by the ﬁller metal, Aﬁller. One way to deﬁne the meltingefﬁciency of the welding arc, hm, is as follows: ( AbaseVt weld )H base + ( AﬁllerVt weld )H ﬁller hm = (2.5) hEIt weldwhere V is the welding speed, Hbase the energy required to raise a unit volumeof base metal to the melting point and melt it, and Hﬁller the energy required toraise a unit volume of ﬁller metal to the melting point and melt it. The quantityinside the parentheses represents the volume of material melted while thedenominator represents the heat transfer from the heat source to the workpiece. Figures 2.9a and b show the transverse cross section of two steel welds dif-fering in the melting efﬁciency (7). Here, EI = 3825 W and V = 10 mm/s for theshallower weld of lower melting efﬁciency (Figure 2.9a) and EI = 10170 W andV = 26 mm/s for the deeper weld of higher melting efﬁciency (Figure 2.9b).Note that the ratio EI/V is equivalent in each case. 0.7 −175 0.6 η m = 0.50exp ηEIV /(Hαν) Melting efficiency 0.5 0.4 0.3 PAW GTAW 0.2 GMAW 0.1 SAW (c) 0.0 0 1000 2000 3000 4000 5000 ηEIV/(Hαν)Figure 2.9 Melting efﬁciency: (a) lower at lower heat input and welding speed; (b)higher at higher heat input and welding speed; (c) variation with dimensionless para-meter hEIV/Ha. Reprinted from DuPont and Marder (7). Courtesy of AmericanWelding Society.
HEAT SOURCE 45 Fuerschbach and Knorovsky (5) proposed the following empirical equationfor the melting efﬁciency: Ê -B ˆ hm = A exp (2.6) Ë hEIV Han ¯where A and B are constants, H = Hbase + Hﬁller, a is the thermal diffusivity, and is the kinematic viscosity of the weld pool. The results of DuPont and Marder(7) shown in Figure 2.9c conﬁrms the validity of Equation (2.6). As thedimensionless parameter hEIV/Ha increases, the melting efﬁciency increasesrapidly ﬁrst and then levels off. If the arc efﬁciency h is known, hEIV/Ha isalso known and the melting efﬁciency can be predicted from Figure 2.9. Withthe help of the following equation for determining Aﬁller, Abase can then becalculated from Equation (2.5): AﬁllerVtweld = pR2ﬁllerVﬁllertweld (2.7)or 2 pRﬁllerVﬁller Aﬁller = (2.8) VIn the above equations Rﬁller and Vﬁller are the radius and feeding speed of theﬁller metal, respectively. The left-hand side of Equation (2.7) is the volume ofthe weld metal contributed by the ﬁller metal while the right-hand side is thevolume of ﬁller metal used during welding. It should be noted that the melting efﬁciency cannot be increased indeﬁ-nitely by increasing the welding speed without increasing the power input. Todo so, the power input must be increased along with the welding speed. Itshould also be noted that in the presence of a surface-active agent suchas sulfur in steel, the weld pool can become much deeper even thoughthe welding parameters and physical properties in Equation (2.6) remainunchanged (Chapter 4).2.1.3 Power Density Distribution of Heat SourceA. Effect of Electrode Tip Angle In GTAW with DCEN, the shape of theelectrode tip affects both the shape and power density distribution of thearc. As the electrode tip becomes blunter, the diameter of the arc decreasesand the power density distribution increases, as illustrated in Figure 2.10.Glickstein (15) showed, in Figure 2.11, that the arc becomes more constrictedas the conical tip angle of the tungsten electrode increases. Savage et al. (16) observed that, under the same welding current, speed, andarc gap, the weld depth–width ratio increases with increasing vertex angle of
46 HEAT FLOW IN WELDING Tungsten electrode Arc (a) (c) Power Power density density (b) (d) Radial Radial distance distanceFigure 2.10 Effect of electrode tip angle on shape and power density distribution ofgas–tungsten arc.Figure 2.11 Effect of electrode tip angle on shape of gas–tungsten arc. Reprinted fromGlickstein (15).
ANALYSIS OF HEAT FLOW IN WELDING 47 Electrode tip angle (truncation, mm) 30o 60o 90o 180o (0.125) (0.125) (0.500) (0)Figure 2.12 Effect of electrode tip geometry on shape of gas–tungsten arc welds instainless steel (pure Ar, 150 A, 2.0 s, spot-on-plate). Reprinted from Key (17). Courtesyof American Welding Society. 60 Lu and Kou (1988) Tsai (1983) Power Density, W/mm 2 40 -0.1r2 q(r) = 32e electrode (+) 100 A,14.2 V 4.7 mm arc 20 100% Ar 3.2 mm electrode o -0.1r2 75 tip angle q(r) = 30e 0 0 2 4 6 8 Radius, mmFigure 2.13 Measured power density distributions. Reprinted from Lu and Kou (3).Courtesy of American Welding Society.the conical tip of the tungsten electrode. Key (17) reported a similar effect ofthe tip angle, at least with Ar shielding, as shown in Figure 2.12.B. Measurements Several investigators have measured the power densitydistribution (and current density distribution) in the gas tungsten arc by usingthe split-anode method (2, 18–20). Figure 2.13 shows the results of Tsai (20)and Lu and Kou (3). For simplicity, the Gaussian-type distribution is often usedas an approximation (21–23).2.2 ANALYSIS OF HEAT FLOW IN WELDINGFigure 2.14 is a schematic showing the welding of a stationary workpiece (24).The origin of the coordinate system moves with the heat source at a constantspeed V in the negative-x direction. Except for the initial and ﬁnal transients
48 HEAT FLOW IN WELDINGFigure 2.14 Coordinate system (x, y, z) moving with heat source. From Kou and Le(24).of welding, heat ﬂow in a workpiece of sufﬁcient length is steady, or quasi-stationary, with respect to the moving heat source. In other words, for anobserver moving with the heat source, the temperature distribution and thepool geometry do not change with time. This steady-state assumption was ﬁrstused by Rosenthal (25) to simplify the mathematical treatment of heat ﬂowduring welding.2.2.1 Rosenthal’s EquationsRosenthal (25) used the following simplifying assumptions to derive analyti-cal equations for heat ﬂow during welding: 1. steady-state heat ﬂow, 2. point heat source, 3. negligible heat of fusion, 4. constant thermal properties, 5. no heat losses from the workpiece surface, and 6. no convection in the weld pool.A. Rosenthal’s Two-Dimensional Equation Figure 2.15 is a schematicshowing the welding of thin sheets. Because of the small thickness of the work-piece, temperature variations in the thickness direction are assumed negligi-ble and heat ﬂow is assumed two dimensional. Rosenthal (25) derived thefollowing equation for two-dimensional heat ﬂow during the welding of thinsheets of inﬁnite width:
ANALYSIS OF HEAT FLOW IN WELDING 49 heat source, Q welding T speed, V weld pool o T(x,y) x fusion zo y = 4 cm ne 2 -3 -2 -1 0 1 thickness, g 2 34 5 y thin sheets at T(x,y) shown at x = -1 cm and y = 4 cm temperature T 0 before welding Figure 2.15 Two-dimensional heat ﬂow during welding of thin workpiece. 2p (T - T0 )kg Ê Vx ˆ Ê Vr ˆ = exp K (2.9) Q Ë 2a ¯ 0 Ë 2a ¯where T = temperature T0 = workpiece temperature before welding k = workpiece thermal conductivity g = workpiece thickness Q = heat transferred from heat source to workpiece V = travel speed a = workpiece thermal diffusivity, namely, k/rC, where r and C are density and speciﬁc heat of the workpiece, respectively K0 = modiﬁed Bessel function of second kind and zero order, as shown in Figure 2.16 (26) r = radial distance from origin, namely, (x2 + y2)1/2 Equation (2.9) can be used to calculate the temperature T(x, y) at any loca-tion in the workpiece (x, y) with respect to the moving heat source, forinstance, at x = -1 cm and y = 4 cm shown in Figure 2.15. The temperatures atother locations along y = 4 cm can also be calculated, and the temperature dis-tribution along y = 4 cm can thus be determined. Table 2.1 lists the thermalproperties for several materials (27).B. Rosenthal’s Three-Dimensional Equation The analytical solutionderived by Rosenthal for three-dimensional heat ﬂow in a semi-inﬁnite work-piece during welding, Figure 2.17, is as follows (25): 2p (T - T0 )kR È -V (R - x) ˘ = exp Í ˙ (2.10) Q Î 2a ˚
50 HEAT FLOW IN WELDING 2.8 Modified Bessel function 2.4 of second kind zero order 2.0 K 0 [Vr/(2α )] 1.6 1.2 0.8 0.4 0 0 1 2 3 4 Vr/(2α ) Figure 2.16 Modiﬁed Bessel function of second kind and zero order (26).TABLE 2.1 Thermal Properties for Several Materials Volume Thermal Thermal Thermal Melting Diffusivity, Capacity, Conductivity, PointMaterial a (m2/s) rCs (J/m3 K) k (J/m s K) (K)Aluminum 8.5 ¥ 10-5 2.7 ¥ 106 229.0 933Carbon steel 9.1 ¥ 10-6 4.5 ¥ 106 41.0 18009% Ni steel 1.1 ¥ 10-5 3.2 ¥ 106 35.2 1673Austenitic 5.3 ¥ 10-6 4.7 ¥ 106 24.9 1773 stainless steelInconel 600 4.7 ¥ 10-6 3.9 ¥ 106 18.3 1673Ti alloy 9.0 ¥ 10-6 3.0 ¥ 106 27.0 1923Copper 9.6 ¥ 10-5 4.0 ¥ 106 384.0 1336Monel 400 8.0 ¥ 10-6 4.4 ¥ 106 35.2 1573Source: Gray et al. (27).where R is the radial distance from the origin, namely, (x2 + y2 + z2)1/2. For agiven material and a given welding condition, an isotherm T on a plane at agiven x has a radius of R. In other words, Equation (2.10) implies that on thetransverse cross section of the weld all isotherms, including the fusion bound-ary and the outer boundary of the heat-affected zone, are semicircular inshape. Equation (2.10) can be used to calculate the steady-state temperatureT(x, y, z), with respect to the moving heat source, at any location in the work-piece (x, y, z), for instance, at x = 1 cm, y = 4 cm, and z = 0 cm, as shown inFigure 2.17. The temperatures at other locations along y = 4 cm can also be
ANALYSIS OF HEAT FLOW IN WELDING 51 heat source, Q welding T(x,y,z) speed, V weld pool T fusion zone o x y = 4 cm 1 -2 y 0 2 4 z semi-infinite plates T(x,y,z) shown at x = 1 cm, y = 4 at temperature T0 cm and z = 0 cm before weldingFigure 2.17 Three-dimensional heat ﬂow during welding of semi-inﬁnite workpiece.calculated, and the temperature distribution along y = 4 cm can thus bedetermined.C. Thermal Cycles and Temperature Distributions Equations (2.9) and(2.10) can be used to calculate the temperature distribution in the workpieceduring welding. The temperature distribution in the welding direction, forinstance, the T–x curves in Figures 2.15 and 2.17, are of particular interest.They can be readily converted into temperature–time plots, namely, thethermal cycles, by converting distance x into time t through t = (x - 0)/V.Figures 2.18 and 2.19 show calculated thermal cycles and temperature distri-butions at the top surface (z = 0) of a thick 1018 steel at two different sets ofheat input and welding speed. The inﬁnite peak temperature at the origin ofthe coordinate system is the result of the singularity problem in Rosenthal’ssolutions caused by the point heat source assumption. It should be mentioned, however, that Rosenthal’s analytical solutions,though based on many simplifying assumptions, are easy to use and have beengreatly appreciated by the welding industry.2.2.2 Adams’ EquationsAdams (28) derived the following equations for calculating the peak temper-ature Tp at the workpiece surface (z = 0) at a distance Y away from the fusionline (measured along the normal direction): 1 4.13VYgrC 1 = + (2.11) Tp - T0 Q Tm - T0for two-dimensional heat ﬂow and
52 HEAT FLOW IN WELDINGFigure 2.18 Calculated results from Rosenthal’s three-dimensional heat ﬂow equa-tion: (a) thermal cycles; (b) isotherms. Welding speed: 2.4 mm/s; heat input: 3200 W;material: 1018 steel. 2 1 5.44pka È Ê VY ˆ ˘ 1 = Í2 + Ë + (2.12) Tp - T0 QV Î ¯ ˙ Tm - T0 2a ˚for three-dimensional heat ﬂow. Several other analytical solutions have also been derived for two-dimensional (29–34) and three-dimensional (31, 35–37) welding heat ﬂow.Because of the many simplifying assumptions used, analytical solutions havehad limited success.2.2.3 Computer SimulationMany computer models have been developed to study two-dimensional heatﬂow (e.g., refs. 38–43) and three-dimensional heat ﬂow (e.g., refs. 44–55) duringwelding. Most assumptions of Rosenthal’s analytical solutions are no longerrequired. Figure 2.20 shows the calculated results of Kou and Le (24) for theGTAW of 3.2-mm-thick sheets of 6061 aluminum alloy. The agreement withobserved fusion boundaries and thermal cycles appears good.
EFFECT OF WELDING PARAMETERS 53Figure 2.19 Calculated results similar to those in Figure 2.18 but with welding speedof 6.2 mm/s and heat input of 5000 W.2.3 EFFECT OF WELDING PARAMETERS2.3.1 Pool ShapeAs the heat input Q and welding speed V both increase, the weld pool becomesmore elongated, shifting from elliptical to teardrop shaped. Figure 2.21 showsthe weld pools traced from photos taken during autogenous GTAW of 304stainless steel sheets 1.6 mm thick (56). Since the pools were photographedfrom the side at an inclined angle (rather than vertically), the scale bar appliesonly to lengths in the welding direction. In each pool the cross indicates theposition of the electrode tip relative to the pool. The higher the welding speed,the greater the length–width ratio becomes and the more the geometric centerof the pool lags behind the electrode tip. Kou and Le (57) quenched the weld pool during autogenous GTAW of1.6-mm 309 stainless steel sheets and observed the sharp pool end shown in Figure2.22. The welding current was 85A, voltage 10V, and speed 4.2mm/s [10in./min(ipm)]. The sharp end characteristic of a teardrop-shaped weld pool is evident. The effect of the welding parameters on the pool shape is more signiﬁcantin stainless steel sheets than in aluminum sheets. The much lower thermal con-
54 HEAT FLOW IN WELDINGFigure 2.20 Computer simulation of GTAW of 3.2-mm-thick 6061 aluminum, 110 A,10 V, and 4.23 mm/s: (a) fusion boundaries and isotherms; (b) thermal cycles. From Kouand Le (24). 304 stainless steel sheets 2mm 35A, 7.4V 0.42 mm/s 70A, 8.4V 2.5 mm/s 100A, 9.0V 4.2 mm/sFigure 2.21 Weld pool shapes in GTAW of 304 stainless steel sheets. Courtesy ofSmolik (56).
EFFECT OF WELDING PARAMETERS 55Figure 2.22 Sharp pool end in GTAW of 309 stainless steel preserved by ice quench-ing during welding. From Kou and Le (57). 1200 1100 (a) V:10 cm/min; EI/V:15.4 kJ/cm (b) V:15 cm/min; EI/V:9.79 kJ/cm 1000 (c) V:20 cm/min; EI/V:7.34 kJ/cm (d) V:30 cm/min; EI/V:4.76 kJ/cm Temperature ( oC) 900 (e) V:40 cm/min; EI/V:3.57 kJ/cm 800 (f) V:60 cm/min; EI/V:2.38 kJ/cm 700 600 (a) 500 (b) 400 (c) 300 (d) (e) 200 (f) 100 0 0.4 0.8 1.2 1.6 2 2.4 2.8 3.2 3.6 4 Time (sec)Figure 2.23 Variation in cooling rates with heat input per unit length of weld (EI/V).Reprinted from Lee et al. (58).ductivity of stainless steels makes it more difﬁcult for the weld pool to dissi-pate heat and solidify.2.3.2 Cooling Rate and Temperature GradientThe ratio EI/V represents the amount of heat input per unit length of weld.Lee et al. (58) measured the cooling rate in GTAW of 2024 aluminum by stick-ing a thermocouple into the weld pool. Figure 2.23 shows that increasing EI/V
56 HEAT FLOW IN WELDING 1925 3500 Temperature, oF 1650 3000 Temperature, oC 1370 Electroslag 2500 weld 1095 2000 815 1500 Arc weld 540 1000 260 500 -18 0 0 2 4 6 8 10 12 14 Time, minFigure 2.24 Thermal cycles of electroslag and arc welds. Reprinted from Liu et al.(60).decreases the cooling rate (the slope). Kihara et al. (59) showed that thecooling rate decreases with increasing EI/V and preheating. Figure 2.24 showsthat the cooling rate in ESW, which is known to have a very high Q/V, is muchsmaller than that in arc welding (60). The effects of the heat input, weldingspeed, and preheat on the cooling rate and temperature gradient can be illus-trated by considering the following example.Example: Bead-on-plate welding of a thick steel plate is carried out usingGTAW at 200 A, 10 V, and 2 mm/s. Based on Rosenthal’s three-dimensionalequation, calculate the 500°C cooling rates along the x axis of the workpiecefor zero and 250°C preheating. The arc efﬁciency is 70% and the thermal con-ductivity is 35 W/m°C. Along the x axis of the workpiece, y=z=0 and R=x (2.13)Therefore, Equation (2.10) becomes Q T - T0 = (2.14) 2pkxTherefore, the temperature gradient is 2 Ê ∂T ˆ Q -1 (T - T0 ) = = -2pk (2.15) Ë ∂ x ¯ t 2px x 2 QFrom the above equation and Ê ∂xˆ =V (2.16) Ë ∂t ¯ T
EFFECT OF WELDING PARAMETERS 57the cooling rate is 2 Ê ∂T ˆ Ê ∂T ˆ Ê ∂ x ˆ (T - T0 ) = = -2pkV (2.17) Ë ∂t ¯ x Ë ∂ x ¯ t Ë ∂t ¯ T QWithout preheating the workpiece before welding, 2Ê ∂T ˆ (500 ∞C - 25∞C) = (-2p ¥ 35 W m ∞C ¥ 2 ¥ 10 -3 m s) = 71 ∞C s (2.18)Ë ∂t ¯ x 0.7 ¥ 200 A ¥ 10 VWith 250°C preheating, 2Ê ∂T ˆ (500∞C - 250∞C) = (-2p ¥ 35 W m ∞C ¥ 2 ¥ 10 -3 m s) = 20 ∞C s (2.19)Ë ∂t ¯ x 0.7 ¥ 200 A ¥ 10 V It is clear that the cooling rate is reduced signiﬁcantly by preheating. Pre-heating is a common practice in welding high-strength steels because it reducesthe risk of heat-affected zone cracking. In multiple-pass welding the inter-pass temperature is equivalent to the preheat temperature T0 in single-passwelding. Equation (2.17) shows that the cooling rate decreases with increasing Q/V,and Equation (2.15) shows that the temperature gradient decreases withincreasing Q.2.3.3 Power Density DistributionFigure 2.25 shows the effect of the power density distribution of the heatsource on the weld shape (24). Under the same heat input and welding speed,weld penetration decreases with decreasing power density of the heat source.As an approximation, the power density distribution at the workpiece surfaceis often considered Gaussian, as shown by the following equation: 3Q È r2 ˘ q= exp Í 2 ˙ (2.20) pa 2 Î-a 3˚where q is the power density, Q the rate of heat transfer from the heat sourceto the workpiece, and a the effective radius of the heat source.2.3.4 Heat Sink Effect of WorkpieceKihara et al. (59) showed that the cooling rate increases with the thickness ofthe workpiece. This is because a thicker workpiece acts as a better heat sinkto cool the weld down. Inagaki and Sekiguchi (61) showed that, under the
58 HEAT FLOW IN WELDINGFigure 2.25 Effect of power density distribution on weld shape in GTAW of 3.2-mm6061 aluminum with 880 W and 4.23 mm/s. From Kou and Le (24).same heat input and plate thickness, the cooling time is shorter for ﬁlletwelding (a T-joint between two plates) than for bead-on-plate welding becauseof the greater heat sink effect in the former.2.4 WELD THERMAL SIMULATOR2.4.1 The EquipmentThe thermal cycles experienced by the workpiece during welding can be dupli-cated in small specimens convenient for mechanical testing by using a weldthermal simulator called Gleeble, a registered trademark of Dynamic Systems.
WELD THERMAL SIMULATOR 59Figure 2.26 A weld simulator specimen held between two water-cooled jaws andresistance heated by electric current passing through it. Courtesy of Dynamic SystemsInc. (63).These simulators evolved from an original device developed by Nippes andSavage in 1949 (62). Figure 2.26 shows a specimen being resistance heated bythe electric current passing through the specimen and the water-cooled jawsholding it (63). A thermocouple spot welded to the middle of the specimen isconnected to a feedback control system that controls the amount of electriccurrent passing through the specimen such that a speciﬁc thermal cycle can beduplicated.2.4.2 ApplicationsThere are many applications for weld thermal simulators. For instance, aweld thermal simulator can be used in conjunction with a high-speeddilatometer to help construct continuous-cooling transformation diagramsuseful for studying phase transformations in welding and heat treating ofsteels. By performing high-speed tensile testing during weld thermal simulation,the elevated-temperature ductility and strength of metals can be evaluated.This is often called the hot-ductility test. Nippes and Savage (64, 65), forinstance, used this test to investigate the heat-affected zone ﬁssuring inaustenitic stainless steels. Charpy impact test specimens can also be prepared from specimens (1 ¥1 cm in cross section) subjected to various thermal cycles. This synthetic-specimen or simulated-microstructure technique has been employed bynumerous investigators to study the heat-affected-zone toughness.
60 HEAT FLOW IN WELDING2.4.3 LimitationsWeld thermal simulators, though very useful, have some limitations and draw-backs. First, extremely high cooling rates during electron and laser beamwelding cannot be reproduced, due to the limited cooling capacity of the sim-ulators. Second, because of the surface heat losses, the temperature at thesurface can be lower than that at the centerline of the specimen, especially ifthe peak temperature is high and the thermal conductivity of the specimen islow (66). Third, the temperature gradient is much lower in the specimenthan in the weld heat-affected zone, for instance, 10°C/mm, as opposed to300°C/mm near the fusion line of a stainless steel weld. This large differencein the temperature gradient tends to make the specimen microstructure differfrom the heat-affected-zone microstructure. For example, the grain size tendsto be signiﬁcantly larger in the specimen than in the heat-affected zone, espe-cially at high peak temperatures such as 1100°C and above.REFERENCES 1. Kou, S., and Le, Y., Metall. Trans. A, 15A: 1165, 1984. 2. Kou, S., and Lu, M. J., in Welding Metallurgy, 1st ed., S. Kou, 1987, Wiley, New York, p. 32; Lu, M. J., Ph.D. Thesis, Department of Materials Science and Engineering, University of Wisconsin, Madison, WI, 1988. 3. Lu, M., and Kou, S., Weld. J., 67: 29s, 1988. 4. Giedt, W. H., Tallerico, L. N., and Fuerschbach, P. W., Weld. J., 68: 28s, 1989. 5. Fuerschbach, P. W., and Knorovsky, G. A., Weld. J., 70: 287s, 1991. 6. Fuerschbach, P. W., Weld. J., 77: 76s, 1998. 7. Dupont, J. N., and Marder, A. R., Weld. J., 74: 406s, 1995. 8. Dupont, J. N., and Marder, A. R., Metall. Mater. Trans., 27B: 481s, 1996. 9. Evans, D. M., Huang, D., McClure, J. C., and Nunes, A. C., Weld. J., 77: 53s, 1998.10. Lu, M., and Kou, S., Weld. J., 68: 452s, 1989.11. Lu, M., and Kou, S., Weld. J., 68: 382s, 1989.12. Essers, W. G., and Van Gompel, M. R. M., Weld. J., 63: 26s, 1984.13. Hasegawa, M., and Goto, H., IIW Document 212-212-71, International Welding Institute, London, 1971.14. Xie, J., and Kar, A., Weld. J., 78: 343s, 1999.15. Glickstein, S. S., Weld. J., 55: 222s, 1976.16. Savage, W. F., Strunk, S. S., and Ishikawa, Y., Weld. J., 44: 489s, 1965.17. Key, J. F., Weld. J., 59: 365s, 1980.18. Nestor, O. H., J. Appl. Phys., 33: 1638, 1962.19. Schoeck, P. A., in Modern Developments in Heat Transfer, Warren Ibele, Academic, New York, 1963, p. 353.20. Tsai, N., Ph.D. Thesis, Department of Materials Science and Engineering, MIT, Cambridge, MA, 1983.
REFERENCES 6121. Kou, S., and Sun, D. K., Metall. Trans. A, 16A: 203, 1985.22. Oreper, G., Eagar, T. W., and Szekely, J., Weld. J., 62: 307s, 1983.23. Pavelic, V., Tan Bakuchi, L. R., Uyechara, O. A., and Myers, P. S., Weld. J., 48: 295s, 1969.24. Kou, S., and Le, Y., Metall. Trans. A, 14A: 2245, 1983.25. Rosenthal, D., Weld. J., 20: 220s, 1941.26. Abramowitz, M., and Stegun, I.A., Eds., Handbook of Mathematical Functions, National Bureau of Standards, Washington, DC, 1964.27. Gray, T. F. G., Spence, J., and North, T. H., Rational Welding Design, Newnes- Butterworth, London, 1975.28. Adams, C. M., Jr., Weld. J., 37: 210s, 1958.29. Grosh, R. J., Trabant, E. A., and Hawskins, G. A., Q. Appl. Math., 13: 161, 1955.30. Swift-Hook, D. T., and Gick, A. E. F., Weld. J., 52: 492s, 1973.31. Jhaveri, P., Moffatt, W. G., and Adams C. M., Jr., Weld. J., 41: 12s, 1962.32. Myers, P. S., Uyehara, O. A., and Borman, G. L., Weld. Res. Council Bull., 123: 1967.33. Ghent, H. W., Hermance, C. E., Kerr, H. W., and Strong, A. B., in Proceedings of the Conference on Arc Physics and Weld Pool Behavior, Welding Institute, Arbington Hall, Cambridge, 1979, p. 389.34. Trivedi, R., and Shrinivason, S. R., J. Heat Transfer, 96: 427, 1974.35. Grosh, R. J., and Trabant, E. A., Weld. J., 35: 396s, 1956.36. Malmuth, N. D., Hall, W. F., Davis, B. I., and Rosen, C. D., Weld. J., 53: 388s, 1974.37. Malmuth, N. D., Int. J. Heat Mass Trans., 19: 349, 1976.38. Kou, S., Kanevsky, T., and Fyﬁtch, S., Weld. J., 62: 175s, 1982.39. Pavelic, V., and Tsao, K. C., in Proceedings of the Conference on Arc Physics and Weld Pool Behavior, Vol. 1, Welding Institute, Arbington Hall, Cambridge, 1980, p. 251.40. Kou, S., and Kanevsky, T., in Proceedings of the Conference on New Trends of Welding Research in the United States, Ed. S. David, ASM International, Materials Park, OH, 1982, p. 77.41. Friedman, E., Trans. ASME; J. Pressure Vessel Techn., Series J, No. 3, 97: 206, 1965.42. Grill, A., Metall. Trans. B, 12B: 187, 1981.43. Grill, A., Metall. Trans. B, 12B: 667, 1981.44. Ushio, M., Ishmimura, T., Matsuda, F., and Arata, Y., Trans. Japan Weld. Res. Inst., 6: 1, 1977.45. Kou, S., in Proceedings of the Conference on Modeling of Casting and Welding Processes, Metall. Society of AIME, Warrendale, PA, 1980.46. Friedman, E., and Glickstein, S. S., Weld. J., 55: 408s, 1976.47. Friedman, E., in Numerical Modeling of Manufacturing Processes, Ed. R. F. Jones, Jr., American Society of Mechanical Engineers, New York, 1977, p. 35.48. Lewis, R. W., Morgan, K., and Gallagher, R. H., in Numerical Modeling of Manu- facturing Processes, Ed. R. F. Jones, Jr., American Society of Mechanical Engineers, New York, 1977, p. 67.49. Hsu, M. B., in Numerical Modeling of Manufacturing Processes, Ed. R. F. Jones, Jr., American Society of Mechanical Engineers, New York, 1977, p. 97.
62 HEAT FLOW IN WELDING50. Glickstein, S. S., and Friedman, E., Weld. J., 60: 110s, 1981.51. Krutz, G. W., and Segerlind, L. J., Weld. J., 57: 211s, 1978.52. Paley, Z., and Hibbert, P. D., Weld. J., 54: 385s, 1975.53. Hibbitt, H. D., and Marcal, P. V., Comput. Struct., 3: 1145, 1973.54. Mazumder, J., and Steen, W. M., J. Appl. Phys., 51: 941, 1980.55. Tsai, N. S., and Eagar, T. W., Weld. J., 62: 82s, 1983.56. Smolik, G., private communication, Idaho National Engineering Laboratories, Idaho Falls, Idaho, 1984.57. Kou, S., and Le, Y., Metall. Trans. A, 13A: 1141, 1982.58. Lee, J. Y., Park, J. M., Lee, C. H., and Yoon, E. P., in Synthesis/Processing of Light- weight Metallic Materials II, Eds. C. M. Ward-Close, F. H. Froes, S. S. Cho, and D. J. Chellman, The Minerals, Metals and Materials Society, Warrendale, PA, 1996, p. 49.59. Kihara, H., Suzuki, H., and Tamura, H., Researches on Weldable High-Strength Steels, 60th Anniversary Series, Vol. 1, Society of Naval Architects of Japan, Tokyo, 1957.60. Liu, S., Brandi, S. D., and Thomas, R. D., in ASM Handbook, Vol. 6, ASM Interna- tional, Materials Park, OH, 1993, p. 270.61. Inagaki, M., and Sekiguchi, H., Trans. Nat. Res. Inst. Metals, Tokyo, Japan, 2(2): 102 (1960).62. Nippes, E. F., and Savage, W. F., Weld. J., 28: 534s, 1949.63. HAZ 1000, Duffers Scientiﬁc, Troy, NY, now Dynamic System, Inc.64. Nippes, E. F., Savage, W. F., Bastian, B. J., Mason, H. F., and Curran, R. M., Weld. J., 34: 183s, 1955.65. Nippes, E. F., Savage, W. F., and Grotke, G. E., Weld. Res. Council Bull., 33: Febru- ary 1957.66. Widgery, D. J., in Weld Thermal Simulators for Research and Problem Solving, Welding Institute, Cambridge, 1972, p. 14.FURTHER READING1. Rykalin, N. N., Calculation of Heat Flow in Welding, Trans. Z. Paley and C. M.Adams, Jr., Document 212-350-74, 1974, International Institute of Welding, London.2. Rosenthal, D., Weld. J., 20: 220s (1941).3. Meyers, P. S., Uyehara, O. A., and Borman, G. L., Weld. Res. Council Bull. 123: 1967.4. Kou, S., Transport Phenomena and Materials Processing, Wiley, New York, 1996.PROBLEMS2.1 In one welding experiment, 50-mm-thick steel plates were joined using electroslag welding. The current and voltage were 480 A and 34 V, res- pectively. The heat losses to the water-cooled copper shoes and by
PROBLEMS 63 radiation from the surface of the slag pool were 1275 and 375 cal/s, respectively. Calculate the heat source efﬁciency.2.2 It has been reported that the heat source efﬁciency in electroslag welding increases with increasing thickness of the workpiece. Explain why.2.3 (a) Consider the welding of 25.4-mm-thick steel plates. Do you prefer to apply Rosenthal’s two- or three-dimensional heat ﬂow equation for full-penetration electron beam welds? What about bead-on- plate gas–tungsten arc welds? (b) Suppose you are interested in studying the solidiﬁcation structure of the weld metal and you wish to calculate the temperature distri- bution in the weld pool. Do you expect Rosenthal’s equations to provide reliable thermal information in the pool? Why or why not? (c) In multipass welding do you expect a higher or lower cooling rate in the ﬁrst pass than in the subsequent passes? Why?2.4 Large aluminum sheets 1.6 mm thick are butt welded using GTAW with alternating current. The current, voltage, and welding speed are 100 A, 10 V, and 2 mm/s, respectively. Calculate the peak temperatures at distance of 1.0 and 2.0 mm from the fusion boundary. Assume 50% arc efﬁciency.2.5 Bead-on-plate welding of a thick-section carbon steel is carried out using 200 A, 20 V, and 2 mm/s. The preheat temperature and arc efﬁ- ciency are 100°C and 60%, respectively. Calculate the cross-sectional area of the weld bead.2.6 (a) Do you expect to have difﬁculty in achieving steady-state heat ﬂow during girth (or circumferential) welding of tubes by keeping constant heat input and welding speed? Explain why. What is the consequence of the difﬁculty? (b) Suggest two methods that help achieve steady-state heat ﬂow during girth welding.2.7 A cold-rolled AISI 1010 low-carbon steel sheet 0.6 mm thick was tested for surface reﬂectivity in CO2 laser beam welding under the following different surface conditions: (a) as received; (b) oxidized in air furnace at 1000°C for 20 s; (c) oxidized in air furnace at 1000°C for 40 s; (d) covered with steel powder. In which order does the reﬂectivity rank in these surface conditions and why?2.8 It was observed in YAG laser beam welding of AISI 409 stainless steel that under the same power the beam size affected the depth–width ratio of the resultant welds signiﬁcantly. Describe and explain the effect.2.9 Calculate the thermal cycle at the top surface of a very thick carbon steel plate at 5 mm away from the centerline of the weld surface. The
64 HEAT FLOW IN WELDING power of the arc is 2 kW, the arc efﬁciency 0.7, the travel speed 2 mm/s, and the preheat temperature 100°C.2.10 Is the transverse cross section of the weld pool at a ﬁxed value of x perfectly round according to Rosenthal’s three-dimensional heat ﬂow equation? Explain why or why not based on the equation. What does your answer tell you about the shape of the transverse cross section of a weld based on Rosenthal’s three-dimensional equation?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-43 Chemical Reactions in WeldingBasic chemical reaction during fusion welding will be described in this chapter,including gas–metal reactions and slag–metal reactions. The effect of thesechemical reactions on the weld metal composition and mechanical propertieswill be discussed.3.1 OVERVIEW3.1.1 Effect of Nitrogen, Oxygen, and HydrogenNitrogen, oxygen, and hydrogen gases can dissolve in the weld metal duringwelding. These elements usually come from air, the consumables such as theshielding gas and ﬂux, or the workpiece such as the moist or dirt on its surface.Nitrogen, oxygen, and hydrogen can affect the soundness of the resultant weldsigniﬁcantly. Some examples of the effect of these gases are summarized inTable 184.108.40.206.2 Techniques for Protection from AirAs described in Chapter 1, various techniques can be used to protect the weldpool during fusion welding. These techniques are summarized in Table 3.2.Figure 3.1 shows the weld oxygen and nitrogen levels expected from severaldifferent arc welding processes (1, 2). As will be explained below, techniquesprovide different degrees of weld metal protection.A. GTAW and GMAW Gas–tungsten arc welding is the cleanest arc weldingprocess because of the use of inert shielding gases (Ar or He) and a short,stable arc. Gas shielding through the torch is sufﬁcient for welding most mate-rials. However, as shown in Figure 3.2, additional gas shielding to protect thesolidiﬁed but still hot weld is often provided both behind the torch and underthe weld of highly reactive metals such as titanium (3, 4). Welding can also beconducted inside a special gas-ﬁlled box. Although also very clean, GMAW isnot as clean as GTAW due to the less stable arc associated with the use of con-sumable electrodes. Furthermore, the greater arc length in GMAW reducesthe protective effects of the shielding gas. Carbon dioxide is sometimesemployed as shielding gas in GMAW. Under the high temperature of the arc, 65
66 CHEMICAL REACTIONS IN WELDINGTABLE 3.1 Effect of Nitrogen, Oxygen, and Hydrogen on Weld Soundness Nitrogen Oxygen HydrogenSteels Increases strength but Reduces toughness Induces hydrogen reduces toughness but improves it if cracking acicular ferrite is promotedAustenitic or Reduces ferrite andduplex promotes solidiﬁcationstainless steels crackingAluminum Forms oxide ﬁlms Forms gas porosity that can be trapped and reduces both as inclusions strength and ductilityTitanium Increases strength but Increases strength reduces ductility but reduces ductility TABLE 3.2 Protection Techniques in Common Welding Processes Protection Technique Fusion Welding Process Gas Gas tungsten arc, gas metal arc, plasma arc Slag Submerged arc, electroslag Gas and slag Shielded metal arc, ﬂux- cored arc Vacuum Electron beam Self-protection Self-shielded arcdecomposition into CO and O is favored, potentially increasing the weldoxygen level.B. SMAW The ﬂow of gas in SMAW is not as well directed toward the weldpool as the ﬂow of inert gas in GTAW or GMAW. Consequently, the protec-tion afforded the weld metal is less effective, resulting in higher weld oxygenand nitrogen levels. Carbon dioxide, produced by the decomposition of car-bonate or cellulose in the electrode covering, can potentially increase the weldoxygen level.C. Self-Shielded Arc Welding Self-shielded arc welding uses strong nitrideformers such as Al, Ti, and Zr in the electrode wire alone to protect againstnitrogen. Since these nitride formers are also strong deoxidizers, the weld
OVERVIEW 67Figure 3.1 Oxygen and nitrogen levels expected from several arc welding processes.From Rein (1); reproduced from Eagar (2). Torch Trailing (HP Argon) shield(Argon) (Air-Argon) (CO2-Argon) Work Backing shield(Argon)Figure 3.2 Gas–tungsten arc welding of titanium with additional gas shielding.Reprinted from Harwig et al. (3). Courtesy of American Welding Society.oxygen levels are slightly lower than in SMAW. Unfortunately, as can be seenin Figure 3.1, the weld nitrogen content is still rather high.D. SAW The weld oxygen level in submerged arc welds can vary signiﬁ-cantly, depending on the composition of the ﬂux; the very high oxygen levelsassociated with acidic ﬂuxes containing large percentages of SiO2, accordingto Eagar (2), are the result of SiO2 decomposition. This is consistent with thelarge increase in the weld metal silicon content when acidic ﬂuxes are used(2). If atmospheric contamination were the reason for the weld metal oxygencontent, the nitrogen content would also have been high.
68 CHEMICAL REACTIONS IN WELDING3.2 GAS–METAL REACTIONSThe gas–metal reactions here refer to chemical reactions that take place at theinterface between the gas phase and the liquid metal. They include the disso-lution of nitrogen, oxygen, and hydrogen in liquid metal and the evolution ofcarbon monoxide.3.2.1 Thermodynamics of ReactionsIn steelmaking, exposure of molten steel to molecular nitrogen, N2, can resultin dissolution of nitrogen atoms in the molten steel, that is, 1 N 2 (g ) = N (3.1) 2where the underlining bar denotes dissolution in molten metal. From ther-modynamics (5), the equilibrium concentration of dissolved nitrogen, [N], atany given temperature T can be determined from the following relationship: d Ê [N ] ˆ - DG∞ ln K N = ln = (3.2) Ë pN 2 ¯ RT dwhere KN is the equilibrium constant for reaction (3.1) based on dissolutionfrom a diatomic gas N2, pN2 the partial pressure (in atmospheres) of N2 abovethe molten metal, DG° the standard free energy of formation (in caloriesper mole), and R the gas constant 1.987 cal/(K mol). Table 3.3 shows the valuesof DG° for several chemical reactions involving nitrogen, oxygen, and hydro-gen (6–9). From Equation (3.2), the well-known Sievert law (10) for the dis-solution of a diatomic gas in molten metal can be written asTABLE 3.3 Free Energy of Reactions Involving Nitrogen, Oxygen, and Hydrogen Free Energy of Reaction,Gas Reaction DG° (cal/mol) Reference 1Nitrogen /2N2(g) = N(g) 86596.0 - 15.659T (K) 6 N(g) = N(wt % in steel) -85736.0 + 21.405T 1 /2N2(g) = N(wt % in steel) 860.0 + 5.71T 7 1Oxygen /2O2(g) = O(g) 60064 - 15.735T 6 O(g) = O(wt % in steel) -88064 + 15.045 T 1 /2O2(g) = O(wt % in steel) -28000 - 0.69T 8 1Hydrogen /2H2(g) = H(g) 53500.0 - 14.40T 9 H(g) = H(ppm in steel) -44780.0 + 3.38T 9 1 /2H2(g) = H(ppm in steel) 8720.0 - 11.02T 8
GAS–METAL REACTIONS 69 [N ] = K N pN2 d (3.3) In arc welding, however, a portion of the N2 molecules can dissociate (oreven ionize) under the high temperature of the arc plasma. The atomic N soproduced can dissolve in the molten metal as follows: N=N (3.4) m Ê [N ] ˆ - DG∞ ln K N = ln = (3.5) Ë pN ¯ RT mwhere KN is the equilibrium constant for reaction (3.4) based on dissolutionfrom a monatomic gas N and pN the partial pressure (in atmospheres) of Nabove the molten metal. It is interesting to compare dissolution of nitrogen in molten steel frommolecular nitrogen to that from atomic nitrogen. Consider an arbitrary tem-perature of 1600°C for molten steel for the purpose of discussion. Based onthe free energy of reaction DG° shown in Table 3.3, for molecular nitrogen apressure of pN2 = 1 atm is required in order to have [N] = 0.045 wt %. For atomicnitrogen, however, only a pressure of pN = 2 ¥ 10-7 atm is required to dissolvethe same amount of nitrogen in molten steel. Similarly, for the dissolution of oxygen and hydrogen from O2(g) and H2(g), 1 O2 (g) = O (3.6) 2 1 H 2 (g ) = H (3.7) 2However, as in the case of nitrogen, a portion of the O2 and H2 molecules candissociate (or even ionize) under the high temperature of the arc plasma. Theatomic O and H so produced can dissolve in the molten metal as follows: O=O (3.8) H=H (3.9) DebRoy and David (11) showed, in Figure 3.3, the dissolution of mono-atomic, rather than diatomic, nitrogen and hydrogen dominates in molten iron.As they pointed out, several investigators have concluded that the species con-centration in the weld metal can be signiﬁcantly higher than those calculatedfrom dissolution of diatomic molecules. Dissociation of such molecules toneutral atoms and ions in the arc leads to enhanced dissolution in the moltenmetal. In the case of hydrogen the calculated results are consistent with the earlierones of Gedeon and Eagar (9) shown in Figure 3.4. The calculation is based
70 CHEMICAL REACTIONS IN WELDING 0.12 0.3 Weight percent solute Weight percent solute (a) (b) 0.10 O 0.08 0.2 N N 0.06 0.04 0.1 H O 0.02 H 0 0 1,850 2,050 2,250 2,450 1,850 2,050 2,250 2,450 Temperature (K) Temperature (K)Figure 3.3 Equilibrium concentration of nitrogen, oxygen, and hydrogen in liquid ironas a function of temperature: (a) N2(g) with pN2 = 1 atm, O2(g) with pO2 = 10-9 atm, H2(g)with pH2 = 1 atm; (b) N(g) with pN = 10-6 atm, O(g) with pO = 10-8 atm, H(g) with pH =5 ¥ 10-2 atm. From DebRoy and David (11). 30 Hydrogen absorbed (ppm) Monatomic absorption Diatomic absortion 25 20 15 10 5 0 -10 -5 0 5 10 Weld pool width (mm)Figure 3.4 Equilibrium concentration of hydrogen as a function of weld pool loca-tion. Reprinted from Gedeon and Eagar (9). Courtesy of American Welding Society.on a dissociation temperature of 2500°C, 0.01 atm hydrogen added to the argonshielding gas, and the pool surface temperature distribution measured byKrause (12). As shown, the majority of hydrogen absorption appears to takeplace around the outer edge of the weld pool, and monatomic hydrogenabsorption dominates the contribution to the hydrogen content. This contra-dicts predictions based on Sievert’s law that the maximum absorption occursnear the center of the pool surface where the temperature is highest. However,as they pointed out, the dissolution process alone does not determine thehydrogen content in the resultant weld metal. Rejection of the dissolvedhydrogen atoms by the solidiﬁcation front and diffusion of the hydrogen atomsfrom the weld pool must also be considered. It is interesting to note that
GAS–METAL REACTIONS 71 0.4 Nitrogen content (mass%) 0.3 0.2 0.1 0 0.02 0.04 0.06 0.08 0.1 Nitrogen partial pressure (MPa)Figure 3.5 Effect of nitrogen partial pressure in Ar–N2 shielding gas on nitrogencontent in welds of duplex stainless steel. Reprinted from Sato et al. (14).Hooijmans and Den Ouden (13) suggested that a considerable amount ofhydrogen absorbed by the liquid metal during welding leaves the weld metalimmediately after the extinction of the arc.3.2.2 NitrogenFor metals that neither dissolve nor react with nitrogen, such as copper andnickel, nitrogen can be used as the shielding gas during welding. On the otherhand, for metals that either dissolve nitrogen or form nitrides (or both), suchas Fe, Ti, Mn, and Cr, the protection of the weld metal from nitrogen shouldbe considered.A. Sources of Nitrogen The presence of nitrogen in the welding zone isusually a result of improper protection against air. However, nitrogen is some-times added purposely to the inert shielding gas. Figure 3.5 shows the weldnitrogen content of a duplex stainless steel as a function of the nitrogen partialpressure in the Ar–N2 shielding gas (14). Nitrogen is an austenite stabilizer foraustenitic and duplex stainless steels. Increasing the weld metal nitrogencontent can decrease the ferrite content (Chapter 9) and increase the risk ofsolidiﬁcation cracking (Chapter 11).B. Effect of Nitrogen The presence of nitrogen in the weld metal can sig-niﬁcantly affect its mechanical properties. Figure 3.6 shows the needlelikestructure of iron nitride (Fe4N) in a ferrite matrix (15). The sharp ends of such
72 CHEMICAL REACTIONS IN WELDING Figure 3.6 Iron nitride in a ferrite matrix (¥500). From Seferian (15).Figure 3.7 Effect of nitrogen on the room temperature mechanical properties of mildsteel welds. From Seferian (15).a brittle nitride act as ideal sites for crack initiation. As shown in Figure 3.7,the ductility and the impact toughness of the weld metal decrease with increas-ing weld metal nitrogen (15). Figure 3.8 shows that nitrogen can decrease theductility of Ti welds (4).C. Protection against Nitrogen In the self-shielded arc welding process,strong nitride formers (such as Ti, Al, Si, and Zr) are often added to the ﬁllerwire (16). The nitrides formed enter the slag and nitrogen in the weld metalis thus reduced. As already shown in Figure 3.1, however, the nitrogen con-
GAS–METAL REACTIONS 73 35 30 % Elongation 25 o 20 .03Fe, 10 C/sec o 15 .03Fe, 28 C/sec o 10 .07Fe, 15 C/sec o .07Fe, 10oC/sec 5 .11Fe, 11 C/sec 0 0.15 0.2 0.25 0.3 0.35 0.4 0.45 OE = 2C+3.5N+O-0.14FeFigure 3.8 Effect of oxygen equivalence (OE) on ductility of titanium welds.Reprinted from Harwig et al. (4). Courtesy of American Welding Society.tents of self-shielded arc welds can still be rather high, and other arc weldingprocesses such as GTAW, GMAW, or SAW should be used if weld nitrogencontamination is to be minimized.3.2.3 OxygenA. Sources of Oxygen Oxygen in the weld metal can come from the air, theuse of excess oxygen in oxyfuel welding, and the use of oxygen- or CO2-containing shielding gases. It can also come from the decomposition of oxides(especially SiO2 and MnO and FeO) in the ﬂux and from the slag–metal reac-tions in the weld pool, which will be discussed subsequently. In GMAW of steels the addition of oxygen or carbon dioxide to argon (e.g.,Ar–2% O2) helps stabilize the arc, reduce spatter, and prevent the ﬁller metalfrom drawing away from (or not ﬂowing out to) the fusion line (17). Carbondioxide is widely used as a shielding gas in FCAW, the advantages being lowcost, high welding speed, and good weld penetration. Baune et al. (18) pointedout that CO2 can decompose under the high temperature of the welding arcas follows: 1 CO2 (g) = CO(g) + O2 (g) (3.10) 2 1 CO(g) = C ( s) + O2 (g) (3.11) 2B. Effect of Oxygen Oxygen can oxidize the carbon and other alloyingelements in the liquid metal, modifying their prevailing role, depressinghardenability, and producing inclusions. The oxidation of carbon is asfollows: C + O = CO(g) (3.12)
74 CHEMICAL REACTIONS IN WELDINGTABLE 3.4 Effect of Oxygen–Acetylene Ratio on Weld Metal Composition andProperties of Mild Steel a = O2/C2H2 > 1 a£1 Before a = 1.14 a = 1.33 a=2 a = 2.37 a=1 a = 0.82C 0.155 0.054 0.054 0.058 0.048 0.15 1.56Mn 0.56 0.38 0.265 0.29 0.18 0.29 0.375Si 0.03S 0.030P 0.018O — 0.04 0.07 0.09 — 0.02 0.01N — 0.015 0.023 0.030 — 0.012 0.023Impact value, — 5.5 1.40 1.50 1.30 6.9 2.3 kg/cm2Hardness, HB — 130 132 115 100 140 320Grain size — 6 5 4 4 4 5Source: Seferian (15).The oxidation of other alloying elements, which will be discussed subse-quently in slag–metal reactions, forms oxides that either go into the slag orremain in the liquid metal and become inclusion particles in the resultantweld metal. Table 3.4 shows the effect of gas composition in oxyacetylene welding ofmild steel on the weld metal composition and properties (15). When too muchoxygen is used, the weld metal has a high oxygen level but low carbon level.On the other hand, when too much acetylene is used, the weld metal has a lowoxygen level but high carbon level (the ﬂame becomes carburizing). In eithercase, the weld mechanical properties are poor. When the oxygen–acetyleneratio is close to 1, both the impact toughness and strength (proportional tohardness) are reasonably good. If oxidation results in excessive inclusion formation in the weld metal orsigniﬁcant loss of alloying elements to the slag, the mechanical properties ofthe weld metal can deteriorate. Figure 3.9 shows that the strength, toughness,and ductility of mild steel welds can all decrease with increasing oxygen con-tamination (15). In some cases, however, ﬁne inclusion particles can act asnucleation sites for acicular ferrite to form and improve weld metal toughness(Chapter 9). For aluminum and magnesium alloys, the formation of insolubleoxide ﬁlms on the weld pool surface during welding can cause incompletefusion. Heavy oxide ﬁlms prevent a keyhole from being established properlyin conventional PAW of aluminum, and more advanced DC variable-polarityPAW has to be used. In the latter, oxide ﬁlms are cleaned during the electrode-positive part of the current cycle. Bracarense and Liu (19) discovered in SMAW that the metal transferdroplet size can increase gradually during welding, resulting in increasing Mn
GAS–METAL REACTIONS 75Figure 3.9 Effect of the oxygen content on the mechanical properties of mild steelwelds. From Seferian (15).and Si transfer to the weld pool and hence increasing weld metal hardnessalong the weld length, as shown in Figure 3.10. As the electrode is heated upmore and more during welding, the droplet size increases gradually (becomesmore globular). This reduces the surface area (per unit volume) for oxygen toreact with Mn and Si and hence improves the efﬁciency of Mn and Si trans-fer to the weld pool.3.2.4 HydrogenA. Steels The presence of hydrogen during the welding of high-strengthsteels can cause hydrogen cracking (Chapter 17).A.1. Sources of Hydrogen Hydrogen in the welding zone can come fromseveral different sources: the combustion products in oxyfuel welding; decom-position products of cellulose-type electrode coverings in SMAW; moisture orgrease on the surface of the workpiece or electrode; and moisture in the ﬂux,electrode coverings, or shielding gas. As mentioned previously in Chapter 1, in SMAW high-cellulose electrodescontain much cellulose, (C6H10O5)x, in the electrode covering. The coveringdecomposes upon heating during welding and produces a gaseous shield richin H2, for instance, 41% H2, 40% CO, 16% H2O, and 3% CO2 in the case ofE6010 electrodes (20). On the other hand, low-hydrogen electrodes containmuch CaCO3 in the electrode covering. The covering decomposes duringwelding and produces a gaseous shield low in H2, for example, 77% CO, 19%CO2, 2% H2, and 2% H2O in the case of E6015 electrodes. As such, to reduceweld metal hydrogen, low-hydrogen electrodes should be used.
76 CHEMICAL REACTIONS IN WELDING 100 430 manganese [Mn] and [Si] x 10-2, wt % 420 80 410 [O], ppm ox yge 60 n 400 40 silicon 390 (a) 20 380 0 20 40 60 80 100 120 140 160 weld length position, mm 50 Hardness, H RC 40 (b) 30 0 20 40 60 80 100 120 weld length position, mmFigure 3.10 Variations of weld metal along the length of a weld made with an E7018electrode: (a) composition; (b) hardness. Reprinted from Bracarense and Liu (19).Courtesy of American Welding Society.A.2. Measuring Hydrogen Content Various methods have been developedfor measuring the hydrogen content in the weld metal of steels. The mercurymethod and the gas chromatography method are often used. Figure 3.11 showsthe mercury method (21). A small test specimen (13 ¥ 25 ¥ 127 mm, or 1/2 ¥ 1¥ 5 in.) is welded in a copper ﬁxture. The welded test specimen is thenimmersed in mercury contained in a eudiometer tube. As hydrogen diffusesout of the welded test specimen, the mercury level in the eudiometer tube con-tinues to drop. From the ﬁnal mercury level, H (in millimeters), the amountof hydrogen that diffuses out of the specimen, that is, the so-called diffusiblehydrogen, can be measured. This method, however, can take days because ofthe slow diffusion of hydrogen at room temperature. In the gas chromatogra-phy method (22), the specimen is transferred to a leak-tight chamber after
GAS–METAL REACTIONS 77Figure 3.11 Mercury method for measuring diffusible hydrogen in welds. Reprintedfrom Shutt and Fink (21). Courtesy of American Welding Society.welding, which can be heated to accelerate the hydrogen evolution from thespecimen. After that, the chamber can be connected to a gas chromatographanalyzer to measure the total amount of hydrogen present. The advantagesare that it can separate other gases present and measure only hydrogen andit takes hours instead of days. One disadvantage is the relatively high cost ofthe equipment. Newer methods have also been developed. Albert et al. (23) developed anew sensor for detecting hydrogen. The sensor is a conducting polymer ﬁlmcoated with Pd on one side to be exposed to a hydrogen-containing gas andthe other side to air. The current going through the sensor is directionally pro-portional to the hydrogen content in the gas. Figure 3.12 shows the hydrogencontents measured by the new sensor as well as gas chromatography (GC).These are gas–tungsten arc welds of a 0.5Cr–0.5Mo steel made with Ar–H2 asthe shielding gas. Smith et al. (24) developed a new hydrogen sensor that gen-erates results in less than 1 h and allows analysis to be done on the actualwelded structure. The sensor is a thin porous ﬁlm of tungsten oxide, whichchanges color upon reacting with hydrogen.
78 CHEMICAL REACTIONS IN WELDING 55.0 Hydrogen in weld metal (ml/100cc) 45.0 35.0 25.0 sensor gas chromatography 15.0 0.0 1.0 2.0 3.0 4.0 5.0 6.0 Concentration of hydrogen in shielding gas (%)Figure 3.12 Hydrogen content in gas–tungsten arc welds of 0.5Cr–0.5Mo steel as afunction of volume percent of hydrogen in Ar–H2 shielding gas. Reprinted from Albertet al. (23). Courtesy of American Welding Society. 30 ml/100g deposited metal As baked Diffusible hydrogen 25 Exposed at 80% relative humidity at 20 28oC for 24 h 15 10 5 0 0 100 200 300 400 500 Baking temperature oCFigure 3.13 Effect of electrode baking temperature on weld metal diffusible hydro-gen levels. Reprinted from Fazackerley and Gee (25).A.3. Hydrogen Reduction Methods The weld hydrogen content can bereduced in several ways. First, avoid hydrogen-containing shielding gases,including the use of hydrocarbon fuel gases, cellulose-type electrode cover-ings, and hydrogen-containing inert gases. Second, dry the electrode coveringand ﬂux to remove moisture and clean the ﬁller wire and workpiece to removegrease. Figure 3.13 shows the effect of the electrode baking temperature onthe weld metal hydrogen content (25). Third, adjust the composition of theconsumables if feasible. Figure 3.14 shows that CO2 in the shielding gas helpsreduce hydrogen in the weld metal (22), possibly because of reaction betweenthe two gases. Increasing the CaF2 content in the electrode covering or the ﬂux
GAS–METAL REACTIONS 79 3 (a) fused metal deposited metal 2 Diffusible Hydrogen (mL/100g) 1 0 Ar Ar+20%CO2 CO Ar+5%CO2 2 10 (b) 8 6 4 2 fused metal deposited metal 0 Ar Ar+20%CO2 Ar+5%CO2 CO2 Shielding gasFigure 3.14 Effect of shielding gases on weld metal hydrogen content: (a) GMAW;(b) FCAW. Reprinted from Mirza and Gee (22).Figure 3.15 Effect of postweld heating on the weld metal hydrogen content of mildsteel. Reprinted from Flanigan (27).has been reported to reduce the weld hydrogen content. This reduction inhydrogen has been ascribed to the reaction between hydrogen and CaF2 (26).Fourth, as shown in Figure 3.15, use postweld heating to help hydrogen diffuseout of the weld (27).
80 CHEMICAL REACTIONS IN WELDING Figure 3.16 Solubility of hydrogen in aluminum. From Eastwood (28).B. Aluminum Hydrogen can cause porosity in aluminum welds (Chapter10). The oxide ﬁlms on the surface of the workpiece or electrode can absorbmoisture from the air and introduce hydrogen into molten aluminum duringwelding. Grease on the surface of the workpiece or electrode and moisture inshielding gas can also be the sources of hydrogen. Figure 3.16 shows the sol-ubility of hydrogen in aluminum (28). Since the solubility of hydrogen is muchhigher in liquid aluminum than in solid aluminum, hydrogen is rejected intothe weld pool by the advancing solid–liquid interface. Consequently, hydrogenporosity is often observed in aluminum welds. Devletian and wood (29) havereviewed the factors affecting porosity in aluminum welds.B.1. Effect of Hydrogen Porosity As shown in Figure 3.17, excessive hydro-gen porosity can severely reduce both the strength and ductility of aluminumwelds (30). It has also been reported to reduce the fatigue resistance ofaluminum welds (31).B.2. Reducing Hydrogen Porosity To reduce hydrogen porosity, the surfaceof Al–Li alloys has been scrapped, milled, or even thermovacuum degassed toremove hydrogen present in the form of hydrides or hydrated oxides (32, 33).Similarly, Freon (CCl2F2) has been added to the shielding gas to reduce hydro-gen in aluminum welds. The weld pool has been magnetically stirred to helphydrogen bubbles escape and thus reduce hydrogen porosity (34). Keyholeplasma arc welding, with variable-polarity direct current, has been used toreduce hydrogen porosity in aluminum welds (35). The cleaning action of theDCEP cycle helps remove hydrated oxides and hydrides. The keyhole, on theother hand, helps eliminate entrapment of oxides and foreign materials inthe weld, by allowing contaminants to enter the arc stream instead ofbeing trapped in the weld. Consequently, the welds produced are practicallyporosity free.
GAS–METAL REACTIONS 81Figure 3.17 Effect of porosity on tensile properties of aluminum welds. From Shore(30). Consider the reduction of severe gas porosity in the welding of a high-strength, lightweight Al–5Mg–2Li alloy (33, 36). The presence of Li in the alloypromotes the formation of lithium hydride during heat treatment as well asthe hydration of the surface oxide at room temperature. Surface cleaning andthermovacuum treatment before welding, which help reduce the hydrogencontent of the workpiece surface, have been reported to reduce the porositylevel of the weld metal. Reduction in porosity has also been achieved by usingan alternating magnetic ﬁeld to stir the weld pool and by using variable-polarity keyhole PAW (33). Consider also the reduction of severe gas porosity in the welding of PM(powder metallurgy) parts of Al–8.0Fe–1.7Ni alloy (33, 36). Oxidation and sub-sequent hydration of the aluminum powder during and after powder produc-tion by air atomization result in a high surface moisture content. When thepowder is consolidated into PM parts, the moisture is trapped inside the parts.Because of the difﬁculty in removing the moisture from deep inside the work-piece, thermovacuum treatments at temperatures as high as 595°C have beenfound necessary. Unfortunately, the use of such a high temperature causesunacceptable degradation in the base-metal strength. Therefore, atomizationand consolidation techniques that minimize powder oxidation and hydrationare required for producing porosity-free welds.
82 CHEMICAL REACTIONS IN WELDINGC. Copper Hydrogen can also cause problems in copper welding. It can reactwith oxygen to form steam, thus causing porosity in the weld metal. It can alsodiffuse to the HAZ and react with oxygen to form steam along the grainboundaries. This can cause microﬁssuring in the HAZ. These problems can beminimized if deoxidized copper is used for welding.3.3 SLAG–METAL REACTIONS3.3.1 Thermochemical ReactionsThe thermochemical slag–metal reactions here refer to thermochemical reac-tions that take place at the interface between the molten slag and the liquidmetal. Examples of such reactions are decomposition of metal oxides in theﬂux, oxidation of alloying elements in the liquid metal by the oxygen dissolvedin the liquid metal, and desulfurization of the weld metal.A. Decomposition of Flux In studying SAW, Chai and Eagar (37) suggestedthat in the high-temperature environment near the welding plasma, all oxidesare susceptible to decomposition and produce oxygen. It was found that thestability of metal oxides during welding decreases in the following order: (i)CaO, (ii) K2O, (iii) Na2O and TiO2, (iv) Al2O3, (v) MgO, and (vi) SiO2 and MnO(FeO was not included but can be expected to be rather unstable, too). Forinstance, SiO2 and MnO can decompose as follows (2): 1 (SiO2 ) = SiO(g) + O2 (g) (3.13) 2 1 (MnO) = Mn(g) + O2 (g) (3.14) 2 It was concluded that in ﬂuxes of low FeO content (<10% FeO), SiO2 andMnO are the primary sources of oxygen contamination and the stability ofmetal oxides in welding is not directly related to their thermodynamic stabil-ity. It was also concluded that CaF2 reduces the oxidizing potential of weldingﬂuxes due to dilution of the reactive oxides by CaF2 rather than to reactivityof the CaF2 itself and signiﬁcant losses of Mn may occur by evaporation fromthe weld pool due to the high vapor pressure of Mn.B. Oxidation by Oxygen in Metal Mn + O = (MnO) (3.15) Si + 2O = (SiO2 ) (3.16) Ti + 2O = (TiO2 ) (3.17) 2 Al + 3O = ( Al 2O3 ) (3.18)
SLAG–METAL REACTIONS 83C. Desulfurization of Liquid Metal S + (CaO) = (CaS) + O (3.19)3.3.2 Effect of Flux on Weld Metal CompositionBurck et al. (38) welded 4340 steel by SAW with manganese silicate ﬂuxes,keeping SiO2 constant at 40 wt % and adding CaF2, CaO, and FeO separatelyat the expense of MnO. Figure 3.18 shows the effect of such additions on theextent of oxygen transfer from the ﬂux to the weld metal, expressed in D(weldmetal oxygen). A positive D quantity means transfer of an element (oxygen inthis case) from the ﬂux to the weld metal, while a negative D quantity meansloss of the element from the weld metal to the ﬂux. The FeO additions, at theexpense of MnO, increase the extent of oxygen transfer to the weld metal. Thisis because FeO is less stable than MnO and thus decomposes and producesoxygen in the arc more easily than MnO. The CaO additions at the expenseof MnO decrease the extent of oxygen transfer to the weld metal becauseCaO is more stable than MnO. The CaF2 additions at the expense of MnO alsodecrease the extent of oxygen transfer to the weld metal but more signiﬁcantly.It is worth noting that Chai and Eagar (37) reported previously that 0.08 -SiO2-MnO-CaF Flux 2 -SiO2-MnO-CaO Flux AISI 4340 Delta weld metal oxygen (wt.%) -SiO2-MnO-FeO Flux 0.06 SiO2 = 40 w/o (constant) FeO 0.04 CaO 0.02 CaF2 0.0 0 10 20 30 40 Flux addition (wt.%) 60 50 40 30 20 MnO in the flux (wt.%)Figure 3.18 Effect of ﬂux additions to manganese silicate ﬂux on extent of oxygentransfer to the weld metal in submerged arc welding of 4340 steel. Reprinted fromBurck et al. (38). Courtesy of American Welding Society.
84 CHEMICAL REACTIONS IN WELDING 0.6 -SiO2-MnO-CaF Flux 2 -SiO2-MnO-CaO Flux AISI 4340 -SiO2-MnO-FeO Flux Delta weld metal manganese (wt.%) SiO2 = 40 w/o (constant) CaO 0.4 CaF2 0.2 FeO 0.0 -0.2 0 10 20 30 40 Flux addition (wt.%) 60 50 40 30 20 MnO in the flux (wt.%)Figure 3.19 Effect of ﬂux additions to manganese silicate ﬂux on extent of manganesetransfer to the weld metal in submerged arc welding of 4340 steel. Reprinted fromBurck et al. (38). Courtesy of American Welding Society.CaF2 reduces oxygen transfer by acting as a diluent rather than an activespecies. Figure 3.19 shows the effect of ﬂux additions on the manganese changeof the weld metal (38). It is surprising that the CaO additions at the expenseof MnO do not decrease the extent of manganese transfer from the ﬂux to theweld metal. From the steelmaking data shown in Figure 3.20, it appears thatthe CaO additions do not reduce the activity of MnO (39), as indicated by thedots along the constant MnO activity of about 0.30. The additions of FeO andCaF2 at the expense of MnO decrease the extent of manganese transferfrom the ﬂux to the weld metal, as expected. Beyond 20% FeO, D(weldmetal manganese) becomes negative, namely, Mn is lost from the weld metalto the slag. This is likely to be caused by the oxidation of Mn by the oxygenintroduced into the liquid metal from FeO, namely, Mn + O = (MnO). The ﬂuxadditions also affect the extents of loss of alloying elements such as Cr, Mo,and Ni. Therefore, the ﬂux composition can affect the weld metal composition andhence mechanical properties rather signiﬁcantly. The loss of alloying elementscan be made up by the addition of ferroalloy powder (e.g., Fe–50% Si andFe–80% Mn) to SAW ﬂuxes or SMAW electrode coverings. In doing so, the
SLAG–METAL REACTIONS 85 SiO2 SiO2 saturation 0.4 0.6 X SiO 6 7 O 0 0. 0.13 0.1 .21 0.25 Ca 0 2 X 0.6 0.4 0.41 0.59 0.37 0.67 lime and lime silicate saturation MnO saturation CaO 0.2 0.4 0.6 MnO XMnOFigure 3.20 Activity of MnO in CaO–MnO–SiO2 melts at 1500°C. Reprinted fromBurck et al. (38). Courtesy of American Welding Society.alloying element recovery, that is, the percentage of the element transferredacross the arc and into the weld metal, should be considered. The recoveryvaries signiﬁcantly from element to element. In SMAW, for example, it can beabout 100% for Ni and Cr, 75% for Mn, 70% for Nb, 45% for Si, and 5% forTi (40).3.3.3 Types of Fluxes, Basicity Index, and Weld Metal PropertiesThe use of proper welding ﬂuxes during fusion welding helps control the com-position of the weld metal as well as protect it from air. Welding ﬂuxes can becategorized into the following three groups according to the types of mainconstituents (26): (a) Halide-type ﬂuxes: for example, CaF2–NaF, CaF2–BaCl2–NaF, KC1–NaCl–Na3AlF6, and BaF2–MgF2–CaF2–LiF. (b) Halide–oxide-type ﬂuxes: for example, CaF2–CaO–Al2O3, CaF2–CaO–SiO2, CaF2–CaO–Al2O3–SiO2, and CaF2–CaO–MgO– Al2O3. (c) Oxide-type ﬂuxes: for example, MnO–SiO2, FeO–MnO–SiO2, and CaO–TiO2–SiO2. The halide-type ﬂuxes are oxygen free and are used for welding titaniumand aluminum alloys (26, 41). The halide–oxide-type ﬂuxes, which are slightlyoxidizing, are often used for welding high-alloy steels. The oxide-type ﬂuxes,which are mostly oxidizing, are often used for welding low-carbon or low-alloysteels. When oxide-type ﬂuxes are used for welding a reactive metal such astitanium, the weld metal can be contaminated with oxygen. The oxides in a welding ﬂux can be roughly categorized into the followingthree groups (26):
86 CHEMICAL REACTIONS IN WELDING (a) Acidic oxides, in the order of decreasing acidity: SiO2, TiO2, P2O5, V2O5. (b) Basic oxides, in the order of decreasing basicity: K2O, Na2O, CaO, MgO, BaO, MnO, FeO, PbO, Cu2O, NiO. (c) Amphoteric oxides: Al2O3, Fe2O3, Cr2O3, V2O3, ZnO. Oxides that are donors of free oxide ions, O2-, are considered as basicoxides, CaO being the most well known example. Oxides that are acceptors ofO2- are considered as acidic oxides, SiO2 being the most well known example.Oxides that are neutral are considered as amphoteric oxides.3.3.4 Basicity IndexThe concept of the basicity index (BI) was adopted in steelmaking toexplain the ability of the slag to remove sulfur from the molten steel. Itwas later broadened to indicate the ﬂux oxidation capability. The BI of a ﬂux(especially an oxide-type one) can be deﬁned in the following general form(42): BI = Â (% basic oxides) (3.20) Â (% nonbasic oxides) The concept of the BI was applied to welding. Tuliani et al. (43) used thefollowing well-known formula for the ﬂuxes in SAW: CaF2 + CaO + MgO + BaO + SrO + Na 2O + K 2O + Li2O + 0.5(MnO + FeO) BI = (3.21) SiO2 + 0.5( Al 2O3 + TiO2 + ZrO2 )where components are in weight fractions. Using the above expression, theﬂux is regarded as acidic when BI < 1, as neutral when 1.0 < BI < 1.2, and asbasic when BI > 1.2. The formula correlates well with the oxygen content insubmerged arc welds. Eagar and Chai (44, 45), however, modiﬁed Equation (3.21) by consideringCaF2 as neutral rather than basic and omitting the CaF2 term. As shown inFigure 3.21, the formula correlates well with the oxygen content in submergedarc welds (44, 45). The oxygen content decreases as the basicity index increasesup to about 1.25 and reaches a constant value around 250 ppm at larger basic-ity values. Baune et al. (18, 46) modiﬁed Equation (3.21) for FCAW electrodes byusing the composition of the solidiﬁed slag after welding rather than the com-position of the ﬂux before welding. Furthermore, mole fraction was used ratherthan weight fraction, and FeO was replaced by Fe2O3. The composition of thesolidiﬁed slag was thought to provide more information about the extent of
SLAG–METAL REACTIONS 87Figure 3.21 Weld metal oxygen content in steel as a function of ﬂux basicity insubmerged arc welding. From Chai and Eagar (45). 515 510 [o]=-199.69B.l.+895.37 R2 =0.9941 505 Weld metal oxygen Wire #1 Wire #3 500 content(ppm) Bl=1.94 Bl=1.982 495 Wire #2 490 Bl=1.976 485 Wire #5 Wire #4 480 Bl=2.13 Bl=2.02 475 470 465 1.9 1.95 2 2.05 2.1 2.15 Basicity index based on measured composition of solidified slagFigure 3.22 Weld metal oxygen content in steel as a function of ﬂux basicity in ﬂux-core arc welding. Reprinted from Baune et al. (46). Courtesy of American WeldingSociety.the slag–metal reactions during welding than the composition of the ﬂuxbefore welding. The Fe2O3 was thought to be the iron oxide that forms in awelding slag. As shown in Figure 3.22, the weld oxygen content correlates wellwith the new basicity index (46). Oxide inclusions in steel welds can affect the formation of acicular ferrite,which improves the weld metal toughness (47–50). It has been reported thatacicular ferrite forms in the range of about 200–500 ppm oxygen (51–53). Thiswill be discussed later in Chapter 9. For SAW of high-strength, low-alloy steels with the CaF2–CaO–SiO2 ﬂuxsystem, Dallam et al. (47) used the following simple formula for the basicityindex:
88 CHEMICAL REACTIONS IN WELDING CaO BI = (3.22) SiO2 Figure 3.23 shows the effect of the basicity index on sulfur transfer (47).As the basicity index increases from 0 to 5, Dsulfur becomes increasinglynegative, namely, more undesirable sulfur is transferred from the weld metalto the slag (desulfurization). This is because CaO is a strong desulfurizer,as shown previously by Equation (3.19). Excessive weld metal oxygen and hence oxide inclusions can deteriorateweld metal mechanical properties. As shown in Figure 3.24, some inclusion -0.004 -0.008 ∆ sulfur (wt%) -0.012 -0.016 -0.020 0 1 2 3 4 5 ∞ CaO/SiO2Figure 3.23 Desulfurization of high-strength, low-alloy steel welds as a function ofbasicity index CaO/SiO2 of CaF2–CaO–SiO2 type ﬂux. Reprinted from Dallam et al.(47). Courtesy of American Welding Society.Figure 3.24 Fracture initiation at an inclusion in ﬂux-cored arc weld of high-strength,low-alloy steel. Reprinted from Bose et al. (54).
SLAG–METAL REACTIONS 89particles can act as a fracture initiation site (54). Besides oxide inclusions,oxygen in the weld pool can also react with carbon to form CO gas duringsolidiﬁcation. As shown in Figure 3.25, this can result in gas porosity in steelwelds (55). The addition of deoxidizers such as Al, Ti, Si, and Mn in the ﬁllermetal helps reduce the amount of porosity. Figure 3.26 shows that thetoughness of the weld metal decreases with increasing oxygen content (56).However, if the content of the acicular ferrite in the weld metal increases withthe weld oxygen content, the weld metal toughness may in fact increase(Chapter 9). Basic ﬂuxes, however, can have some drawbacks. They are often found tohave a greater tendency to absorb moisture, which can result in hydrogenembrittlement unless they are dried before welding.The slag detachability may Figure 3.25 Wormhole porosity in weld metal. From Jackson (55).Figure 3.26 Relationship between the toughness at 20°C and the oxygen content ofsteel welds. Reprinted from North et al. (56). Courtesy of American Welding Society.
90 CHEMICAL REACTIONS IN WELDINGnot be very good in a fully basic ﬂux. This makes slag removal more difﬁcult,especially in multiple-pass or narrow-groove welding. In the case of FCAW,basic ﬂuxes have also been observed to generate unstable arcs (57).3.3.5 Electrochemical ReactionsKim et al. (58, 59) studied the effect of electrochemical reactions on the weldmetal composition in SAW, and signiﬁcant composition differences wereobserved when the electrode polarity was varied in DC welding. The follow-ing anodic oxidation reactions were proposed: M (metal) + nO 2- (slag) = MOn (slag) + 2 ne - (3.23) O 2- (slag) = O(metal) + 2e - (3.24)These reactions occur at the electrode tip–slag interface in the electrode-positive polarity or the weld pool–slag interface in the electrode-negativepolarity. Therefore, oxidation losses of alloying elements and pickup of oxygenare expected at the anode. The following cathodic reduction reactions were also proposed: M 2+ (slag) + 2e - = M (metal) (3.25) Si 4+ (slag) + 4e - = Si(metal) (3.26) O(metal) + 2e - = O 2- (slag) (3.27)The ﬁrst two reactions are the reduction of metallic cations from the slag,and the third reaction is the removal (reﬁning) of oxygen from the metal.These reactions occur at the electrode tip–slag interface in the electrode-negative polarity or the weld pool–slag interface in the electrode-positivepolarity. The current density is much higher at the electrode tip–slag interfacethan at the weld pool–slag interface. Therefore, reactions at the electrode tipmay exert a greater inﬂuence on the weld metal composition than those at theweld pool. A carbon steel containing 0.18% C, 1.25% Mn, and 0.05% Si was sub-merged arc welded with a low-carbon steel wire of 0.06% C, 1.38% Mn, and0.05% Si and a ﬂux of 11.2% SiO2, 18.14% Al2O3, 33.2% MgO, 25.3% CaF2,6.9% CaO, and 1.2% MnO. Figure 3.27 shows the oxygen contents of themelted electrode tips and the detached droplets for both polarities, the 20 ppmoxygen content of the wire being included as a reference (58). A signiﬁcantoxygen pickup in the electrode tips is evident for both polarities, suggestingthat the excess oxygen came from decomposition of oxide components in theﬂux and the surrounding atmosphere. The anodic electrode tip has about twiceas much oxygen as the cathodic electrode tip, suggesting the signiﬁcant effectof electrochemical reactions. The difference in the oxygen content is due to
SLAG–METAL REACTIONS 91 1200 Anode Oxygen Concentration (ppm) 1000 Wire Cathode 800 600 400 200 0 Wire Electrode Droplet TipFigure 3.27 Oxygen contents of the welding wire, melted electrode tips, and detacheddroplets for both electrode-positive and electrode-negative polarities. Reprinted fromKim et al. (58). Courtesy of American Welding Society.oxygen pickup at the anode and oxygen removal (reﬁning) at the cathode. Ineither polarity the detached droplets contain more oxygen than the meltedelectrode tip. This suggests that the electrochemical reactions cease after thedroplets separate from the electrode tips, but the droplets pick up more oxygenfrom decomposed oxides while falling through the arc plasma. The higheroxygen content in the droplets separated from the anodic electrode tip is dueto the higher oxygen content of the melted anodic electrode tip. Figure 3.28 shows the silicon change in the weld pool for both polarities(58). Since there is plenty of oxygen from the decomposition of oxides, lossof silicon from the weld pool due to the thermochemical reaction Si + 2O =(SiO2) is likely. But the silicon loss is recovered by the cathodic reduction(Si4+) + 4e- = Si and worsened by the anodic oxidation Si + 2(O2-) = (SiO2) +4e-. Consequently, the silicon loss is more signiﬁcant at the anode than at thecathode. Figure 3.29 shows the manganese change in the weld pool for both polari-ties (58). The manganese loss from the weld pool to the slag is signiﬁcant inboth cases. This is because manganese is the richest alloying element in theweld pool (judging from the compositions of the workpiece and the ﬁllermetal) and MnO is among the poorest oxides in the ﬂux. As such, the ther-mochemical reaction Mn + O = (MnO) can shift to the right easily and causemuch manganese loss. Since manganese is known to have a high vapor pres-sure (Chapter 4), evaporation from the liquid can be another reason for muchmanganese loss. However, the manganese loss is partially recovered by thecathodic reduction (Mn2+) + 2e- = Mn and worsened by the anodic oxidationMn + (O2-) = (MnO) + 2e-. Consequently, the manganese loss is more signiﬁ-cant at the anode than at the cathode.
92 CHEMICAL REACTIONS IN WELDING 0.15 Silicon change in weld pool 0.10 ∆ silicon (wt.%) 0.05 Cathode 0.00 -0.05 Anode -0.10 -0.15 0.0 0.8 1.6 2.4 3.2 Travel speed (cm/s)Figure 3.28 Gain or loss of weld metal silicon due to reactions in weld pool forelectrode-positive and electrode-negative polarities as a function of welding speed.Reprinted from Kim et al. (58). Courtesy of American Welding Society. Manganese change in weld pool 0.00 -0.15 Cathode ∆ manganese (wt.%) -0.10 -0.15 -0.20 -0.25 -0.30 Anode -0.35 0.0 0.8 1.6 2.4 3.2 Travel speed (cm/s)Figure 3.29 Loss of weld metal manganese due to reactions in weld pool for elec-trode-positive and electrode-negative polarities as a function of welding speed.Reprinted from Kim et al. (58). Courtesy of American Welding Society.REFERENCES 1. Rein, R. H., in Proceedings of a Workshop on Welding Research Opportunities, Ed. B. A. McDonald, Ofﬁce of Naval Research, Washington, DC, 1974, p. 92.
REFERENCES 93 2. Eagar, T. W., in Weldments: Physical Metallurgy and Failure Phenomena, Proceed- ings of the Fifth Bolton Landing Conference, General Electric Co., Schenectady, NY, 1979, p. 31. 3. Harwig, D. D., Fountain, C., Ittiwattana, W., and Castner, H., Weld. J., 79: 305s, 2000. 4. Harwig, D. D., Ittiwattana, W., and Castner, H., Weld. J., 80: 126s, 2001. 5. Darken, L. S., and Gurry, R. W., Physical Chemistry of Metals, McGraw-Hill, New York, 1953. 6. Elliott, J. F., and Gleiser, M., Thermochemistry for Steelmaking, Vol. I, Addison Wesley, Reading, MA, 1960. 7. Pehlke, R. D., and Elliott, J. F., Trans. Metall. Soc. AIME., 218: 1091, 1960. 8. Elliott, J. F., Gleiser, M., and Ramakrishna, V., Thermochemistry for Steelmaking, Vol. II, Addison Wesley, Reading, MA, 1963. 9. Gedeon, S. A., and Eagar, T. W., Weld. J., 69: 264s, 1990.10. Pehlke, R. D., Unit Processes in Extractive Metallurgy, Elsevier, New York, 1979.11. DebRoy, T., and David, S. A., Rev. Modern Phys., 67: 85, 1995.12. Krause, H. G., Weld. J., 66: 353s, 1987.13. Hooijmans, J. W., and Den Ouden, G., Weld. J., 76: 264s, 1997.14. Sato, Y. S., Kokawa, H., and Kuwana, T., in Trends in Welding Research, Eds. J. M. Vitek, S. A. David, J. A. Johnson, H. B. Smartt, and T. DebRoy, ASM International, Materials Park, OH, June 1998, p. 131.15. Seferian, D., The Metallurgy of Welding, Wiley, New York, 1962.16. Atarashi, N., Welding Metallurgy, Maruzen, Tokyo, 1972 (in Japanese).17. Welding Handbook, Vol. 2, 7th ed., American Welding Society, Miami, FL, 1978, p. 134.18. Baune, E., Bonnet, C., and Liu, S., Weld. J., 79: 57s, 2000.19. Bracarense, A. Q., and Liu, S., Weld. J., 72: 529s, 1993.20. Christensen, N., Welding Metallurgy, Lecture Notes, Colorado School of Mines, 1979.21. Shutt, R. C., and Fink, D. A., Weld. J., 64: 19, 1985.22. Mirza, R. M., and Gee, R., Sci. Technol. Weld. Join., 4: 104, 1999.23. Albert, S. K., Remash, C., Murugesan, N., Gill, T. P. S., Periaswami, G., and Kulkarni, S. D., Weld. J., 76: 251s, 1997.24. Smith, R. D., Benson, D. K., Maroef, I., Olson, D. L., and Wildeman, T. R., Weld. J., 80: 122s, 2001.25. Fazackerley, W., and Gee, R., in Trends in Welding Research, Eds. H. B. Smartt, J. A. Johnson, and S. A. David, ASM International, Materials Park, OH, June 1995, p. 435.26. Principles and Technology of the Fusion Welding of Metal, Vol. 1., Mechanical Engineering Publishing Company, Peking, 1979 (in Chinese).27. Flanigan, A. E., Weld. J., 26: 193s, 1947.28. Eastwood, L. W., Gases in Non-ferrous Metals and Alloys, American Society for Metals, Cleveland, OH, 1953.29. Devletian, J. H., and Wood, W. E., Weld. Res. Council Bull., 290: December 1983.30. Shore, R. J., M.S. Thesis, Ohio State University, Columbus, OH, 1968.
94 CHEMICAL REACTIONS IN WELDING31. Pense, A. W., and Stout, R. D., Weld. Res. Council Bull., 152: July 1970.32. Fedoseev, V. A., Ryazantsev, V. I., Shiryaeva, N. V., and Arbuzov,Y. U. P., Svar. Proiz., 6: 15, 1978.33. Ishchenko, A. Y., and Chayun, A. G., paper presented at the Second Interna- tional Conference on Aluminum Weldments, Paper 110, Munich, F.R.G., May 1982.34. Matsuda, F., Nakata, K., Miyanaga, Y., Kayano, T., and Tsukamoto, K., Trans. Jpn. Weld. Res. Inst., 7: 181, 1978.35. Tomsic, M., and Barhorst, S., Weld. J., 63: 25, 1984.36. Baeslak, W. A. III, paper presented at the 1982 American Welding Society Con- vention, Kansas City, MO, 1982.37. Chai, C. S., and Eagar, T. W., Weld. J., 61: 229s, 1982.38. Burck, P. A., Indacochea, J. E., and Olson, D. L., Weld. J., 69: 115s, 1990.39. Abraham, K. P., Davies, M. W., and Richardson, F. D., J. Iron Steel Inst., 196: 82, 1960.40. Linnert, G. E., in Welding Metallurgy, Vol. 1, American Welding Society, Miami, FL, 1965, Chapter 8, p. 367.41. Gurevich, S. M., Metallurgy and Technology of Welding Titanium and Its Alloys, Naukova Dumka Publishing House, Kiev, 1979 (in Russian).42. Schenck, H., Physical Chemistry of Steelmaking, British Iron and Steel Research Association, London, 1945.43. Tuliani, S. S., Boniszewski, T., and Eaton, N. F., Weld. Metal Fab., 37: 327, 1969.44. Eagar, T. W., Weld. J., 57: 76s, 1978.45. Chai, C. S., and Eagar, T. W., Metall. Trans., 12B: 539, 1981.46. Baune, E., Bonnet, C., and Liu, S., Weld. J., 79: 66s, 2000.47. Dallam, C. B., Liu, S., and Olson, D. L., Weld. J., 64: 140s, 1985.48. Lathabai, S., and Stout, R. D., Weld. J., 64: 303s, 1985.49. Fleck, N. A., Grong, O., Edwards, G. R., and Matlock, D. K., Weld. J., 65: 113s, 1986.50. Liu, S., and Olson, D. L., Weld. J., 65: 139s, 1986.51. Ito, Y., and Nakanishi, M., Sumitomo Search, 15: 42, 1976.52. Abson, D. J., Dolby, R. E., and Hart, P. M. H., Trend in Steel and Consumables fore Welding, pp. 75–101, 1978.53. Cochrane, R. C., and Kirkwood, P. R., Trend in Steel and Consumables fore Welding, pp. 103–121, 1978.54. Bose, W. W., Bowen, P., and Strangwood, M., in Trends in Welding Research, Eds. H. B. Smartt, J. A. Johnson, and S. A. David, ASM International, Materials Park, OH, June 1995, p. 603.55. Jackson, C. E., in Weldability of Steels, 3rd. ed., Eds. R. D. Stout and W. D. Doty, Welding Research Council, New York, 1978, p. 48.56. North, T. H., Bell, H. B., Nowicki, A., and Craig, I., Weld. J., 57: 63s, 1978.57. Siewert, T. A., and Ferree, S. E., Metal Prog., 119: 58, 1981.58. Kim, J. H., Frost, R. H., Olson, D. L., and Blander, M., Weld. J., 69: 446s, 1990.59. Kim, J. H., Frost, R. H., and Olson, D. L., Weld. J., 77: 488s, 1998.
PROBLEMS 95FURTHER READING1. Olson, D. L., Liu, S., Frost, R. H., Edwards, G. R., and Fleming, D. A., in ASM Hand- book, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, p. 55.2. Gaskell, D. R., Introduction to Metallurgical Thermodynamics, 2nd ed., McGraw- Hill, New York, 1983.3. Richardson, F. D., Physical Chemistry of Melts in Metallurgy, Vols. 1 and 2. Academic, London, 1974.PROBLEMS3.1 Lithium alloys are known to have severe hydrogen porosity problems due to the hydration of oxides and formation of hydrides on the work- piece surface. If you were to do GMAW of these alloys using Al–Li wires, can you avoid porosity? If so, how?3.2 Do you prefer using an oxidizing or reducing ﬂame in gas welding of high-carbon steels? Explain why or why not.3.3 (a) Will decreasing welding speed help reduce weld porosity in gas–tung- sten arc welds of aluminum if the source of hydrogen is on the work- piece surface? (b) What about if the source of hydrogen is in the shielding gas? Explain why or why not.3.4 When welding rimmed steels or when doing GMAW of carbon steels using CO2 as the shielding gas, Mn- or Si-containing electrodes are used to prevent gas porosity. Explain why.3.5 Austenitic stainless steels usually contain very low levels of carbon, around or below 0.05 wt %. When welding stainless steels using CO2 as the shielding gas or covered electrodes containing abundant CaCO3, the weld metal often tends to carburize. Explain why and indicate how to avoid the problem.3.6 It has been reported that gas–tungsten arc welds of aluminum made in the overhead position tend to have a signiﬁcantly higher porosity level than those made in the ﬂat position. Explain why.3.7 The GTAW of pure iron with Ar–5% H2 as the shielding gas showed that the weld metal hydrogen content increased with increasing heat input per unit length of the weld. Explain why.3.8 Electromagnetic stirring has been reported to reduce hydrogen porosity in aluminum welds. Explain why.
96 CHEMICAL REACTIONS IN WELDING3.9 A steel container was welded by SAW with a ﬁller wire containing 1.38% Mn and 0.05% Si and a ﬂux containing 11.22% SiO2 and 1.15% MnO. Is the electrode tip Mn content expected to be greater or smaller than the wire Mn content and why? What about the Si content?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-44 Fluid Flow and MetalEvaporation in WeldingIn this chapter ﬂuid ﬂow in both the welding arc and the weld pool willbe described. The effect of weld pool ﬂuid ﬂow on the geometry of theresultant weld will be discussed. Evaporation of alloying elements from theweld pool and its effect on the weld metal composition will be presented.Finally, the effect of active ﬂuxes on weld penetration in GTAW will bediscussed.4.1 FLUID FLOW IN ARCSFigure 4.1 shows a gas–tungsten arc in GTAW with DC electrode negative (1).The shape of the electrode tip is characterized by the tip angle (also calledincluded or vertex angle) and the extent to which the sharp point is removed,that is, the truncation.4.1.1 Driving Force for Fluid FlowThe welding arc is an ionic gas, that is, a plasma, with an electric current passingthrough. The driving force for ﬂuid ﬂow in the arc is the electromagnetic forceor Lorentz force.The buoyancy force is negligible. Mathematically, the Lorentzforce F = J ¥ B, where J is the current density vector and B is the magneticﬂux vector. The current density vector J is in the direction the electric currentﬂows. According to the right-hand rule for the magnetic ﬁeld, if the thumbpoints in the direction of the current, the magnetic ﬂux vector B is in the direc-tion that the ﬁngers curl around the path of the current. Vectors F, J, and Bare perpendicular to each other. According to the right-hand rule for the elec-tromagnetic force, F is in the direction out of and perpendicular to the palmif the thumb points in the direction of J and the ﬁngers stretch out and pointin the direction of B.4.1.2 Effect of Electrode Tip GeometryThe welding arc is more or less bell shaped. The tip angle of a tungstenelectrode in GTAW is known to have a signiﬁcant effect on the shape of 97
98 FLUID FLOW AND METAL EVAPORATION IN WELDINGFigure 4.1 Gas–tungsten welding arc. Reprinted from Tsai and Kou (1). Copyright1990 with permission from Elsevier Science.the arc (Chapter 2)—it tends to become more constricted as the electrodetip changes from sharp to blunt. The change in the shape of the electrode tipchanges ﬂuid ﬂow in the arc plasma, which in turn changes the shape of thearc.A. Sharp Electrode Consider the case of GTAW with DC electrode nega-tive. The electric current converges from the larger workpiece to the smallerelectrode tip. It tends to be perpendicular to the electrode tip surface and theworkpiece surface, as illustrated in Figure 4.2a. The electric current inducesa magnetic ﬁeld, and its direction is out of the plane of the paper (as indicatedby the front view of an arrow) on the left and into the paper (as indicatedby the rear view of an arrow) on the right. The magnetic ﬁeld and the con-verging electric current ﬁeld together produce a downward and inwardforce F to push the ionic gas along the conical surface of the electrode tip.The downward momentum is strong enough to cause the high-temperatureionic gas to impinge on the workpiece surface and turn outward alongthe workpiece surface, thus producing a bell-shaped arc, as illustrated inFigure 4.2b. Fluid ﬂow in welding arcs has been studied by computer simulation (1–6).Tsai and Kou (1) investigated the effect of the electrode tip geometry on heatand ﬂuid ﬂow in GTAW arcs. Figure 4.3 (left) shows the current density dis-tribution in a 2-mm-long, 200-A arc produced by a 3.2-mm-diameter electrode
FLUID FLOW IN ARCS 99 Tungsten Tungsten electrode (-) electrode (-) Shielding gas Electric Arc current F F Workpiece (+) Workpiece (+) (a) (b)Figure 4.2 Arc produced by a tungsten electrode with a sharp tip: (a) Lorentz force(F); (b) ﬂuid ﬂow. 1.0 x 10 8 5.0 x 10 6 Tungsten A/m2 electrode (-) N/m3 0.5 mm 0.5 mm current density Lorentz forceFigure 4.3 Current density ﬁeld (left) and Lorentz force ﬁeld (right) in an arc pro-duced by a tungsten electrode with a 60° tip angle. Modiﬁed from Tsai and Kou (1).with a 60° angle tip. The electric current near the electrode tip is essentiallyperpendicular to the surface. The electromagnetic force, shown in Figure 4.3(right), is downward and inward along the conical surface of the electrode tip.As shown in Figure 4.4, this force produces a high-velocity jet of more than200 m/s maximum velocity and the jet is deﬂected radially outward along theworkpiece surface. This deﬂection of the high-temperature jet causes theisotherms to push outward along the workpiece surface, thus resulting in abell-shaped arc.
100 FLUID FLOW AND METAL EVAPORATION IN WELDING Tungsten 200 m/sec electrode (-) 0.5 mm velocity field and isothermsFigure 4.4 Velocity and temperature ﬁelds in an arc produced by a tungsten electrodewith a 60° tip angle. The isotherms from right to left are 11,000, 13,000, 15,000, 17,000,19,000, and 21,000 K. Modiﬁed from Tsai and Kou (1).B. Flat-End Electrode With a ﬂat-end electrode, on the other hand, thereis no longer an electrode tip to act as a ﬁxed cathode spot, where the electriccurrent enters the electrode. Consequently, the cathode spot moves aroundrather randomly and quickly in the ﬂat electrode end. The time-averageddiameter of the area covered by the moving spot can be considered as theeffective cathode spot size. Without a conical surface at the electrode end, theresultant Lorentz force is still inward and downward but the downward com-ponent is reduced, as illustrated in Figure 4.5a. Consequently, the resultant arccan be expected to be more constricted, as shown in Figure 4.5b. Figure 4.6 (left) shows the current density distribution in a 2-mm-long, 200-A arc produced by a 3.2-mm-diameter electrode with a ﬂat end and a 2.4-mm-diameter cathode spot. The electromagnetic force, shown in Figure 4.6 (right),is less downward pointing than that in the case of a 60° electrode (Figure 4.3).As shown in Figure 4.7, the isotherms are not pushed outward as much andthe resultant arc is thus more constricted.C. Power Density and Current Density Distributions These distributions atthe anode surface can be measured by the split-anode method (7–10). Figure4.8 shows such distributions for a 100-A, 2.7-mm-long gas–tungsten arc mea-sured by Lu and Kou (10). These distributions are often approximated by thefollowing Gaussian distributions:
FLUID FLOW IN ARCS 101 Tungsten Tungsten electrode (-) electrode (-) Shielding gas Electric current F F Workpiece (+) Workpiece (+) (a) (b)Figure 4.5 Arc produced by a tungsten electrode with a ﬂat end: (a) Lorentz force(F); (b) ﬂuid ﬂow. 5.0 x 10 7 Tungsten 1.2 x 10 6 A/m2 electrode (-) N/m3 0.5 mm 0.5 mm current density Lorentz forceFigure 4.6 Current density ﬁeld (left) and Lorentz force ﬁeld (right) in an arc pro-duced by a tungsten electrode with a ﬂat end. Modiﬁed from Tsai and Kou (1). 3Q Ê r2 ˆ q= expÁ 2 ˜ (4.1) pa 2 Ë -a 3¯ 3I Ê r2 ˆ j= expÁ 2 ˜ (4.2) pb 2 Ë -b 3 ¯where q is the power density, Q the power transfer to the workpiece, a theeffective radius of the power density distribution, j the current density, I thewelding current, and b the effective radius of the current density distribution.
102 FLUID FLOW AND METAL EVAPORATION IN WELDING Tungsten 200 m/sec electrode (-) 0.5 mm velocity field and isothermsFigure 4.7 Velocity and temperature ﬁelds in an arc produced by a tungsten electrodewith a ﬂat end. The isotherms from right to left are 11,000, 13,000, 15,000, 17,000, 19,000,and 21,000 K. Modiﬁed from Tsai and Kou (1). Experiment Experiment Gaussian 30 Gaussian Current density, amp/mm 2 Power density, W/mm 2 80 approximation approximation DC electrode negative 100 A, 12 V, Ar 60 20 2.7 mm arc length 2.4 mm electrode 50o tip angle 40 10 -0.27r2 20 q(r)=65.0e j(r)=17.6e-0.54r2 0 0 0 2 4 6 0 2 4 6 Radius, mm Radius, mm (a) (b)Figure 4.8 Gas–tungsten welding arc: (a) power density distribution; (b) currentdensity distribution. Reprinted from Lu and Kou (10). Courtesy of American WeldingSociety.The effective radius represents the location where q or j drops to 5% of itsmaximum value. Equation (4.1) is identical to Equation (2.20). Lee and Na (6) studied, by computer simulation, the effect of the arc lengthand the electrode tip angle on gas–tungsten arcs. Figure 4.9 shows that boththe power and current density distributions at the anode (workpiece) ﬂattenand widen as the arc length increases.
FLUID FLOW IN WELD POOLS 103 100 3.2 mm I = 200 A o θ e = 30 Heat flux, W/mm 2 80 6.3 mm Calculated 60 Measured 40 12.7 mm arc length 20 (a) 0 0 1 2 3 4 5 6 7 8 9 10 r-axis along base plate, mm 100 I = 200 A Current density, A/mm 2 3.2 mm o 80 θ e = 30 6.3 mm Calculated 60 Measured 40 12.7 mm arc length 20 (b) 0 0 1 2 3 4 5 6 7 8 9 10 r-axis along base plate, mmFigure 4.9 Effect of arc length on gas–tungsten welding arcs: (a) power density dis-tributions; (b) current density distributions. Modiﬁed from Lee and Na (6).4.2 FLUID FLOW IN WELD POOLS4.2.1 Driving Forces for Fluid FlowThe driving forces for ﬂuid ﬂow in the weld pool include the buoyancy force,the Lorentz force, the shear stress induced by the surface tension gradientat the weld pool surface, and the shear stress acting on the pool surface by thearc plasma. The arc pressure is another force acting on the pool surface, butits effect on ﬂuid ﬂow is small, especially below 200 A (11, 12), which is usuallythe case for GTAW. The driving forces for ﬂuid ﬂow in the weld pool, shownin Figure 4.10, are explained next.A. Buoyancy Force The density of the liquid metal (r) decreases withincreasing temperature (T). Because the heat source is located above thecenter of the pool surface, the liquid metal is warmer at point a and cooler atpoint b. Point b is near the pool boundary, where the temperature is lowest atthe melting point. As shown in Figure 4.10a, gravity causes the heavier liquid
104 FLUID FLOW AND METAL EVAPORATION IN WELDING Buoyancy Force a b b ρ weld pool F F b a base metal (a) T (b) Lorentz Force F F electric current (c) (d) Surface Tension Force b a b γ F F b a (e) (f) T Arc Shear Stress F F (g) (h)Figure 4.10 Driving forces for weld pool convection: (a, b) buoyancy force; (c, d)Lorentz force; (e, f ) shear stress caused by surface tension gradient; (g, h) shear stresscaused by arc plasma.metal at point b to sink. Consequently, the liquid metal falls along the poolboundary and rises along the pool axis, as shown in Figure 4.10b.B. Lorentz Force Gas–tungsten arc welding with DC electrode negative isused as an example for the purpose of discussion. The electric current in theworkpiece converges toward the tungsten electrode (not shown) and hencenear the center of the pool surface. This converging current ﬁeld, together withthe magnetic ﬁeld it induces, causes a downward and inward Lorentz force, asshown in Figure 4.10c. As such, the liquid metal is pushed downward along thepool axis and rises along the pool boundary, as shown in Figure 4.10d. The areaon the pool surface where the electric current goes through is called the anodespot (pb2, where b is the effective radius of the current density distribution).
FLUID FLOW IN WELD POOLS 105The smaller the anode spot, the more the current ﬁeld converges from theworkpiece (through the weld pool) to the anode spot, and hence the greaterthe Lorentz force becomes to push the liquid metal downward.C. Shear Stress Induced by Surface Tension Gradient In the absence of asurface-active agent, the surface tension (g) of the liquid metal decreases withincreasing temperature (T), namely, ∂g /∂T < 0. As shown in Figure 4.10e, thewarmer liquid metal with a lower surface tension at point a is pulled outwardby the cooler liquid metal with a higher surface tension at point b. In otherwords, an outward shear stress is induced at the pool surface by the surfacetension gradient along the pool surface. This causes the liquid metal to ﬂowfrom the center of the pool surface to the edge and return below the poolsurface, as shown in Figure 4.10f. Surface-tension-driven convection is alsocalled thermocapillary convection or Marangoni convection.D. Shear Stress Induced by Plasma Jet The plasma moving outward at highspeeds along a pool surface (Figure 4.4) can exert an outward shear stress atthe pool surface, as shown in Figure 4.10g. This shear stress causes the liquidmetal to ﬂow from the center of the pool surface to the pool edge and returnbelow the pool surface, as shown in Figure 4.10h. These driving forces are included either in the governing equations or asboundary conditions in the computer modeling of ﬂuid ﬂow in the weld pool(13). Oreper et al. (14) developed the ﬁrst two-dimensional ﬂuid ﬂow modelfor stationary arc weld pools of known shapes. Kou and Sun (15) developed asimilar model but allowed the unknown pool shape to be calculated. Kou andWang (16–18) developed the ﬁrst three-dimensional ﬂuid ﬂow model formoving arc and laser weld pools. Numerous computer models have beendeveloped subsequently for ﬂuid ﬂow in weld pools.4.2.2 Buoyancy ConvectionFigure 4.11 shows the buoyancy convection in a stationary weld pool of an alu-minum alloy calculated by Tsai and Kou (19). The liquid metal rises along thepool axis and falls along the pool boundary. The maximum velocity is alongthe pool axis and is only about 2 cm/s. The pool surface is slightly above theworkpiece surface because of the expansion of the metal upon heating andmelting.4.2.3 Forced Convection Driven by Lorentz ForceA. Flow Field Figure 4.12 shows the calculated results of Tsai and Kou (20)for a stationary weld pool in an aluminum alloy. The liquid metal falls alongthe pool axis and rises along the pool boundary (Figure 4.12a). The electriccurrent converges from the workpiece to the center of the pool surface (Figure4.12b). The Lorentz force is inward and downward (Figure 4.12c), thus pushing
106 FLUID FLOW AND METAL EVAPORATION IN WELDINGFigure 4.11 Buoyancy convection in aluminum weld pool. From Tsai and Kou (19). fluid flow current 0.4 m/sec density 1 mm 5 x 107A/m2 (a) (b) Lorentz force 5 x 10 5 N/m3 (c)Figure 4.12 Convection in an aluminum weld pool caused by Lorentz force: (a)ﬂow ﬁeld; (b) current density ﬁeld; (c) Lorentz force ﬁeld. Modiﬁed from Tsai and Kou(20).
FLUID FLOW IN WELD POOLS 107the liquid downward along the pool axis. The maximum velocity, about 40 cm/s,is one order of magnitude greater than that in the case of buoyancy convec-tion (Figure 4.11). The parameters used for the calculation include 150 A forthe welding current, 1800 W for the power input, 2 mm for the effective radiusof the power density distribution, and 4 mm for the effective radius of thecurrent density distribution.B. Deep Penetration Caused by Lorentz Force The Lorentz force (Figure4.12) makes the weld pool much deeper, as compared to the buoyancy force(Figure 4.11). The liquid pushed downward by the Lorentz force carries heatfrom the heat source to the pool bottom and causes a deep penetration.C. Physical Simulation of Effect of Lorentz Force Kou and Sun (15) weldedWoods metal (a low-melting-point alloy) with a heated copper rod in contactwith it, as shown in Figure 4.13a. The weld became much deeper when a 75-A current was passed through to the weld pool (no arcing and negligible re-sistance heating), as shown in Figure 4.13b. This conﬁrms the effect of theLorentz force on weld penetration.4.2.4 Marangoni ConvectionA. Heiple’s Model Heiple et al. (21–25) proposed that, when a surface-active agent is present in the liquid metal in a small but signiﬁcant amount,∂g /∂T can be changed from negative to positive, thus reversing Marangoni con-vection and making the weld pool much deeper. Examples of surface-active Heated rod Weld 75 A current Heated rod (b) Weld (a) Woods metal Woods metalFigure 4.13 Welds in Woods metal produced under the inﬂuence of (a) buoyancyforce and (b) Lorentz force. Modiﬁed from Kou and Sun (15).
108 FLUID FLOW AND METAL EVAPORATION IN WELDINGagents in steel and stainless steel are S, O, Se, and Te. Figure 4.14 shows thesurface tension data of two different heats of the stainless steel, one withapproximately 160 ppm more sulfur than the other (26). Figure 4.15 shows twoYAG laser welds made in 6.4-mm- (1/4-in.-) thick 304 stainless steel plates at3000 W and 3.39 mm/s (8 ipm). The plate with the shallower weld containsabout 40 ppm sulfur and that with the deeper weld contains about 140 ppmsulfur (27). Heiple’s model is explained in Figure 4.16. In the absence of a surface-activeagent (Figures 4.16a–c), the warmer liquid metal of lower surface tension nearthe center of the pool surface is pulled outward by the cooler liquid metal ofhigher surface tension at the pool edge. In the presence of a surface-activeagent (Figures 4.16d–f ), on the other hand, the cooler liquid metal of lowersurface tension at the edge of the pool surface is pulled inward by the warmerliquid metal of higher surface tension near the center of the pool surface. Theﬂow pattern in Figure 4.16e favors convective heat transfer from the heatsource to the pool bottom. In other words, the liquid metal carries heat from 2000 Surface Tension (mN/m) low sulfur stainless steel 1900 1800 1700 high sulfur 1600 stainless steel 1400 1600 1800 2000 2200 o Temperature ( C)Figure 4.14 Surface tension data of two different heats of 316 stainless steel, one with160 ppm more sulfur than the other. Modiﬁed from Heiple and Burgardt (26).Figure 4.15 YAG laser welds in two 304 stainless steels with (a) 40 ppm sulfur and(b) 140 ppm sulfur. From Limmaneevichitr and Kou (27).
FLUID FLOW IN WELD POOLS 109 γ surface tension, γ 2 1 1 2 distance, l 2 1 temperature,T (a) (b) (c) welding γ direction surface tension, γ 1 2 l 1 1 2 2 temperature,T (d) (e) (f)Figure 4.16 Heiple’s model for Marangoni convection in a weld pool: (a, b, c) low-sulfur steel; (d, e, f) high-sulfur steel.Figure 4.17 Marangoni convection with an outward surface ﬂow in a NaNO3 pool.Reprinted from Limmaneevichitr and Kou (28). Courtesy of American WeldingSociety.the heat source to the pool bottom more effectively, thus increasing the weldpenetration.B. Physical Simulation of Marangoni Convection Limmaneevichitr andKou (28) induced Marangoni convection in a transparent pool of NaNO3 witha defocused CO2 laser beam. The NaNO3 has a ∂g/∂T = -0.056 dyn/cm/°C. Sinceits transmission range is from 0.35 to 3 mm, NaNO3 is opaque to CO2 laser (10.6mm wavelength) just like a metal weld pool is opaque to an arc. Figure 4.17
110 FLUID FLOW AND METAL EVAPORATION IN WELDINGshows the ﬂow pattern induced by a CO2 laser beam of 2.5 W power and3.2 mm diameter (28). The pool surface is just below the two arrows thatindicate the directions of ﬂow at the pool surface. The two counterrotatingcells are, in fact, the two intersections between the donut-shaped ﬂow patternand the meridian plane of the pool. The outward surface ﬂow is much fasterthan the inward return ﬂow, which is typical of Marangoni convection. Asthe beam diameter is reduced, convection grows stronger and penetratesdeeper. It is worth noting that in conduction-mode (no-keyholing) laser beamwelding, the pool surface can be concave due to Marangoni convection andsurface tension (29) and, in fact, this has been shown to be the case experi-mentally (30) and by computer simulation (31). The concave NaNO3 poolsurface, however, is just a coincidence; the melt wets the container wall andthe meniscus makes the pool surface concave. Limmaneevichitr and Kou (32) added C2H5COOK to the NaNO3 pool andreversed the direction of Marangoni convection. The C2H5COOK is a surface-active agent of NaNO3 and, like S reduces the surface tension of liquid steel,it reduces the surface tension of NaNO3, ∂g /∂C being -22 dyn/(cm/mol %) (33).The NaNO3 pool shown in Figure 4.18 contains 2 mol % of C2H5COOK andits surface ﬂow is inward. This ﬂow reversion is because the surface tensionis now higher at the center of the pool surface than at the pool edge. At thecenter of the pool surface, C2H5COOK is lower in concentration because itdecomposes under the heating of the CO2 laser beam. Blocks of solid NaNO3, both pure and with C2H5COOK, were welded witha defocused CO2 laser beam. As shown in Figure 4.19, the weld in pure NaNO3is shallow and wide (32). This is because the thermal conductivity of NaNO3is low and heat transfer is dominated by the outward surface ﬂow to the poolFigure 4.18 Marangoni convection with an inward surface ﬂow in a NaNO3 poolcontaining 2 mol % C2H5COOK as a surface-active agent. Reprinted fromLimmaneevitchitr and Kou (32). Courtesy of American Welding Society.
FLUID FLOW IN WELD POOLS 111 CO2 laser (12.4 W) 0 weld mm -1 -2 base material -3 -7 -6 -5 -4 -3 -2 -1 0 1 2 3 4 5 6 7 mm : with surface-active agent; : withoutFigure 4.19 Laser welds in solid blocks of pure NaNO3 (open circles) and NaNO3 with2 mol % C2H5COOK (solid squares). Reprinted from Limmaneevichitr and Kou (32).Courtesy of American Welding Society. Surface Tension x 10 (N/mK) Temperature Coefficient of (a) 5 (b) Surface Tension (N/m) 2.2 3 4 150 ppm 1 1.7 0 -1 40 ppm 20 ppm -3 1.2 0 2020 0.0 Tem 0 .01 ulfur -5 pe 2420 1620 2020 2420 2820 rat .02 nt S ure 2820 0 erce Temperature (K) (K) PFigure 4.20 Liquid iron with various levels of sulfur: (a) surface tension; (b) tem-perature coefﬁcient of surface tension. Reprinted from Pitscheneder et al. (36).Courtesy of American Welding Society.edge. The weld in NaNO3 with 2 mol % C2H5COOK is deeper and slightlynarrower, which is consistent with the inward surface ﬂow observed duringwelding.C. Thermodynamic Analysis of Surface Tension Sahoo et al. (34) andMcNallan and DebRoy (35) calculated the surface tension of liquid metalsbased on thermodynamic data. Figure 4.20 shows the surface tension of liquidiron as a function of temperature and the sulfur content (36). For pure Fe,∂g/∂T is negative at all temperatures. For sulfur-containing Fe, however, ∂g /∂Tcan be positive at lower temperatures, which is consistent with the surfacetension measurements by Sundell et al. (37). Based on the surface tension data in Figure 4.20, Pitscheneder et al. (36)calculated Marangoni convection in stationary steel weld pools. Figure 4.21shows the results for a laser power of 5200 W and an irradiation time of 5 s.
112 FLUID FLOW AND METAL EVAPORATION IN WELDINGFigure 4.21 Convection in stationary laser weld pools of steels with (a) 20 ppm sulfurand (b) 150 ppm sulfur. Reprinted from Pitscheneder et al. (36). Courtesy of AmericanWelding Society.For the steel containing only 20 ppm sulfur, the outward surface ﬂow carriesheat from the heat source to the pool edge and results in a shallow and widepool (Figure 4.21a). For the steel containing 150 ppm sulfur, on the other hand,the inward surface ﬂow turns downward to deliver heat to the pool bottomand results in a much deeper pool (Figure 4.21b). In the small area near thecenterline of the pool surface, the temperature is above 2000 K and the surfaceﬂow is outward because of negative ∂g /∂T (Figure 4.20). It is worth noting thatZacharia et al. (38) showed that computer simulations based on a positive∂g /∂T for liquid steel at all temperatures can overpredict the pool depth.4.2.5 Forced Convection Driven by Plasma JetMatsunawa and Shinichiro (39, 40) demonstrated that the plasma shear stressinduced by a long arc in GTAW can outweigh both the Lorentz force in the
FLUID FLOW IN WELD POOLS 113 2 mm arc length 8 mm arc length 150 s 180 s 210 s 5 0 5 mm 5 0 5 mmFigure 4.22 Stationary gas–tungsten arc welds in a mild steel made with a 2-mm arc(left) and an 8-mm arc (right) for 150, 180, and 210 s. Modiﬁed from Matsunawa et al.(39). 2 mm arc length S: 18 ppm S: 77 ppm (a) 5 mm 8 mm arc length S: 18 ppm S: 77 ppm (b) ∂σ ∂Τ < 0 ∂σ ∂Τ = 0Figure 4.23 Stationary GTA welds in 304 stainless steels with 18 ppm sulfur and77 ppm sulfur made with an arc length of (a) 2 mm and (b) 8 mm. Modiﬁed fromMatsunawa et al. (39).weld pool and the surface tension gradients along the pool surface. Figure 4.22shows two series of stationary gas–tungsten arc welds in mild steel with 150,180, and 210 s of welding times, one with a 2-mm-long arc and the other witha 8-mm-long arc (39, 40). The 8-mm-arc welds are much wider and shallowerthan the 2-mm-arc welds. For a longer and thus wider arc, the Lorentz forcein the weld pool is smaller because of ﬂatter and wider current density distri-bution at the pool surface (Figure 4.9b). The surface tension gradients are alsosmaller because of the ﬂatter and wider power density distribution (Figure4.9a). However, location of the maximum shear stress shifts outward, thusallowing the shear stress to act on a greater portion of the pool surface. As shown in Figure 4.23, with a 2-mm-arc length the gas–tungsten arc weldis much deeper in the 304 stainless steel containing 77 ppm sulfur (39, 40). This
114 FLUID FLOW AND METAL EVAPORATION IN WELDING (a) (b)Figure 4.24 Weld pool shapes and isotherms in a 304 stainless steel with 50 ppm sul-fur calculated based on (a) laminar ﬂow and (b) turbulent ﬂow. Reprinted from Honget al. (42).is expected because sulfur makes ∂g/∂T either less negative or even positive.With a longer arc of 8 mm, however, the welds are shallow regardless of thesulfur level. This further demonstrates that forced convection driven by thearc plasma dominates in the welds made with the 8-mm-long arc.4.2.6 Effect of TurbulenceChoo and Szekely (41) ﬁrst considered turbulence in gas–tungsten arc weldpools and showed that turbulence can affect the pool depth signiﬁcantly.Hong et al. (42) demonstrated that a ﬂuid ﬂow model based on laminarcan over-predict the pool depth, as shown in Figure 4.24a for a GTA weldin a 304 stainless steel. When turbulence is considered, however, the effec-tive viscosity increases (meff > m) and convection slows down. Furthermore,the effective thermal conductivity (keff > k) increases and the effect of con-vection on the pool shape thus decreases. Consequently, the calculatedpool depth decreases and agrees better with the observed one, as shown inFigure 4.24b.4.3 METAL EVAPORATION4.3.1 Loss of Alloying ElementsDue to the intense heating of pool surface, evaporation from the weld poolcan be signiﬁcant with some alloying elements. Evaporation-induced Mg losses
METAL EVAPORATION 115Figure 4.25 Magnesium loss in a laser weld of an Al–Mg alloy. Reprinted from Pastoret al. (45). Courtesy of American Welding Society.from laser welds of aluminum alloys have been reported (43–45), and Figure4.25 is an example (45). Since Al–Mg alloys are solution strengthened by alloy-ing with Mg, Mg loss can result in substantial reduction in the tensile strengthof the weld metal. Similarly, Figure 4.26 shows evaporation-induced Mn lossesin laser welds of stainless steels (46). Figure 4.27 shows the vapor pressure of several metals (47). It is clear thatMg has a much higher vapor pressure than Al at any temperature; that is, Mghas a greater tendency to evaporate than Al.This explains Mg losses from laserwelds of aluminum alloys. It is also clear that Mn has a much higher vaporpressure than Fe, which explains Mn losses from laser welds of stainless steels.The Langmuir equation has been used to predict the evaporation rate of metalfrom the weld pool surface (47). However, according to DebRoy et al. (48–51),it can overpredict by a factor of 10 or more.4.3.2 Explosion of Metal DropletsEvaporation can also occur as metal droplets transfer from the ﬁller wire tothe weld pool through the arc, considering the very high temperature of the
116 FLUID FLOW AND METAL EVAPORATION IN WELDING 17 AISI 202 16 AISI 201 15 USS Weight % Mn TENELON 7 6 5 4 BASE METAL WELD ZONE 3 0 0.4 0.8 1.2 1.6 1.8 Horizontal Distance (mm)Figure 4.26 Manganese losses in laser welds of stainless steels. Reprinted fromDebRoy (46). 1x102 Zn Vapor pressure (mm Hg) Mg 1x100 Mn Li 1x10-2 Fe -4 1x10 1x10-6 Al 1x10-8 800 1000 1200 1400 1600 1800 2000 Temperature (K) Figure 4.27 Vapor pressure of several metals as a function of temperature.arc. Unstable metal transfer has been reported in GMAW with Al–Mgand Al–Mg–Zn ﬁller wires (52). In fact, high-speed photography revealedin-ﬂight explosions of metal droplets, resulting in much spattering. Figure4.27 shows that Zn has an even higher vapor pressure than Mg. Obviously,the high vapor pressures of Mg and Zn are likely to have contributed to theexplosions.4.4 ACTIVE FLUX GTAWThe use of ﬂuxes in GTAW has been found to dramatically increase weldpenetration in steels and stainless steels (53–58). The ﬂux usually consists ofoxides and halides, and it is mixed with acetone or the like to form a paste and
REFERENCES 117Figure 4.28 Gas–tungsten arc welds of 6-mm-thick 316L stainless steel: (a) without aﬂux; (b) with a ﬂux. Reprinted from Howse and Lucas (56).painted as a thin coating over the area to be welded. Figure 4.28 shows gas–tungsten arc welds made, without and with a ﬂux, in a 6-mm-thick 316L stain-less steel containing low S (0.005 wt %) (56). Howse and Lucus (56) observed that the arc becomes more constrictedwhen a ﬂux is used. Consequently, they proposed that the deeper penetrationis caused by arc constriction and the vaporized ﬂux constricts the arc by cap-turing electrons in the cooler outer region of the arc. For the same weldingcurrent, the more the arc is constricted, the smaller the area (pb2, where b isthe effective radius of the current density distribution) on the pool surface towhich the current ﬁeld converges from the workpiece (through the weld pool),and hence the greater the Lorentz force (F in Figure 4.10c) and deeperpenetration. Tanaka et al. (57), however, proposed that the inward surface ﬂow in thepresence of the oxygen from the oxide-containing ﬂux causes the deeperpenetration. They gas–tungsten arc welded a 304 stainless steel containinglittle (0.002 wt %) S, with He for shielding and TiO2 as the ﬂux (TiO2 is a mainingredient in several commercial ﬂuxes). They observed both an inwardsurface ﬂow and a signiﬁcant decrease in the surface tension when the ﬂux isused. As mentioned previously, ∂g/∂T can become positive and cause inwardsurface ﬂow in the presence of a surface-active agent such as oxygen. Theyobserved a steep temperature gradient across the pool surface caused by theinward surface ﬂow. Spectroscopic analysis of the arc showed that the blueluminous plasma appears to be mainly composed of metal vapor (Cr, Fe, etc.)from the weld pool. The steeper temperature gradient across the smaller poolsurface suggests a more localized metal evaporation and hence a more con-stricted arc, which also help increase the penetration.REFERENCES 1. Tsai, M. C., and Kou, S., Int. J. Heat Mass Transfer, 33: 2089, 1990. 2. Ushio, M., and Matsuda, F., Trans. JWM, 11: 7, 1982.
118 FLUID FLOW AND METAL EVAPORATION IN WELDING 3. Ushio, M., and Matsuda, F., J. Jpn. Weld. Soc., 6: 91, 1988. 4. McKelliget, J., and Szekely, J., Metall. Trans. A, 17A: 1139, 1986. 5. Choo, R. T. C., Szekely, J., and Westhoff, R. C., Weld. J., 69: 346, 1990. 6. Lee, S.-Y., and Na, S.-J., Weld. J., 75: 269, 1996. 7. Nestor, O. H., J. Appl. Phys., 33: 1638 (1962). 8. Schoeck, P. A., in Modern Developments in Heat Transfer, Ed. W. Ibele, Academic, New York, 1963, p. 353. 9. Tsai, N., Ph.D. Thesis, MIT, Cambridge, MA, 1983.10. Lu, M., and Kou, S., Weld. J., 67: 29s, 1988.11. Lawson, W. H. S., and Kerr, H. W., Welding Research International, Vol. 6, p. 1, 1976.12. Lin, M. L., and Eagar, T. W., Weld. J., 64: 63s, 985.13. Kou, S., Transport Phenomena in Materials Processing, Wiley, New York, 1996, pp. 3–115.14. Oreper, G. M., Eagar, T. W., and Szekely, J., Weld. J., 62: 307s, 1983.15. Kou, S., and Sun, D. K., Metall. Trans., 16A: 203, 1985.16. Kou, S., and Wang, Y. H., Weld. J., 65: 63s, 1986.17. Kou, S., and Wang, Y. H., Metall. Trans., 17A: 2265, 1986.18. Kou, S., and Wang, Y. H., Metall. Trans., 17A: 2271, 1986.19. Tsai, M. C., and Kou, S., Numerical Heat Transfer, 17A: 73, 1990.20. Tsai, M. C., and Kou, S., Weld. J., 69: 241s, 1990.21. Heiple, C. R., and Roper, J. R., Weld. J., 61: 97s, 1982.22. Heiple, C. R., and Roper, J. R., in Trends in Welding Research in the United States, Ed. S. A. David, American Society for Metals, Metals Park, OH, 1982, pp. 489– 520.23. Heiple, C. R., Roper, J. R., Stagner, R. T., and Aden, R. J., Weld. J., 62: 72s, 1983.24. Heiple, C. R., Burgardt, P., and Roper, J. R., in Modeling of Casting and Welding Processes, Vol. 2, Eds. J. A. Dantzig and J. T. Berry, TMS-AIME, Warrendale, PA, 1984, pp. 193–205.25. Heiple, C. R., and Burgardt, P., Weld. J., 64: 159s, 1985.26. Keene, B. J., Mills, K. C., and Brooks, R. F., Mater. Sci. Technol., 1: 568–571, 1985; Heiple, C. R., and Burgardt, P., ASM Handbook, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, p. 19.27. Limmaneevichitr, C., and Kou, S., unpublished research, University of Wisconsin, Madison, WI, 2000.28. Limmaneevichitr, C., and Kou, S., Weld. J., 79: 126s, 2000.29. Duley, W. W., Laser Welding, Wiley, New York, 1999, p. 76.30. Mazumder, J., and Voekel, D., in Laser Advanced Materials Processing—Science and Applications, Vol. 1, Eds. A. Matsunawa and S. Katayama, High Temperature Society of Japan, Osaka, Japan, 1992, pp. 373–380.31. Tsai, M. C., and Kou, S., Internal J. Numerical Methods Fluids, 9: 1503, 1989.32. Limmaneevichitr, C., and Kou, S., Weld. J., 79: 324s, 2000.33. Smechenko, V. K., and Shikobalova, L. P., Zh. Fiz. Khim., 21: 613, 1947.
FURTHER READING 11934. Sahoo, P., DebRoy, T., and McNallan, M. J., Metall. Trans. B., 19B: 483–491, 1988.35. McNallan, M. J., and DebRoy, T., Metall. Trans. B, 22B: 557–560, 1991.36. Pitscheneder, W., DebRoy, T., Mundra, K., and Ebner, R., Weld. J., 75: 71s–80s, 1996.37. Sundell, R. E., Correa, S. M., Harris, L. P., Solomon, H. D., and Wojcik, L. A., Report 86SRD013, General Electric Company, Schenectady, NY, December 1986.38. Zacharia, T., David, S. A., Vitek, J. M., and DebRoy, T., Weld. J., 68: 510s–519s, 1989.39. Matsunawa, A., and Shinichiro, Y., in Recent Trends in Welding Science and Tech- nology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, 1990, pp. 31–35.40. Matsunawa, A., in International Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, 1993, pp. 3–16.41. Choo, R. T. C., and Szekely, J., Weld. J., 73: 25s, 1994.42. Hong, K., Weckman, D. C., Strong, A. B., and Zheng, W., Science and Technology of Welding and Joining, in press; Weckman, D. C., in Trends in Welding Research, Eds. J. M. Vitek, S. A. David, J. A. Johnson, H. S. Smartt, and T. DebRoy, ASM Interna- tional, Materials Park, OH, p. 3, 1999.43. Moon, D. W., and Metzbower, E. A., Weld. J., 62: 53s, 1983.44. Cieslak, M. J., and Fuerschbach, P. W., Metall. Trans., 19B: 319, 1988.45. Pastor, M., Zhaq, H., Martukanitz, R. P., and Debroy, T., Weld. J, 78: 207s, 1999.46. DebRoy, T., in International Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, 1993, p. 18.47. Block-Bolten, A., and Eagar, T. W., Metall. Trans., 15B: 461, 1984.48. Mundra, K., and DebRoy, T., Weld. J., 72: 1s, 1991.49. Mundra, K., and DebRoy, T., Metall. Trans., 24B: 146, 1993.50. Yang, Z., and DebRoy, T., Metall. Trans., 30B: 483, 1999.51. Zhao, H., and DebRoy, T., Metall. Trans., 32B: 163, 2001.52. Woods, R. A., Weld. J., 59: 59s, 1980.53. Gurevich, S. M., Zamkov, V. N., and Kushnirenko, N. A., Avtomat Svarka, Automat. Weld., 9: 1, 1965.54. Gurevich, S. M., and Zamkov, V. N., Automat. Weld., 12: 13, 1966.55. Paskell, T., Lundin, C., and Castner, H., Weld, J., 76: 57, 1997.56. Howse, D. S., and Lucas, W., Sci. Technol. Weld. Join., 5: 189, 2000.57. Tanaka, M., Shimizu, T., Terasaki, H., Ushio, M., Koshi-ishi, F., and Yang, C.-L., Sci. Technol. Weld. Join., 5: 397, 2000.58. Kuo, M., Sun, Z., and Pan, D., Sci. Technol. Weld. Join., 6: 17, 2001.FURTHER READING1. Szekely, J., Fluid Flow Phenomena in Metals Processing, Academic, New York, 1979.2. Kou, S., Transport Phenomena and Materials Processing, Wiley, New York, 1996.3. Lancaster, J. F., The Physics of Welding, Pergamon, Oxford, 1984.
120 FLUID FLOW AND METAL EVAPORATION IN WELDINGPROBLEMS4.1 Experimental results show that the depth–width ratio of stainless steel welds increases with increasing electrode tip angle. How does the angle affect the effective radius of the electric current at the pool surface (the anode spot)? How does this radius in turn affect weld pool convection and the weld depth–width ratio?4.2 Experimental results show that the depth–width ratio of stainless steel welds decreases with increasing arc length. Explain why.4.3 It has been suggested that the weldability of stainless steels can be improved by oxidizing the surface by subjecting it to an elevated tem- perature in an oxidizing environment. From the penetration point of view, do you agree or disagree, and why?4.4 Two heats of a stainless steel with the same nominal composition but signiﬁcantly different sulfur contents are butt welded by autogenous GTAW. Which side of the weld is deeper and why?4.5 Two GTA welds of the same 304 stainless steel were made, one with a shielding gas of Ar and the other with Ar plus 700 ppm SO2 gas. Which weld was deeper and why?4.6 Consider Marangoni convection in a simulated weld pool of NaNO3 such as that shown in Figure 4.17. As the laser beam diameter is reduced at the same power from 5.9 to 1.5 mm, does Marangoni convection in the pool become faster or slower and why?4.7 In electron beam welding with the surface melting mode, which driving force for ﬂow is expected to dominate?4.8 In conduction-mode laser beam welding of a 201 stainless steel sheet 7 mm thick, the welding speed was 3 mm/s. The power was increased from 400 to 600 W. It was found that: (a) the Mn evaporation rate increased, (b) the weld pool grew signiﬁcantly larger in volume, and (c) the Mn concentration decrease in the resultant weld metal decreased. The Mn concentration was uniform in the resultant weld metal. Explain (c) based on (a) and (b).4.9 (a) Name the four different driving forces for weld pool convection. (b) In GMAW with spray metal transfer, is there an additional driving force for weld pool convection besides the four in (a)? If so, explain what it is and sketch the ﬂow pattern in the pool caused by this force alone.4.10 Parafﬁn has been used to study weld pool Marangoni convection. The surface tension of molten parafﬁn decreases with increasing tempera- ture, and convection is dominated by the surface tension effect. A thin
PROBLEMS 121 Figure P4.10slice of parafﬁn is sandwiched between two pieces of glass, and its topsurface is in contact with the tips of two hot soldering irons to producea weld pool that penetrates downward into the thin slice, as shown inFigure P4.10. Sketch and explain the ﬂow pattern and the shape of thepool.
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-45 Residual Stresses, Distortion,and FatigueIn this chapter the causes of residual stresses, distortion, and fatigue failure inweldments will be discussed, and the remedies will be described.5.1 RESIDUAL STRESSESResidual stresses are stresses that would exist in a body if all external loadswere removed. They are sometimes called internal stresses. Residual stressesthat exist in a body that has previously been subjected to nonuniform tem-perature changes, such as those during welding, are often called thermalstresses (1).5.1.1 Development of Residual StressesA. Three-Bar Arrangement The development of residual stresses can beexplained by considering heating and cooling under constraint (2). Figure 5.1shows three identical metal bars connected to two rigid blocks. All three barsare initially at room temperature. The middle bar alone is heated up, but itsthermal expansion is restrained by the side bars (Figure 5.1a). Consequently,compressive stresses are produced in the middle bar, and they increase withincreasing temperature until the yield stress in compression is reached. Theyield stress represents the upper limit of stresses in a material, at which plasticdeformation occurs. When heating stops and the middle bar is allowed to cooloff, its thermal contraction is restrained by the side bars (Figure 5.1b). Con-sequently, the compressive stresses in the middle bar drop rapidly, change totensile stresses, and increase with decreasing temperature until the yield stressin tension is reached. Therefore, a residual tensile stress equal to the yieldstress at room temperature is set up in the middle bar when it cools down toroom temperature. The residual stresses in the side bars are compressivestresses and equal to one-half of the tensile stress in the middle bar.B. Welding Roughly speaking, the weld metal and the adjacent base metalare analogous to the middle bar, and the areas farther away from the weldmetal are analogous to the two side bars (Figure 5.1c). This is because the122
RESIDUAL STRESSES 123 after (a) heating (b) stops middle bar: heated, middle bar: cooled, in tension in compression residual tensile stresses side bars in tension side bars: residual compressive stresses weld metal and adjacent base metal: residual tensile stresses (c) areas farther away from weld metal: residual compressive stressesFigure 5.1 Thermally induced stresses: (a) during heating; (b) during cooling;(c) residual stresses in weld.expansion and contraction of the weld metal and the adjacent base metal arerestrained by the areas farther away from the weld metal. Consequently, aftercooling to the room temperature, residual tensile stresses exist in the weldmetal and the adjacent base metal, while residual compressive stresses existin the areas farther away from the weld metal. Further explanations are givenas follows. Figure 5.2 is a schematic representation of the temperature change (DT)and stress in the welding direction (sx) during welding (2). The crosshatchedarea M–M¢ is the region where plastic deformation occurs. Section A–A isahead of the heat source and is not yet signiﬁcantly affected by the heat input;the temperature change due to welding, DT, is essentially zero. Along sectionB–B intersecting the heat source, the temperature distribution is rather steep.Along section C–C at some distance behind the heat source, the temperaturedistribution becomes less steep and is eventually uniform along section D–Dfar away behind the heat source. Consider now the thermally induced stress along the longitudinal direction,sx. Since section A–A is not affected by the heat input, sx is zero. Along sectionB–B, sx is close to zero in the region underneath the heat source, since theweld pool does not have any strength to support any loads. In the regionssomewhat away from the heat source, stresses are compressive (sx is negative)because the expansion of these areas is restrained by the surrounding metalof lower temperatures. Due to the low yield strength of the high-temperaturemetal in these areas, sx reaches the yield strength of the base metal at
124 RESIDUAL STRESSES, DISTORTION, AND FATIGUEFigure 5.2 Changes in temperature and stresses during welding. Reprinted fromWelding Handbook (2). Courtesy of American Welding Society.corresponding temperatures. In the areas farther away from the weld sx istensile, and sx is balanced with compressive stresses in areas near the weld. Along section C–C the weld metal and the adjacent base metal have cooledand hence have a tendency to contract, thus producing tensile stresses (sx ispositive). In the nearby areas sx is compressive. Finally, along section D–D theweld metal and the adjacent base metal have cooled and contracted further,thus producing higher tensile stresses in regions near the weld and compres-sive stresses in regions away from the weld. Since section D–D is well behindthe heat source, the stress distribution does not change signiﬁcantly beyond it,and this stress distribution is thus the residual stress distribution.5.1.2 Analysis of Residual StressesFigure 5.3 shows typical distributions of residual stresses in a butt weld.According to Masubuchi and Martin (3), the distribution of the longitudinalresidual stress sx can be approximated by the equation È Ê yˆ 2 ˘ È 1 Ê yˆ 2 ˘ s x ( y) = s m Í1 - ˙ exp Í- Ë ¯ ˙ (5.1) Î Ë b¯ ˚ Î 2 b ˚
RESIDUAL STRESSES 125 x in tension in compression in compression in tension σx weld y b σy base base metal weld metal with external constraint (a) (b)Figure 5.3 Typical distributions of longitudinal (sx) and transverse (sy) residualstresses in butt weld. Modiﬁed from Welding Handbook (2).where sm is the maximum residual stress, which is usually as high as the yieldstrength of the weld metal. The parameter b is the width of the tension zoneof sx (Figure 5.3a). The distribution of the transverse residual stress sy along the length of theweld is shown in Figure 5.3b. As shown, tensile stresses of relatively low mag-nitude are produced in the middle part of the weld, where thermal contrac-tion in the transverse direction is restrained by the much cooler base metalfarther away from the weld. The tensile stresses in the middle part of the weldare balanced by compressive stresses at the ends of the weld. If the lateral con-traction of the joint is restrained by an external constraint (such as a ﬁxtureholding down the two sides of the workpiece), approximately uniform tensilestresses are added along the weld as the reaction stress (1). This external con-straint, however, has little effect on sx. Figure 5.4 shows measured and calculated distributions of residual stressessx in a butt joint of two rectangular plates of 5083 aluminum (60 cm long, 27.5cm wide, and 1 cm thick) welded by GMAW (4). The calculated results arebased on the ﬁnite-element analysis (FEA), and the measured results are fromSatoh and Terasaki (5). The measurement and calculation of weld residualstresses have been described in detail by Masubuchi (1) and will not berepeated here. Residual stresses can cause problems such as hydrogen-inducedcracking (Chapter 17) and stress corrosion cracking (Chapter 18). Postweldheat treatment is often used to reduce residual stresses. Figure 5.5 shows theeffect of temperature and time on stress relief in steel welds (2). Table 5.1 listthe temperature ranges used for postweld heat treatment of various types ofmaterials (2). Other techniques such as preheat, peening, and vibration havealso been used for stress relief.
126 RESIDUAL STRESSES, DISTORTION, AND FATIGUE 1.2 1 Residual Stress, Sy/Sys 0.8 F.E.A. 0.6 Satoh et al. 1976 0.4 0.2 0 -0.2 -0.4 0 0.2 0.4 0.6 0.8 1 Distance along x-axis, x/WFigure 5.4 Measured and calculated distributions of residual stress in butt joint of5083 aluminum. Reprinted from Tsai et al. (4). Courtesy of American Welding Society.Figure 5.5 Effect of temperature and time on stress relief of steel welds. Reprintedfrom Welding Handbook (2). Courtesy of American Welding Society.5.2 DISTORTION5.2.1 CauseBecause of solidiﬁcation shrinkage and thermal contraction of the weld metalduring welding, the workpiece has a tendency to distort. Figure 5.6 illustratesseveral types of weld distortions (2). The welded workpiece can shrink in thetransverse direction (Figure 5.6a). It can also shrink in the longitudinal direc-tion along the weld (Figure 5.6b). Upward angular distortion usually occurswhen the weld is made from the top of the workpiece alone (Figure 5.6c). Theweld tends to be wider at the top than at the bottom, causing more solidiﬁca-tion shrinkage and thermal contraction at the top of the weld than at thebottom. Consequently, the resultant angular distortion is upward. In electron
DISTORTION 127 TABLE 5.1 Typical Thermal Treatments for Stress Relieving Weldments Soaking Material Temperature (°C) Carbon steel 595–680 Carbon–1/2% Mo steel 595–720 1 /2% Cr–1/2% Mo steel 595–720 1% Cr–1/2% Mo steel 620–730 11/4% Cr–1/2% Mo steel 705–760 2% Cr–1/2% Mo steel 705–760 21/4% Cr–1% Mo steel 705–770 5% Cr–1/2% Mo (Type 502) steel 705–770 7% Cr–1/2% Mo steel 705–760 9% Cr–1% Mo steel 705–760 12% Cr (Type 410) steel 760–815 16% Cr (Type 430) steel 760–815 11/4% Mn–1/2% Mo steel 605–680 Low-alloy Cr–Ni–Mo steels 595–680 2–5% Ni steels 595–650 9% Ni steels 550–585 Quenched and tempered steels 540–550 Source: Welding Handbook (2). (a) Transverse shrinkage (b) Longitudinal in butt weld shrinkage in butt weld (c) Angular distortion (d) Angular distortion in butt weld in fillet welds Figure 5.6 Distortion in welded structures. Modiﬁed from Welding Handbook (2).beam welding with a deep narrow keyhole, the weld is very narrow both atthe top and the bottom, and there is little angular distortion. When ﬁllet weldsbetween a ﬂat sheet at the bottom and a vertical sheet on the top shrink, theypull the ﬂat sheet toward the vertical one and cause upward distortion in the
128 RESIDUAL STRESSES, DISTORTION, AND FATIGUEFigure 5.7 Distortion in butt welds of 5083 aluminum with thicknesses of6.4–38 mm. Reprinted from Gibbs (6). Courtesy of American Welding Society.ﬂat sheet (Figure 5.6d). Figure 5.7 shows angular distortions in butt weldsof 5083 aluminum of various thicknesses (6). As shown, angular distortionincreases with workpiece thickness because of increasing amount of the weldmetal and hence increasing solidiﬁcation shrinkage and thermal contraction.The quantitative analysis of weld distortion has also been described in detailby Masubuchi (1) and hence will not be repeated here.5.2.2 RemediesSeveral techniques can be used to reduce weld distortion. Reducing thevolume of the weld metal can reduce the amount of angular distortion andlateral shrinkage. Figure 5.8 shows that the joint preparation angle and theroot pass should be minimized (7). The use of electron or laser beam weldingcan minimize angular distortion (Chapter 1). Balancing welding by using adouble-V joint in preference to a single-V joint can help reduce angular dis-tortion. Figure 5.9 shows that welding alternately on either side of the double-V joint is preferred (7). Placing welds about the neutral axis also helps reducedistortion. Figure 5.10 shows that the shrinkage forces of an individual weld
DISTORTION 129 larger angle more distortion smaller angle less distortion no angle little distortion (a) (b)Figure 5.8 Reducing angular distortion by reducing volume of weld metal and byusing single-pass deep-penetration welding. Modiﬁed from TWI (7). before welding one side alternating welded first welding more less distortion distortionFigure 5.9 Reducing angular distortion by using double-V joint and weldingalternately on either side of joint. Modiﬁed from TWI (7). Neutral Neutral axis axis more less distortion distortionFigure 5.10 Reducing distortion by placing welds around neutral axis. Modiﬁed fromTWI (7).
130 RESIDUAL STRESSES, DISTORTION, AND FATIGUEcan be balanced by placing another weld on the opposite side of the neutralaxis (7). Figure 5.11 shows three other techniques to reduce weld distortion(2, 8). Presetting (Figure 5.11a) is achieved by estimating the amount ofdistortion likely to occur during welding and then assembling the job withmembers preset to compensate for the distortion. Elastic prespringing (Figure5.11b) can reduce angular changes after the removal of the restraint. Pre-heating (Figure 5.11c), thermal management during welding, and postweldheating can also reduce angular distortion (4).Figure 5.11 Methods for controlling weld distortion: (a) presetting; (b) prespringing;(c) preheating (8). (a), (b) Reprinted from Welding Handbook (2). Courtesy ofAmerican Welding Society.
FATIGUE 1315.3 FATIGUE5.3.1 MechanismFailure can occur in welds under repeated loading (9, 10). This type of failure,called fatigue, has three phases: crack initiation, crack propagation, and frac-ture. Figure 5.12 shows a simple type of fatigue stress cycling and how it canresult in the formation of intrusions and extrusions at the surface of a mater-ial along the slip planes (10). A discontinuity point in the material (e.g., inclu-sions, porosity) can serve as the source for a slip to initiate. Figure 5.13 showsa series of intrusions and extrusions at the free surfaces due to the alternat-ing placement of metal along slip planes (10). Eventually, these intrusions andextrusions become severe enough and initial cracks form along slip planes. The Stress cyclic loading 2 σmax 1 0 Time 3 σmin 4 tensile tensile compressive compressive force force force force 1 2 3 4 source extrusion slip plane intrusion intrusionFigure 5.12 Fatigue stress cycling (top) and formation of intrusions and extrusions(bottom). Figure 5.13 Fatigue surface showing extrusions and intrusions. From Hull (10).
132 RESIDUAL STRESSES, DISTORTION, AND FATIGUEdirection of crack propagation is along the slip plane at the beginning and thenbecomes macroscopically normal to the maximum tensile stress (11).5.3.2 FractographyAs pointed out by Colangelo and Heiser (11), the appearance of fatigue fail-ures is often described as brittle because of the little gross plastic deformationand the fairly smooth fracture surfaces. Fatigue failures are usually easy to dis-tinguish from other brittle failures because they are progressive and they leavecharacteristic marks. Macroscopically, they appear as “beach,” “clam-shell,” or“conchoidal” marks, which represent delays in the fatigue loading cycle. Figure5.14 shows a fatigue fracture surface, where the arrow indicates the origin offracture (12).5.3.3 S–N CurvesFatigue data are often presented in the form of S–N curves, where the appliedstress (S) is plotted against number of cycles to failure (N). As the appliedstress decreases, the number of cycles to failure increases. There are manyfactors (13) that affect the fatigue behavior, such as material properties, jointconﬁguration, stress ratio, welding procedure, postweld treatment, loadingcondition, residual stresses, and weld reinforcement geometry. Figures5.15–5.17 show the effect of some of these factors observed by Sanders andDay (14) in aluminum welds.Figure 5.14 Fatigue fracture surface showing beach marks and origin of fracture.Reprinted, with permission, from Wulpi (12).
FATIGUE 133 100 Log maximum stress - MPa Log maximum stress - Ksi 500 50 5456-H116 100 10 5056 5052 -O -H32 50 5 6061 -T6 As welded transverse square butt joint 10 1 1 10 100 1,000 10,000 100,000 Number of kilocyclesFigure 5.15 Effect of alloy and material properties on fatigue of transverse butt joint.Modiﬁed from Sanders and Day (14). Longitudinal butt weld Transverse butt weld Transverse attachment Double transverse strap Cruciform 100 500 50 Log maximum stress - MPa Log maximum stress - Ksi Transve Longitu rs butt welde dinal b utt weld Transve 100 10 rse atta Double chment transve 50 Cruciform rse stra 5 p As welded 5083-O S.R. =0 10 1 10 1,000 10,000 100,000 Number of kilocyclesFigure 5.16 Effect of joint conﬁgurations on fatigue of 5083–O aluminum. Modiﬁedfrom Sanders and Day (14).
134 RESIDUAL STRESSES, DISTORTION, AND FATIGUE 100 500 Log maximum stress - Ksi Log maximum stress - MPa 50 Rein for testecement d in re salt moved 100 10 As we wate ; lded r Tested 50 in salt 5 water Transverse butt weld 5456-H117 S.R. = -1.0 10 1 10 100 1,000 10,000 Number of kilocyclesFigure 5.17 Effect of reinforcement removal and saltwater environment on fatigue of5456-H117 aluminum. Modiﬁed from Sanders and Day (14).5.3.4 Effect of Joint GeometryAs pointed out by Sanders and Day (14), in developing any fatigue behaviorcriteria for welding, the severity of joint geometry is probably the most criti-cal factor. The more severe the geometry, the lower the fatigue strength, asshown in Figure 5.16. The severity level of the longitudinal butt weld is lowestbecause both the weld and the base metal carry the load. The severity level ofthe cruciform, on the other hand, is highest since the welds alone carry theload and the parts are joined perpendicular to each other.5.3.5 Effect of Stress RaisersIt is well known that stress raisers tend to reduce fatigue life, namely, the so-called notch effect. Stress raisers can be mechanical, such as toes with a highreinforcement, lack of penetration, and deep undercuts. They can also be met-allurgical, such as microﬁssures (microcracks), porosity, inclusions, and brittleand sharp intermetallic compounds. Figure 5.18 shows a fatigue crack origi-nating from the toe (Chapter 1) of a gas–metal arc weld of a carbon steel (15).Figure 5.19 shows a fatigue failure originating from an undercut at the top ofan electron beam weld in a carbon steel and how undercutting can reducefatigue life (16).5.3.6 Effect of CorrosionAs also shown in Figure 5.17, a corrosive environment (salt water in this case)can often reduce fatigue life (14). This is called corrosion fatigue (17, 18). Ithas been reported that the damage can be almost always greater than the sumof the damage by corrosion and fatigue acting separately.
FATIGUE 135Figure 5.18 Fatigue crack originating from weld toe of gas–metal arc weld of carbonsteel. Reprinted from Itoh (15). Courtesy of American Welding Society.Figure 5.19 Effect of undercutting on fatigue in electron beam welds of carbon steel:(a) photograph; (b) fatigue life. Reprinted from Elliott (16). Courtesy of AmericanWelding Society.5.3.7 RemediesA. Shot Peening Welding and postweld grinding can create tensile residualstresses at the weld surface and promote fatigue initiation when under cyclicloading. Shot and hammer peening, on the other hand, can introduce surfacecompressive stresses to suppress the formation of intrusions and extrusionsand hence fatigue initiation (13). In shot peening, the metal surface is bom-barded with small spherical media called shot (19). Each piece of shot strik-
136 RESIDUAL STRESSES, DISTORTION, AND FATIGUEing the surface acts as a tiny peening hammer, producing a tiny indentation ordimple on the surface. Overlapping indentations or dimples develop a uniformlayer of residual compressive stresses. Figure 5.20 shows the residual stressesas a function of depth, namely, the distance below the surface (19). It is clearthat tensile residual stresses (>0) in the as-welded condition can be reducedby stress-relieving heat treatment and reversed to become highly compressiveresidual stresses (<0) by shot peening.B. Reducing Stress Raisers Figure 5.21 shows stress raisers caused byimproper welding and how they can be reduced or eliminated. Figure 5.17shows that removing the reinforcement improves the fatigue life (14). This isconsistent with the results of Nordmark et al. (20) shown in Figure 5.22 for Depth (inches) Residual stress (ksi) 0 0.01 0.02 0.03 Residual stress (MPa) 20 100 0 0.0 -100 -20 -200 -300 -40 -400 -60 0 0.25 0.50 0.75 Depth (mm) welded condition welded & stress relieved (SR) welded & shot peened (SP) welded, SR & SPFigure 5.20 Effect of stress relieving and shot peening on residual stresses near themetal surface. Modiﬁed from Molzen and Hornbach (19). reinforcement stress concentration undercut stress concentration lack of penetration Higher stress- Lower stress- concentration welds concentration welds Figure 5.21 Stress raisers in butt and T-welds and their corrections.
CASE STUDIES 137 reinforcement removed incomplete penetration reinforcement intact reinforcement removed reinforcement complete intact penetration 4 5 6 10 10 10 Cycles to failureFigure 5.22 Effect of weld reinforcement and penetration on fatigue life of transversebutt welds of 5456 aluminum. Reprinted from Nordmark et al. (20). Courtesy ofAmerican Welding Society.transverse butt welds of 6.4-mm- (1/4-in.-) thick 5456-H116 aluminum.However, in the case of incomplete penetration, removing the reinforcementcan dramatically reduce the fatigue life.5.4 CASE STUDIES5.4.1 Failure of a Steel Pipe Assembly (21)Figure 5.23a is a sketch showing a steel pipe of 10 mm wall thickness bent toturn in 90° and welded at the ends (b) to connecting ﬂanges. The pipe–ﬂangeassembly was connected to a bottle-shaped container (a) and a heavy over-hanging valve weighing 95 kg (e). The working pressure was 425 kg/cm2 andthe operating temperature was 105°C. The assembly was subjected to vibra-tions from the compressors provided at intervals along the pipe system.Graphical recorders showed evidence of the vibrations. The assembly failedafter a service time of about 2500 h. Examination of the failed assembly showed two fractures: fracture A atposition c and fracture B at the weld at position d. Both fractures exhibitedradial lines and striations typical of a fatigue fracture. Fracture A (Figure5.23b) originated in small craters accidentally formed in the ﬂange during arcwelding. Fracture B (Figure 5.23c) started at the weld toe, namely, the junc-tion between the weld reinforcement and the base metal surface. The fracturesurface (Figure 5.23d) shows the radial lines and striations of fatigue. The composition of the steel was unavailable, though metallographyshowed that it had a ferrite–pearlite structure, and the grains are ﬁne and
138 RESIDUAL STRESSES, DISTORTION, AND FATIGUEFigure 5.23 Failure of a steel pipe assembly (21): (a) pipe system; (b) fracture Acaused by craters at position c; (c) fracture B at weld at position d; (d) surface offracture B.equiaxed. Regarding fracture A, many cracks were observed in the fused metalin the craters and in the martensitic structure of the heat-affected zone. Underthe cyclic loading from the vibrations, these cracks served as the initiation sitesfor fatigue. As for fracture B, the notch effect due to reinforcement of the weldpromoted the fatigue failure.5.4.2 Failure of a Ball Mill (22)Figure 5.24 shows part of a ball mill used for ore crushing. The cylindrical shellof the ball mill was 10.3 m in length, 4.4 m in diameter, and 50 mm in thickness.
CASE STUDIES 139Figure 5.24 Failure of a ball mill: (a) design; (b) fatigue cracks (indicated by whitearrows); (c) origin of fatigue cracks. From Wallner (22).
140 RESIDUAL STRESSES, DISTORTION, AND FATIGUEA ﬂange with 100 mm wall thickness was welded to each end of the cylindri-cal shell (left half of Figure 5.24a). Both the cylindrical shell and the ﬂangeswere made from a killed steel with the composition of the steel being 0.19%C, 0.25% Si, 0.65% Mn, 0.025% P, and 0.028% S. The entire weight of the millcharge was approximately 320 tons and the drum operated at a rotation speedof 14 rpm.After about 3000 h of operation, long cracks appeared on the outsidesurface of the drum (Figure 5.24b). The failed drum was emptied, its inside inspected, and cracks ranging from100 to 1000 mm long were observed. It was found that these cracks had orig-inated from nearby tack welds, which had been made for holding insulationduring stress relieving of the drum (Figure 5.24c). Apparently, the high notcheffect has greatly reduced the fatigue life of the drum. It was subsequently sug-gested that the new joint design shown in the right half of Figure 5.24a be usedand a new stress relief method be employed in order to avoid the use of similartack welds.REFERENCES 1. Masubuchi, K., Analysis of Welded Structures, Pergamon, Elmsford, NY, 1980. 2. Welding Handbook, 7th ed., Vol. 1, American Welding Society, Miami, FL, 1976. 3. Masubuchi, K., and Martin, D. C., Weld. J., 40: 553s, 1961. 4. Tsai, C. L., Park, S. C., and Cheng, W. T., Weld. J., 78: 156s, 1999. 5. Satoh, K., and Terasaki, T., J. Jpn. Weld. Soc., 45: 42, 1976. 6. Gibbs, F. E., Weld. J., 59: 23, 1980. 7. TWI Job Knowledge for Welders, Part 34, Welding Institute, Cambridge, UK, March 21, 1998. 8. Watanabe, M., Satoh, K., Morii, H., and Ichikawa, I., J. Jpn. Weld. Soc., 26: 591, 1957. 9. Hertzberg, R. W., Deformation and Fracture Mechanics of Engineering Materials, Wiley, New York, 1976, p. 422.10. Hull, D., J. Inst. Met., 86: 425, 1957.11. Colangelo, V. J., and Heiser, F. A., Analysis of Metallurgical Failures, Wiley, New York, 1974.12. Wulpi, D., Understanding How Components Fail, American Society for Metals, Metals Park, OH, 1985, p. 144.13. Sanders, W. W. Jr., Weld. Res. Council Bull., 171: 1972.14. Sanders, W. W. Jr., and Day, R. H., in Proceedings of the First International Aluminum Welding Conference, Welding Research Council, New York, 1982.15. Itoh, Y., Weld. J., 66: 50s, 1987.16. Elliott, S., Weld. J., 63: 8s, 1984.17. Uhlig, H. H., Corrosion and Corrosion Control, 2nd ed., Wiley, New York, 1971.18. Fontana, M. G., and Greene, N. D., Corrosion Engineering, 2nd ed., McGraw-Hill, New York, 1978.19. Molzen, M. S., and Hornbach, D., Weld. J., 80: 38, 2001.
PROBLEMS 14120. Nordmark, G. E., Herbein, W. C., Dickerson, P. B., and Montemarano, T. W., Weld. J., 66: 162s, 1987.21. Fatigue Fractures in Welded Constructions, Vol. II, International Institute of Welding, London, 1979, p. 56.22. Wallner, F., in Cracking and Fracture in Welds, Japan Welding Society, Tokyo, 1972, P. IA3.1.FURTHER READING1. Masubuchi, K., Analysis of Welded Structures, Pergamon, Elmsford, NY, 1980.2. Fatigue Fractures in Welded Constructions, Vol. II, International Institute of Welding, London, 1979.3. Cracking and Fracture in Welds, Japan Welding Society, Tokyo, 1972.4. Gurney, T. R., Ed., Fatigue of Welded Structures, 2nd ed., Cambridge University Press, Cambridge, 1979.PROBLEMS5.1 (a) Austenitic stainless steels have a high thermal expansion coefﬁcient and a low thermal conductivity. Do you expect signiﬁcant distortion in their welds? (b) Name a few welding processes that help reduce weld distortion.5.2 Aluminum alloys have a high thermal expansion coefﬁcient, high thermal conductivity, and high solidiﬁcation shrinkage. Do you expect signiﬁcant distortion in their welds?5.3 The lower the weld reinforcement usually means the less the stress con- centration at the weld toe. One quick way to reduce the height of the reinforcement is to grind its upper half ﬂat without changing its contact angle with the workpiece surface. In this a proper treatment of the rein- forcement? Explain why or why not.
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-4PART IIThe Fusion Zone
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-46 Basic Solidiﬁcation ConceptsIn order to help explain the weld metal microstructure and chemical inho-mogeneities in subsequent chapters, some basic solidiﬁcation concepts will bepresented ﬁrst in this chapter. These concepts include solute redistribution,solidiﬁcation modes, constitutional supercooling, microsegregation and band-ing, the dendrite-arm or cell spacing, and the solidiﬁcation path.6.1 SOLUTE REDISTRIBUTION DURING SOLIDIFICATIONWhen a liquid of uniform composition solidiﬁes, the resultant solid is seldomuniform in composition. The solute atoms in the liquid are redistributed duringsolidiﬁcation. The redistribution of the solute depends on both thermody-namics, that is, the phase diagram, and kinetics, that is, diffusion, undercooling,ﬂuid ﬂow, and so on.6.1.1 Phase DiagramFigure 6.1a is a portion of a phase diagram near the corner of a pure metal ofmelting point Tm, with S denoting the solid phase and L the liquid phase. Con-sider the solidiﬁcation of alloy C0, that is, with initial melt composition C0. Avertical line through C0 intersects the liquidus line at the liquidus temperature,TL, and the solidus line at the solidus temperature, TS. Assume that under-cooling is negligible so that the solid begins to form when the liquid cools toTL. Also assume that equilibrium between the solid and the liquid is main-tained at the solid–liquid (S/L) interface throughout solidiﬁcation. This meansat any temperature T the composition of the solid at the interface, CS, and thecomposition of the liquid at the interface, CL, follow the solidus line and theliquidus line, respectively.A. Equilibrium Partition Ratio At any temperature T the equilibrium par-tition ratio, or the equilibrium segregation coefﬁcient, k, is deﬁned as CS k= (6.1) CLwhere CS and CL are the compositions of the solid and liquid at the S/L inter-face, respectively. The value of k depends on temperature T. For simplicity, 145
146 BASIC SOLIDIFICATION CONCEPTS melt of initial Equilibrium composition, CO Tm segregation TL coefficient: k = C S/C L < 1 Temperature, T T TS CS CL L (a) S S+L solidus line liquidus line; slope m L < 0 kC O CO Solute concentration, C liquidus line; slope m L > 0 solidus line CO Temperature, T L S+L TL CL S T (b) TS CS Tm k = C S/C L > 1 CO kC O Solute concentration, CFigure 6.1 Portion of a binary phase diagram showing the equilibrium partitionratio k.k is assumed constant; that is, the solidus and liquidus lines are both assumedstraight lines. The ﬁrst solid to form will have the composition kC0 according toEquation (6.1) and the phase diagram, that is, CL = C0 at T = TL. Considerthe case of k < 1 ﬁrst. As the phase diagram in Figure 6.1a shows, the solidcannot accommodate as much solute as the liquid does, and the solid thusrejects the solute into the liquid during solidiﬁcation. Consequently, the solutecontent of the liquid continues to rise during solidiﬁcation. Since the solidgrows from the liquid, its solute content also continues to rise. As indicated bythe arrowheads on the solidus and liquidus lines in Figure 6.1a for k < 1, CSand CL both increase as temperature T of the S/L interface drops duringsolidiﬁcation. Consider now the case of k > 1. As the phase diagram in Figure 6.1b shows,the solid can accommodate more solute than the liquid does, and the solid thusabsorbs the solute from the liquid during solidiﬁcation. Consequently, thesolute content of the liquid continues to drop during solidiﬁcation. Since thesolid grows from the liquid, its solute content also continues to drop. As indi-cated by the arrowheads on the solidus and liquidus lines in Figure 6.1b fork > 1, CS and CL both decrease as temperature T of the S/L interface dropsduring solidiﬁcation.
SOLUTE REDISTRIBUTION DURING SOLIDIFICATION 147 rising Directional Solidification tubular Experiment furnace distance, z (rising) R: growth rate L G: temperature gradient R dT/dz at S/L cooler S/L (solid/liquid interface) s (rising) L: liquid metal water S: solid metal container (stationary) temperature, T Figure 6.2 Directional solidiﬁcation experiment.B. Slope of Liquidus Line The slope of the liquidus line, mL, is less than zerowhen k < 1 and vice versa, as shown in Figure 6.1. If the liquidus line is straight,a temperature T on the liquidus line can be expressed as T = Tm + mLCL (6.2)6.1.2 Complete Diffusion in Solid and LiquidTo help understand solute redistribution during solidiﬁcation, consider theone-dimensional solidiﬁcation experiment shown in Figure 6.2. A metal heldin a stationary container of an aluminum oxide tube is heated by a tubularfurnace at the top and cooled by a water cooler at the bottom. As thefurnace–cooler assembly rises steadily, the metal in the container solidiﬁesupward with a planar S/L interface. The growth rate R of the metal, that is,the travel speed of the S/L interface, can be adjusted by adjusting the risingspeed of the furnace–cooler assembly. The temperature gradient G in theliquid metal at the S/L interface can be adjusted by adjusting heating andcooling. This case of complete diffusion in both the solid and the liquid is shown inFigure 6.3, where a liquid metal of uniform initial composition C0 is allowedto solidify in one direction with a planar S/L interface, just like in the direc-tional solidiﬁcation experiment shown in Figure 6.2. This case is also calledequilibrium solidiﬁcation because equilibrium exists between the entire solidand the entire liquid, not just at the interface. Diffusion is complete in the solidand the liquid, and the solid and liquid are thus uniform in composition.Uniform composition in the liquid requires either complete mixing by strongconvection or complete diffusion in the liquid. Complete diffusion of thesolute in the liquid requires DLt >> l2, where l is the initial length of the liquid,DL the diffusion coefﬁcient of the solute in the liquid, and t the time available
148 BASIC SOLIDIFICATION CONCEPTS initial melt Tm composition,Co Temperature, T TL CL k<1 (a) T TS CS L S S+L kCo Co Co/k Concentration, C C Equilibrium Co/k solidification C L(f S) (b) Co C S(f S) kCo 0 Fraction of solid, f S 1 C SfS + C LfL = Co C solid liquid total fS fL = 1 - f S CL Co CS solid liquid (c) 0 S/L fS 1 solid liquid total volume of materialFigure 6.3 Solute redistribution during solidiﬁcation with complete diffusion in solidand liquid: (a) phase diagram; (b) CL(fs) and CS(fs); (c) composition proﬁles in solidand liquid.for diffusion. This is because the square root of Dt is often considered as anapproximation for the diffusion distance, where D is the diffusion coefﬁcient.This requirement can be met when l is very small, when solidiﬁcation is so slowthat the solute has enough time to diffuse across the liquid, or when the dif-fusion coefﬁcient is very high. Similarly, complete solute diffusion in the solidrequires DSt >> l2, where DS is the diffusion coefﬁcient of the solute in thesolid. Since DS is much smaller than DL, complete diffusion is much more dif-ﬁcult to achieve in solid than in liquid. Interstitial solutes (such as carbon insteel) tend to have a much higher DS than substitutional solutes (such as Crin steel) and are more likely to approach complete diffusion in solid. During solidiﬁcation the composition of the entire solid follows the solidusline and that of the entire liquid follows the liquidus line (Figure 6.3a). Thecomposition of the solid is a function of the fraction of the solid, that is, CS(fS).Likewise the composition of the liquid is a function of the fraction of the solid,
SOLUTE REDISTRIBUTION DURING SOLIDIFICATION 149that is, CL(fS). At the onset of solidiﬁcation at TL, the fraction of solid fs = 0,and the compositions of the solid and the liquid are kC0 and C0, respectively.As solidiﬁcation continues and temperature drops from TL to TS, the compo-sition of the entire solid rises from kC0 to C0 and that of the entire liquid fromC0 to C0/k (Figure 6.3b). At any time during solidiﬁcation, the compositions ofthe solid and liquid are uniform (as shown by the thick horizontal lines inFigure 6.3c). Solidiﬁcation ends at the solidus temperature TS and the resul-tant solid has a uniform composition of C0; that is, there is no solute segrega-tion at all. In Figure 6.3c the hatched areas CS fS and CL fL represent the amountsof solute in the solid and liquid, respectively, where fS and fL are the fractionsof solid and liquid, respectively. The area C0(fS + fL) represents the amount ofsolute in the liquid before solidiﬁcation. Based on the conservation of soluteand the fact that fS + fL = 1, CS fS + C L fL = C0 ( fS + fL ) = C0 (6.3)Substituting fS = 1 - fL into the above equation, the following equilibrium leverrule is obtained: C0 - CS fL = (6.4) C L - CS C L - C0 fS = (6.5) C L - CSand the composition of the liquid is C0 CL = (6.6) fL + k(1 - fL )6.1.3 No Solid Diffusion and Complete Liquid DiffusionThis case is shown in Figure 6.4. Diffusion in the solid is assumed negligible,and the solid is thus not uniform in composition. This requires that DSt << l 2.On the other hand, diffusion in the liquid is assumed complete, and the liquidis thus uniform in composition. This requires that DLt >> l 2. If mixing causedby strong convection is complete in the liquid, the liquid composition can alsobe uniform. Equilibrium exists between the solid and the liquid only at theinterface. Unlike the case of equilibrium solidiﬁcation, the solute cannot backdiffuse into the solid and all the solute rejected by the growing solid has togo into the liquid. Consequently, CL rises more rapidly during solidiﬁcationthan in the case of equilibrium solidiﬁcation. Since the solid grows from theliquid, its composition at the S/L interface CS also rises more rapidly than in
150 BASIC SOLIDIFICATION CONCEPTS initial melt Tm composition,C o TL Temperature, T CL k<1 T TS (a) CS L S S+L kCo Co Co /k Concentration, C f (c) Complete C C Liquid Diffusion c CL Co /k C L(f S) (b) Co Co CS solid liquid C S(f S) 0 1 kC o 0 S/L fS Fraction of Solid, f s 1 solid liquid (C L - CS )df S = (1 - f S )dC L total volume of material area 1 area 2 k<1 c dC L area 2 d Concentration, C c CL area 1 d Co dfS CS a b (d) b kCo fS fL = 1 - f S 0 solid S/L liquid 1 Fraction of Solid, f SFigure 6.4 Solute redistribution during solidiﬁcation with complete diffusion in liquidand no diffusion in solid: (a) phase diagram; (b) CL(fs) and CS(fs); (c) composition pro-ﬁles in solid and liquid; (d) conservation of solute.the case of equilibrium solidiﬁcation. When CL rises beyond C0 /k, CS risesbeyond C0 (Figure 6.4b). The two hatched areas in Figure 6.4c represent the amounts of solute in thesolid and liquid, and their sum equals the amount of solute in the liquid beforesolidiﬁcation, C0. Consider the conservation of solute shown in Figure 6.4d.Since the total amount of solute in the system (total hatched area) is con-served, the area under abcd equals the area ab¢ c ¢d ¢ under. As such, hatchedarea 1 equals hatched area 2 and, therefore,
SOLUTE REDISTRIBUTION DURING SOLIDIFICATION 151 (C L - CS ) dfS = (1 - fS ) dC L (6.7)Substituting CS = kCL into the above equation and integrating from CL = C0at fs = 0, k -1 CS = kC0 (1 - fS ) (6.8)or C L = C0 fL -1 k (6.9)The above two equations are the well-known Scheil equation for solute seg-regation (1). Equation (6.9) can be written for the fraction liquid as follows: 1 ( k -1) 1 ( 1- k ) Ê CL ˆ Ê C0 ˆ fL = = (6.10) Ë C0 ¯ Ë CL ¯ The nonequilibrium lever rule, that is, the counterpart of Equation (6.5), canbe written as C L - C0 fS = (6.11) C L - CSFrom the Scheil equation the average composition of the solid, C S , can bedetermined as Ú0 kC0 (1 - fS ) dfS C0 [1 - (1 - fS ) ] fS k -1 k CS = f = (6.12) S fS Ú0 dfS As already mentioned, the solidus and liquidus lines are both assumedstraight. From Figure 6.1a, it can be shown that (TL - Tm)/C0 = mL. Furthermore,based on the proportional property between two similar right triangles, it canbe shown that (Tm - TL)/(Tm - T) = C0/CL. Based on these relationships andEquation (6.10), the Scheil equation can be rewritten as follows: 1 1- k 1 1- k Ê Tm - TL ˆ Ê (- mL )Co ˆ fL = 1 - fS = = (6.13) Ë Tm - T ¯ Ë Tm - T ¯This equation can be used to determine the fraction of solid fs at a tempera-ture T below the liquidus temperature TL.
152 BASIC SOLIDIFICATION CONCEPTS6.1.4 No Solid Diffusion and Limited Liquid DiffusionThis case is shown in Figure 6.5. In the solid diffusion is assumed negligible.In the liquid diffusion is assumed limited, and convection is assumed negligi-ble. Consequently, neither the solid nor the liquid is uniform in compositionduring solidiﬁcation. Because of limited liquid diffusion, the solute rejected bythe solid piles up and forms a solute-rich boundary layer ahead of the growthfront, as shown in Figure 6.5c. Again, equilibrium exists between the solid andthe liquid only at the interface. initial melt composition,Co k<1 Limited Liquid Tm Diffusion Temperature, T TL (a) initial transient steady TS state L final transient S S+L transient Concentration, C final kC o Co Co /k steady transient C state initial C o/ k C L(f S) (b) Co C S(f S) kCo 0 Fraction Solid, f S 1 C solute-rich C o/ k boundary layer Co solid liquid (c) kCo 0 S/L fS 1 solid liquid total volume of materialFigure 6.5 Solute redistribution during solidiﬁcation with limited diffusion in liquidand no diffusion in solid: (a) phase diagram; (b) CL(fs) and CS(fs); (c) composition pro-ﬁles in solid and liquid.
SOLUTE REDISTRIBUTION DURING SOLIDIFICATION 153 Unlike the previous case of complete liquid diffusion and no solid diffu-sion, the solute rejected by the growing solid forms a solute-rich boundarylayer ahead of the growth front, rather than spreading uniformly in the entireliquid. Consequently, CL and hence CS rise more rapidly than those in the caseof complete liquid diffusion and no solid diffusion. The period of rising CL andCS is called the initial transient (Figure 6.5b). When CL and CS reach C0 /k andC0, respectively, a steady-state period is reached, within which CL, CS, and theboundary layer (Figure 6.5c) remain unchanged. As the boundary layer movesforward, it takes in a liquid of composition C0 and it leaves behind a solid ofthe same composition C0. Since the input equals the output, the boundary layerremains unchanged. This steady-state condition continues until the boundarylayer touches the end of the liquid, that is, when the thickness of the remain-ing liquid equals that of the steady-state boundary layer. Here the volumeof the remaining liquid is already rather small, and any further decrease involume represents a very signiﬁcant percentage drop in volume. As such,the remaining liquid quickly becomes much more concentrated in solute assolidiﬁcation continues, and CL and hence CS rise sharply. This ﬁnal period ofrapidly rising CL and CS is called the ﬁnal transient, and its length equals thethickness of the steady-state boundary layer. The solute-rich boundary layer is further examined in Figure 6.6. It has beenshown mathematically (2) that the steady-state composition proﬁle in theboundary layer is initial melt composition,Co k<1 Tm Temperature, T TL Limited Liquid L Diffusion S S+L TS (a) Concentration, C kCo Co Co/k growth rate, R C solid liquid S/L solute-rich Co/k boundary Co layer kCo δ= (b) DL /R Z distance, xFigure 6.6 Solidiﬁcation with limited diffusion in liquid and no diffusion in solid: (a)phase diagram; (b) solute-rich boundary layer.
154 BASIC SOLIDIFICATION CONCEPTS C L - C0 = e - ( R DL )Z (6.14) C0 k - C0where R is the growth rate and Z the distance from the S/L interfacepointing into the liquid. At Z = 0, CL - C0 has a maximum value of C0 /k -C0 and at Z = DL/R it drops to 1/e (about one-third) of the maximumvalue. As such, the thickness of the boundary layer at the steady state can betaken as d ഠ DL/R. As such, the characteristic length of the ﬁnal transient isDL/R. It also has been shown mathematically (3, 4) that, for k << 1, the composi-tion proﬁle in the initial transient can be expressed as C0 - CS = e - k ( R DL ) x (6.15) C0 - kC0where x is the distance from the starting point of solidiﬁcation. At x = 0, C0 -CS has a maximum value of C0 - kC0 and at x = DL/kR it drops to 1/e ofthe maximum value. As such, the characteristic length of the initial transientis DL/kR, which is much greater than that of the ﬁnal transient because k issigniﬁcantly less than 1. Equation (6.15) can be rearranged as follows: CS 1- = (1 - k)e - k ( R DL ) x (6.16) C0Upon taking the logarithm on both sides, the above equation becomes Ê CS ˆ Ê log e ˆ log 1 - = log(1 - k) - x (6.17) Ë C0 ¯ Ë DL kR ¯The left-hand-side of Equation (6.17) can be plotted against the distancex. From the intercept the value of k can be checked, and from the slopethe length of the initial transient DL/kR can be found. From this thegrowth rate R can be found if the diffusion coefﬁcient DL is known or viceversa. Figure 6.7 shows three different types of solute of redistributions thatcan occur when diffusion in the solid is negligible during solidiﬁcation. Intype 1 either liquid diffusion or convection-induced mixing in the liquidis complete, and the resultant solute segregation is most severe (Figure 6.7d).In type 3, on the other hand, liquid diffusion is limited and there is noconvection-induced mixing in the liquid, and the resultant solute segrega-tion is least severe. Type 2 is intermediate, so is the resultant solutesegregation.
SOLIDIFICATION MODES AND CONSTITUTIONAL SUPERCOOLING 155 solid liquid Type 1: complete liquid diffusion or mixing C o kC (a) o solid liquid Solute concentration, C Type 2: limited liquid diffusion, some convection C o kC solid liquid (b) o Type 3: limited liquid diffusion, C /k no convection o C o kC solid liquid o (c) solid C Type 3 (least segregation) C o kC Type 1 (most o (d) Type 2 segregation) Fraction Solid, f sFigure 6.7 Solute redistributions in the absence of solid diffusion: (a) type 1; (b) type2; (c) type 3; (d) resultant segregation proﬁles.6.2 SOLIDIFICATION MODES ANDCONSTITUTIONAL SUPERCOOLING6.2.1 Solidiﬁcation ModesDuring the solidiﬁcation of a pure metal the S/L interface is usually planar,unless severe thermal undercooling is imposed. During the solidiﬁcation of analloy, however, the S/L interface and hence the mode of solidiﬁcation can beplanar, cellular, or dendritic depending on the solidiﬁcation condition and thematerial system involved. In order to directly observe the S/L interface duringsolidiﬁcation, transparent organic materials that solidify like metals have beenused. Shown in Figure 6.8 are the four basic types of the S/L interfacemorphology observed during the solidiﬁcation of such transparent materials:planar, cellular, columnar dendritic, and equiaxed dendritic (5, 6). Typical
156 BASIC SOLIDIFICATION CONCEPTSFigure 6.8 Basic solidiﬁcation modes (magniﬁcation 67¥): (a) planar solidiﬁcation ofcarbon tetrabromide (5); (b) cellular solidiﬁcation of carbon tetrabromide with a smallamount of impurity (5); (c) columnar dendritic solidiﬁcation of carbon tetrabromidewith several percent impurity (5); (d) equiaxed dendritic solidiﬁcation of cyclohexanolwith impurity (6). From Solidiﬁcation (5), pp. 132–134, with permission.microstructures resulting from the cellular, columnar dendritic, and equiaxeddendritic modes of solidiﬁcation in alloys are shown in Figures 6.9a, b, and c,respectively (7–9). A three-dimensional view of dendrites is shown in Figure6.9d (10).6.2.2 Constitutional SupercoolingTwo major theories have been proposed to quantitatively describe the break-down of a planar S/L interface during solidiﬁcation: the constitutional super-cooling theory by Chalmer and co-workers (11, 12) and the interface stabilitytheory by Mullins and Sekerka (13–15). The former theory considers only thethermodynamic aspect of the problem while the latter incorporates the inter-face kinetic and heat transfer aspects. For simplicity, however, only the con-stitutional supercooling theory will be described here. Consider the solidiﬁcation of alloy C0 at the steady state with a planar S/Linterface, as shown in Figure 6.10. As shown previously in Figure 6.6, the com-position distribution in the solute-rich boundary layer is shown in Figure 6.10b.
SOLIDIFICATION MODES AND CONSTITUTIONAL SUPERCOOLING 157Figure 6.9 Nonplanar solidiﬁcation structure in alloys. (a) Transverse section of a cel-lularly solidiﬁed Pb–Sn alloy from Journal of Crystal Growth (7) (magniﬁcation 48¥).(b) Columnar dendrites in a Ni alloy. From New Trends in Materials Processing (8),with permission. (c) Equiaxed dendrites of a Mg–Zn alloy from Journal of Inst. ofMetals (9) (magniﬁcation 55¥). (d) Three-dimensional view of dendrites in a Ni-basesuperalloy. Reprinted from International Trends in Welding Science and Technology(10).The liquidus temperature distribution corresponding to this composition dis-tribution can be constructed point by point from the liquidus line of the phasediagram and is shown in Figure 6.10c. A boundary layer consisting of the liquidphase alone is thermodynamically stable only if its temperature is above theliquidus temperature. If its temperature is below the liquidus temperature,solid and liquid should coexist. This means that the planar S/L interface should
158 BASIC SOLIDIFICATION CONCEPTS growth rate, R S/L S L ∆T initial melt solute-rich slope of tangent = composition,Co boundary layer DL /R ∆T Temperature, T L T actual slope G < TL DL /R L region of ∆T constitutional ∆T G ∆ + or < T S supercooling R DL TS S solidus liquidus Co Co/k Concentration, C (c) distance from S/L (a) C To avoid constitutional Co /k supercooling: G ∆T > Co R DL δ = D /R L (b) distance from S/LFigure 6.10 Constitutional supercooling: (a) phase diagram; (b) composition proﬁlein liquid; (c) liquidus temperature proﬁle in liquid.break down to a cellular or dendritic one so that solid cells or dendrites cancoexist with the intercellular or interdendritic liquid (Figures 6.8b–d). Theshaded area under the liquidus temperature distribution in Figure 6.10c indi-cates the region where the actual liquid temperature is below the liquidus tem-perature, that is, the region of constitutional supercooling. The shaded areabelow the liquidus line in Figure 6.10a, which depends on DL and R, indicatesthe corresponding region of constitutional supercooling in the phase diagram.Obviously, this area lies within the solid–liquid region of the phase diagram,that is, liquid alone is unstable and solid and liquid should coexist. The temperature difference across the boundary layer is the equilibriumfreezing range DT = TL - TS. As shown previously, the thickness of the bound-ary layer at the steady state is DL/R. As such, the slope of the tangent to theliquidus temperature distribution at the S/L interface is DT/(DL/R) or RDT/DL.To ensure that a planar S/L interface is stable, the actual temperature gradientG at the S/L interface must be at least RDT/DL. Therefore, for a planar S/Linterface to be stable at the steady state, the following criterion must be met: G DT ≥ (6.18) R DL
SOLIDIFICATION MODES AND CONSTITUTIONAL SUPERCOOLING 159This is the steady-state form of the criterion for planar growth. It says that foran alloy to be able to grow with a planar solidiﬁcation mode, the ratio G/Rmust be no less than DT/DL. The constitutional supercooling theory has beenveriﬁed experimentally by many investigators (16–23). In general, this theorypredicts fairly closely the conditions required to initiate the breakdown of aplanar S/L interface in alloys with isotropic surface energy. According to Equation (6.18), the higher the temperature gradient G andthe lower the growth rate, the easier for a planar S/L interface to be stable.On the other hand, the higher the freezing range DT and the lower the diffu-sion coefﬁcient DL, the more difﬁcult for a planar S/L interface to be stable.For an Al–4% Cu alloy, for example, TL, TS and DL, are 650°C, 580°C, and 3 ¥10-5 cm2/s, respectively. If the temperature gradient G is 700°C/cm, the growthrate R has to be less than or equal to 3 ¥ 10-4 cm/sec in order to have planarsolidiﬁcation. If the growth rate is higher than this, the planar S/L interfacewill break down and cellular or dendritic solidiﬁcation will take place. Figure 6.11 shows that the solidiﬁcation mode changes from planar to cel-lular, to columnar dendritic, and ﬁnally to equiaxed dendritic as the degree ofconstitutional supercooling continues to increase. The region where dendrites(columnar or equiaxed) and the liquid phase coexist is often called the mushyzone (2). It is interesting to note that at a very high degree of constitutionalsupercooling (Figure 6.11d) the mushy zone can become so wide that it iseasier for equiaxed dendrites to nucleate than for columnar dendrites tostretch all the way across the mushy zone. Unfortunately, simple theories l tua Ac Increasing constitutional supercooling Equilibrium (a) S L Planar S L Cellular (b) Columnar dendritic (c) S L constitutional M supercooling Equiaxed (d) dendritic S L MFigure 6.11 Effect of constitutional supercooling on solidiﬁcation mode: (a) planar;(b) cellular; (c) columnar dendritic; (d) equiaxed dendritic (S, L, and M denote solid,liquid, and mushy zone, respectively).
160 BASIC SOLIDIFICATION CONCEPTSFigure 6.12 Breakdown of a planar S/L interface during the solidiﬁcation of pivalicacid–ethanol: (a) 0 s, (b) 120 s, (c) 210 s, (d) 270 s, (e) 294 s, (f) 338 s, (g) 378 s, (h) 456 s,(i) 576 s, and (j) 656 s. Reprinted from Liu and Kirkaldy (24). Copyright 1994 with per-mission from Elsevier Science.similar to the constitutional supercooling theory are not available for pre-dicting the transitions from the cellular mode to the columnar dendritic modeand from the columnar dendritic mode to the equiaxed dendritic mode. Figure 6.12 is a series of photographs showing the breakdown of a planarS/L interface into a cellular one during the solidiﬁcation of a pivalic acidalloyed with 0.32 mol % ethanol (24). The temperature gradient G was15°C/mm, and the growth rate R was suddenly raised to a higher level of5.7 mm/s, to suddenly lower the G/R ratio and trigger the breakdown by con-stitutional supercooling.6.3 MICROSEGREGATION AND BANDING6.3.1 MicrosegregationSolute redistribution during solidiﬁcation results in microsegregation acrosscells or dendrite arms. The analysis of solute redistribution during the direc-
MICROSEGREGATION AND BANDING 161tional solidiﬁcation of a liquid metal (Section 6.1) can be applied to soluteredistribution during the solidiﬁcation of an intercellular or interdendriticliquid during welding (or casting). The total volume of material in directionalsolidiﬁcation (Figures 6.3–6.5) is now a volume element in a cell or a dendritearm, as shown in Figure 6.13. Within the volume element the S/L interfaceis still planar even though the overall structure is cellular or dendritic. Thevolume element covers the region from the centerline of the cell or dendritearm to the boundary between cells or dendrite arms. Solidiﬁcation beginsin the volume element when the tip of the cell or dendrite arm reaches thevolume element. The case of the equilibrium partition ratio k < 1 is shown in Figure 6.14a.No segregation occurs when diffusion is complete in both the liquid and solid. volume element L L S S (a) (b)Figure 6.13 Volume elements for microsegregation analysis: (a) cellular solidiﬁcation;(b) dendritic solidiﬁcation. complete liquid & complete liquid & k<1 solid diffusion k>1 solid diffusion Co Co composition composition complete liquid diffusion, complete liquid diffusion, no solid diffusion kCo no solid diffusion Co Co kCo limited liquid diffusion, limited liquid diffusion, no solid diffusion kCo Co no solid diffusion Co kCo distance distance dendrite arm dendrite arm cell or cell or centerline of cell volume boundary between cells or dendrite arm element or dendrite arms (a) (b)Figure 6.14 Microsegregation proﬁles across cells or dendrite arms: (a) k < 1; (b) k > 1.
162 BASIC SOLIDIFICATION CONCEPTSThis requires that DLt >> l 2 and that DSt >> l 2, where l is now half the cell ordendrite arm spacing (the length of the volume element). Segregation is worstwith complete diffusion in the liquid but no diffusion in the solid. This requiresthat DLt >> l 2 and that DSt << l 2. Segregation is intermediate with limited dif-fusion in the liquid and no diffusion in the solid. When this occurs, there isa clear concentration minimum at the centerline of the cell or dendrite arm.Usually, there is some diffusion in the solid and the concentration minimummay not always be clear. The case of k > 1 is shown in Figure 6.14b. The seg-regation proﬁles are opposite to those of k < 1. Consider the case of a eutectic phase diagram, which is common amongaluminum alloys. Assume complete liquid diffusion and no solid diffusion. Asshown in Figure 6.15, the solid composition changes from kC0 to CSM, themaximum possible solute content in the solid, when the eutectic temperatureTE is reached. The remaining liquid at this point has the eutectic composition initial melt T composition,Co m T (a) L L Temperature, T T S eutectic S+L S T E C E Concentration, C kC C C SM o o CE Complete C Liquid Diffusion C SM (b) C L(f S) C o C S(f S) fE kC 0 Fraction of Solid, f 1 o s volume solid eutectic elementFigure 6.15 Solute redistribution during solidiﬁcation with complete diffusion inliquid and no diffusion in solid: (a) eutectic phase diagram; (b) composition proﬁles inliquid and solid.
EFFECT OF COOLING RATE 163 Solute concentration, C R = R1 R = R 2 > R1 R = R 1 < R2 Co /k solute- solute- rich band depleted band Co Time, t Figure 6.16 Formation of banding due to changes in the solidiﬁcation rate R.CE and, therefore, solidiﬁes as solid eutectic at TE. The fraction of eutectic, fE,can be calculated from Equation (6.13) with fL = fE and T = TE, that is, 1 ( 1- k ) Ê Tm - TL ˆ fE = (6.19) Ë Tm - TE ¯6.3.2 BandingIn addition to microsegregation, solute segregation can also occur as a resultof growth rate ﬂuctuations caused by thermal ﬂuctuations. This phenomenon,shown in Figure 6.16, is known as banding (2). As shown, steady-state solidi-ﬁcation occurs at the growth rate R1. When the growth rate is suddenlyincreased from R1 to R2, an extra amount of solute is rejected into the liquidat the S/L interface, causing its solute content to rise. As a result, the materialsolidiﬁes right after the increase in the growth rate has a higher solute con-centration than that before the increase. The boundary layer at R2 is thinnerthan that at R1 because, as mentioned previously, the boundary layer thicknessis about DL/R. The solute concentration eventually resumes its steady value ifno further changes take place. If, however, the growth rate is then decreasedsuddenly from R2 back to R1, a smaller amount of solute is rejected into theliquid at the S/L interface, causing its solute content to drop. As a result, thematerial solidiﬁes right after the decrease in the growth rate has a lower soluteconcentration than that just before the decrease. In practice, the growth ratecan vary as a result of thermal ﬂuctuations during solidiﬁcation caused byunstable ﬂuid ﬂow in the weld pool, and solute-rich and solute-depleted bandsform side by side along the solidiﬁcation path. When the ﬂow carrying heatfrom the heat source and impinging on the growth front suddenly speeds up,the growth rate is reduced and vice versa.6.4 EFFECT OF COOLING RATEIt has been observed that the higher the cooling rate, that is, the shorter thesolidiﬁcation time, the ﬁner the cellular or dendritic structure becomes (2).
164 BASIC SOLIDIFICATION CONCEPTSFigure 6.17 shows the dendrite arm spacing as a function of the cooling rateor solidiﬁcation time in three different materials (25–27). The relationship canbe expressed as (2) -n d = at n = b(e ) f (6.20)where d is the secondary dendrite arm spacing, tf is the local solidiﬁcation time,e is the cooling rate, and a and b are proportional constants. Figure 6.18 depicts the growth of a dendrite during solidiﬁcation (2). Thewindow for viewing the growing dendrite remains stationary as the dendritetip advances. As can be seen through the window, large dendrite arms grow atthe expense of smaller ones as solidiﬁcation proceeds. Since smaller dendritearms have more surface area per unit volume, the total surface energy of thesolidifying material in the window can be reduced if larger dendrite arms growat the expense of the smaller ones. The slower the cooling rate during solidi- Secondary dendrite arm spacing, µm 104 Al-4.5Cu 102 1 10-4 10-2 1 102 104 106 108 (a) Average local cooling rates, oC/s Secondary dendrite arm spacing, µ m 100 Brower et al. Abdulgadar 10 1 201 stainless steel 0.1 100 101 102 103 104 105 106 (b) Cooling rate, oC/s 10 Secondary dendrite 8 arm spacing, µ m 6 4 2 310 stainless steel 1 .01 .02 .04.06 .10 .20 (c) Solidification time, secFigure 6.17 Effect of cooling rate or solidiﬁcation time on dendrite arm spacing: (a)For Al–4.5Cu. From Munitz (25), (b) For 201 stainless steel. From Paul and DebRoy(26). (c) For 310 stainless steel. From Kou and Le (27).
EFFECT OF COOLING RATE 165Figure 6.18 Schematic showing dendritic growth of an alloy at a ﬁxed position atvarious stages of solidiﬁcation. Note that several smaller arms disappear while largerones grow. Reprinted from Flemings (2). 100 Cell spacing (microns) 80 60 40 20 0 10 20 30 50 70 100 200 (GR)-1 (oC/sec)-1Figure 6.19 Effect of GR on cell spacing in Sn–Pb alloys. Modiﬁed from Flemings (2)based on data from Plaskett and Winegard (28).ﬁcation, the longer the time available for coarsening and the larger the den-drite arm spacing (Figure 6.17). Figure 6.19 shows how GR affects the cell spacing in Sn–Pb alloys solidi-ﬁed in the cellular mode (2, 28). The product GR (°C/cm times cm/s) is, in fact,the cooling rate, judging from its unit of °C/s. As shown, the higher the coolingrate, that is, the lower (GR)-1, the ﬁner the cells become. The effect of the temperature gradient G and the growth rate R on thesolidiﬁcation microstructure of alloys is summarized in Figure 6.20. Together,G and R dominate the solidiﬁcation microstructure. The ratio G/R determinesthe mode of solidiﬁcation while the product GR governs the size of the solid-iﬁcation structure.
166 BASIC SOLIDIFICATION CONCEPTS hi gh a SL high G/R determines morphology SL er c G/R of solidification structure finer oolin cture GxR determines size of low coar Temperature gradient, G solidification structure stru g ra er c ser te (G ool stru ing xR); rate ture c (Gx R); ar Plan r la r na llu lum ritic Ce Co end D ed Equiax ic Low D endrit G/R b Growth rate, RFigure 6.20 Effect of temperature gradient G and growth rate R on the morphologyand size of solidiﬁcation microstructure.6.5 SOLIDIFICATION PATHConsider the eutectic phase diagram of a binary system A–B shown by thebroken lines in Figure 6.21a. To the left of the eutectic point, the primarysolidiﬁcation phase is g, namely, g is the ﬁrst thing to solidify. To the right, theprimary solidiﬁcation phase is a. The solid line represents the solidiﬁcationpath of alloy C0. The arrow in the solidiﬁcation path indicates the directionin which the liquid composition changes as temperature decreases. At step 1,where the fraction of the liquid phase L is fL = 1, g begins to form from theliquid phase, assuming negligible undercooling before solidiﬁcation. The com-position of the liquid phase follows the solid line representing L Æ g. At step2, solidiﬁcation is complete and fL = 0. In the case of a ternary system A–B–C, the phase diagram is three dimen-sional, with the base plane showing the composition and the vertical directionshowing the temperature. The liquidus is a surface (curved) instead of a lineas in a binary phase diagram (Figure 6.21a). The intersection between two liq-uidus surfaces is a line called the line of twofold saturation, instead of a pointintersection between two liquidus lines in a binary phase diagram. As shownin Figure 6.21b, when projected vertically downward to the base plane, theliquidus surfaces show areas of primary solidiﬁcation phases with the lines oftwofold saturation separating them. The solid line shows the solidiﬁcation path of alloy C0. At step 1, where thefraction of the liquid phase L is fL = 1, the solid phase g begins to form from
REFERENCES 167 primary γ primary α liquidus line 1 solidification Temperature, T path fL = 1 L L+ γ γ L L + α γ α (a) 2 fL = 0 A Co wt % B B to pure C solidification lines of twofold saturation: path m m3, 3n and 34 primary γ 2 γ primary α L γ+ L n 3 (b) wt % C α primary γ primary β L 1 fL = 1 γ+β fL = 0 A wt % B 4 to pure BFigure 6.21 Solidiﬁcation paths: (a) a binary A–B system; (b) a ternary A–B–Csystem.the liquid phase. As temperature decreases, the composition of the liquidphase follows the solid line representing L Æ g until the line of twofold satu-ration m3 is reached. At step 2, the a phase begins to form from the liquid,too. As temperature decreases further, the composition of the liquid phasefollows the solid line representing the ternary eutectic reaction L Æ g + a untilthe line of twofold saturation 3n is reached. At step 3, the formation of a fromthe liquid stops and is taken over by the formation of b. As temperaturedecreases still further, the composition of the liquid phase follows the solidline representing the ternary eutectic reaction L Æ g + b. This can go on untilthe line representing binary A–B (the abscissa) is reached, if there is still liquidavailable to get there. The fraction of liquid fL = 0 when solidiﬁcation iscomplete.REFERENCES 1. Scheil, E., Z. Metallk., 34: 70, 1942. 2. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974. 3. Pohl, R. G., J. Appl. Phys., 25: 668, 1954.
168 BASIC SOLIDIFICATION CONCEPTS 4. Kou, S., Transport Phenomena and Materials Processing, Wiley, New York, 1996. 5. Jackson, K. A., in Solidiﬁcation, American Society for Metals, Metals Park, OH, 1971, p. 121. 6. Jackson, K. A., Hunt, J. D., Uhlmann, D. R., Sewand III, T. P., Trans. AIME, 236: 149, 1966. 7. Morris, L. R., and Winegard, W. C., J. Crystal Growth, 5: 361, 1969. 8. Giamei, A. F., Kraft, E. H., and Lernkey, F. D., in New Trends in Materials Pro- cessing, American Society for Metals, Metals Park, OH, 1976, p. 48. 9. Kattamis, T. Z., Holmber, U. T., and Flemings, M. C., J. Inst. Metals, 55: 343, 1967.10. David, S. A., and Vitek, J. M., in International Trends in Welding Science and Tech- nology, Eds. by S. A. David and J. M. Vitek, ASM International, Materials Park, OH, 1993, p. 147.11. Rutter, J. W., and Chalmer, B., Can. J. Physiol., 31: 15, 1953.12. Tiller, W. A., Jackson, K. A., Rutter, J. W., and Chalmer, B., Acta Met., 1: 428, 1953.13. Mullins, W. W., and Sekerka, R. F., J. Appl. Physiol., 34: 323, 1963; 35: 444, 1964.14. Sekerka, R. F., J. Appl. Physiol., 36: 264, 1965.15. Sekerka, R. F., J. Phys. Chem. Solids, 28: 983, 1967.16. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.17. Jackson, K. A., and Hunt, J. S., Acta Met., 13: 1212, 1965.18. Walton, D., Tiller, W. A., Rutter, J. W., and Winegard, W. C., Trans. AIME, 203: 1023, 1955.19. Cole, G. S., and Winegard, W. C., J. Inst. Metals, 92: 323, 1963.20. Hunt, M. D., Spittle, J. A., and Smith, R. W., The Solidiﬁcation of Metals, Publica- tion No. 110, Iron and Steel Institute, London, 1968, p. 57.21. Plaskett, T. S., and Winegard, W. C., Can. J. Physiol., 37: 1555, 1959.22. Bardsley, W., Callan, J. M., Chedzey, H. A., and Hurle, D. T. J., Solid-State Electron, 3: 142, 1961.23. Coulthard, J. O, and Elliott, R., The Solidiﬁcation of Metals, Publication No. 110, Iron and Steel Institute, 1968, p. 61.24. Liu, L. X., and Kirkaldy, J. S., J. Crystal Growth, 144: 335, 1994.25. Munitz, A., Metall. Trans., 16B: 149, 1985.26. Paul, A. J., and DebRoy, T., Rev. Modern Phys., 67: 85, 1995.27. Kou, S., and Le, Y., Metall. Trans., 13A: 1141, 1982.28. Plaskett, T. S., and Winegard, W. C., Can. J. Physiol., 38: 1077, 1960.FURTHER READING1. Chalmers, B., Principles of Solidiﬁcation, Wiley, New York, 1964.2. Davies, G. J., Solidiﬁcation and Casting, Wiley, New York, 1973.3. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20: 83, 1975.4. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.5. Savage, W. F., Weld. World, 18: 89, 1980.
PROBLEMS 169PROBLEMS6.1 From the Al–Mg phase diagram, the equilibrium freezing range of 5052 aluminum (essentially Al–2.5Mg) is about 40°C. Suppose the welding speed is 4 mm/s and the diffusion coefﬁcient DL is 3 ¥ 10-5 cm2/s. Calcu- late the minimum temperature gradient required for planar solidiﬁcation at the weld centerline. What is the corresponding cooling rate? Can this level of cooling rate be achieved in arc welding.6.2 Let CE and CSM be respectively 35% and 15% Mg, and both the solidus and liquidus lines are essentially straight in the Al–Mg system. The melting point of pure Al is 660°C, and the eutectic temperature is 451°C. What is the approximate volume fraction of the aluminum-rich dendrites in the fusion zone of autogenous 5052 aluminum weld?6.3 It has been observed that aluminum alloys welded with the electron beam welding process show much ﬁner secondary dendrite arm spacing in the weld metal than those welded with GMAW. Explain why.6.4 Which alloy has a greater tendency for planar solidiﬁcation to break down, Al-0.01Cu or Al-6.3Cu and why?6.5 How would preheating of the workpiece affect the secondary dendrite arm spacing in welds of aluminum alloys and why?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-47 Weld Metal Solidiﬁcation I:Grain StructureIn this chapter we shall discuss the development of the grain structure in thefusion zone and the effect of welding parameters on the grain structure. Then,we shall discuss various mechanisms of and techniques for grain reﬁning. Thegrain structure of the fusion zone can signiﬁcantly affect its susceptibility tosolidiﬁcation cracking during welding and its mechanical properties afterwelding.7.1 EPITAXIAL GROWTH AT FUSION BOUNDARY7.1.1 Nucleation TheoryFigure 7.1 shows the nucleation of a crystal from a liquid on a ﬂat substratewith which the liquid is in contact (1, 2). The parameters gLC, gLS, and gCS arethe surface energies of the liquid–crystal interface, liquid–substrate interface,and crystal–substrate interface, respectively. According to Turnbull (2), theenergy barrier DG for the crystal to nucleate on the substrate is 3 2 4pg LCTm DG = 2 (2 - 3 cosq + cos3 q ) (7.1) 3(DH m DT )where Tm is the equilibrium melting temperature, DHm the latent heat ofmelting, DT the undercooling below Tm, and q the contact angle. If the liquidwets the substrate completely, the contact angle q is zero and so is DG. Thismeans that the crystal can nucleate on the substrate without having to over-come any energy barrier required for nucleation. The energy barrier can besigniﬁcant if no substrate is available or if the liquid does not wet the substratecompletely. In fusion welding the existing base-metal grains at the fusion line act as thesubstrate for nucleation. Since the liquid metal of the weld pool is in intimatecontact with these substrate grains and wets them completely (q = 0), crystalsnucleate from the liquid metal upon the substrate grains without difﬁculties.When welding without a ﬁller metal (autogenous welding), nucleation occursby arranging atoms from the liquid metal upon the substrate grains without170
EPITAXIAL GROWTH AT FUSION BOUNDARY 171 Liquid (L) γ LC Crystal (C) θ γ LS γ CS Substrate (S) (r) s diu RaFigure 7.1 Spherical cap of a crystal nucleated on a planar substrate from a liquid. Fusion Line Grain (crystal) Welding Direction Base Metal Weld Pool (substrate) (liquid) <100> Epitaxial Growth Figure 7.2 Epitaxial growth of weld metal near fusion line.altering their existing crystallographic orientations. Such a growth initiationprocess, shown schematically in Figure 7.2, is called epitaxial growth or epi-taxial nucleation. The arrow in each grain indicates its <100> direction. Formaterials with a face-centered-cubic (fcc) or body-centered-cubic (bcc) crystalstructure, the trunks of columnar dendrites (or cells) grow in the <100> direc-tion. As shown, each grain grows without changing its <100> direction.
172 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREFigure 7.3 Epitaxial growth during the “welding” of camphene in the area indicatedby the square (magniﬁcation 75¥). Modiﬁed from Savage (6).7.1.2 Epitaxial Growth in WeldingSavage et al. (3–8) ﬁrst discovered epitaxial growth in fusion welding. By usingthe Laue x-ray back-reﬂection technique, they conﬁrmed the continuity ofcrystallographic orientation across the fusion boundary. Savage and Hrubec(6) also studied epitaxial growth by using a transparent organic material(camphene) as the workpiece, as shown in Figure 7.3. Three grains are visiblein the base metal at the fusion line. All dendrites growing from each grainpoint in one direction, and this direction varies from one grain to another.From the welds shown in Figure 7.4 epitaxial growth at the fusion line isevident (9). Epitaxial growth can also occur when the workpiece is a material of morethan one phase. Elmer et al. (10) observed epitaxial growth in electron beamwelding of an austenitic stainless steel consisting of both austenite and ferrite.As shown in Figure 7.5, both austenite (A) and ferrite (F) grow epitaxially atthe fusion line (dotted line) from the base metal to the weld metal (resolidi-ﬁed zone).7.2 NONEPITAXIAL GROWTH AT FUSION BOUNDARYWhen welding with a ﬁller metal (or joining two different materials), the weldmetal composition is different from the base metal composition, and the weldmetal crystal structure can differ from the base metal crystal structure. When
NONEPITAXIAL GROWTH AT FUSION BOUNDARY 173 FL GB 1 GB 2 weld metal GB 1 base (b) metal 100 µm GB 2 FLFigure 7.4 Epitaxial growth. (a) Near the fusion boundary of electron beam weld ofC103 alloy (magniﬁcation 400¥). Reprinted from O’Brien (9). Courtesy of AmericanWelding Society. (b) Near the fusion boundary of as-cast Al–4.5Cu welded with 4043ﬁller (Al–5Si).this occurs, epitaxial growth is no longer possible and new grains will have tonucleate at the fusion boundary. Nelson et al. (11) welded a type 409 ferritic stainless steel of the bcc struc-ture with a Monel (70Ni–30Cu) ﬁller metal of the fcc structure and produceda fcc weld metal. Figure 7.6 shows the fusion boundary microstructure. Theyproposed that, when the base metal and the weld metal exhibit two differentcrystal structures at the solidiﬁcation temperature, nucleation of solid weldmetal occurs on heterogeneous sites on the partially melted base metal at thefusion boundary. The fusion boundary exhibits random misorientationsbetween base metal grains and weld metal grains as a result of heterogeneousnucleation at the pool boundary. The weld metal grains may or may not follow
174 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE resolidified zone FA 20 µmFigure 7.5 Epitaxial growth of austenite (A) and ferrite (F) from the fusion line ofan austenitic stainless steel containing both phases. From Elmer et al. (10).special orientation relationships with the base metal grains they are in contactwith, namely, orient themselves so that certain atomic planes are parallel tospeciﬁc planes and directions in the base-metal grains.7.3 COMPETITIVE GROWTH IN BULK FUSION ZONEAs described in the previous section, the grain structure near the fusion line ofa weld is dominated either by epitaxial growth when the base metal and the weldmetal have the same crystal structure or by nucleation of new grains when theyhave different crystal structures. Away from the fusion line, however, the grainstructure is dominated by a different mechanism known as competitive growth. During weld metal solidiﬁcation grains tend to grow in the direction per-pendicular to pool boundary because this is the direction of the maximum tem-perature gradient and hence maximum heat extraction. However, columnardendrites or cells within each grain tend to grow in the easy-growth direction.Table 7.1 shows the easy-growth directions in several materials (12) and, asshown, it is <100> for both fcc and bcc materials. Therefore, during solidiﬁca-tion grains with their easy-growth direction essentially perpendicular to thepool boundary will grow more easily and crowd out those less favorablyoriented grains, as shown schematically in Figure 7.7. This mechanism ofcompetitive growth dominates the grain structure of the bulk weld metal.7.4 EFFECT OF WELDING PARAMETERS ONGRAIN STRUCTUREThe weld pool becomes teardrop shaped at high welding speeds and ellipticalat low welding speeds (Chapter 2). Since the trailing pool boundary of a
Figure 7.6 Fusion boundary microstructure in 409 ferritic stainless steel (bcc) weldedwith Monel ﬁller wire (fcc): (a) optical micrograph; (b) scanning electron micrograph.White arrows: fusion boundary; dark arrows: new grains nucleated along fusion bound-ary. Reprinted from Nelson et al. (11). Courtesy of American Welding Society.TABLE 7.1 Easy-Growth DirectionsCrystal Structure Easy-Growth Direction ExamplesFace-centered-cubic (fcc) <100> Aluminum alloys, austenitic stainless steelsBody-centered-cubic (bcc) <100> Carbon steels, ferritic stainless steelsHexagonal-close-packed (hcp) ¯ <1010> Titanium, magnesiumBody-centered-tetragonal (bct) <110> TinSource: From Chalmers (12).
176 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE Fusion Line Welding Direction Base Weld Metal Pool <100> Competitive Growth Epitaxial Growth Figure 7.7 Competitive growth in bulk fusion zone.Figure 7.8 Effect of welding speed on columnar-grain structure in weld metal: (a, b)regular structure; (c, d) with axial grains.teardrop-shaped weld pool is essentially straight, the columnar grains are alsoessentially straight in order to grow perpendicular to the pool boundary, asshown schematically in Figure 7.8a. On the other hand, since the trailingboundary of an elliptical weld pool is curved, the columnar grains are also
EFFECT OF WELDING PARAMETERS ON GRAIN STRUCTURE 177Figure 7.9 Gas–tungsten arc welds of 99.96% aluminum: (a) 1000 mm/min weldingspeed; (b) 250 mm/min welding speed. From Arata et al. (13).curved in order to grow perpendicular to the pool boundary, as shown inFigure 7.8b. Figure 7.9 shows the gas–tungsten arc welds of high-purity(99.96%) aluminum made by Arata et al. (13). At the welding speed of1000 mm/min straight columnar grains point toward the centerline, while at250 mm/min curved columnar grains point in the welding direction. Axial grains can also exist in the fusion zone. Axial grains can initiate fromthe fusion boundary at the starting point of the weld and continue along thelength of the weld, blocking the columnar grains growing inward from thefusion lines. Like other columnar grains, these axial grains also tend to growperpendicular to the weld pool boundary. With a teardrop-shaped pool, onlya short section of the trailing pool boundary can be perpendicular to the axialdirection, and the region of axial grains is thus rather narrow, as shown inFigure 7.8c. With an elliptical weld pool, however, a signiﬁcantly longer sectionof the trailing pool boundary can be perpendicular to the axial direction, andthe region of axial grains can thus be signiﬁcantly wider, as shown in Figure7.8d. Figure 7.10 shows aluminum welds with these two types of grain
178 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREFigure 7.10 Axial grains in GTAW: (a) 1100 aluminum at 12.7 mm/s welding speed;(b) 2014 aluminum at 3.6 mm/s welding speed.structure. Axial grains have been reported in aluminum alloys (14–16),austenitic stainless steels (17), and iridium alloys (18).7.5 WELD METAL NUCLEATION MECHANISMSThe mechanisms of nucleation of grains in the weld metal will be discussedin the present section. In order to help understand these mechanisms,the microstructure of the material around the weld pool will be discussedﬁrst. Figure 7.11 shows a 2219 aluminum (essentially Al–6.3% Cu) weldpool quenched with ice water during GTAW (19). The S + L region aroundthe weld pool consists of two parts (Figure 7.11a): the partially melted material
WELD METAL NUCLEATION MECHANISMS 179Figure 7.11 Weld pool of 2219 aluminum quenched during GTAW: (a) overall view;(b) microstructure at position 1; (c) microstructure at position 2. Modiﬁed from Kouand Le (19). Courtesy of American Welding Society.(clear) associated with the leading portion of the pool boundary and themushy zone (shaded) associated with the trailing portion. Area 1 (Figure7.11b) covers a small portion of the partially melted material. Area 2 (Figure7.11c) covers a small portion of the mushy zone as well as the partially meltedmaterial. Based on Figure 7.11, the microstructure around the weld pool boundaryof an alloy is shown schematically in Figure 7.12, along with thermal cycles atthe weld centerline and at the fusion line and a phase diagram. The eutectic-type phase diagram is common among aluminum alloys. As shown, the mushy
180 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE T Temperature, T centerline fusion line TL L (b) S S+L TE A Co time, t Concentration, C (a) distance, x welding fusion line zone (S) direction fusion (c) pool (L) centerline partially melted TL fusion line material (S+L) partially melted zone base metal (S) TE mushy zone (S+L)Figure 7.12 Microstructure around the weld pool boundary: (a) phase diagram; (b)thermal cycles; (c) microstructure of solid plus liquid around weld pool.zone behind the trailing portion of the pool boundary consists of solid den-drites (S) and the interdendritic liquid (L). The partially melted materialaround the leading portion of the pool boundary, on the other hand, consistsof solid grains (S) that are partially melted and the intergranular liquid (L).In summary, there is a region of solid–liquid mixture surrounding the weldpool of an alloy. Figure 7.13a shows three possible mechanisms for new grains to nucleateduring welding: dendrite fragmentation, grain detachment, and heterogeneousnucleation (19). Figure 7.13b shows the fourth nucleation mechanism, surfacenucleation. These mechanisms, which have been well documented in metalcasting, will be described brieﬂy below. The techniques for producing newgrains in the weld metal by these mechanisms will be discussed in a subse-quent section.7.5.1 Dendrite FragmentationWeld pool convection (Chapter 4) can in principle cause fragmentation of den-drite tips in the mushy zone, as illustrated in Figure 7.13a. These dendrite frag-ments are carried into the bulk weld pool and act as nuclei for new grains toform if they survive the weld pool temperature. It is interesting to note thatthis mechanism has been referred to frequently as the grain reﬁning mecha-nism for weld metals without proof.
WELD METAL NUCLEATION MECHANISMS 181Figure 7.13 Nucleation mechanisms during welding: (a) top view; (b) side view.Reprinted from Kou and Le (19). Courtesy of American Welding Society.7.5.2 Grain DetachmentWeld pool convection can also cause partially melted grains to detach them-selves from the solid–liquid mixture surrounding the weld pool, as shown inFigure 7.13a. Like dendrite fragments, these partially melted grains, if theysurvive in the weld pool, can act as nuclei for the formation of new grains inthe weld metal.7.5.3 Heterogeneous NucleationForeign particles present in the weld pool upon which atoms in the liquidmetal can be arranged in a crystalline form can act as heterogeneous nuclei.Figure 7.14 depicts heterogeneous nucleation and the growth of new grains inthe weld metal. Figure 7.15a shows two (dark) heterogeneous nuclei at thecenters of two equiaxed grains in an autogenous gas–tungsten arc weld of a6061 aluminum containing 0.043% titanium (20). Energy dispersive spec-trometry (EDS) analysis, shown in Figure 7.15b, indicates that these nuclei arerich in titanium (boron is too light to be detected by EDS). A scanning elec-tron microscopy (SEM) image of a nucleus is shown in Figure 7.15c. The
182 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE Equiaxed dendrite Nucleus TE Welding Direction Pool TLFigure 7.14 Heterogeneous nucleation and formation of equiaxed grains in weldmetal.Figure 7.15 Heterogeneous nuclei in GTAW of 6061 aluminum: (a) optical micro-graph; (b) EDS analysis; (c) SEM image; (d) SEM image of TiB2 particles in a grainreﬁner for aluminum casting. (a, b) From Kou and Le (20). (d) Courtesy of Granger(21).
WELD METAL NUCLEATION MECHANISMS 183 (c) Figure 7.15 Continuedmorphology of the nucleus is similar to that of the agglomerated TiB2 parti-cles, shown in Figure 7.15d, in an Al–5% Ti–0.2% B grain reﬁner for ingotcasting of aluminum alloys (21). This suggests that the TiB2 particles in theweld metal are likely to be from the Al–Ti–B grain reﬁner in aluminum ingotcasting. Figure 7.16 shows a heterogeneous nucleus of TiN at the center of anequiaxed grain in a GTA weld of a ferritic stainless steel (22). As mentioned previously, Nelson et al. (11) have observed nucleation ofsolid weld metal on heterogeneous sites on the partially melted base metal atthe fusion boundary when the weld metal and the base metal differ in crystalstructure. Gutierrez and Lippold (23) have also studied the formation of thenondendritic equiaxed zone in a narrow region of the weld metal adjacent tothe fusion boundary of 2195 aluminum (essentially Al–4Cu–1Li). Figure 7.17shows an example of the equiaxed zone in a 2195 weld made with a 2319(essentially Al–6.3Cu) ﬁller metal. The width of the equiaxed zone was foundto increase with increasing Zr and Li contents in the alloy. They proposed thatnear the pool boundary the cooler liquid is not mixed with the warmer bulkweld pool. Consequently, near the pool boundary heterogeneous nuclei suchas Al3Zr and Al3(LixZr1-x), which are originally present as dispersoids in the
184 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREFigure 7.16 TiN particle as heterogeneous nucleus in GTAW of ferritic stainless steel.Reprinted from Villafuerte and Kerr (22).Figure 7.17 Nondendritic equiaxed zone in narrow region adjacent to fusion bound-ary of 2195 Al–Cu–Li alloy. Reprinted from Gutierrez and Lippold (23). Courtesy ofAmerican Welding Society.base metal, are able to survive and form the nondendritic equiaxed zone, asillustrated in Figure 7.18. By using a Gleeble thermal simulator, Kostrivas andLippold (24) found that the equiaxed zone could be formed by heating in thetemperature range of approximately 630–640°C and at temperatures above640°C the normal epitaxial growth occurred. This is consistent with the pro-posed mechanism in the sense that the heterogeneous nuclei can only survivenear the cooler pool boundary and not in the warmer bulk weld pool. In the metal casting process the metal is superheated during melting beforeit is cast. Since the nuclei are unstable at higher temperatures, they dissolve inthe superheated liquid in the casting process. As such, there is no equiaxed
WELD METAL NUCLEATION MECHANISMS 185 welding direction nuclei unable weak flow near to survive in pool boundary warmer bulk weld pool cooler unmixed liquid containing nuclei base metal containing fusion nuclei boundary zone of nondendritic normal dendritic equiaxed grains formed structure by hetrogeneous nucleationFigure 7.18 Mechanism for formation of nondendritic equiaxed zone in Al–Cu–Liweld according to Gutierrez and Lippold (23).zone in the weld of an as-cast alloy 2195. However, the equiaxed zone occursagain if the as-cast alloy 2195 is solution heat treated ﬁrst and then welded.Gutierrez and Lippold (23) proposed that because of the relatively low solu-bility of Zr in solid aluminum, Al3Zr and Al3(LixZr1-x) particles precipitate outof the solid solution during heat treating.7.5.4 Surface NucleationThe weld pool surface can be undercooled thermally to induce surface nucle-ation by exposure to a stream of cooling gas or by instantaneous reduction orremoval of the heat input. When this occurs, solid nuclei can form at the weldpool surface, as illustrated in Figure 7.13b. These solid nuclei then grow intonew grains as they shower down from the weld pool surface due to their higherdensity than the surrounding liquid metal.7.5.5 Effect of Welding Parameters on Heterogeneous NucleationBefore leaving this section, an important point should be made about theeffect of welding parameters on heterogeneous nucleation. Kato et al. (25),Arata et al. (26), Ganaha et al. (16), and Kou and Le (20) observed in com-mercial aluminum alloys that the formation of equaixed grains is enhanced byhigher heat inputs and welding speeds. As shown in Figure 7.19, equiaxedgrains can form a band along the centerline of the weld and block off colum-nar grains as the heat input and welding speed are increased (20). Kou and Le(27) showed in Figure 7.20 that, as the heat input and the welding speed areincreased, the temperature gradient (G) at the end of the weld pool is reduced.Furthermore, as the welding speed is increased, the solidiﬁcation rate of the
186 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREFigure 7.19 Effect of welding parameters on grain structure in GTAW of 6061aluminum: (a) 70 A ¥ 11 V heat input and 5.1 mm/s welding speed; (b) 120 A ¥ 11 Vheat input and 12.7 mm/s welding speed. From Kou and Le (20). Welding direction Pool Pool 1100 aluminum Temperature, oC Temperature, oC 1000 175 A 1000 60 A 15 V 10 V 20 mm/sec 1.7 mm/sec 500 500 0 50 100 0 50 Distance, mm Distance, mm (a) (b)Figure 7.20 Effect of welding parameters on temperature gradient at weld pool endof 1100 aluminum: (a) higher welding speed and heat input; (b) lower welding speedand heat input. From Kou and Le (27).weld metal (R) is also increased. As illustrated in Figure 7.21, the ratio G/Rshould be decreased and the constitutional supercooling (28) in front of theadvancing solid–liquid interface should, therefore, be increased. Kato et al.(25) and Arata et al. (26) proposed that the transition to an equiaxed grain
GRAIN STRUCTURE CONTROL 187Figure 7.21 Effect of welding parameters on heterogeneous nucleation: (a) lowconstitutional supercooling at low welding speed and heat input; (b) heterogeneousnucleation aided by high constitutional supercooling at high welding speed and heatinput.structure is due to the existence of a sufﬁciently long constitutionally under-cooled zone in the weld pool. Ganaha et al. (16), however, indicated that thetransition is not due to constitutional supercooling alone. In fact, it wasobserved that signiﬁcant amounts of equiaxed grains formed only in thosealloys containing around or more than 0.01 wt % Ti or 0.10 wt % Zr. Further-more, tiny second-phase particles rich in titanium and/or zirconium (possiblyTixZryC compounds) existed at the dendrite centers of the equiaxed grains.Consequently, it was proposed that equiaxed grains in the fusion zone formby heterogeneous nucleation aided by constitutional supercooling. The obser-vation of Ganaha et al. (16) was conﬁrmed by Kou and Le (19, 20, 29). Theeffect of welding parameters on grain reﬁning in aluminum welds was dis-cussed by Kou and Le (20).7.6 GRAIN STRUCTURE CONTROLThe weld metal grain structure can affect its mechanical properties signiﬁ-cantly. Arata et al. (13) tensile tested aluminum welds in the welding direc-tion. The weld metal ductility of 99.96% aluminum dropped greatly when thecolumnar grains pointed to the weld centerline (Figure 7.9a), that is, when thegrains became nearly normal to the tensile axis. Also, the weld metal tensilestrength of 5052 aluminum increased as the amount of equiaxed grainsincreased.
188 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE The formation of ﬁne equiaxed grains in the fusion zone has two mainadvantages. First, ﬁne grains help reduce the susceptibility of the weld metalto solidiﬁcation cracking during welding (Chapter 11). Second, ﬁne grains canimprove the mechanical properties of the weld, such as the ductility and frac-ture toughness in the case of steels and stainless steels. Therefore, much efforthas been made to try to grain reﬁne the weld fusion zone. This includes theapplication of grain reﬁning techniques that were originally developed forcasting. Described below are several techniques that have been used to controlthe weld metal grain structure.7.6.1 InoculationThis technique has been used extensively in metal casting. It involves the addi-tion of nucleating agents or inoculants to the liquid metal to be solidiﬁed. Asa result of inoculation, heterogeneous nucleation is promoted and the liquidmetal solidiﬁes with very ﬁne equiaxed grains. In the work by Davies andGarland (1), inoculant powders of titanium carbide and ferrotitanium–titanium carbide mixtures were fed into the weld pool during the submergedarc welding of a mild steel and very ﬁne grains were obtained. Similarly,Heintze and McPherson (30) grain reﬁned submerged arc welds of C-Mn andstainless steels with titanium. Figure 7.22 shows the effect of inoculation onthe grain structure of the weld fusion zone of the C-Mn steel. It is interestingto note that Petersen (31) has grain reﬁned Cr–Ni iron base alloys with alu-minum nitride and reported a signiﬁcant increase in the ductility of the resul-tant welds, as shown in Figure 7.23. Pearce and Kerr (32), Matsuda et al. (33), Yunjia et al. (34), andSundaresan et al. (35) grain reﬁned aluminum welds by using Ti and Zr asinoculants. Yunjia et al. (34) showed the presence of TiAl3 particles at theorigins of equiaxed grains in Ti microalloyed 1100 aluminum welds. Figure 7.24shows grain reﬁning in a 2090 Al–Li–Cu alloy gas–tungsten arc welded with a2319 Al–Cu ﬁller inoculated with 0.38% Ti (35).7.6.2 External ExcitationDifferent dynamic grain reﬁning techniques, such as liquid pool stirring, moldoscillation, and ultrasonic vibration of the liquid metal, have been employedin metal casting, and recently similar techniques, including weld pool stirring,arc oscillation, and arc pulsation, have been applied to fusion welding.A. Weld Pool Stirring Weld pool stirring can be achieved by electromag-netic stirring, as shown in Figure 7.25, by applying an alternating magnetic ﬁeldparallel to the welding electrode (36). Matsuda et al. (37, 38) and Pearce andKerr (32) increased the degree of grain reﬁnement in aluminum alloys con-taining small amounts of titanium by electromagnetic pool stirring. Pearce andKerr (32) suggested that the increased grain reﬁnement was due to heteroge-
GRAIN STRUCTURE CONTROL 189Figure 7.22 Effect of inoculation on grain structure in submerged arc welds of C–Mnsteel (magniﬁcation 6¥): (a) without inoculation; (b) inoculation with titanium.Reprinted from Heintze and McPherson (30). Courtesy of American Welding Society. 400 Elongation, % 300 200 100 0 0 0.04 0.08 0.12 0.16 Grain size, mmFigure 7.23 Effect of grain size on weld metal ductility of a Cr–Ni iron base alloy at925°C. Modiﬁed from Petersen (31).neous nucleation, rather than to dendrite fragmentation. This is because inGTAW, unlike ingot casting, the liquid pool and the mushy zone are rathersmall, and it is therefore difﬁcult for the liquid metal in the pool to penetrateand break away dendrites, which are so short and so densely packed together.
190 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREFigure 7.24 Effect of inoculation on grain structure in GTAW of 2090 Al–Li–Cu alloy:(a) 2319 Al–Cu ﬁller metal; (b) 2319 Al–Cu ﬁller metal inoculated with 0.38% Ti.Reprinted from Sundaresan et al. (35). tungsten electrode magnetic field welding direction workpiece weld pool current field coilFigure 7.25 Schematic sketch showing application of external magnetic ﬁeld duringautogenous GTAW. Modiﬁed from Matsuda et al. (36).Stirring of the weld pool tends to lower the weld pool temperature, thushelping heterogeneous nuclei survive. Figure 7.26 shows the increased grainreﬁnement by weld pool stirring in an Al–2.5 wt % Mg alloy containing0.11 wt % Ti (32). As shown in Figure 7.27, Villafuerte and Kerr (39) grainreﬁned a weld of 409 ferritic stainless steel containing 0.32% Ti by the sametechnique. The higher the Ti content, the more effective grain reﬁning was.Titanium-rich particles were found at the origin of equiaxed grains, suggest-ing heterogeneous nucleation as the grain reﬁning mechanism. Pearce and Kerr (32) also found that by applying weld pool stirring, thepartially melted grains along the leading portion of the pool boundary, if theyare only loosely held together, could be swept by the liquid metal into the weld
GRAIN STRUCTURE CONTROL 191Figure 7.26 Widening of equiaxed zone in GTAW of alloy Al–2.5Mg–0.011Ti bymagnetic stirring (at dotted line). Reprinted from Pearce and Kerr (32).Figure 7.27 Effect of electromagnetic pool stirring on grain structure in GTAW of409 ferritic stainless steel: (a) without stirring; (b) with stirring. Reprinted from Villa-fuerte and Kerr (39). Courtesy of American Welding Society.
192 WELD METAL SOLIDIFICATION I: GRAIN STRUCTUREpool, where they served as nuclei. Signiﬁcant amounts of equiaxed grains wereso produced in gas–tungsten arc welds of a 7004 aluminum alloy containingvery little Ti.B. Arc Oscillation Arc oscillation, on the other hand, can be produced bymagnetically oscillating the arc column using a single- or multipole magneticprobe or by mechanically vibrating the welding torch. Davies and Garland (1)produced grain reﬁning in gas–tungsten arc welds of Al–2.5 wt % Mg alloy bytorch vibration. Resistance to weld solidiﬁcation cracking was improved inthese welds. Figure 7.28 shows the effect of the vibration amplitude on thegrain size (1). Dendrite fragmentation was proposed as the grain reﬁningmechanism. It is, however, suspected that heterogeneous nucleation couldhave been the real mechanism, judging from the fact that the Al–2.5 wt % Mgused actually contained about 0.15 wt %Ti. Venkataraman et al. (40, 41)obtained grain reﬁning in the electroslag welds of steels by electrode vibra-tion and enhanced electromagnetic stirring of the weld pool and improvedtheir toughness and resistance to centerline cracking. Dendrite fragmentationwas also considered as the mechanism for grain reﬁning. Sharir et al. (42) obtained grain reﬁnement in gas–tungsten arc welds ofpure tantalum sheets by arc oscillation. Due to the high melting point of puretantalum (about 3000°C), the surface heat loss due to radiation was rather sig-niﬁcant. As a result, the liquid metal was cooled down rapidly and was in factundercooled below its melting point when the heat source was deﬂected awayduring oscillated arc welding. This caused surface nucleation and resulted ingrain reﬁnement. 0.5 150A, 200 mm/min Arc gap 2.4 mm 0.4 Arc vibration frequency 10 Hz Parallel to welding direction Perpendicular to welding Grain size, mm 0.3 direction 0.2 0.1 0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 Arc vibration amplitude, mmFigure 7.28 Effect of arc vibration amplitude on grain size in Al–2.5Mg welds. Mod-iﬁed from Davies and Garland (1).
GRAIN STRUCTURE CONTROL 193 Sundaresan and Janaki Ram (43) grain reﬁned Ti alloys by magnetic arcoscillation and improved the weld metal tensile ductility. No speciﬁc grainreﬁning mechanism was identiﬁed.C. Arc Pulsation Arc pulsation can be obtained by pulsating the weldingcurrent. Sharir et al. (42) also obtained grain reﬁnement in gas–tungsten arcwelds of pure tantalum sheets by arc pulsation. The liquid metal was under-cooled when the heat input was suddenly reduced during the low-current cycleof pulsed arc welding. This caused surface nucleation and resulted in grainreﬁnement. Figure 7.29 shows grain reﬁning in a pulsed arc weld of a 6061 aluminumalloy containing 0.04 wt % Ti (44). Heterogeneous nucleation, aided by thermalundercooling resulting from the high cooling rate produced by the relativelyhigh welding speed used and arc pulsation, could have been responsible forthe grain reﬁnement in the weld.7.6.3 Stimulated Surface NucleationStimulated surface nucleation was originally used by Southin (45) to obtaingrain reﬁnement in ingot casting. A stream of cool argon gas was directed onthe free surface of molten metal to cause thermal undercooling and inducesurface nucleation. Small solidiﬁcation nuclei formed at the free surface andshowered down into the bulk liquid metal. These nuclei then grew and becamesmall equiaxed grains. This technique was used to produce grain reﬁning inAl–2.5Mg welds by Davies and Garland (1) and in Ti alloys by Wells (46).Figure 7.29 Equiaxed grains in pulsed arc weld of 6061 aluminum (magniﬁcation 9¥).From Kou and Le (44).
194 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE7.6.4 Manipulation of Columnar GrainsKou and Le (14, 15, 47) manipulated the orientation of columnar grains inaluminum welds by low-frequency arc oscillation. Figure 7.30a shows a 2014aluminum weld made with 1 Hz transverse arc oscillation, that is, with arcoscillating normal to the welding direction (14). Similarly, Figure 7.30b showsa 5052 aluminum weld made with 1 Hz circular arc oscillation (15). In bothFigure 7.30 Grain structures in oscillated arc welds of aluminum alloys. (a) For alloy2014 with transverse arc oscillation. From Kou and Le (14). (b) For alloy 5052 withcircular arc oscillation. From Kou and Le (15).
REFERENCES 195Figure 7.31 Effect of gravity on grain structure in GTAW of 2090 Al–Li–Cu alloy: (a)1 g; (b) 10 g and with equiaxed zone (EQZ) near the fusion boundary eliminated.Reprinted from Aidun and Dean (48). Courtesy of American Welding Society.cases, columnar grains grew perpendicular to the trailing portion of the weldpool, and the weld pool in turn followed the path of the moving oscillatingarc. As will be discussed later in Chapter 11, periodic changes in grain orienta-tion, especially that produced by transverse arc oscillation at low frequencies,can reduce solidiﬁcation cracking and improve both the strength and ductil-ity of the weld metal (47).7.6.5 GravityAidun and Dean (48) gas–tungsten arc welded 2195 aluminum under the highgravity produced by a centrifuge welding system and eliminated the narrowband of nondendritic equiaxed grains along the fusion boundary. As shown inFigure 7.31, the band disappeared when gravity was increased from 1 g to10 g. It was suggested that buoyancy convection enhanced by high gravitycaused Al3Zr and Al3(LixZr1-x) nuclei near the pool boundary to be swept intothe bulk pool and completely dissolved, thus eliminating formation ofequiaxed grains by heterogeneous nucleation.REFERENCES 1. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20(196): 83, 1975. 2. Turnbull, D., J. Chem. Physiol., 18: 198, 1950. 3. Savage, W. F., Lundin, C. D., and Aronson, A. H., Weld. J., 44: 175s, 1965. 4. Savage, W. F., and Aronson, A. H., Weld. J., 45: 85s, 1966. 5. Savage, W. F., Lundin, C. D., and Chase, T. F., Weld. J., 47: 522s, 1968. 6. Savage, W. F., and Hrubec, R. J., Weld. J., 51: 260s, 1972.
196 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE 7. Savage, W. F., Weld. World, 18: 89, 1980. 8. Savage, W. F., in Weld Imperfections, Eds. A. R. Hunger and R. E. Lewis, Addison- Wesley, Reading, MA, 1968, p. 13. 9. 18th ed., O’brien R. L., Ed., Jefferson’s Welding Encyclopedia, American Welding Society, Miami, FL, 1997, p. 316.10. Elmer, J. W., Allen, S. M., and Eagar, T. W., Metall. Trans. A, 20A: 2117, 1989.11. Nelson, T. W., Lippold, J. C., and Mills, M. J., Weld. J., 78: 329s, 1999.12. Chalmers, B., Principles of Solidiﬁcation, Wiley, New York, 1964, p. 117.13. Arata, Y., Matsuda, F., Mukae, S., and Katoh, M., Trans. JWRI, 2: 55, 1973.14. Kou, S., and Le, Y., Metall. Trans., 16A: 1887, 1985.15. Kou, S., and Le, Y., Metall. Trans., 16A: 1345, 1985.16. Ganaha, T., Pearce, B. P., and Kerr, H. W., Metall. Trans., 11A: 1351, 1980.17. Kou, S., and Le, Y., Metall. Trans., 13A: 1141, 1982.18. David, S. A., and Liu, C. T., Metals Technol., 7: 102, 1980.19. Kou, S., and Le, Y., Weld. J., 65: 305s, 1986.20. Kou, S., and Le, Y., Metall. Trans., 19A: 1075, 1988.21. Granger, D. A., Practical Aspects of Grain Reﬁning Aluminum Alloy Melts, paper presented at International Seminar on Reﬁning and Alloying of Liquid Aluminum and Ferro-Alloys, Trondheim, Norway, August 26–28, 1985.22. Villafuerte, J. C., and Kerr, H. W., in International Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, March 1993, p. 189.23. Gutierrez, A., and Lippold, J. C., Weld. J., 77: 123s, 1998.24. Kostrivas, A., and Lippold, J. C., Weld. J., 79: 1s, 2000.25. Kato, M., Matsuda, F., and Senda, T., Weld. Res. Abroad, 19: 26, 1973.26. Arata, Y., Matsuda, F., and Matsui, A., Trans. Jpn. Weld. Res. Inst., 3: 89, 1974.27. Kou, S., and Le, Y., unpublished research, University of Wisconsin, Madison, 1985.28. Rutter, J. W., and Chalmer, B., Can. J. Physiol., 31: 15, 1953.29. Le, Y., and Kou, S., in Advances in Welding Science and Technology, Ed. S. A. David, ASM International, Metals Park, OH, 1986, p. 139.30. Heintze, G. N., and McPherson, R., Weld. J., 65: 71s, 1986.31. Petersen, W. A., Weld. J., 53: 74s, 1973.32. Pearce, B. P., and Kerr, H. W., Metall. Trans., 12B: 479, 1981.33. Matsuda, F., Nakata, K., Tsukamoto, K., and Arai, K., Trans. JWRI, 12: 93, 1983.34. Yunjia, H., Frost, R. H., Olson, D. L., and Edwards, G. R., Weld. J., 68: 280s, 1983.35. Sundaresan, S., Janaki Ram, G. D., Murugesan, R., and Viswanathan, N., Sci. Technol. Weld. Join., 5: 257, 2000.36. Matsuda, F., Ushio, M., Nakagawa, H., and Nakata, K., in Proceedings of the Conference on Arc Physics and Weld Pool Behavior, Vol. 1, Welding Institute, Cambridge, 1980, p. 337.37. Matsuda, F., Nakagawa, H., Nakata, K., and Ayani, R., Trans. JWRI, 7: 111, 1978.38. Matsuda, F., Nakata, K., Miyawaga, Y., Kayano, T., and Tsukarnoto, K., Trans. JWRI, 7: 181, 1978.39. Villafuerte, J. C., and Kerr, H. W., Weld. J., 69: 1s, 1990.
PROBLEMS 19740. Venkataraman, S., Devietian, J. H., Wood, W. E., and Atteridge, D. G., in Grain Reﬁnement in Castings and Welds, Eds. G. J. Abbaschian and S. A. David, Metallurgical Society of AIME, Warrendale, PA, 1983, p. 275.41. Venkataraman, S., Wood, W. E., Atteridge, D. G., and Devletian, J. H., in Trends in Welding Research in the United States, Ed. S.A. David,American Society for Metals, Metals Park, OH, 1982.42. Sharir, Y., Pelleg, J., and Grill, A., Metals Technol., 5: 190, 1978.43. Sundaresan, S., and Janaki Ram, G. D., Sci. Technol. Weld. Join., 4: 151, 1999.44. Kou, S., and Le, Y., unpublished research, University of Wisconsin, Madison, 1986.45. Southin, R. T., Trans. AIME, 239: 220, 1967.46. Wells, M. E., and Lukens, W. E., Weld. J., 65: 314s, 1986.47. Kou, S., and Le, Y., Weld. J., 64: 51, 1985.48. Aidun, D. K., and Dean, J. P., Weld. J., 78: 349s, 1999.FURTHER READING1. Chalmers, B., Principles of Solidiﬁcation, Wiley, New York, 1964.2. Davies, G. J., Solidiﬁcation and Casting, Wiley, New York, 1973.3. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20(196): 83, 1975.4. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.5. Savage, W. F., Weld. World, 18: 89, 1980.6. Abbaschian, G. J., and David, S. A., Eds., Grain Reﬁnement in Castings and Welds, Metallurgical Society of AIME, Warrendale, PA, 1983.PROBLEMS7.1 In aluminum alloys such as 6061 and 5052, which often contain small amounts of Ti (say about 0.02 wt %), the Ti-rich particles in the workpiece can be dissolved with a gas–tungsten arc by multipass melting. If the preweld is a multipass weld intended to dissolve such particles and the grain structure is shown in Figure P7.1, what is the grain reﬁning mech- anism in the test weld and why?7.2 Equiaxed grains can often be found in the crater of a weld that exhibits an essentially purely columnar grain structure, as shown in Figure P7.2. Explain why. test weld preweld Figure P7.1
198 WELD METAL SOLIDIFICATION I: GRAIN STRUCTURE weld crater Figure P7.2 test weld preweld Figure P7.3 (a) Ni ingot (b) Ni ingot Figure P7.4 welding direction pulsed arc weld Figure P7.57.3 Gutierrez and Lippold (23) made a preweld in aluminum alloy 2195 and then a test weld perpendicular to it, as shown in Figure P7.3. (a) Do you expect to see a nondendritic equiaxed zone near the fusion boundary of the test weld in the overlap region and why or why not? (b) Same as (a) but with the workpiece and the preweld solution heat treated before making the test weld.7.4 Part of a pure Ni ingot with large columnar grains is welded perpendic- ular to the grains, as shown in Figure P7.4. Sketch the grain structure in the weld.7.5 A pulsed arc weld is shown in Figure P7.5. Sketch the grain structure in the area produced by the last pulse.
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-48 Weld Metal Solidiﬁcation II:Microstructure within GrainsIn this chapter we shall discuss the microstructure within the grains in thefusion zone, focusing on the solidiﬁcation mode, dendrite spacing and cellspacing, how they vary across the weld metal, and how they are affected bywelding parameters. The advantages of ﬁne microstructure and techniques formicrostructural reﬁning will also be discussed.8.1 SOLIDIFICATION MODESAs constitutional supercooling increases, the solidiﬁcation mode changes fromplanar to cellular and from cellular to dendritic (Chapter 6). Figure 8.1 showsschematically the effect of constitutional supercooling on the microstructurewithin the grains in the weld metal. The solidiﬁcation mode changes fromplanar to cellular, columnar dendritic, and equiaxed dendritic as the degree ofconstitutional supercooling at the pool boundary increases. Heterogeneousnucleation aided by constitutional supercooling promotes the formation ofequiaxed grains in the weld metal (Chapter 7).8.1.1 Temperature Gradient and Growth RateWhile the solidiﬁcation mode can vary from one weld to another (Figure 8.1),it can also vary within a single weld from the fusion line to the centerline. Thiswill be explained following the discussion on the growth rate R and the tem-perature gradient G. Figure 8.2 shows the relationship between the growth rate R and thewelding speed V. The distance a given point on the pool boundary travels inthe normal direction n during a very small time interval dt is Rn dt = (V dt ) cos a = (R dt ) cos(a - b ) (8.1)Dividing the above equation by dt cos(a - b) yields V cos a R= (8.2) cos(a - b ) 199
200 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINS weld welding pool direction magnified l tua weld fusion metal ac T T line equilibrium S+L S L base S L welding direction x metal x weld pool <100> Planar Cellular 0> (b) (a) <10 T T S+L constitutional supercooling S L S S+L L x x Columnar Equiaxed dendritic dendritic (c) (d)Figure 8.1 Effect of constitutional supercooling on solidiﬁcation mode duringwelding: (a) planar; (b) cellular; (c) columnar dendritic; (d) equiaxed dendritic.Constitutional supercooling increases from (a) through (d). pool boundary pool boundary at time, t+dt at time, t welding speed, V pool n centerline R V dendrite fusion line n R Rn Rd t dt α β V Vdt t+dt dendrite t Figure 8.2 Relationship between growth rate R and welding speed V.
SOLIDIFICATION MODES 201where a is the angle between the welding direction and the normal to the poolboundary and b is the angle between the welding direction and the growthdirection of a dendrite at the point (<100> in fcc and bcc materials). This rela-tionship has been shown by Nakagawa et al. (1). If the difference between thetwo angles is neglected (cos 0° = 1) as an approximation, Equation (8.2)becomes R = V cosa (8.3) As shown in Figure 8.3, a = 0° and 90° at the weld centerline and the fusionline, respectively. Therefore, the solidiﬁcation rate at the centerline RCL = V(maximum) while that at the fusion line RFL = 0 (minimum). As shown inFigure 8.4, the distance between the maximum pool temperature (Tmax) andthe pool boundary (TL) is greater at the centerline than at the fusion line pool boundary pool boundary at time t + dt at time t welding speed, V pool centerline fusion line Rdt ഠ 0 Rdt α Rdt Vdt Vdt Vdt α = 900 α = 00 Rdt = (Vdt) cosα cos900 = 0 cos 00 = 1 RFL ഠ V cos α = 0 R ഠ V cos α RCLഠ V cos α = V at fusion line anywhere at centerline Figure 8.3 Variation in growth rate along pool boundary. weld pool welding Tmax speed, V R CL=V G CL centerline (CL) G FL G TL R FL≈ 0 fusion line (FL)Figure 8.4 Variations in temperature gradient G and growth rate R along poolboundary.
202 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINSbecause the weld pool is elongated. Consequently, the temperature gradientnormal to the pool boundary at the centerline, GCL, is less than that at thefusion line, GFL. Since GCL < GFL and RCL >> RFL, Ê Gˆ Ê Gˆ << (8.4) Ë R ¯ CL Ë R ¯ FL8.1.2 Variations in Growth Mode across WeldAccording to Equation (8.4), the ratio G/R decreases from the fusion linetoward the centerline. This suggests that the solidiﬁcation mode may changefrom planar to cellular, columnar dendritic, and equiaxed dendritic across thefusion zone, as depicted in Figure 8.5. Three grains are shown to grow epitax-ially from the fusion line. Consider the one on the right. It grows with theplanar mode along the easy-growth direction <100> of the base-metal grain.A short distance away from the fusion line, solidiﬁcation changes to thecellular mode. Further away from the fusion line, solidiﬁcation changes tothe columnar dendritic mode. Some of the cells evolve into dendrites andtheir side arms block off the neighboring cells. Near the weld centerlineequiaxed dendrites nucleate and grow, blocking off the columnar dendrites.The solidiﬁcation-mode transitions have been observed in several differentmaterials (2–4). Figure 8.6 shows the planar-to-cellular transition near the weld fusion lineof an autogenous gas–tungsten weld of Fe–49Ni (2). Figure 8.7 shows theplanar-to-cellular transition and the cellular-to-dendritic transition in 1100 alu-minum (essentially pure Al) welded with a 4047 (Al–12Si) ﬁller metal. Figure8.8 shows the transition from columnar to equiaxed dendrites in an electronbeam weld of a Fe–15Cr–15Ni single crystal containing some sulfur (4). Thesecolumnar dendrites, with hardly visible side arms, follow the easy-growth centerline equiaxed welding dendritic direction weld columnar pool dendritic pool boundary cellular planar base fusion <10 0 > 0> <100> <10 metal line Figure 8.5 Variation in solidiﬁcation mode across the fusion zone.
SOLIDIFICATION MODES 203 solidified liquid weld fusion weld metal metal line ͗100͘ weld pool boundary region of cellular growth region of planar growthFigure 8.6 Planar-to-cellular transition in an autogenous weld of Fe–49Ni. Modiﬁedfrom Savage et al. (2).Figure 8.7 Planar-to-cellular and cellular-to-dendritic transitions in 1100 Al weldedwith 4047 ﬁller.direction <100> of the single crystal, which happens to be normal to the fusionline in this case. Before leaving the subject of the solidiﬁcation mode, it is desirable tofurther consider the weld metal microstructure of a workpiece with only oneand very large grain, that is, a single-crystal workpiece. Figure 8.9 shows thecolumnar dendritic structure in a Fe–15Cr–15Ni single crystal of high purityelectron beam welded along a  direction on a (001) surface (5). The weldis still a single crystal because of epitaxial growth. However, it can have
204 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINSFigure 8.8 Electron beam weld of single crystal of Fe–15Cr–15Ni with sulfur showingtransition from columnar to equiaxed dendrites. Reprinted from David and Vitek (4).colonies of columnar dendrites of different orientations, as shown by the topweld pass in Figure 8.9b (f is one of the angles characterizing the normal tothe pool boundary). This is because of competitive growth between columnardendrites along the three <100> easy-growth directions , , and .Dendrites with an easy-growth direction closest to the heat ﬂow direction(normal to the pool boundary) compete better.8.2 DENDRITE AND CELL SPACINGThe spacing between dendrite arms or cells, just as the solidiﬁcation mode, canalso vary across the fusion zone. As already mentioned in the previous section,GCL < GFL and RCL >> RFL. Consequently, (G ¥ R)CL > (G ¥ R) FL (8.5)where G ¥ R is the cooling rate, as explained previously in Chapter 6. Accord-ing to Equation (8.5), the cooling rate (G ¥ R) is higher at the weld centerlineand lower at the fusion line. This suggests that the dendrite arm spacingdecreases from the fusion line to the centerline because the dendrite armspacing decreases with increasing cooling rate (Chapter 6). The variation in the dendrite arm spacing across the fusion zone can befurther explained with the help of thermal cycles (Chapter 2). Figure 8.10
DENDRITE AND CELL SPACING 205Figure 8.9 Electron beam weld of single crystal of pure Fe–15Cr–15Ni made in a direction on a (001) surface: (a) top cross section; (b) transverse cross section.Reprinted from Rappaz et al. (5).shows a eutectic-type phase diagram and the thermal cycles at the weld cen-terline and fusion line of alloy C0. As shown, the cooling time through the ¯solidiﬁcation temperature range is shorter at the weld centerline (24 /V) and ¯longer at the fusion line (13 /V). As such, the cooling rate through the solidiﬁ-cation temperature range increases and the dendrite arm spacing decreasesfrom the fusion line to the centerline. As shown by the aluminum weld in
206 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINS T shorter solidification time, b, at centerline Temperature, T L 1 longer solidification TL 2 time, a, at fusion line S 3 4 TE (b) S+L a b A Co time Concentration, C distance (a) 3 1 welding direction centerline (finer weld 2 microstructure) TL pool 4 fusion line (c) (coarser TE microstructure)Figure 8.10 Variation in dendrite arm spacing across fusion zone: (a) phase diagram;(b) thermal cycles; (c) top view of weld pool.Figure 8.11 Transverse cross-section of gas–tungsten arc weld in 6061 aluminum:(a) ﬁner microstructure near centerline; (b) coarser microstructure near fusion line.Magniﬁcation 115¥. Reprinted from Kou et al. (6). Courtesy of American WeldingSociety.Figure 8.11, the solidiﬁcation microstructure gets ﬁner from the fusion line tothe centerline (6). The same trend was observed in other aluminum welds byKou et al. (6, 7) and Lanzafame and Kattamis (8).8.3 EFFECT OF WELDING PARAMETERS8.3.1 Solidiﬁcation ModeThe heat input and the welding speed can affect the solidiﬁcation mode of theweld metal signiﬁcantly. The solidiﬁcation mode changes from planar to cel-
EFFECT OF WELDING PARAMETERS 207TABLE 8.1 Effect of Welding Parameters on Weld Metal MicrostructureTravel speed 150 A 300 A 450 A0.85 mm/s Cellular Cellular dendritic Coarse cellular(2 ipm) dendritic1.69 mm/s Cellular Fine cellular Coarse cellular(4 ipm) dendritic dendritic3.39 mm/s Fine cellular Cellular, slight Severe undercutting(8 ipm) undercutting6.77 mm/s Very ﬁne cellular Cellular, Severe undercutting(16 ipm) undercuttingSource: From Savage et al. (9).lular and dendritic as the ratio G/R decreases (Chapter 6). Table 8.1 summa-rizes the observations of Savage et al. (9) in HY-80 steel. At the welding speedof 0.85 mm/s (2 ipm), the weld microstructure changes from cellular to den-dritic when the welding current increases from 150 to 450 A. According toEquation (2.15), the higher the heat input (Q) under the same welding speed(V), the lower the temperature gradient G and hence the lower the ratio G/R.Therefore, at higher heat inputs G/R is lower and dendritic solidiﬁcation pre-vails, while at lower heat inputs G/R is higher and cellular solidiﬁcation pre-vails. Although analytical equations such as Equations (2.15) and (2.17) areoversimpliﬁed, they can still qualitatively tell the effect of welding parameters.8.3.2 Dendrite and Cell SpacingThe heat input and the welding speed can also affect the spacing between den-drite arms and cells. The dendrite arm spacing or cell spacing decreases withincreasing cooling rate (Chapter 6). As compared to arc welding, the coolingrate in laser or electron beam welding is higher and the weld metal microstruc-ture is ﬁner. The 6061 aluminum welds in Figure 8.12 conﬁrm that this is thecase (10). As shown in Table 8.1, at the welding current of 150 A, the cells becomeﬁner as the welding speed increases. From Equation (2.17), under the sameheat input (Q), the cooling rate increases with increasing welding speed V.Therefore, at higher welding speeds the cooling rate is higher and the cells areﬁner, while at lower welding speeds the cooling rate is lower and the cells arecoarser. Elmer et al. (11) also observed this trend in EBW of two austeniticstainless steels of similar compositions, as shown in Figure 8.13. The differencein the cell spacing can be seen even though the magniﬁcations of the micro-graphs are different. According to Equation (2.17), the cooling rate increases with decreasingheat input–welding speed ratio Q/V. This ratio also represents the amount
208 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINSFigure 8.12 Autogenous welds of 6061 aluminum: (a) coarser solidiﬁcation structurein gas–tungsten arc weld: (b) ﬁner solidiﬁcation structure in electron beam weld.Reprinted from Metals Handbook (10).Figure 8.13 Effect of welding speed on cell spacing in EBW of austenitic stainlesssteels: (a) 100 mm/s; (b) 25 mm/s. From Elmer et al. (11).
REFINING MICROSTRUCTURE WITHIN GRAINS 209 14 just above toe of weld Dendrite spacing, µ m 12 level with surface of plate 10 8 6 4 (a) 2 0 10 20 30 40 50 60 70 80 Heat input cal/cm length (Heat input/welding speed, J/mm) 1/2 0 30 60 90 Dendrite arm spacing, µ m 20 10 (b) 0 10 20 30 40 (Heat input/welding speed, W/mm) 1/2Figure 8.14 Effect of heat input per unit length of weld on dendrite arm spacing.(a) For Al–Mg–Mn alloy. From Jordan and Coleman (13). (b) For 2014 Al–Cu alloy.Modiﬁed from Lanzafame and Kattamis (14). Courtesy of American Welding Society.of heat per unit length of the weld (J/cm or cal/cm). Therefore, the dendritearm spacing or cell spacing can be expected to increase with increasingQ/V or amount of heat per unit length of the weld. This has been observedin several aluminum alloys (7, 8, 12–14), including those shown in Fig-ure 220.127.116.11 REFINING MICROSTRUCTURE WITHIN GRAINSIt has been shown in aluminum alloys that the ﬁner the dendrite arm spacing,the higher the ductility (15) and yield strength (8, 15) of the weld metal andthe more effective the postweld heat treatment (8, 12, 15), due to the ﬁnerdistribution of interdendritic eutectics.
210 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINS8.4.1 Arc OscillationKou and Le (16) studied the microstructure in oscillated arc welds of 2014 alu-minum alloy. It was observed that the dendrite arm spacing was reduced sig-niﬁcantly by transverse arc oscillation at low frequencies, as shown in Figure8.15. This reduction in the dendrite arm spacing has contributed to the signif-icant improvement in both the strength and ductility of the weld, as shown inFigure 8.16. As illustrated in Figure 8.17, when arc oscillation is applied, the weld poolgains a lateral velocity, v, in addition to its original velocity u in the weldingdirection (16). The magnitude of v can be comparable with that of u depend-ing on the amplitude and frequency of arc oscillation. As shown, the resultant velocity of the weld pool, w, is greater than that ofthe unoscillated weld pool, u. Furthermore, the temperature gradient aheadof the solid–liquid interface, G, could also be increased due to the smallerdistance between the heat source and the pool boundary. Consequently, theproduct GR or the cooling rate is increased signiﬁcantly by the action of arcoscillation. This explains why the microstructure is ﬁner in the oscillated arcweld.Example: Suppose the welding speed of a regular weld is 4.2 mm/s (10 ipm).Calculate the increase in the velocity of the weld pool if the arc is oscillated NO TRANSVERSE OSCILLATION OSCILLATION (a) (b)Figure 8.15 Microstructures near fusion line of gas-tungsten arc welds of 2014 alu-minum: (a) coarser dendrites in weld made without arc oscillation; (b) ﬁner dendritesin weld made with transverse arc oscillation. Magniﬁcation 200¥. Reprinted from Kouand Le (16). Courtesy of American Welding Society.
REFINING MICROSTRUCTURE WITHIN GRAINS 211Figure 8.16 Tensile testing of two gas–tungsten arc welds of 2014 aluminum madewithout arc oscillation and with transverse arc oscillation. From Kou and Le (16). No oscillation u (a) w v u (b) Transverse oscillationFigure 8.17 Increase in weld pool travel speed due to transverse arc oscillation. Mod-iﬁed from Kou and Le (16). Courtesy of American Welding Society.transversely at a frequency of 1 Hz and an amplitude (the maximum deﬂec-tion of the arc from the weld centerline) of 1.9 mm. Do you expect the den-drite arm spacing to keep on decreasing if the frequency keeps on increasingto, say, 100 Hz?
212 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINS Since the arc travels a distance equal to four oscillation amplitudesper second, v = 4 ¥ 1.9 mm/s = 7.6 mm/s. Therefore, the resultant velocity w =(u2 + v2)1/2 = (4.22 + 7.62)1/2 = 8.7 mm/s. The increase in the weld pool velocityis 8.7 - 4.2 = 4.5 mm/s. The increase in the weld pool velocity and hence thedecrease in the dendrite arm spacing cannot keep on going with increasingoscillation frequency. This is because when the arc oscillates too fast, say at100 Hz, the weld pool cannot catch up with it because there is not enough timefor melting and solidiﬁcation to occur. It is interesting to point out that Kou and Le (16) also observed that themicrostructure in oscillated arc welds is much more uniform than that in weldswithout oscillation. In oscillated arc welds the weld centerline is no longer alocation where the cooling rate (or GR) is clearly at its maximum. Tseng and Savage (17) studied the microstructure in gas–tungsten arcwelds of HY-80 steel made with transverse and longitudinal arc oscillation.Reﬁning of the grain structure was not obtained, but reﬁning of the dendriticstructure within grains (subgrain structure) was observed and solidiﬁcationcracking was reduced, as shown in Figure 8.18. It is possible that solidiﬁcationcracking was reduced because the crack-causing constituents were dilutedto a greater extent by the larger interdendritic area in the welds with a ﬁnerdendritic structure. Half-amplitude = Subgrain diameter 30 1.65mm (0.065in) (microns) 20 10 0 0 0.23 0.42 1.20 (a) Frequency of oscillation-Hz Amplitude =1.65mm crack length (mils) crack length (mm) 0.75 30 Mean maximum (0.065in) Mean maximum 0.50 20 0.25 10 0 0 No 0.42 1.19 oscillation Hz Hz (b) Oscillation frequencyFigure 8.18 Effect of magnetic arc oscillation on gas–tungsten arc welds of HY-80steel: (a) reﬁning of microstructure within grains; (b) solidiﬁcation cracking. Modiﬁedfrom Tseng and Savage (17).
FURTHER READING 2138.4.2 Arc PulsationBecker and Adams (18) studied the microstructure in pulsed arc welds oftitanium alloys. It was observed that the cell spacing varied periodicallyalong the weld, larger where solidiﬁcation took place during the high-currentportion of the cycle. Obviously, the cooling rate was signiﬁcantly lower dur-ing the high-current portion of the cycle. This is because, from Equation(2.17), the cooling rate can be expected to decrease with increasing heatinput, though, strictly speaking, this equation is for steady-state conditionsonly.REFERENCES 1. Nakagawa, H., et al., J. Jpn. Weld. Soc., 39: 94, 1970. 2. Savage, W. F., Nippes, E. F., and Erickson, J. S., Weld. J., 55: 213s, 1976. 3. Kou, S., and Le, Y., unpublished research, University of Wisconsin, Madison, 1983. 4. David, S. A., and Vitek, J. M., Int. Mater. Rev., 34: 213, 1989. 5. Rappaz, M., David, S. A., Vitek, J. M., and Boatner, L. A., in Recent Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM Interna- tional, Materials Park, OH, May 1989, p. 147. 6. Kou, S., Kanevsky, T., and Fyﬁtch, S., Weld. J., 61: 175s, 1982. 7. Kou, S., and Le, Y., Metall. Trans. A, 14A: 2245, 1983. 8. Lanzafame, J. N., and Kattamis, T. Z., Weld. J., 52: 226s, 1973. 9. Savage, W. F., Lundin, C. D., and Hrubec, R. J., Weld. J., 47: 420s, 1968.10. Metals Handbook, Vol. 7, 8th ed., American Society for Metals, Metals Park, OH, 1972, pp. 266, 269.11. Elmer, J. W., Allen, S. M., and Eagar, T. W., Metall. Trans., 20A: 2117, 1989.12. Brown, P. E., and Adams, C. M. Jr., Weld. J., 39: 520s, 1960.13. Jordan, M. F., and Coleman, M. C., Br. Weld. J., 15: 552, 1968.14. Lanzafame, J. N., and Kattamis, T. Z., Weld. J., 52: 226s, 1973.15. Fukui, T., and Namba, K., Trans. Jpn. Weld. Soc., 4: 49, 1973.16. Kou, S., and Le, Y., Weld. J., 64: 51, 1985.17. Tseng, C., and Savage, W. F., Weld. J., 50: 777, 1971.18. Becker, D. W., and Adams, C. M. Jr., Weld. J., 58: 143s, 1979.19. Savage, W. F., in Weldments: Physical Metallurgy and Failure Phenomena, Eds. R. J. Christoffel, E. F. Nippes, and H. D. Solomon, General Electric Co., Schenec- tady, NY, 1979, p. 1.FURTHER READING1. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20: 83, 1975.2. Savage, W. F., Weld. World, 18: 89, 1980.
214 WELD METAL SOLIDIFICATION II: MICROSTRUCTURE WITHIN GRAINS3. David, S. A., and Vitek, J. M., Int. Mater. Rev., 34: 213, 1989.4. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.PROBLEMS8.1 It has been suggested that the secondary dendrite arm spacing d along the weld centerline can be related quantitatively to the heat input per unit length of weld, Q/V. Based on the data of the dendrite arm spacing d as a function of cooling rate e, similar to those shown in Figure 6.17a, it can be shown that d = ae-1/b, where a and b are constant with b being in the range of 2–3. (a) Express the dendrite arm spacing in terms of Q/V for bead-on-plate welds in thick-section aluminum alloys. (b) How do the preheat temperature and thermal conductivity affect the dendrite arm spacing? (c) Do you expect the relationship obtained to be very accurate?8.2 The size of the mushy zone is often an interesting piece of information for studying weld metal solidiﬁcation. Let d = ae-1/b, where d is the den- drite arm spacing and e the cooling rate. Consider how measurements of the dendrite arm spacing across the weld metal can help determine the size of the mushy zone. Express the width of the mushy zone in the welding direction Dx, as shown in Figure P8.2, in terms of the dendrite arm spacing d, the welding speed V, and the freezing temperature range DT (= TL - TE).8.3 It has been observed that the greater the heat input per unit length of weld (Q/V), the longer it takes to homogenize the microsegregation in the weld metal of aluminum alloys for improving its mechanical proper- ties. Let d = ae-1/b, where d is the dendrite arm spacing and e the cooling rate. Express the time required for homogenization (t) in terms of Q/V.8.4 An Al–1% Cu alloy is welded autogenously by GTAW, and an Al–5% Cu alloy is welded under identical condition. Which alloy is expected to develop more constitutional supercooling and why? Which alloy is likely to have more equiaxed dendrites in the weld metal and why?8.5 An Al–5% Cu alloy is welded autogenously by GTAW and by EBW under the same welding speed but different heat inputs (much less in the TL TE V ∆x weld pool mushy zone Figure P8.2
PROBLEMS 215 Figure P8.8 case of EBW). Which weld is expected to experience more constitutional supercooling and why? Which weld is likely to have more equiaxed den- drites and why?8.6 In autogenous GTAW of aluminum alloys, how do you expect the amount of equiaxed grains in the weld metal to be affected by preheating and why?8.7 In autogenous GTAW of aluminum alloys, how do you expect the den- drite arm spacing of the weld metal to be affected by preheating and why?8.8 Figure P8.8 is a micrograph near the fusion line of an autogenous gas–tungsten arc weld in a Fe–49% Ni alloy sheet (19). Explain the solid- iﬁcation microstructure, which is to the right of the fusion line (dark ver- tical line).
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-49 Post-Solidiﬁcation PhaseTransformationsPost-solidiﬁcation phase transformations, when they occur, can change thesolidiﬁcation microstructure and properties of the weld metal. It is, there-fore, essential that post-solidiﬁcation phase transformations be understoodin order to understand the weld metal microstructure and properties. Inthis chapter two major types of post-solidiﬁcation phase transformations inthe weld metal will be discussed. The ﬁrst involves the ferrite-to-austenitetransformation in welds of austenitic stainless steels, and the second involvesthe austenite-to-ferrite transformation in welds of low-carbon, low-alloysteels.9.1 FERRITE-TO-AUSTENITE TRANSFORMATION INAUSTENITIC STAINLESS STEEL WELDS9.1.1 Primary Solidiﬁcation ModesThe welds of austenitic stainless steels normally have an austenite (fcc) matrixwith varying amounts of d-ferrite (bcc) (1–7). A proper amount of d-ferrite inaustenitic stainless steel welds is essential—too much d-ferrite (տ10 vol %)tends to reduce the ductility, toughness, and corrosion resistance, while toolittle d-ferrite (Շ5 vol %) can result in solidiﬁcation cracking.A. Phase Diagram Figure 9.1 shows the ternary phase diagram of theFe–Cr–Ni system (8). The heavy curved line in Figure 9.1a represents thetrough on the liquidus surface, which is called the line of twofold saturation.The line declines from the binary Fe–Ni peritectic reaction temperatureto the ternary eutectic point at 49Cr–43Ni–8Fe. Alloys with a composition onthe Cr-rich (upper) side of this line have d-ferrite as the primary solidiﬁcationphase, that is, the ﬁrst solid phase to form from the liquid. On the other hand,alloys with a composition on the Ni-rich (lower) side have austenite as theprimary solidiﬁcation phase. The heavy curved 1ines on the solidus surface inFigure 9.1b more or less follow the trend of the liquidus trough and convergeat the ternary eutectic temperature. The development of weld metal microstructure in austenitic stainless steelsis explained in Figure 9.2. The weld metal ferrite can have three different types216
Figure 9.1 The Fe–Cr–Ni ternary system: (a) liquidus surface; (b) solidus surface. Reprinted from Metals Handbook (8).217
218 POST-SOLIDIFICATION PHASE TRANSFORMATIONS Primary austenite Primary ferrite solidification solidification liquid liquid liquid γ δ δ interdendritic γ γ vermicular lathy γ ferrite ferrite or ferrite (a) (b) (c) liquid, L 1 4 Temperature 2 3 L+ γ L+ δ L+ γ + δ austenite, γ δ+γ ferrite, δ increasing Ni increasing Cr (d)Figure 9.2 Schematics showing solidiﬁcation and postsolidiﬁcation transformation inFe–Cr–Ni welds: (a) interdendritic ferrite; (b) vermicular ferrite; (c) lathy ferrite; (d)vertical section of ternary-phase diagram at approximately 70% Fe.of morphology: interdendritic (Figure 9.2a), vermicular (Figure 9.2b), andlathy (Figure 9.2c). Figure 9.2d shows a schematic vertical (isoplethal) sectionof the ternary phase diagram in Figure 9.1, for instance, at 70 wt % Fe andabove 1200°C. This has also been called a pseudo-binary phase diagram. Theapex (point 1) of the three-phase eutectic triangle (L + g + d) corresponds tothe intersection between the vertical section and the heavy curved line inFigure 9.1a. The two lower corners (points 2 and 3) of the triangle, on the otherhand, correspond to the intersections between the vertical section and the twoheavy curved lines in Figure 9.1b.B. Primary Austenite For an alloy on the Ni-rich (left-hand) side of the apexof the three-phase eutectic triangle, austenite (g) is the primary solidiﬁcationphase. The light dendrites shown in Figure 9.2a are austenite, while the darkparticles between the primary dendrite arms are the d-ferrite that forms when
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 219the three-phase triangle is reached during the terminal stage of solidiﬁcation.These are called the interdendritic ferrite. For dendrites with long secondaryarms, interdendritic ferrite particles can also form between secondary dendritearms.C. Primary Ferrite For an alloy on the Cr-rich (right-hand) side of the apexof the three-phase eutectic triangle, d-ferrite is the primary solidiﬁcation phase.The dark dendrites shown in Figure 9.2b are d-ferrite. The core of the d-ferritedendrites, which forms at the beginning of solidiﬁcation, is richer in Cr (point4), while the outer portions, which form as temperature decreases, have lowerchromium contents. Upon cooling into the (d + g) two-phase region, the outerportions of the dendrites having less Cr transform to austenite, thus leavingbehind Cr-rich “skeletons” of d-ferrite at the dendrite cores. This skeletalferrite is called vermicular ferrite. In addition to vermicular ferrite, primaryd-ferrite dendrites can also transform to lathy or lacy ferrite upon coolinginto the (d + g) two-phase region, as shown in Figure 9.2c.D. Weld Microstructure Figure 9.3a shows the solidiﬁcation structure at thecenterline of an autogenous gas–tungsten arc weld of a 310 stainless steelsheet, which contains approximately 25% Cr, 20% Ni, and 55% Fe by weight(9). The composition is on the Ni-rich (left) side of the apex of the three-phaseeutectic triangle, as shown in Figure 9.4a, and solidiﬁcation occurs as primaryaustenite. The microstructure consists of austenite dendrites (light etching;mixed-acids etchant) and interdendritic d-ferrite (dark etching; mixed-acidsetchant) between the primary and secondary dendrite arms, similar to thoseshown in Figure 9.2a. Figure 9.3b, on the other hand, shows the solidiﬁcation structure at thecenterline of an autogenous gas–tungsten arc weld of a 309 stainless steelsheet, which contains approximately 23 wt % Cr, 14 wt % Ni, and 63 wt % Fe.The composition lies just to the Cr-rich side of the apex of the three-phaseeutectic triangle, as shown in Figure 9.4b, and solidiﬁes as primary d-ferrite.The microstructure consists of vermicular ferrite (dark etching; mixed-acids etchant) in an austenite matrix (light etching; mixed-acids etchant)similar to those shown in Figure 9.2b. In both welds columnar dendrites growessentially perpendicular to the teardrop-shaped pool boundary as revealedby the columnar dendrites. Kou and Le (9) quenched welds during welding in order to preservethe as-solidiﬁed microstructure, that is, the microstructure before post-solidiﬁcation phase transformations. For stainless steels liquid-tin quenchingis more effective than water quenching because steam and bubbles reduce heattransfer. With the help of quenching, the evolution of microstructure duringwelding can be better studied. Figure 9.5 shows the d-ferrite dendrites (lightetching; mixed-chloride etchant) near the weld pool of an autogenous gas–tungsten arc weld of 309 stainless steel, quenched in during welding with liquidtin before the d Æ g transformation changed it to vermicular ferrite like that
220 POST-SOLIDIFICATION PHASE TRANSFORMATIONSFigure 9.3 Solidiﬁcation structure at the weld centerline: (a) 310 stainless steel; (b)309 stainless steel. Magniﬁcation 190¥. Reprinted from Kou and Le (9). L L L 1400 Temperature, o C δ δ δ L γ+δ + γ γ δ δ δ+γ + 1000 γ γ + γ 600 55%Fe 63%Fe 73%Fe (a) (b) (c) 15 25 35 10 20 30 5 15 25 wt%Cr 30 20 10 27 17 7 22 12 2 wt%NiFigure 9.4 The Fe–Cr–Ni pseudo-binary phase diagrams: (a) at 55 wt % Fe; (b) at 63wt % Fe; (c) at 73 wt % Fe. Reprinted from Kou and Le (9).
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 221Figure 9.5 Liquid-tin quenched solidiﬁcation structure near the pool of an auto-genous gas–tungsten arc weld of 309 stainless steel. Magniﬁcation 70ϫ. Mixed-chlorideetchant. Reprinted from Kou and Le (9).shown in Figure 9.3b. Liquid-tin quenching was subsequently used by otherinvestigators to study stainless steel welds (10, 11).9.1.2 Mechanisms of Ferrite FormationInoue et al. (11) studied vermicular and lathy ferrite in autogenous GTAW ofaustenitic stainless steels of 70% Fe with three different Cr–Ni ratios. It wasfound that, as the Cr–Ni ratio increases, the ratio of lathy ferrite to total ferritedoes not change signiﬁcantly even though both increase. A schematic of theproposed formation mechanism of vermicular and lathy ferrite is shown inFigure 9.6. Austenite ﬁrst grows epitaxially from the unmelted austenite grainsat the fusion boundary, and d-ferrite soon nucleates at the solidiﬁcation front.The crystallographic orientation relationship between the d-ferrite and theaustenite determines the ferrite morphology after the postsolidiﬁcation trans-formation. If the closed-packed planes of the d-ferrite are parallel to those ofthe austenite, the d Æ g transformation occurs with a planar d/g interface,resulting in vermicular ferrite. However, if the so-called Kurdjumov–Sachs ori- ¯ ¯ ¯¯ ¯¯entation relationships, namely, (110)d //(111)g and d //g, exist betweenthe d-ferrite and the austenite, the transformation occurs along the austenitehabit plane into the d-ferrite dendrites. The resultant ferrite morphology islathy, as shown in Figure 9.7. For the lathy ferrite to continue to grow, the
222 POST-SOLIDIFICATION PHASE TRANSFORMATIONSFigure 9.6 Mechanism for the formation of vermicular and lathy ferrite. Reprintedfrom Inoue et al. (11).Figure 9.7 Lathy ferrite in an autogenous gas–tungsten arc weld of Fe–18.8Cr–11.2Ni.Reprinted from Inoue et al. (11).
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 223preferred growth direction <100> of both d-ferrite and austenite must bealigned with the heat ﬂow direction.9.1.3 Prediction of Ferrite ContentSchaefﬂer (12) ﬁrst proposed the quantitative relationship between the com-position and ferrite content of the weld metal. As shown by the constitutiondiagram in Figure 9.8, the chromium equivalent of a given alloy is determinedfrom the concentrations of ferrite formers Cr, Mo, Si, and Cb, and the austen-ite equivalent is determined from the concentrations of austenite formers Ni,C, and Mn. DeLong (13) reﬁned Schaefﬂer’s diagram to include nitrogen, astrong austenite former, as shown in Figure 9.9. Also, the ferrite content isexpressed in terms of the ferrite number, which is more reproducible than theferrite percentage and can be determined nondestructively by magneticmeans. Figure 9.10 shows that nitrogen, introduced into the weld metal byadding various amounts of N2 to the Ar shielding gas, can reduce the weldferrite content signiﬁcantly (14). Cieslak et al. (6), Okagawa et al. (7), andLundin et al. (15) have reported similar results previously. The WRC-1992 diagram of Kotecki and Siewert (16), shown in Figure 9.11,was from the Welding Research Council in 1992. It was modiﬁed from theWRC-1988 diagram of McCowan et al. (17) by adding to the nickel equiva-lent the coefﬁcient for copper (18) and showing how the axes could beextended to make Schaefﬂer-like calculations for dissimilar metal joining. 30 28 e rit 26 Fer %Ni + 30 X %C + 0.5 X %Mn 24 Austenite 0% 22 5% Nickel equivalent = % 20 10 18 % A +M 20 16 % 14 A+F 40 12 80% 10 Martensite 8 A+M+F 100% 6 4 F+ M+F Ferrite 2 M 0 0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30 32 34 36 38 40 Chromium equivalent = %Cr + %Mo + 1.5 X %Si + 0.5 X %CbFigure 9.8 Schaefﬂer diagram for predicting weld ferrite content and solidiﬁcationmode. From Schaefﬂer (12).
224 POST-SOLIDIFICATION PHASE TRANSFORMATIONS WRC ferrite number 21 %Ni + 30 X %C + 30 X %N + 0.5 X %Mn 0 2 4 6 8 20 0 12 Austenite 1 19 14 18 1 6 18 Nickel equivalent = 17 Prior magnetic ferrite % 16 15 Sc 14 ha 0 eff A+ ler 4 13 M 2 line 6 2 Austenite 12 9. .3 plus ferrite 6 7. .7 12 11 0 .8 1 3 10 1 16 17 18 19 20 21 22 23 24 25 26 27 Chromium equivalent = %Cr + %Mo + 1.5 X %Si + 0.5 X %CbFigure 9.9 DeLong diagram for predicting weld ferrite content and solidiﬁcationmode. Reprinted from DeLong (13). Courtesy of American Welding Society. 80 Ferrite content (%) 60 40 20 0 0.1 0.2 0.3 0.4 Nitrogen content (mass%)Figure 9.10 Effect of nitrogen on ferrite content in gas–tungsten arc welds of duplexstainless steel. Reprinted from Sato et al. (14).Kotecki (19, 20) added the martensite boundaries to the WRC-1992 diagram,as shown in Figure 9.12. More recent investigations of Kotecki (21, 22) haverevealed that the boundaries hold up well with Mo and N variation butnot as well with C variation. Balmforth and Lippold (23) proposed theferritic–martensitic constitution diagram shown in Figure 9.13. Vitek et al. (24,
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 225Figure 9.11 WRC-1992 diagram for predicting weld ferrite content and solidiﬁcationmode. Reprinted from Kotecki and Siewert (16). Courtesy of American WeldingSociety.Figure 9.12 WRC-1992 diagram with martensite boundaries for 1, 4, and 10% Mn.Reprinted from Kotecki (20). Courtesy of American Welding Society.
226 POST-SOLIDIFICATION PHASE TRANSFORMATIONS 6 Martensite A+M+ F 5 20 40 60 70 80 90 Ni + 35C + 20N 10 30 50 4 M+F 3 2 Ferrite 1 0 8 10 12 14 16 18 20 22 Cr + 2Mo + 10(Al + Ti)Figure 9.13 Ferritic–martensitic stainless steel constitution diagram containing aboundary for austenite formation and with iso-ferrite lines in volume percent of ferrite.Reprinted from Balmforth and Lippold (23).Figure 9.14 Experimentally measured ferrite number (FN) versus predicted FN: (a)FNN-1999; (b) WRC-1992. Reprinted from Vitek et al. (25). Courtesy of AmericanWelding Society.25) developed a model FNN-1999 using artiﬁcial neural networks to improveferrite number prediction, as shown in Figure 9.14. Twelve alloying elementsbesides Fe were considered: C, Cr, Ni, Mo, N, Mn, Si, Cu, Ti, Cb, V, and Co. Themodel is not in a simple pictorial form, such as the WRC-1992 diagram,because it allows nonlinear effects and element interactions.9.1.4 Effect of Cooling RateA. Changes in Solidiﬁcation Mode The prediction of the weld metal ferritecontent based on the aforementioned constitution diagrams can be inaccurate
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 227when the cooling rate is high, especially in laser and electron beam welding(3, 26–37). Katayama and Matsunawa (28, 29), David et al. (31), and Brooksand Thompson (37) have compared microstructures that form in slow-cooling-rate arc welds with those that form in high-cooling-rate, high-energy-beamwelds. Their studies show two interesting trends. For low Cr–Ni ratio alloys theferrite content decreases with increasing cooling rate, and for high Cr–Ni ratioalloys the ferrite content increases with increasing cooling rate. Elmer et al.(33) pointed out that in general low Cr–Ni ratio alloys solidify with austeniteas the primary phase, and their ferrite content decreases with increasingcooling rate because solute redistribution during solidiﬁcation is reduced athigh cooling rates. On the other hand, high Cr–Ni ratio alloys solidify withferrite as the primary phase, and their ferrite content increases with increas-ing cooling rate because the d Æ g transformation has less time to occur athigh cooling rates. Elmer et al. (33, 34) studied a series of Fe–Ni–Cr alloys with 59% Fe andthe Cr–Ni ratio ranging from 1.15 to 2.18, as shown in Figure 9.15. The apexof the three-phase triangle is at about Fe–25Cr–16Ni. Figure 9.16 summarizesthe microstructural morphologies of small welds made by scanning an elec-tron beam over a wide range of travel speeds and hence cooling rates (33). Atlow travel speeds such as 0.1–1 mm/s, the cooling rates are low and the alloyswith a low Cr–Ni ratio (especially alloys 1 and 2) solidify as primary austen-ite. The solidiﬁcation mode is either single-phase austenite (A), that is, noferrite between austenite dendrites or cells (cellular–dendritic A), or primaryaustenite with second-phase ferrite (AF), that is, only a small amount of ferritebetween austenite dendrites (interdendritic F). The alloys with a high Cr–Ni 1550 L 59% Fe 1500 1 23 4 5 6 7 1450 Temperature, oC L+F 1400 L+A 1350 A A+F F 1300 1250 1200 Cr 21 23 25 27 29 31 Ni 20 18 16 14 12 10 Composition, wt%Figure 9.15 Vertical section of Fe–Ni–Cr phase diagram at 59% Fe showing sevenalloys with Cr–Ni ratio ranging from 1.15 to 2.18. Modiﬁed from Elmer et al. (33).
228 POST-SOLIDIFICATION PHASE TRANSFORMATIONS Cr Ni 30 11 alloys Widmanstatten A 7 cellular F blocky A 28 13 Composition, wt% 6 5 lacy F intercellular A massive A 26 15 4 vermicular F 3 2 interdendritic F intercellular F 24 17 cellular A 1 22 19 cellular-dendritic A 20 21 10-1 100 101 102 103 104 Electron-beam travel speed, mm/sFigure 9.16 Electron beam travel speed (cooling rate) versus composition map ofmicrostructural morphologies of the seven alloys in Figure 9.15 (A and F denoteaustenite and ferrite, respectively). The solid lines indicate the regions of the fourprimary solidiﬁcation modes, while the dashed lines represent the different morpholo-gies resulting from postsolidiﬁcation transformation from ferrite to austenite. Modiﬁedfrom Elmer et al. (33).ratio (especially alloys 5–7), on the other hand, solidify as primary ferrite. Thesolidiﬁcation mode is primary ferrite with second-phase austenite (FA), thatis, vermicular ferrite, lacy ferrite, small blocks of austenite in a ferrite matrix(blocky A), or Widmanstatten austenite platelets originating from ferrite grainboundaries (Widmanstatten A). At very high welding speeds such as 2000 mm/s, however, the cooling ratesare high and the alloys solidify in only the single-phase austenite mode (A) orthe single-phase ferrite mode (F). An example of the former is the alloy 3(about Fe–24.75Cr–16.25Ni) shown in Figure 9.17a. At the travel speed of25 mm/s (2 ¥ 103 °C/s cooling rate) the substrate solidiﬁes as primary austen-ite in the AF mode, with austenite cells and intercellular ferrite. At the muchhigher travel speed of 2000 mm/s (1.5 ¥ 106 °C/s cooling rate) the weld at thetop solidiﬁes as primary austenite in the A mode, with much smaller austen-ite cells and no intercellular ferrite (cellular A). An example of the latter isalloy 6 (about Fe–27.5Cr–13.5Ni) shown in Figure 9.17b. At 25 mm/s the sub-strate solidiﬁes as primary ferrite in the FA mode, with blocky austenite in aferrite matrix. At 2000 mm/s the weld at the top solidiﬁes as primary ferrite inthe F mode, with ferrite cells alone and no austenite (cellular F). Figure 9.16 also demonstrates that under high cooling rates an alloy thatsolidiﬁes as primary ferrite at low cooling rates can change to primary austen-ite solidiﬁcation. For instance, alloy 4 (about Fe–25.5Cr–15.5Ni) can solidifyas primary ferrite at low cooling rates (vermicular F) but solidiﬁes as primary
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 229Figure 9.17 Microstructure of the low-cooling-rate substrate (2 ¥ 103 °C/s) and thehigh-cooling-rate electron beam weld at the top: (a) alloy 3 in Figure 9.15; (b) alloy 6.Reprinted from Elmer et al. (34).austenite at higher cooling rates (intercellular F or cellular A). Another inter-esting point seen in the same ﬁgure is that at high cooling rates alloy 5 cansolidify in the fully ferritic mode and undergoes a massive (diffusionless) trans-formation after solidiﬁcation to austenite (massive A). Under very highcooling rates there is no time for diffusion to occur.B. Dendrite Tip Undercooling Vitek et al. (27) attributed the change solid-iﬁcation mode, from primary ferrite to primary austenite, at high cooling ratesto dendrite tip undercooling. Brooks and Thompson (37) explained this under-cooling effect based on Figure 9.18. Alloy C0 solidiﬁes in the primary ferritemode at low cooling rates. Under rapid cooling in laser or electron beamwelding, however, the melt can undercool below the extended austeniteliquidus (CLg), and it becomes thermodynamically possible for the melt tosolidify as primary austenite. The closer C0 is to the apex of the three-phasetriangle, the easier sufﬁcient undercooling can occur to switch the solidiﬁca-tion mode from primary ferrite to primary austenite.
230 POST-SOLIDIFICATION PHASE TRANSFORMATIONS CL δ δ+ L γ+ L Temperature CLγ CS δ CS γ δ γ δ+γ Co Composition Ni CrFigure 9.18 Vertical section of Fe–Cr–Ni phase diagram showing change in solidiﬁ-cation from ferrite to austenite due to dendrite tip undercooling. Reprinted fromBrooks and Thompson (37).Figure 9.19 Weld centerline austenite in an autogenous gas–tungsten arc weld of 309stainless steel solidiﬁed as primary ferrite. From Kou and Le (9). Kou and Le (9) made autogenous gas–tungsten arc welds in 309 stainlesssteel, which has a composition close to the apex of the three-phase triangle,as shown in Figure 9.4b. At 2 mm/s (5 ipm) welding speed, primary ferrite wasobserved across the entire weld (similar to that shown in Figure 9.3b). At ahigher welding speed of 5 mm/s (12 ipm), however, primary austenite wasobserved along the centerline, as shown in Figure 9.19. Electron probe micro-analysis (EPMA) revealed no apparent segregation of either Cr or Ni nearthe weld centerline to cause the change in the primary solidiﬁcation phase.From Equation (8.3) the growth rate R = V cos a, where a is the angle betweenthe welding direction and the normal to the pool boundary. Because of theteardrop shape of the weld pool during welding (Figure 2.22), a drops to zero
TRANSFORMATION IN AUSTENITIC STAINLESS STEEL WELDS 231and R increases abruptly at the weld centerline. As such, the cooling rate (GR)increases abruptly at the weld centerline, as pointed out subsequently byLippold (38). Elmer et al. (34) calculated the dendrite tip undercooling for the alloys inFigure 9.16 under various electron beam travel speeds. An undercooling of45.8°C was calculated at the travel speed of 175 mm/s, which is sufﬁcient todepress the dendrite tip temperature below the solidus temperature (Figure9.15). This helps explain why alloy 4 can change from primary ferrite solidiﬁ-cation at low travel speeds to primary austenite solidiﬁcation at much highertravel speeds.9.1.5 Ferrite Dissolution upon ReheatingLundin and Chou (39) observed ferrite dissolution in multiple-pass or repairaustenitic stainless steel welds. This region exists in the weld metal of a previ-ous deposited weld bead, adjacent to but not contiguous with the fusion zoneof the deposited bead under consideration. Both the ferrite number and duc-tility are lowered in this region, making it susceptible to ﬁssuring under strain.This is because of the dissolution of d-ferrite in the region of the weld metalthat is reheated to below the g-solvus temperature. Chen and Chou (40)reported, in Figure 9.20, a signiﬁcant ferrite loss in a 316 stainless steel weldFigure 9.20 Effect of thermal cycles on ferrite content in 316 stainless steel weld: (a)as welded; (b) subjected to thermal cycle of 1250°C peak temperature three times afterwelding. Reprinted from Chen and Chou (40).
232 POST-SOLIDIFICATION PHASE TRANSFORMATIONSsubjected to three postweld thermal cycles with a 1250°C peak temperature,which is just below the g + d two-phase region of about 1280–1425°C.9.2 AUSTENITE-TO-FERRITE TRANSFORMATION INLOW-CARBON, LOW-ALLOY STEEL WELDS9.2.1 Microstructure DevelopmentThe dendrites or cells in the weld metal are not always discernible. First, sig-niﬁcant solute partitioning does not occur during solidiﬁcation if the partitionratio k is too close to 1. The miscrosegregation, especially solute segregationto the interdendritic or intercellular regions, in the resultant weld metal canbe too little to bring out the dendritic or cellular structure in the grain inte-rior even though the grain structure itself can still be very clear. Second, ifsolid-state diffusion occurs rapidly, microsegregation either is small or ishomogenized quickly, and the dendrites or cells in the resultant weld metalcan be unclear. Third, post-solidiﬁcation phase transformations, if they occur,can produce new microstructures in the grain interior and/or along grainboundaries and the subgrain structure in the resultant weld metal can beovershadowed. Several continuous-cooling transformation (CCT) diagrams have beensketched schematically to explain the development of the weld metalmicrostructure of low-carbon, low-alloy steels (41–45). The one shown inFigure 9.21 is based on that of Onsoien et al. (45). The hexagons represent thetransverse cross sections of columnar austenite grains in the weld metal. Asaustenite (g) is cooled down from high temperature, ferrite (a) nucleates atthe grain boundary and grows inward. The grain boundary ferrite is also called“allotriomorphic” ferrite, meaning that it is a ferrite without a regular faceted austenite grain boundary grain inclusion particle cooling Temperature curve ry fe rrite grain bounda austenite sideplate ferrite rrite accicular fe bainite martensite log TimeFigure 9.21 Continuous-cooling transformation diagram for weld metal of low-carbon steel.
TRANSFORMATION IN LOW-CARBON, LOW-ALLOY STEEL WELDS 233shape reﬂecting its internal crystalline structure. At lower temperatures themobility of the planar growth front of the grain boundary ferrite decreasesand Widmanstatten ferrite, also called side-plate ferrite, forms instead. Theseside plates can grow faster because carbon, instead of piling up at the planargrowth front, is pushed to the sides of the growing tips. Substitutional atomsdo not diffuse during the growth of Widmanstatten ferrite. At even lower tem-peratures it is too slow for Widmanstatten ferrite to grow to the grain interiorand it is faster if new ferrite nucleates ahead of the growing ferrite. This newferrite, that is, acicular ferrite, nucleates at inclusion particles and has randomlyoriented short ferrite needles with a basket weave feature. Figure 9.22 shows the microstructure of the weld metal of a low-carbon,low-alloy steel (46). It includes in Figure 9.22a grain boundary ferrite (A), (a) (b)Figure 9.22 Micrographs showing typical weld metal microstructures in low-carbonsteels: A, grain boundary ferrite; B, polygonal ferrite; C, Widmanstatten ferrite; D,acicular ferrite; E, upper bainite; F, lower bainite. Reprinted from Grong and Matlock(46).
234 POST-SOLIDIFICATION PHASE TRANSFORMATIONSWidmanstatten ferrite (C), and acicular ferrite (D) and in Figure 9.22bupper bainite (E) and lower bainite (F). A polygonal ferrite (B) is also found.Examination with transmission electron microscopy (TEM) is usually neededto identify the upper and lower bainite. The microstructure of a low-carbonsteel weld containing predominately acicular ferrite is shown in Figure 9.23and at a higher magniﬁcation in Figure 9.24 (47). The dark particles areinclusions.9.2.2 Factors Affecting MicrostructureBhadeshia and Suensson (48) showed in Figure 9.25 the effect of severalfactors on the development of microstructure of the weld metal: the weldmetal composition, the cooling time from 800 to 500°C (Dt8–5), the weld metaloxygen content, and the austenite grain size. The vertical arrows indicate thedirections in which these factors increase in strength. This will be explainedwith the help of CCT curves.A. Cooling Time Consider the left CCT curves (broken lines) in Figure 9.26.As cooling slows down (Dt8–5 increases) from curve 1 to curve 2 and curve 3,and the transformation product can change from predominately bainite(Figure 9.25c), to predominately acicular ferrite (Figure 9.25b) to predomi-nately grain boundary and Widmanstatten ferrite (Figure 9.25a).Figure 9.23 Predominately acicular ferrite microstructure of a low-carbon, low-alloysteel weld. Reprinted from Babu et al. (47).
TRANSFORMATION IN LOW-CARBON, LOW-ALLOY STEEL WELDS 235Figure 9.24 Acicular ferrite and inclusion particles in a low-carbon, low-alloy steelweld. Reprinted from Babu et al. (47).Figure 9.25 Schematic showing effect of alloy additions, cooling time from 800 to500°C, weld oxygen content, and austenite grain size. Reprinted from Bhadeshia andSvensson (48).B. Alloying Additions An increase in alloying additions (higher harden-ability) will shift the CCT curves toward longer times and lower temperatures.Consider now cooling curve 3 in Figure 9.26. The transformation product canchange from predominately grain boundary and Widmanstatten ferrite (leftCCT curves) to predominately acicular ferrite (middle CCT curves) to pre-dominately bainite (right CCT curves). This is like what Figure 9.25 shows.
236 POST-SOLIDIFICATION PHASE TRANSFORMATIONS austenite increasing alloying additions increasing grain size decreasing oxygen Temperature grain boundary ferrite sideplate ferrite acicular ferrite 1 2 bainite 3 log TimeFigure 9.26 Effect of alloying elements, grain size, and oxygen on CCT diagrams forweld metal of low-carbon steel. 110 Q&T C-Mn-Mo-Nb Prior austenite grain plate 3.0 MJ/m welds 100 diameter, µ m 90 80 70 0.01 0.02 0.03 0.04 0.05 Weld metal oxygen content, wt %Figure 9.27 Prior austenite grain diameter as a function of weld metal oxygen contentin submerged arc welds. Reprinted from Fleck et al. (49). Courtesy of AmericanWelding Society.C. Grain Size Similar to the effect of alloying additions, an increase in theaustenite grain size (less grain boundary area for ferrite nucleation) will alsoshift the CCT curves toward longer times and lower temperatures.D. Weld Metal Oxygen Content The effect of the weld metal oxygencontent on the weld metal microstructure is explained as follows. First, asshown in Figure 9.27, Fleck et al. (49) observed in submerged arc welds thatthe austenite grain size before transformation decreases with increasingweld metal oxygen content. Liu and Olson (50) observed that increasing theweld metal oxygen content increased the inclusion volume fraction anddecreased the average inclusion size. In fact, a large number of smaller sizeinclusions of diameters less than 0.1 mm was found. Since ﬁne second-phaseparticles are known to increasingly inhibit grain growth by pinning the grainboundaries as the particles get smaller and more abundant (51), increasing theweld metal oxygen content should decrease the prior austenite grain size.
TRANSFORMATION IN LOW-CARBON, LOW-ALLOY STEEL WELDS 237Therefore, the effect of decreasing the weld metal oxygen content is similar tothat of increasing the prior austenite grain size. This is just like what Figure9.25 shows. Second, larger inclusions, which are favored by lower weld metal oxygencontents, can act as favorable nucleation sites for acicular ferrite (50). Appro-priate inclusions appear to be in the size range 0.2–2.0 mm, and the mean sizeof about 0.4 mm has been suggested to be the optimum value (49, 51–53). Foxet al. (54) suggested in submerged arc welds of HY-100 steel that insufﬁcientinclusion numbers are generated for the nucleation of acicular ferrite if theoxygen content is too low (<200 ppm). On the other hand, many small oxideinclusions (<0.2 mm) can be generated if the oxygen content is too high(>300 ppm). These inclusions, though too small to be effective nuclei for aci-cular ferrite, reduce the grain size and thus provide much grain boundary areafor nucleation of grain boundary ferrite. As such, an optimum oxygen contentcan be expected for acicular ferrite to form. This is just like what Figure 9.25bshows. The existence of an optimum oxygen content for acicular ferrite to formhas also been reported by Onsoien et al. (45) in GMAW with oxygen or carbondioxide added to argon, as shown clearly in Figure 9.28. With Ar–O2 as theshielding gas, the shielding gas oxygen equivalent is the volume percentage ofO2 in the shielding gas. With Ar–CO2 as the shielding gas, it becomes thevolume percentage of CO2 in the shielding gas that will produce the sameoxygen content in the weld metal. As expected, the experimental results showthat the higher the shielding gas oxygen equivalent, the more hardenabilityelements such as Mn and Si from the ﬁller wire are oxidized. Consider againcooling curve 3 in Figure 9.26. As the shielding gas oxygen equivalent isreduced, the CCT curves can shift from left (broken lines) to middle (solid 100 Acicular ferrite content (vol. pct.) ER 70S-3, 1.8 MJ/m Oxygen in shielding gas 80 Carbon dioxide in shielding gas 60 40 20 0 0 5 10 15 20 Shielding gas oxygen equivalent (vol. pct.)Figure 9.28 Acicular ferrite content as a function of shielding gas oxygen equivalentfor gas–metal arc welds. Reprinted from Onsoien et al. (45). Courtesy of AmericanWelding Society.
238 POST-SOLIDIFICATION PHASE TRANSFORMATIONSlines) and a predominately acicular microstructure is produced. However, asthe shielding gas oxygen equivalent is reduced further, the CCT curves canshift from middle (solid lines) to right (dotted lines) and acicular ferrite nolonger predominates. Other factors have also been reported to affect amount of acicular ferritein the weld metal. For example, it has been reported that acicular ferriteincreases with increasing basicity index of the ﬂux for submerged arc welding(54), Ti (55, 56), and Mn and Ni (57).9.2.3 Weld Metal ToughnessAcicular ferrite is desirable because it improves the toughness of the weldmetal (55, 56). As shown in Figure 9.29, Dallam et al. (57) observed that the Energy absorbed (ft-lbs) 40 Q&T C-Mn-Mo-Nb plate 3.0 MJ/m welds 50 test temp. -40 oC 30 40 Joules 20 30 20 10 10 7.6 X 7.6 mm izod tests 0 30 40 50 60 70 80 Volume percent acicular ferriteFigure 9.29 Subsize Charpy V-notch toughness values as a function of volumefraction of acicular ferrite in submerged arc welds. Reprinted from Fleck et al. (49).Courtesy of American Welding Society. 0 Transition temperature at -10 -20 35J (deg. C) -30 -40 -50 -60 0 2 4 6 8 10 Shielding gas oxygen equivalent (vol. pct.)Figure 9.30 Weld metal Charpy V-notch toughness expressed as transition tempera-ture as a function of shielding gas oxygen equivalent. Reprinted from Onsoien et al.(45). Courtesy of American Welding Society.
REFERENCES 239weld metal Charpy V-notch toughness in submerged arc welds increases withincreasing volume fraction of acicular ferrite in the weld metal. The inter-locking nature of acicular ferrite, together with its ﬁne grain size, provides themaximum resistance to crack propagation by cleavage. The formation of grainboundary ferrite, ferrite side plates, or upper bainite is detrimental to weldmetal toughness, since these microstructures provide easy crack propagationpaths. Onsoien et al. (45) tested the Charpy V-notch toughness of GMA weldmetal using an energy absorption of 35 J as the criterion for measuring thetransition temperature for ductile-to-brittle fracture. Figure 9.30 showed thatthe maximum toughness (minimum transition temperature)occurs at a shield-ing gas oxygen equivalent of about 2 vol %. This, as can be seen from Figure9.28, essentially corresponds to the maximum amount of acicular ferrite in theweld metal, thus clearly demonstrating the beneﬁcial effect of acicular ferriteon weld metal toughness. Ahlblom (58) has shown earlier a clear minimum inthe plots of Charpy V-notch transition temperature versus weld metal oxygencontent.REFERENCES 1. David, S. A., Goodwin, G. M., and Braski, D. N., Weld. J., 58: 330s, 1979. 2. David, S. A., Weld. J., 60: 63s, 1981. 3. Lippold, J. C., and Savage, W. F., Weld. J., 58: 362s, 1974. 4. Lippold, J. C., and Savage, W. F., Weld. J., 59: 48s, 1980. 5. Cieslak, M. J., and Savage, W. F., Weld. J., 59: 136s, 1980. 6. Cieslak, M. J., Ritter, A. M., and Savage, W. F., Weld. J., 62: 1s, 1982. 7. Okagawa, R. K., Dixon, R. D., and Olson, D. L., Weld. J., 62: 204s, 1983. 8. Metals Handbook, Vol. 8, 8th ed., American Society for Metals, Metals Park, OH, 1973. 9. Kou, S., and Le, Y., Metall. Trans., 13A: 1141, 1982.10. Brooks, J. A., and Garrison, Jr., W. M., Weld. J., 78: 280s, 1999.11. Inoue, H., Koseki, T., Ohkita, S., and Fuji, M., Sci. Technol. Weld. Join., 5: 385, 2000.12. Schaefﬂer, A. L., Metal Prog., 56: 680, 1949.13. Delong, W. T., Weld. J., 53: 273s, 1974.14. Sato, Y. S., Kokawa, H., and Kuwana, T., Sci. Technol. Weld. Join., 4: 41, 1999.15. Lundin, C. D., Chou, C. P. D., and Sullivan, C. J., Weld. J., 59: 226s, 1980.16. Kotecki, D. J., and Siewert, T. A., Weld. J., 71: 171s, 1992.17. McCowan, C. N., Siewert, T. A., and Olson, D. L., WRC Bull., 342: 1–36, 1989.18. Lake, F. B., Expansion of the WRC-1988 Ferrite Diagram and Nitrogen Prediction, Abstracts of Papers, 1988 AWS Convention, Detroit, MI, pp. 214–215.19. Kotecki, D. J., Weld. J., 78: 180s, 1999.20. Kotecki, D. J., Weld. J., 79: 346s, 2000.
240 POST-SOLIDIFICATION PHASE TRANSFORMATIONS21. Kotecki, D. J., Weld Dilution and Martensite Appearance in Dissimilar Metal Welding, IIW Document II-C-195-00, 2000.22. Kotecki, D. J., private communications, Lincoln Electric Company, Cleveland, OH, 2001.23. Balmforth, M. C., and Lippold, J. C., Weld. J., 79: 339s, 2000.24. Vitek, J. M., Iskander, Y. S., and Oblow, E. M., Weld. J., 79: 33s, 2000.25. Vitek, J. M., Iskander, Y. S., and Oblow, E. M., Weld. J., 79: 41s, 2000.26. Vitek, J. M., and David, S. A., in Trends in Welding Research in the United States, Ed. S. A. David, American Society for Metals, Metals Park, OH, 1982.27. Vitek, J. M., DasGupta, A., and David, S. A., Metall. Trans., 14A: 1833, 1983.28. Katayama, S., and Matsunawa, A., Proc. International Congress on Applications of Laser and Electro-Optics 84, 44: 60–67, 1984.29. Katayama, S., and Matsunawa, A., in Proc. International Congress on Applications of Laser and Electro-Optics 85, San Francisco, 1985, IFS Ltd., Kempston, Bedford, UK, 1985, p. 19.30. Olson, D. L., Weld. J., 64: 281s, 1985.31. David, S. A., Vitek, J. M., and Hebble, T. L., Weld. J., 66: 289s, 1987.32. Bobadilla, M., Lacaze, J., and Lesoult, G., J. Crystal Growth, 89: 531, 1988.33. Elmer, J. W., Allen, S. M., and Eagar, T. W., Metall. Trans., 20A: 2117, 1989.34. Elmer, J. W., Eagar, T. W., and Allen, S. M., in Weldability of Materials, Eds. R. A. Patterson and K. W. Mahin, ASM International, Materials Park, OH, 1990, pp. 143–150.35. Lippold, J. C., Weld. J., 73: 129s, 1994.36. Koseki, T., and Flemings, M. C., Metall. Mater. Trans., 28A: 2385, 1997.37. Brooks, J. A., and Thompson, A. W., Int. Mater. Rev., 36: 16, 1991.38. Lippold, J. C., Weld. J., 64: 127s, 1985.39. Lundin, C. D., and Chou, C. P. D., Weld. J., 64: 113s, 1985.40. Chen, M. H., and Chou, C. P., Sci. Technol. Weld. Join., 4: 58, 1999.41. Abson, D. J., and Dolby, R. E., Weld. Inst. Res. Bull., 202: July 1978.42. Dolby, R. E., Metals Technol. 10: 349, 1983.43. Classiﬁcation of Microstructure in Low Carbon Low Alloy Weld Metal, IIW Doc. IX-1282-83, 1983, International Institute of Welding, London, UK.44. Vishnu, P. R., in ASM Handbook, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, pp. 70–87.45. Onsoien, M. I., Liu, S., and Olson, D. L., Weld. J., 75: 216s, 1996.46. Grong, O., and Matlock, D. K., Int. Metals Rev., 31: 27, 1986.47. Babu, S. S., Reidenbach, F., David, S. A., Bollinghaus, Th., and Hoffmeister, H., Sci. Technol. Weld. Join., 4: 63, 1999.48. Bhadeshia, H. K. D. H., and Svensson, L. E., in Mathematical Modelling of Weld Phenomena, Eds. H. Cerjak and K. Easterling, Institute of Materials, 1993.49. Fleck, N. A., Grong, O., Edwards, G. R., and Matlock, D. K., Weld. J., 65: 113s, 1986.50. Liu, S., and Olson, D. L., Weld. J., 65: 139s, 1986.51. Ashby, M. F., and Easterling, K. E., Acta Metall., 30: 1969, 1982.
PROBLEMS 24152. Bhadesia, H. K. D. H., in Bainite in Steels, Institute of Materials, London, 1992, Chapter 10.53. Edwards, G. R., and Liu, S., in Proceedings of the ﬁrst US-Japan Symposium on Advanced Welding Metallurgy, AWA/JWS/JWES, San Francisco, CA, and Yokohama, Japan, 1990, pp. 213–292.54. Fox, A. G., Eakes, M. W., and Franke, G. L., Weld. J., 75: 330s, 1996.55. Dolby, R. E., Research Report No. 14/1976/M, Welding Institute, Cambridge 1976.56. Glover, A. G., McGrath, J. T., and Eaton, N. F., in S Toughness Characterization and Speciﬁcations for HSLA and Structural Steels. ed. P. L. Manganon, Metallurgical Society of AIME, NY, pp. 143–160.57. Dallam, C. B., Liu, S., and Olson, D. L., Weld. J., 64: 140s, 1985.58. Ahlblom, B., Document No. IX-1322-84, International Institute of Welding, London, 1984.FURTHER READING1. Grong, O., and Matlock, D. K., Int. Meter. Rev., 31: 27, 1986.2. Brooks, J. A., and Thompson, A. W., Int. Mater. Rev., 36: 16, 1991.3. Vishnu, P. R., in ASM Handbook, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, pp. 70–87.4. Brooks, J. A., and Lippold, J. C., in ASM Handbook, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, pp. 456–470.PROBLEMS9.1 (a) Construct pseudobinary phase diagrams for 55% and 74% Fe. Mark on the diagrams the approximate compositions of 310 (essentially Fe–25 Cr–20 Ni) and 304 (essentially Fe–18Cr–8Ni) stainless steels. (b) From the diagrams and the approximate compositions, indicate the primary solidiﬁcation phases.9.2 A 308 stainless-steel ﬁller (essentially Fe–20Cr–10Ni) is used to weld 310 stainless steel.What is the primary solidiﬁcation phase if the dilution ratio is about 60%?9.3 A 304 stainless-steel sheet with a composition given below is welded autogenously with the GTAW process. The shielding gas is Ar-2% N2, and the nitrogen content of the weld metal is about 0.13%. The contents of other alloying elements are essentially the same as those in the base metal. (a) Calculate the ferrite numbers for the base metal and the weld metal. (b) The weld metal exhibits the primary solidiﬁcation phase of austen- ite, and the ferrite content measurements indicate essentially zero
242 POST-SOLIDIFICATION PHASE TRANSFORMATIONS ferrite number. Is the calculated ferrite number for the weld metal consistent with the observed one? (Composition: 18.10Cr, 8.49Ni, 0.060C, 0.66Si, 1.76Mn, 0.36Mo, 0.012S, 0.036P, and 0.066N.)9.4 A signiﬁcant amount of ferrite is lost in a 316 stainless steel weld after being subjected to three postweld thermal cycles with a 1250°C peak tem- perature, which is just below the g + d two-phase region of about 1280 to 1425°C. Sketch a curve of ferrite number vs. temperature from 900 to 1400°C and explain it.9.5 Kou and Le (9) quenched 309 stainless steel during autogenous GTAW. The weld metal side of the quenched pool boundary showed dendrites of d-ferrite but the weld pool side showed dendrites of primary austen- ite. Explain why.9.6 It has been observed in welding austenitic stainless steel with a teardrop- shaped weld pool that the weld metal solidiﬁes with primary ferrite except near the centerline, where it solidiﬁes as primary austenite. Sketch a curve of the growth rate R versus the distance y away from the weld centerline. How does your result explain the ferrite content change near the centerline?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-410 Weld Metal ChemicalInhomogeneitiesIn this chapter we shall discuss chemical inhomogeneities in the weld metal,including solute segregation, banding, inclusions, and gas porosity. Solute seg-regation can be either microsegregation or macrosegregation. Microsegrega-tion refers to composition variations across structures of microscopic sizes, forinstance, dendrite arms or cells (Chapter 6). Macrosegregation, on the otherhand, refers to variations in the local average composition (composition aver-aged over many dendrites) across structures of macroscopic sizes, for instance,the weld. Macrosegregation has been determined by removing samples acrossthe weld metal with a small drill for wet chemical analysis (1). Microsegrega-tion, on the other hand, has been determined by electron probe microanalysis(EPMA) (2–8) or scanning transmission electron microscopy (STEM) (9–14).The spacial resolution is lower in the former (e.g., about 1 mm) and higher inthe latter (e.g., about 0.1 mm).10.1 MICROSEGREGATIONAlloying elements with an equilibrium segregation coefﬁcient k < 1 tend tosegregate toward the boundary between cells or dendrite arms, and those withk > 1 tend to segregate toward the core of cells or dendrite arms (Chapter 6).Microsegregation can have a signiﬁcant effect on the solidiﬁcation crackingsusceptibility of the weld metal (Chapter 11).10.1.1 Effect of Solid-State DiffusionMicrosegregation can be reduced signiﬁcantly by solid-state diffusion duringand after solidiﬁcation. Consequently, microsegregation measured afterwelding may not represent the true microsegregation during welding, which ismore relevant to solidiﬁcation cracking (Chapter 11). Kou and Le (15) quenched stainless steels with liquid tin during autoge-nous GTAW in order to preserve the high-temperature microstructure aroundthe pool boundary. In 430 ferritic stainless steel the dendrites were clear nearthe quenched pool boundary but became increasingly blurred away from it,suggesting homogenization of microsegregation by the solid-state diffusion. 243
244 WELD METAL CHEMICAL INHOMOGENEITIESFerrite has a body-centered-cubic (bcc) structure, which is relatively openand thus easy for diffusion. In 310 austenitic stainless steel, however, thedendrites were clear even away from the quenched pool boundary, suggestingmuch less homogenization due to solid-state diffusion. Austenite has a face-centered-cubic (fcc) structure, which is more close packed than bcc and thusmore difﬁcult for diffusion. Brooks and Garrison (8) quenched a precipitation-strengthened marten-sitic stainless steel with liquid tin during GTAW. They measured microsegre-gation across the columnar dendrites, as shown in Figure 10.1a, where thequenched weld pool is in the upper right corner of the micrograph. The weldmetal solidiﬁed as a single-phase ferrite. As shown in Figure 10.1b, near theFigure 10.1 Microsegregation across columnar dendrites near quenched weld pool ina martensitic stainless steel: (a, b) near growth front; (c) 400 mm behind. Reprinted fromBrooks and Garrison (8). Courtesy of American Welding Society.
MICROSEGREGATION 245solidiﬁcation front segregation of Ni, Cu, and Nb toward the boundariesbetween dendrites is clear, the measured equilibrium segregation coefﬁcientsbeing 0.85, 0.9, and 0.36, respectively. The concentration peaks correspond tothe dendrite boundaries. The microsegregation proﬁles at 400 mm behind thesolidiﬁcation front are shown in Figure 10.1c. As shown, microsegregation isreduced signiﬁcantly by solid-state diffusion at elevated temperatures. Instead of using the Scheil equation (Chapter 6), Brooks and Baskes(16–19) calculated weld metal microsegregation considering solid-state diffu-sion and Lee et al. (20) further incorporated the kinetics of dendrite coarsen-ing. Figure 10.2a shows the calculated microsegregation in a Fe–23Cr–12Nistainless steel that solidiﬁes as ferrite (17, 18), where r is the radius of thegrowing cell and R is the ﬁnal cell radius. Since k > 1 for Cr, the cell core (r =0) is rich in Cr. The cell grows to about 60% of its full radius in 0.015 s aftersolidiﬁcation starts and 100% in 0.15 s, with Cr diffusing away from the cell 30 Cr Concentration ( wt % ) t=.015 sec 25 t=.075 sec t=.25 sec t=.75 sec 20 t=.15 sec (a) 15 0 0.2 0.4 0.6 0.8 1 Normalized Distance (r/R) 40 Cr Concentration ( wt % ) 30 t=.18 sec 20 Cr t= 3.2 sec Ni 10 (b) 0 0 0.2 0.4 0.6 0.8 1 Normalized Distance (r/R)Figure 10.2 Calculated microsegregation: (a) Fe–23Cr–12Ni (solid-state diffusion sig-niﬁcant); (b) Fe–21Cr–14Ni. Reprinted from Brooks (18).
246 WELD METAL CHEMICAL INHOMOGENEITIEScore as solidiﬁcation proceeds. Diffusion is fast in ferrite because of itsrelatively loosely packed bcc structure. Chromium diffusion continues aftersolidiﬁcation is over (0.25 s) and the resultant cell is nearly completelyhomogenized in 0.75 s after solidiﬁcation starts. Figure 10.2b, shows the calcu-lated microsegregation in a Fe–21Cr–14Ni stainless steel that solidiﬁes asaustenite at the time of ﬁnal solidiﬁcation (0.18 s) and 3 s later. Both Cr andNi are highly segregated to the cell boundary. Little solid-state diffusion occursduring cooling except near the cell boundary, where some diffusion occursbecause of the steep concentration gradients. Diffusion is slow in austenitebecause of its more densely packed fcc structure. Figure 10.3 shows the STEM microsegregation proﬁles across a dendritearm in the weld metal of 308 austenitic stainless steel (about Fe–20Cr–10Ni)measured by David et al. (10). The primary solidiﬁcation phase is d-ferriteFigure 10.3 Microsegregation in 308 stainless steel weld: (a) phase diagram; (b) TEMmicrograph of a dendrite arm; (c) microsegregation across the arm. Reprinted fromDavid et al. (10). Courtesy of American Welding Society.
MICROSEGREGATION 247(Figure 10.3a), but the dendrite arm has transformed to g except for theremaining d-ferrite core (Figure 10.3b). Nickel (k < 1) segregates toward thedendrite boundary, while Cr (k > 1) segregates toward the dendrite core(Figure 10.3c). Similar microsegregation proﬁles have been measured in weldsof 304L (11, 12) and 309 (13) stainless steels, and it has been conﬁrmed thatdiffusion occurs during the d Æ g transformation (6, 7, 10, 14).10.1.2 Effect of Dendrite Tip UndercoolingIn addition to solid-state diffusion, microsegregation can also be affected bythe extent of dendrite tip undercooling. The difference between the equilib-rium liquidus temperature TL and the dendrite tip temperature Tt is the totalundercooling DT, which can be divided into four parts: DT = DTC + DTR + DTT + DTK (10.1)where DTC = concentration-induced undercooling DTR = curvature-induced undercooling DTT = thermal undercooling DTK = kinetic undercooling The solute rejected by the dendrite tip into the liquid can pile up and causeundercooling at the dendrite tip DTC, similar to constitutional supercooling ata planar growth front (Chapter 6). The equilibrium liquidus temperature in aphase diagram is for a ﬂat solid–liquid interface, and it is suppressed if theinterface has a radius of curvature like a dendrite tip. Thermal undercoolingis present where there is a signiﬁcant nucleation barrier for the liquid totransform to solid. The kinetic undercooling, which is usually negligible, isassociated with the driving force for the liquid atoms to become attached tothe solid. It has been observed that the higher the velocity of the dendrite tip,Vt, the smaller the radius of the dendrite tip, Rt, and the larger the undercoolingat the dendrite tip, DT (21). This is shown schematically in Figure 10.4. Modelshave been proposed for dendrite tip undercooling, including those by Burdenand Hunt (22) and Kurz et al. (23). Brooks et al. (19) calculated weld metal microsegregation in Fe–Nb alloysconsidering dendrite tip undercooling as well as solid-state diffusion. Compo-sition analyses of tin-quenched gas–tungsten arc welds indicated a dendrite tipundercooling of 3.07°C in Fe–1.8Nb and 5.63°C in Fe–3.3Nb. Figure 10.5a showthe calculated results for a Fe–3.3Nb alloy, based on the model of Kurz et al.(23) with k = 0.28 for Nb and DL = 6.8 cm2/s. Undercooling results in a highercore Nb concentration during the initial stages of solidiﬁcation (0.08 s). But assolidiﬁcation proceeds to completion (1.2 s) and the weld cools (5.6 s), the con-centration proﬁles with and without undercooling start to converge due tothe signiﬁcant effect of solid-state diffusion. It was, therefore, concluded that
248 WELD METAL CHEMICAL INHOMOGENEITIES Dendrite Tips: lower tip velocity, larger tip radius, smaller tip Rt1 Vt1 undercooling Liquid higher tip velocity, smaller tip radius, larger tip Rt2 Vt2 undercooling Temperature, T TL ∆T1 Tt1 ∆T2 Tt2 Distance, x Figure 10.4 Dendrite tip undercooling. 5 Nb concentration (wt%) With tip undercooling 4 Without tip undercooling 3 t = 5.6s t = 1.2s 2 t = 0.08s 1 0 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 Fraction solidified ( r/R) (a) 5 Nb concentration (wt%) With tip undercooling 4 Without tip undercooling t = 0.08s 3 2 t = 0.008s 1 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 Fraction solidified (r/R) (b)Figure 10.5 Calculated microsegregation in a Fe–3.3Nb weld: (a) slower cooling rate;(b) higher cooling rate. Reprinted from Brooks et al. (19).
BANDING 249although tip undercooling can result in a higher Nb concentration duringinitial solidiﬁcation, its effect on the ﬁnal microsegregation is small because ofthe overwhelming effect of solid-state diffusion. With a very high cooling rateof 104°C/s such as in high-energy beam welding (less time for solid-state dif-fusion), Figure 10.5b shows that the effect of undercooling can be importantthroughout solidiﬁcation and subsequent cooling. Final microsegregation issigniﬁcantly less with dendrite tip undercooling than without.10.2 BANDING10.2.1 Compositional and Microstructural FluctuationsIn addition to microsegregation across dendrites, microsegregation canalso exist in the weld metal as a result of banding during weld poolsolidiﬁcation (Chapter 6). Banding in welds can cause perturbations in thesolidiﬁcation structure as well as the solute concentration (24). Figure 10.6shows banding and rippling near the centerline of the as-welded top surfaceof a YAG laser weld (conduction mode) in a 304 stainless steel, with alternat-ing bands of dendritic and planarlike structures. Figure 10.7 shows alternat-ing bands of austenite (light) and martensite (dark) in an A36 steelwelded with a E309LSi ﬁller by GTAW (25). The composition of A36 isFe–0.71Mn–0.29Cu–0.18Si–0.17C–0.13Ni–0.09Cr–0.05Mo and that of E309LSiis Fe–23.16Cr–13.77Ni–1.75Mn–0.79Si–0.20Cu–0.16Mo–0.11N–0.02C. Thehigh hardness (smaller indentation marks) in the darker regions reﬂects thepresence of martensite. The hydrogen crack in the martensite near but withinFigure 10.6 Banding and rippling near centerline of as-welded top surface of a 304stainless steel YAG laser welded in conduction mode.
250 WELD METAL CHEMICAL INHOMOGENEITIESFigure 10.7 Banding near fusion boundary of a carbon steel welded with an austeniticstainless steel ﬁller metal. Reprinted from Rowe et al. (25). Courtesy of AmericanWelding Society.the fusion boundary was promoted by the use of Ar–6% H2 as the shieldinggas.10.2.2 CausesBanding in the weld metal can occur due to a number of reasons. Fluctuationsin the welding speed during manual welding or arc pulsing during pulsed arcwelding can cause banding. However, even under steady-state welding condi-tions, banding can still occur, as evidenced by the surface rippling of the weld.Beside ﬂuctuations in the welding speed and the power input, the followingmechanisms also have been proposed: Solidiﬁcation halts due to the rapid evo-lution of latent heat caused by high solidiﬁcation rates during welding (26–28),oscillations of weld pool metal due to uncontrollable variations in arc stabil-ity and the downward stream of the shielding gas (29), and ﬂuctuations in weldpool turbulence due to electromagnetic effects (30, 31).10.3 INCLUSIONS AND GAS POROSITYInclusions and gas porosity tend to deteriorate the mechanical properties of theweld metal. Gas–metal and slag–metal reactions can produce gas porosity andinclusions in the weld metal and affect the weld metal properties (Chapter 3).Inclusions can also result from incomplete slag removal during multiple-passwelding (32), the large dark-etching particle near position D in Figure 10.8being one example (33). Figure 10.9 shows trapped surface oxides as inclusionsin the weld metal and their elimination by modifying the joint design (34).
INCLUSIONS AND GAS POROSITY 251Figure 10.8 Multipass weld with slag inclusions (D) and other defects, including lackof fusion (A), lamellar tearing (B), poor proﬁle (C), and undercut (E). Reprinted fromLochhead and Rodgers (33). Courtesy of American Welding Society.Figure 10.9 Joint designs and trapping of surface oxides in aluminum welding: (a)oxide trapped; (b) oxide not trapped (34). Various ways of reducing gas porosity in the weld metal have already beendescribed in Chapter 3. Gas pores can be round or interdendritic, as shown inFigure 10.10, which shows a gas–metal arc weld in 7075 aluminum made witha 4043 ﬁller metal. Similar gas pores have been reported in other aluminumwelds (35–37). Although round gas pores can be randomly distributed in theweld metal, they can also line up and form bands of porosity when bandingis severe during weld metal solidiﬁcation (35, 36). It is often difﬁcult to tellwhether interdendritic pores are due to gas formation or due to solidiﬁcation
252 WELD METAL CHEMICAL INHOMOGENEITIESFigure 10.10 Porosity in aluminum weld showing both spherical and interdendriticgas pores. One interdendritic pore is enlarged for clarity.shrinkage (21). However, if they are due to gas formation, they must haveformed during the latter stages of solidiﬁcation, where the dendritic structurehas essentially been established.10.4 INHOMOGENEITIES NEAR FUSION BOUNDARYDissimilar metal welding is often encountered in welding, where a ﬁller metaldifferent in composition from the base metal is used or where two base metalsdifferent in composition are welded together. In dissimilar metal welding, theregion near the fusion boundary often differ signiﬁcantly from the bulk weldmetal in composition and sometimes even microstructure and properties. Theregion, ﬁrst discovered by Savage et al. (38, 39), has been called the unmixedzone (38, 39), ﬁller-metal-depleted area (40), partially mixed zone (41), inter-mediate mixed zone (42), and hard zone (43). It has been observed in variouswelds, including stainless steels, alloy steels, aluminum alloys, and superalloys(38–47).10.4.1 Composition ProﬁlesOrnath et al. (46) determined the composition proﬁles across the fusionboundary of a low-alloy steel welded with a stainless steel ﬁller ofFe–18Cr–8Ni–7Mn, as shown in Figure 10.11. Plotting the concentrationagainst the distance from the fusion boundary according to Equation (6.17)(for solute segregation during the initial transient of solidiﬁcation), theyobtained a straight line. As such, they proposed that segregation rather thandiffusion is responsible for the observed composition proﬁles. In other words,the composition proﬁles are caused by the rejection of Cr, Ni, and Mn into themelt by the solid weld metal during the initial stage of solidiﬁcation.
INHOMOGENEITIES NEAR FUSION BOUNDARY 253Figure 10.11 Fusion boundary of a low-alloy steel welded with an austenitic stainlesssteel electrode: (a) microstructure (magniﬁcation 55¥); (b) segregation. Reprinted fromOrnath et al. (46). Courtesy of American Welding Society. Baeslack et al. (45) determined the composition proﬁles across the fusionboundary of a 304L stainless steel welded with a 310 stainless steel ﬁller, asshown in Figure 10.12. Unlike the composition proﬁles shown in Figure 10.11,the weld metal next to the fusion line, labeled as the unmixed zone by theauthors, has essentially the same composition as the base metal, suggestingstagnant melted base metal unmixed with the ﬁller metal. Figure 10.13 is aschematic sketch for an unmixed zone. The arrows show the directions of local
254 WELD METAL CHEMICAL INHOMOGENEITIESFigure 10.12 Unmixed zone in a 304L stainless steel welded with a 310 ﬁller metal:(a) microstructure; (b) composition proﬁles. Reprinted from Baeslack et al. (45). Cour-tesy of American Welding Society. bulk weld metal unmixed zone fusion boundary partially melted zone heat-affected base metal zone Figure 10.13 Zone of unmixed melted base metal along the fusion boundary.
MACROSEGREGATION IN BULK WELD METAL 255ﬂuid ﬂow during welding, which is not strong enough for thorough mixing butstrong enough to move parts of the melted base metal.Also shown in the ﬁgureare the partially melted zone (Chapters 12 and 13) and the heat-affected zone(Chapters 14–18).10.4.2 Effect of InhomogeneitiesInhomogeneities in the region along the fusion boundary have been reportedto cause problems, including hydrogen cracking (48, 49), corrosion (50), andstress corrosion cracking (45). Martensite often exists in the region in carbonor alloy steels welded with austenitic stainless steel ﬁllers. This is because theweld metal composition here can be within the martensite region of the con-stitutional diagrams (Chapter 9). This composition transition shown in Figure10.11 covers compositions in the martensite range of the Schaefﬂer diagram,thus explaining the formation of martensite (46). Linnert (48) observedmartensite and hydrogen cracking in weld metal along the fusion boundary ofa Cr–Ni–Mo steel welded with a 20Cr–10Ni stainless steel ﬁller. Savage et al.(49) reported similar hydrogen cracking in HY-80 welds. Rowe et al. (25)showed hydrogen cracking along the weld metal side of the fusion boundaryin a A36 steel gas–tungsten arc welded with a ER308 stainless steel ﬁller metaland an Ar-6% H2 shielding gas. Omar (43) welded carbon steels to austenitic stainless steels by SMAW.Figure 10.14 shows that the hard martensite layer in the weld metal along thecarbon steel side of the fusion boundary can be eliminated by using a Ni-baseﬁller metal plus preheating and controlling the interpass temperature. Theaustenitic stainless steel electrode E309, which has much less Ni and more Cr,did not work as well.10.5 MACROSEGREGATION IN BULK WELD METALWeld pool convection (Chapter 4) can usually mix the weld pool well tominimize macrosegregation across the resultant weld metal. Houldcroft (1) foundno appreciable macrosegregation in pure aluminum plates single-pass weldedwith Al–5% Cu ﬁller. Similar results were observed in Al–l.0Si–l.0Mg plates single-pass welded using either Al–4.9% Si or Al–1.4% Si as the ﬁller metal (1).However, in single-pass dissimilar-metal welding, macrosegregation can still occurif weld pool mixing is incomplete. In multiple-pass dissimilar-metal welding,macrosegregation can still occur even if weld pool mixing is complete in each pass.10.5.1 Single-Pass WeldsMacrosegregation can occur in a dissimilar weld between two different basemetals because of insufﬁcient mixing in the weld pool. Matsuda et al. (51)showed Cu macrosegregation across an autogenous gas–tungsten arcweld between thin sheets of 1100 aluminum (essentially pure Al) and 2024
256 WELD METAL CHEMICAL INHOMOGENEITIES (a) (b)Figure 10.14 Carbon steel side of weld metal in a weld between a carbon steel andan austenitic stainless steel made with a Ni-based ﬁller metal: (a) martensite alongfusion boundary; (b) martensite avoided by preheating and controlling interpass tem-perature. Reprinted from Omar (43). Courtesy of American Welding Society. (a) (b)Figure 10.15 Macrosegregation in a laser beam weld between Ti–6Al–4V andTi–3Al–8V–6Cr–4Mo–4Zr (bC): (a) transverse cross section; (b) composition proﬁles.Reprinted from Liu et al. (53). Courtesy of American Welding Society.
MACROSEGREGATION IN BULK WELD METAL 257 (a) (b)Figure 10.16 Powder metallurgy Al–10Fe–5Ce alloy gas–tungsten arc welded withAl–5Si ﬁller metal: (a) AC; (b) DCEN. Reprinted from Metzger (54). Courtesy ofAmerican Welding Society. Filler D Base Base metal A d metal B a b c Backing C a+b+c (1) % dilution = × 100 a+b+c+d (2) % element E in weld bead = [a (% E in a) + b (% E in b) + c (% E in c) + d (% E in d)] / (a + b + c + d)Figure 10.17 Filler metal dilution and composition in dissimilar-metal welding.Reprinted from Estes and Turner (55). Courtesy of American Welding Society.aluminum (essentially Al–4.4Cu). Macrosegregation was reduced throughenhanced mixing by magnetic weld pool stirring. In laser or electronbeam welding, the welding speed can be too high to give the weld metalsufﬁcient time to mix well before solidiﬁcation (52, 53). Figures 10.15shows macrosegregation in a laser weld between Ti–6Al–4V (left) andTi–3Al–8V–6Cr–4Mo–4Zr (right) (53). Macrosegregation due to lack of weld pool mixing has also been observedin GTAW of some powder metallurgy alloys. Such alloys are made by con-solidation of rapidly solidiﬁed powder having some special properties, forinstance, extended solubility of alloying elements. Figure 10.16 shows the lack
258 WELD METAL CHEMICAL INHOMOGENEITIESFigure 10.18 Macrosegregation in a multiple-pass weld between 4130 steel and 304stainless steel. Reprinted from Estes and Turner (55). Courtesy of American WeldingSociety.
MACROSEGREGATION IN BULK WELD METAL 259of mixing between an Al–10Fe–5Ce powder metallurgy base metal and a 4043(Al–5Si) ﬁller metal in AC GTAW and improved mixing and reduced gasporosity with DCEN GTAW (54). This may be because in GTAW weld pene-tration is higher with DCEN than with AC (Chapter 1).10.5.2 Multiple-Pass WeldsFigure 10.17 shows the ﬁller metal dilution and composition of the ﬁrst bead(root pass) in a dissimilar-metal weld (55). The composition of the beaddepends not only on the compositions of the base and ﬁller metals but also onthe extent of dilution. Apparently, the second bead to be deposited on top ofthe ﬁrst bead will have a different composition from the ﬁrst bead regardlessof the extent of weld pool mixing. Figure 10.18 shows the composition proﬁles across a multiple-pass weldbetween 4130 alloy steel and 304 stainless steel with a 312 stainless steel asthe ﬁller metal (55). Composition differences between beads are evident. Forinstance, the Cr content varies from 18% in the ﬁrst bead to 25% in the third.As a result of such macrosegregation, the ferrite content (which affects theresistance to solidiﬁcation cracking and corrosion) varies from one bead toanother, as shown in Figure 10.19.Figure 10.19 Variations in microstructure in a multiple-pass weld between 4130 steeland 304 stainless steel. Reprinted from Estes and Turner (55). Courtesy of AmericanWelding Society.
260 WELD METAL CHEMICAL INHOMOGENEITIESREFERENCES 1. Houldcroft, R. T., Br. Weld. J., 1: 468, 1954. 2. Lippold, J. C., and Savage, W. F., Weld. J., 58: 362s, 1979. 3. Takalo, T., Suutala, N., and Moisio, T., Metall. Trans., 10A: 1173, 1979. 4. Suutala, N., Takalo, T., and Moisio, T., Metall. Trans., 10A: 1183, 1979. 5. Ciestak, M. J., and Savage, W. F., Weld. J., 59: 136s, 1980. 6. Suutala, N., Takalo, T., and Moisio, T., Weld. J., 60: 92s, 1981. 7. Leone, G. L., and Kerr, H. W., Weld. J., 61: 13s, 1982. 8. Brooks, J. A., and Garrison, W. M. Jr., Weld. J., 78: 280s, 1999. 9. Gould, J. C., Ph.D. Thesis, Carnegie-Mellon University, Pittsburgh, PA, 1983.10. David, S. A., Goodwin, G. M., and Braski, D. N., Weld. J., 58: 330s, 1979.11. Lyman, C. E., Manning, P. E., Duquette, D. J., and Hall, E., Scan. Electron. Microsc., 1: 213, 1978.12. Lyman, C. E., Weld. J., 58: 189s, 1979.13. Brooks, J. A., Ph.D. Thesis, Carnegie-Mellon University, Pittsburgh, PA, 1982.14. Cieslak, M. J., Ritter, A. M., and Savage, W., Weld. J., 61: 1s, 1982.15. Kou, S., and Le, Y., Metall. Trans. A, 13A: 1141, 1982.16. Brooks, J. A., and Baskes, M. I., in Advances in Welding Science and Technology, Ed. S. A. David, ASM International, Materials Park, OH, March 1986, p. 93.17. Brooks, J. A., and Baskes, M. I., in Recent Trends in Welding Science and Technol- ogy, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, March 1990, p. 153.18. Brooks, J. A., in Weldability of Materials, Eds. R. A. Patterson and K. W. Mahin, ASM International, Materials Park, OH, March 1990, p. 41.19. Brooks, J. A., Li, M., Baskes, M. I., and Yang, N. C. Y., Sci. Technol. Weld. Join., 2: 160, 1997.20. Lee, J. Y., Park, J. M., Lee, C. H., and Yoon, E. P., in Synthesis/Processing of Light- weight Metallic Materials II, Eds. C. M. Ward-Close, F. H. Froes, S. S. Cho, and D. J. Chellman, The Minerals, Metals and Materials Society, Warrendale, PA 1996, p. 49.21. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.22. Burden, M. H., and Hunt, J. D., J. Crystal Growth, 22: 109, 1974.23. Kurz, W., Giovanola, B., and Trivedi, R., Acta Metall., 34: 823, 1986.24. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20: 83, 1975.25. Rowe, M. D., Nelson, T. W., and Lippold, J. C., Weld. J., 78: 31s, 1999.26. Gurev, H. S., and Stout, R. D., Weld. J., 42: 298s, 1963.27. Cheever, D. L., and Howden, D. G., Weld. J., 48: 179s, 1969.28. Morchan, B. A., and Abitdnar, A., Automat. Weld., 21: 4, 1968.29. Ishizaki, K., J. Jpn. Weld. Soc., 38: 1963.30. Jordan, M. F., and Coleman, M. C., Br. Weld. J., 15: 552, 1968.31. Waring, J., Aust. Weld. J., 11: 15, 1967.32. Gurney, T. R., Fatigue of Welded Structures, Cambridge University Press, Cambridge, 1968, p. 156.
PROBLEMS 26133. Lochhead, J. C., and Rodgers, K. J., Weld. J., 78: 49, 1999.34. Inert Gas Welding of Aluminum Alloys, Society of the Fusion Welding of Light Metals, Tokyo, Japan, 1971 (in Japanese).35. D’Annessa, A. T., Weld. J., 45: 569s, 1966.36. D’Annessa, A. T., Weld. J., 49: 41s, 1970.37. D’Annessa, A. T., Weld. J., 46: 491s, 1967.38. Savage, W. F., and Szekeres, E. S., Weld. J., 46: 94s, 1967.39. Savage, W. F., Nippes, E. F., and Szekeres, E. S., Weld. J., 55: 260s, 1976.40. Duvall, D. S., and Owczarski, W. A., Weld. J., 47: 115s, 1968.41. Kadalainen, L. P., Z. Metallkde., 70: 686, 1979.42. Doody, T., Weld. J., 61: 55, 1992.43. Omar, A. A., Weld. J., 67: 86s, 1998.44. Lippold, J. C., and Savage, W. F., Weld. J., 59: 48s, 1980.45. Baeslack, W. A. III, Lippold, J. C., and Savage, W. F., Weld. J., 58: 168s, 1979.46. Ornath, F., Soudry, J., Weiss, B. Z., and Minkoff, I., Weld. J., 60: 227s, 1991.47. Albert, S. K., Gills,T. P. S.,Tyagi,A. K., Mannan, S. L., Kulkarni, S. D., and Rodriguez, P., Weld. J., 66: 135s, 1997.48. Linnert, G. E., Welding Metallurgy, Vol. 2. American Welding Society, Miami, FL, 1967.49. Savage, W. F., Nippes, E. F., and Szekeres, E. S., Weld. J., 55: 276s, 1976.50. Takalo, T., and Moisio, T., IIW Annual Assembly, Tel Aviv, 1975.51. Matsuda, F., Ushio, M., Nakagawa, H., and Nakata, K., in Proceedings of the Conference on Arc Physics and Weld Pool Behavior, Vol. 1, Welding Institute, Arbington Hall, Cambridge, 1980, p. 337.52. Seretsky, J., and Ryba, E. R., Weld. J., 55, 208s, 1976.53. Liu, P. S., Baeslack III, W. A., and Hurley, J., Weld. J., 73: 175s, 1994.54. Metzger, G. E., Weld. J., 71: 297s, 1992.55. Estes, C. L., and Turner, P. W., Weld. J., 43: 541s, 1964.FURTHER READING1. Davies, G. J., Solidiﬁcation and Casting, Wiley, New York, 1973.2. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20: 83, 1975.3. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.4. Savage, W. F., Weld. World, 18: 89, 1980.PROBLEMS10.1 With the help of Schaefﬂer’s diagram, show that martensite can form in the fusion zone at 70 mm from the fusion boundary of the weld shown in Figure 10.11.
262 WELD METAL CHEMICAL INHOMOGENEITIES10.2 Butt welding of 5052 aluminum (Al–2.5Mg) with a single-V joint is carried out with 5556 ﬁller (Al–5.1Mg). The dilution ratio of the ﬁrst pass is 80%. In the second pass 40% of the material comes from the ﬁller wire, 40% from the base metal, and 20% from the ﬁrst pass. Calculate the compositions of the two passes, assuming uniform mixing in both.10.3 Suppose that in the previous problem the workpiece composition is Fe–25Cr–20Ni and the ﬁller composition is Fe–20Cr–10Ni. What is the difference in the ferrite content between the two passes based on Schaefﬂer’s diagram.10.4 Consider the pseudo-binary-phase diagram shown in Figure 10.3a. Sketch the Ni and Cr concentration proﬁles across a dendrite arm for an alloy that has a composition just to the left of point b.10.5 Consider welding Ni to Ti. Can macrosegregation occur in LBW? Why or why not? Is the chance of macrosegregation higher or lower in GTAW than in LBW?10.6 Explain why gas porosity can be severe in the GTAW of powder met- allurgy alloy Al–10Fe–5Ce (Figure 10.16a). Explain why gas porosity can be signiﬁcantly less with DCEN than with AC.10.7 Consider banding in the YAG laser weld of 304 stainless steel (Figure 10.6). What could have caused banding in this weld? Is the growth rate higher during dendritic or planarlike solidiﬁcation and why?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-411 Weld MetalSolidiﬁcation CrackingSolidiﬁcation cracking in the weld metal will be described, the metallurgicaland mechanical factors affecting the crack susceptibility will be discussed, andthe methods for reducing cracking will be presented.11.1 CHARACTERISTICS, CAUSE, AND TESTING11.1.1 Intergranular CrackingSolidiﬁcation cracking, which is observed frequently in castings and ingots, canalso occur in fusion welding, as shown in Figure 11.1. Such cracking, as shownin Figure 11.2, is intergranular, that is, along the grain boundaries of the weldmetal (1). It occurs during the terminal stage of solidiﬁcation, when the tensilestresses developed across the adjacent grains exceed the strength of the almostcompletely solidiﬁed weld metal (2–4). The solidifying weld metal tends tocontract because of both solidiﬁcation shrinkage and thermal contraction. Thesurrounding base metal also tends to contract, but not as much, because it isneither melted nor heated as much on the average. Therefore, the contractionof the solidifying metal can be hindered by the base metal, especially if theworkpiece is constrained and cannot contract freely. Consequently, tensilestresses develop in the solidifying weld metal. The severity of such tensilestresses increases with both the degree of constraint and the thickness of theworkpiece. The various theories of solidiﬁcation cracking (4–7) are effectively identicaland embody the concept of the formation of a coherent interlocking solidnetwork that is separated by essentially continuous thin liquid ﬁlms and thusruptured by the tensile stresses (2). The fracture surface often reveals the den-dritic morphology of the solidifying weld metal, as shown in Figure 11.3 for308 stainless steel fractured under augmented strain during GTAW (8). If asufﬁcient amount of liquid metal is present near the cracks, it can “backﬁll”and “heal” the incipient cracks. The terminal stage of solidiﬁcation mentioned above refers to a fraction ofsolid, fS, close to 1, and not necessarily a temperature near the lower limit ofthe solidiﬁcation temperature range. Depending on how it varies with tem-perature in an alloy, fS can be close to 1 and an essentially coherent inter- 263
264 WELD METAL SOLIDIFICATION CRACKING Figure 11.1 Solidiﬁcation cracking in a gas–metal arc weld of 6061 aluminum.Figure 11.2 Solidiﬁcation cracking in an autogenous bead-on-plate weld of 7075aluminum (magniﬁcation 140¥). From Kou and Kanevsky (1).locking solid network can form even though the temperature is only slightlybelow the liquidus temperature. In fact, Matsuda et al. (9, 10) have reportedthat solidiﬁcation cracking occurs in some carbon and stainless steels at tem-peratures slightly below their liquidus temperatures.11.1.2 Susceptibility TestingA. Houldcroft Test This test, also called the ﬁshbone test, is shown inFigure 11.4 (11, 12). It is often used for evaluating the solidiﬁcation cracking
CHARACTERISTICS, CAUSE, AND TESTING 265Figure 11.3 SEM fracture surface of a 308 stainless steel weld fractured underaugmented strain during GTAW. Reprinted from Li and Messeler (8). Courtesy ofAmerican Welding Society.Figure 11.4 Houldcroft test: (a) design (11); (b) cracking in an aluminum alloyspecimen. Reprinted from Liptax and Baysinger (12). Courtesy of American WeldingSociety.
266 WELD METAL SOLIDIFICATION CRACKING (a) (b) (c)Figure 11.5 Three types of specimens cracking under tension: (a) uniform width alongcrack; (b) decreasing width along crack; (c) uniform width along crack but slotted.susceptibility of sheet gage materials. The crack length from the startingedge of the test specimen is used to indicate the susceptibility to cracking(11–14). The specimen is free from constraints and a progression of slots of vary-ing depth allows the dissipation of stresses within it. In such a test, solidi-ﬁcation cracking initiates from the starting edge of the test specimen andpropagates along its centerline. As the heat source moves inward from thestarting edge of the test specimen, solidiﬁcation begins and the solidifyingstructure is torn apart because the starting edge continues to expand as a resultof continued heat input to the specimen. The reason for using the slots isexplained with the help of specimens cracking under tension, as shownin Figure 11.5. The crack may run all the way through the entire length ofthe specimen (Figure 11.5a). Reducing the width of the specimen can reducethe amount of stress along the length and bring the crack to a stop (Figure11.5b). In order not to dramatically change the heat ﬂow condition alongthe length of the weld, however, the material next to the slots is not cut off(Figure 11.5c).B. Varestraint Test This test was developed by Savage and Lundin (15). Asshown in Figure 11.6a, an augmented strain is applied to the test specimen(usually 12.7 mm thick) by bending it to a controlled radius at an appropriatemoment during welding (15). Both the amount of the applied strain and thecrack length (either the total length of all cracks or the maximum crack length)serve as an index of cracking sensitivity. The specimen can also be bent trans-verse to the welding direction, that is, the transverse Varestraint test, as shownin Figure 11.6b (16). This may promote cracking inside the weld metal morethan that outside. Figure 11.6c shows the cracking pattern observed in a Vare-straint test specimen of a 444 Nb-stabilized ferritic stainless (17). Figure 11.7compares the solidiﬁcation cracking susceptibility of several materials by Vare-straint testing (18). Other methods have also been used for testing the solidiﬁcation crackingsusceptibility of weld metals (19, 20), including the circular patch test (21–23)and Sigamajig test (24).
(c)Figure 11.6 Solidiﬁcation cracking tests: (a) Varestraint (15); (b) transverseVarestraint (16); (c) cracking in a ferritic stainless steel Varestraint specimen (17).(c) Reprinted from Krysiak et al. (17), courtesy of ASM International. 3.0 Maximum crack length, mm 2.5 HR-160 2.0 IN718 1.5 1.0 310SS 0.5 304SS 0 0 1 2 3 4 5 Applied strain, %Figure 11.7 Varestraint test results showing solidiﬁcation cracking susceptibility ofseveral different materials. Reprinted from DuPont et al. (18). Courtesy of AmericanWelding Society.
268 WELD METAL SOLIDIFICATION CRACKING11.2 METALLURGICAL FACTORSMetallurgical factors that have been known to affect the solidiﬁcation crack-ing susceptibility of weld metals include (i) the solidiﬁcation temperaturerange, (ii) the amount and distribution of liquid at the terminal stage of solid-iﬁcation, (iii) the primary solidiﬁcation phase, (iv) the surface tension of thegrain boundary liquid, and (v) the grain structure. All these factors are directlyor indirectly affected by the weld metal composition. The ﬁrst two factors areaffected by microsegregation during solidiﬁcation. Microsegregation in turncan be affected by the cooling rate during solidiﬁcation. In fact, in austeniticstainless steels the primary solidiﬁcation phase can also be affected by thecooling rate. These metallurgical factors will be discussed in what follows.11.2.1 Solidiﬁcation Temperature RangeGenerally speaking, the wider the solidiﬁcation (freezing) temperature range,the larger the (S + L) region in the weld metal or the mushy zone and thusthe larger the area that is weak and susceptible to solidiﬁcation cracking. Thesolidiﬁcation temperature range of an alloy increases as a result of either thepresence of undesirable impurities such as sulfur (S) and phosphorus (P) insteels and nickel-base alloys or intentionally added alloying elements.A. Effect of S and P Impurities such as S and P are known to cause severesolidiﬁcation cracking in carbon and low-alloy steels even at relatively lowconcentrations. They have a strong tendency to segregate at grain boundaries(25) and form low-melting-point compounds (FeS in the case of S), thus widen-ing the solidiﬁcation temperature range. In addition, S and P can cause severesolidiﬁcation cracking in nickel-base alloys (26–28) and ferritic stainless steels(29). In the case of austenitic stainless steels, their detrimental effect on solidi-ﬁcation cracking can be signiﬁcantly affected by the primary solidiﬁcationphase, as will be discussed subsequently. Figure 11.8 shows the effect of various elements, including S and P, on thesolidiﬁcation temperature range of carbon and low-alloy steels (30). As shown,S and P tend to widen the solidiﬁcation temperature range of steels tremen-dously. The wider the solidiﬁcation temperature range, the more grain bound-ary area in the weld metal remains liquid during welding and hence susceptibleto solidiﬁcation cracking, as depicted in Figure 11.9.B. Effect of Reactions during Terminal Solidiﬁcation Reactions, especiallyeutectic reactions, can often occur during the terminal stage of solidiﬁcationand extend the solidiﬁcation temperature range, for instance, in aluminumalloys and superalloys. Dupont et al. (31–35) studied the effect of eutectic reactions on thesolidiﬁcation temperature range and solidiﬁcation cracking. The materialsstudied include some superalloys and stainless steels containing niobium (Nb).
METALLURGICAL FACTORS 269 300 P Freezing range,oC 200 S C 100 B Si 0 0 5 10 Weight %Figure 11.8 Effect of alloying elements on the solidiﬁcation temperature rangeof carbon and low-alloy steels. Modiﬁed from Principles and Technology of the FusionWelding of Metals (30). Pool (L) Weld (S) (a) no grain boundary (GB) liquid GB pure Fe: zero freezing L S temperature range; (b) GB not susceptible grain boundary liquid Fe with silicon: narrow GB freezing temperature (c) L S range; somewhat GB susceptible grain boundary liquid GB Fe with sulfur: wide (d) L S freezing temperature GB range; highly susceptibleFigure 11.9 Effect of impurities on grain boundary liquid of weld metal: (a) weldmetal near pool; (b) no liquid in pure Fe; (c) some liquid with a small amount of Si;(d) much more liquid with a small amount of sulfur.Figure 11.10 shows the weld metal microstructure of a Nb-bearing superalloy(34). Two eutectic-type constituents are present in the microstructure, g-NbCand g-Laves. The liquid solidiﬁes as the primary g and two eutectic reactionsoccur during the terminal stage of solidiﬁcation, ﬁrst L Æ g + NbC and thenL Æ g + Laves. The second eutectic reaction, when it occurs, takes place at aconsiderably lower temperature than the ﬁrst, thus extending the solidiﬁcation
270 WELD METAL SOLIDIFICATION CRACKINGFigure 11.10 Scanning electron micrographs showing weld metal microstructure of aNb-bearing superalloy. Reprinted from DuPont et al. (34). Maximum crack length, mm 3.0 Experimental superalloys 2.5 HR-160 IN718 2.0 1.5 1.0 0.5 0 0 50 100 150 200 250 300 o Solidification temperature range, CFigure 11.11 Maximum crack length as a function of solidiﬁcation temperature rangefor Nb-bearing superalloys and two other materials. Reprinted from DuPont et al. (18).Courtesy of American Welding Society.temperature range signiﬁcantly. For the alloy shown in Figure 11.10, forinstance, solidiﬁcation starts at 1385.6°C (liquidus temperature), L Æ g + NbCtakes place at 1355.2°C and L Æ g + Laves at a considerably lower tempera-ture, 1248.2°C (31). The solidiﬁcation temperature range is 137.4°C. As shownin Figure 11.11, the maximum crack length in Varestraint testing increases withincreasing solidiﬁcation temperature range (17). Before leaving the subject of eutectic reactions, two stainless steel weldswill be used here to illustrate the two eutectic reactions along the solidiﬁca-tion path (35). The ﬁrst weld, containing 0.48 wt % Nb and 0.010 wt % C, is an
METALLURGICAL FACTORS 271 0.25 0.25 Liquid composition, wt% C 20Cb-3 NbC 20Cb-3/ NbC INCO 112 0.20 γ 0.20 fL=0.005 0.15 0.15 γ fL=0.01 fL=0 0.10 0.10 fL=1 0.05 0.05 fL=0.008 fL=1 Laves Laves fL=0 0 0 0 5 10 15 20 25 30 0 5 10 15 20 25 30 (a) Liquid composition, wt% Nb (b)Figure 11.12 Solidiﬁcation paths (solid lines) of Nb-stabilized austenitic stainlesssteels: (a) 20Cb-3; (b) 20Cb-3–INCO 112 composite. Reprinted from DuPont (35).Courtesy of American Welding Society.autogenous gas–tungsten arc weld of a Nb-stabilized austenitic stainless steel20Cb-3. To increase the Nb content, a relatively large composite weld wasmade in alloy 20Cb-3 with an INCO 112 ﬁller wire containing 3.81 wt % Nband then machined ﬂat at the top surface for further welding. The second weld,containing 2.20 wt % Nb and 0.014 wt % C, is an autogenous gas–tungsten arcweld within the 20Cb-3–INCO 112 composite weld. The solidiﬁcation paths of the two welds are shown in Figures 11.12. Asmentioned previously in Chapter 6, the arrows in the solidiﬁcation path indi-cate the directions in which the liquid composition changes as temperaturedecreases. Here, solidiﬁcation of the 20Cb-3 weld initiates by a primary L Æg reaction, as shown in Figure 11.12a. Because of the relatively high C–Nb ratioof the alloy, the interdendritic liquid becomes enriched in C until the g/NbCtwofold saturation line is reached. Here, the L Æ g + NbC reaction takes over.However, since the fraction of liquid is already very small ( fL = 0.005), solidi-ﬁcation is soon over ( fL = 0) at about 1300°C before the L Æ g + Laves reac-tion takes place. In contrast, the lower C–Nb ratio of the 20Cb-3–INCO 112composite weld caused the interdendritic liquid to become more highlyenriched in Nb as shown in Figure 11.12b. The solidiﬁcation path barely inter-sects the g/NbC twofold saturation line (fL = 0.01) before it reaches the g/Lavestwofold saturation line ( fL = 0.008). The L Æ g + NbC reaction takes onlybrieﬂy, and the L Æ g + Laves reaction takes over until solidiﬁcation is com-plete (fL = 0) at about 1223°C, which is signiﬁcantly lower than 1300°C.11.2.2 Amount and Distribution of Liquid during Terminal SolidiﬁcationA. Amount of Liquid Figures 11.13a–d show the effect of composition onthe solidiﬁcation cracking sensitivity of several aluminum alloys (36–41).Figure 11.13e shows the crack sensitivity in pulsed laser welding of Al–Cu
272 WELD METAL SOLIDIFICATION CRACKING (a) Al-Si (Singer et al. 1947) 0 Relative crack sensitivity (b) Al-Cu (Pumphrey et al. 1948 ) Total crack length (mm) 0 30 (c) Al-Mg (Dowd, 1952) 20 0 10 (d) Al-Mg 2Si (e) Al-Cu (Jennings et al. 1948) (Michaud et al. 1995) 0 0 1 2 3 4 5 6 7 8 0 Copper content (wt%) 0 1 2 3 4 5 6 7 8 Composition of weld, % alloying elementFigure 11.13 Effect of composition on crack sensitivity of some aluminum alloys.(a–d) From Dudas and Collins (40). (e) Reprinted from Michaud et al. (41).Figure 11.14 Aluminum welds with three different levels of Cu: (a) almost no Cu; (b)4% Cu; (c) 8% Cu.alloys (41). Figure 11.14a shows an aluminum weld with little Cu (alloy 1100gas–metal arc welded with ﬁller 1100), and there is no evidence of cracking.Figure 11.14b shows a crack in an aluminum weld with about 4% Cu (alloy2219 gas–metal arc welded with ﬁller 1100). Figure 11.14c shows a crack healedby the eutectic liquid in an aluminum weld with about 8% Cu (alloy 2219gas–metal arc welded with ﬁller 2319 plus extra Cu).
METALLURGICAL FACTORS 273 susceptibility II (b) crack Pool (L) Weld (S) III I IV (a) solute content I. pure metal: no grain II: some solute: just enough boundary (GB) liquid; not liquid to form a continuous susceptible to cracking GB film; most susceptible S L L GB (d) S (c) III. more solute: more GB IV. much more solute: much liquid to heal cracks; less GB liquid to heal cracks and susceptible to cracking less rigid dendritic structure; least susceptible to cracking L L (e) (f)Figure 11.15 Effect of composition on crack susceptibility: (a) weld; (b) crack sus-ceptibility curve; (c) pure metal; (d) low solute; (e) more solute; ( f) much more solute. As shown in Figure 11.13, the maximum crack sensitivity occurs somewherebetween pure aluminum and highly alloyed aluminum (say no less than 6 wt% solute). The presence of a maximum in the crack susceptibility compositioncurve (Figure 11.13) is explained qualitatively with the help of Figure 11.15.Pure aluminum is not susceptible to solidiﬁcation cracking because there is nolow-melting-point eutectic present at the grain boundary to cause solidiﬁca-tion cracking. In highly alloyed aluminum, on the other hand, the eutecticliquid between grains can be abundant enough to “heal” incipient cracks (3).Somewhere in between these two composition levels, however, the amount ofliquid between grains can be just large enough to form a thin, continuous grainboundary ﬁlm to make the materials rather susceptible to solidiﬁcation crack-ing but without extra liquid for healing cracks. A ﬁne equiaxed dendritic struc-ture with abundant liquid between grains (Figure 11.15f) can deform moreeasily under stresses than a coarse columnar dendritic structure (Figure11.15e) and thus has a lower susceptibility to cracking.B. Calculation of Fraction Liquid Dupont et al. (31–35) calculated thefraction of the liquid ( fL) as a function of distance (x) within the mushy zonein Nb-bearing superalloys and austenitic stainless steels. The fL–x curve pro-vides the quantitative information for the amount and distribution of inter-dendritic liquid in the mushy zone. The two stainless steel welds discussedpreviously will be considered here, namely, the weld in alloy 20Cb-3 and the
274 WELD METAL SOLIDIFICATION CRACKINGweld in the 20Cb-3–INCO 112 composite weld. According to DuPont et al.(35), Nb, Si, and C are treated as solutes in these alloys and, as an approxi-mation, the remaining elements in the solid solution with g are treated as the“g-solvent.” Assume that the slopes of the liquidus surface with respect to Nb, Si, andC, that is, mL,Nb, mL,Si, and mL,C, respectively, are constant. Equation (6.2) canbe extended to ﬁnd the temperature of a liquid on the liquidus surface T asfollows: T = Tm + mL,NbCL,Nb + mL,SiCL,Si + mL,CCL,C (11.1) Assuming negligible solid diffusion but complete liquid diffusion for Nband Si, the following equations can be written based on the Scheil equation[Equation (6.9)]: C L,Nb = C0,Nb fLkNb -1) ( (11.2) C L,Si = C0,Si fLkSi -1) ( (11.3)Since diffusion in solid and liquid is fast for a small interstitial solute such asC, the following equation can be written based on the equilibrium lever rule[Equation (6.6)]: C0,C C L,C = (11.4) fL + kC (1 - fL )Note that the equilibrium partition ratios kNb, kSi, ans kC have been assumedconstant in Equations (11.2)–(11.4) for simplicity. Inserting these equationsinto Equation (11.1) yields the following relationship between temperatureand fraction liquid: Ê C0 ,C ˆ T = Tm + mL,NbC0,Nb fLkNb -1) + mL,SiC0,Si fLkSi -1) + mL,C ( ( (11.5) Ë fL + kC (1 - fL ) ¯ The cooling rate (e or GR) can be determined from the secondary dendritespacing (d). According to Equation (6.20), -n -n d = at n = b(e ) f = b(GR) (11.6)For instance, from the dendrite arm spacing of the weld metal the cooling rateGR is about 250°C/s. The growth rate at the weld centerline R is the weldingspeed 3 mm/s. As such, the temperature gradient G is about 83°C/mm. Assuming that G is constant in the mushy zone and taking x = 0 at theliquidus temperature of the alloy TL,
METALLURGICAL FACTORS 275 1.0 0.10 20Cb-3/INCO 112 0.8 0.08 Fraction liquid 20Cb-3 0.6 20Cb-3/INCO 112 0.06 0.4 0.04 20Cb-3 γ L 0.2 0.02 L γ 0 0 0 1.0 2.0 3.0 4.0 0 1.0 2.0 3.0 4.0 (a) Distance along centerline, mm (b)Figure 11.16 Fraction liquid as a function of distance within the mushy zone of20Cb-3 and 20Cb-3–INCO 112 composite (a) and enlarged (b). Reprinted fromDuPont (35). Courtesy of American Welding Society. TL - T x= (11.7) Gwhich can be used to ﬁnd the temperature T at any distance x. Equations (11.5) and (11.7) can be combined to determine how the liquidfraction fL varies with distance x within the mushy zone, and the results areshown in Figure 11.16. The liquid fraction drops rapidly with distance near thepool boundary but slowly further into the mushy zone. Also, the mushy zoneis signiﬁcantly wider in the 20Cb-3–INCO 112 composite weld than in the20Cb-3 weld due to the signiﬁcantly larger solidiﬁcation temperature range ofthe former. This explains why the former is more susceptible to solidiﬁcationcracking.C. Liquid Distribution As shown previously in Figure 11.11 for Nb-bearingsuperalloys, the alloys with a narrower solidiﬁcation temperature range areless susceptible to solidiﬁcation cracking. In fact, some of these alloys have awide solidiﬁcation temperature range just like the more susceptible alloys. Asin the more crack-susceptible alloys, the L Æ g + Laves reaction follows the LÆ g + NbC reaction during the terminal stage of solidiﬁcation. However, asshown in Figure 11.17 for one of these less susceptible alloys, the amount ofterminal liquid undergoing the L Æ g + Laves reaction in these alloys is smalland remains isolated. This type of morphology, unlike the continuous grainboundary liquid undergoing the L Æ g + Laves reaction in the more crack-susceptible alloys, should be more resistant to crack propagation throughoutthe mushy zone. Since an isolated L Æ g + Laves reaction does not reallycontribute to solidiﬁcation cracking, it should not have to be included in thesolidiﬁcation temperature range, and the lower bound of the effective solidi-ﬁcation temperature range should more accurately be represented by the LÆ g + NbC reaction (31, 34).
276 WELD METAL SOLIDIFICATION CRACKINGFigure 11.17 Scanning electron micrographs showing morphology of g-NbC and g-Laves constituents in solidiﬁcation cracks of a Nb-bearing superalloy. Reprinted fromDuPont et al. (34).11.2.3 Ductility of Solidifying Weld MetalThe less ductile a solidifying weld metal is, the more likely it will crack duringsolidiﬁcation. Nakata and Matsuda (16) used the transverse Varestraint test(Figure 11.6b) to determine the so-called ductility curve, as illustrated in Figure11.18. At any given strain the ductility curve ranges from the liquidus tem-perature TL to the temperature at the tip of the longest crack. To construct thecurve, a strain of e1 is applied during welding, and the maximum crack lengthis examined after welding (Figure 11.18a). From the temperature distribution
METALLURGICAL FACTORS 277 region of low ductility weld welding pool direction (a) TL Distance tip of longest crack induced by applying strain ε 1 Temperature brittle temperature range (BTR) (b) Strain, ε ductility curve region of low ductility ε1 slope = critical strain rate for ε min temperature drop (CST) TL T1 Temperature BTR 1 CST2 < CST1 : alloy 2 more Strain, ε susceptible to cracking than alloy 1 BTR2 CST1 ε min1 (c) CST2 εmin2 T L1 T L2 Temperature Relative cracking ratio, % 100 A7N01 A2017 A2219 GTAW crater weld test (d) 50 A5083 A5052 A1100(3.75) 0 0 1 2 CST (x 10 -4/ oC)Figure 11.18 Ductility of solidifying weld metal: (a) temperature distribution (tem-perature increases from right to left); (b) ductility curve; (c) ductility curves with dif-ferent crack susceptibility; (d) effect of CST on cracking. (d) From Nakata and Matsuda(16).
278 WELD METAL SOLIDIFICATION CRACKINGalong the weld centerline measured with a thermocouple during welding, thetemperature T1 at the tip of the longest crack and hence the point (T1, e1) canbe determined (Figure 11.18b). By repeating the experiment for variousapplied strains and ﬁnding the corresponding crack tip temperatures, the duc-tility curve can be determined. The maximum crack length and hence the tem-perature range of the ductility curve ﬁrst increase with increasing appliedstrain but then level off as the applied strain increases further. The widest tem-perature range covered by the ductility curve is called the brittle temperaturerange (BTR). The weld metal is “brittle” in the sense that it is much less ductilein this temperature range than either the weld pool or the completely solidi-ﬁed weld metal. The minimum strain required to cause cracking is called emin.The slope of the tangent to the ductility curve is called the critical strain ratefor temperature drop (CST), that is, the critical rate at which the strain varieswith temperature drop. In general, the lower emin, the greater BTR or the smaller CST is, the greaterthe susceptibility to solidiﬁcation cracking (Figure 11.18c). According toNakata and Matsuda (16), CST best correlates with the cracking susceptibil-ity of the weld metal (Figure 11.18d). It should be pointed out, however, thatthe values of CST in Figure 11.18d were not determined exactly as describedabove. Because the emin values were too small to be determined, a slow-bendingtransverse Varestraint test had to be used to modify the ductility curve. For a given material cracking can be avoided if the strain rate for temper-ature drop can be kept below the critical value, that is, if -de/dT < CTS. Math-ematically, -de/dT = (∂e/∂t)/(-∂T/∂t), where t is time. The strain rate (∂e/∂t)consists of both the self-induced tensile strain in the solidifying weld metalwhose contraction is hindered by the adjacent base metal and the augmentedstrain if it is applied. -∂T/∂t is the cooling rate, for instance, 150°C/s. InVarestraint testing an augmented strain is applied essentially instantaneously,and the high ∂e/∂t and hence -de/dT easily cause cracking. If the augmentedstrain were applied very slowly on a solidifying weld metal whose self-inducedstrain rate during solidiﬁcation is low, ∂e/∂t can be small enough to keep -de/dT below the CST, and the weld metal can solidify without cracking. Crack-ing can also be avoided if the cooling rate -∂T/∂t is increased dramatically toreduce -de/dT to below the CST. Yang et al. (42) avoided solidiﬁcation crack-ing in GTAW of 2024 aluminum sheets by directing liquid nitrogen behind theweld pool to increase the cooling rate. They also showed, with ﬁnite-elementmodeling of heat ﬂow and thermal stresses, that the condition -de/dT < CTScan be achieved by cooling the area right behind the weld pool. Before leaving the subject of the ductility curve, the relationship betweenthe BTR and the solidiﬁcation temperature range needs to be discussed.Nakata and Matsuda (16) observed in aluminum alloys such as alloys 2017,2024, and 2219 that the cooling curve showed a clear solidiﬁcation tempera-ture range. A distinct point of arrest (a short ﬂat region) in the curve corre-sponding to the formation of eutectics was observed as well as a discontinuityat the liquidus temperature corresponding to the formation of the aluminum-
METALLURGICAL FACTORS 279rich solid. For these alloys the BTR was found to be the same as the solidiﬁ-cation temperature range, that is, TL to TE. In other words, the region of lowductility behind the weld pool corresponds to the mushy zone discussed in pre-vious chapters. On the other hand, for aluminum alloys such as alloys 5052,5083, and 6061, the cooling curve did not show a distinct point of arrest, andthe inﬂection point in the curve had to be taken as the “nominal” solidus tem-perature TS. For these alloys the BTR was found signiﬁcantly (about 20%)larger than the nominal solidiﬁcation temperature range of TL to TS and wasthus a more realistic representation of the nonequilibrium solidiﬁcation tem-perature range of TL to TE. Presumably, eutectics still formed below TS but notin quantities enough to show a distinct point of arrest in the cooling curve. Itis not clear if differential thermal analysis was tried, which is known to detecteutectic temperatures well. In the case of steels and stainless steels, the solidiﬁcation temperature rangeis relatively narrow, and impurities such as P and S are found to enlarge theBTR, presumably by forming eutectics with a low melting point (16).11.2.4 Primary Solidiﬁcation PhaseFor austenitic stainless steels the susceptibility to solidiﬁcation cracking ismuch lower when the primary solidiﬁcation phase is d-ferrite rather thanaustenite (43–45). As the ratio of the Cr equivalent to the Ni equivalentincreases, the primary solidiﬁcation phase changes from austenite to d-ferrite,and cracking is reduced. As shown by Takalo et al. (44) in Figure 11.19a forarc welding, this change occurs at Creq/Nieq = 1.5. Similarly, as shown by Lienert(45) in Figure 11.19b for pulsed laser welding, this change occurs in theCreq/Nieq range of 1.6–1.7. In both cases Creq = Cr + 1.37Mo + 1.5Si + 2Nb +3Ti and Nieq = Ni + 0.3Mn + 22C + 14.2N + Cu. As discussed previously(Chapter 9), under high cooling rates in laser or electron beam welding, a weldmetal that normally solidiﬁes as primary ferrite can solidify as primary austen-ite because of undercooling, and this is consistent with the change occurringat a higher Creq–Nieq ratio in pulsed laser welding. In general, austenitic stainless steels containing 5–10% d-ferrite are signiﬁ-cantly more resistant to solidiﬁcation cracking than fully austenitic stainlesssteels (46). As mentioned previously in Chapter 9, ferrite contents signiﬁcantlygreater than 10% are usually not recommended, for the corrosion resistancewill be too low (47–50). Furthermore, upon exposure to elevated temperatures(600–850°C), d-ferrite can transform to brittle s-ferrite and impair the me-chanical properties of austenitic stainless steels, unless the ferrite contentis kept low (51). It is generally believed that, since harmful impurities such as sulfur andphosphorus are more soluble in d-ferrite than in austenite (see Table 11.1), theconcentration of these impurities at the austenite grain boundaries, and thustheir damaging effect on solidiﬁcation cracking, can be reduced if d-ferrite ispresent in signiﬁcant amounts (43, 52, 53). In addition, it is also believed that
280 WELD METAL SOLIDIFICATION CRACKING primary austenite primary ferrite susceptible 0.20 somewhat susceptible Total S+P (wt %) not susceptible 0.16 0.12 (a) cracking no cracking 0.08 0.04 0 1.0 1.2 1.4 1.6 1.8 2.0 Cr eq/Nieq 0.08 mixed 0.07 primary primary austenite ferrite 0.06 Total S+P+B (wt %) 0.05 cracking no cracking 0.04 (b) 0.03 0.02 pulsed 0.01 Nd:YAG laser welds 0.00 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 2.0 Cr eq/NieqFigure 11.19 Solidiﬁcation crack susceptibility of austenitic stainless steels:(a) arc welds; (b) laser welds. (a) From Takalo et al. (44). (b) Reprinted fromLienert (45). TABLE 11.1 Solubility of Sulfur and Phosphorus in Ferrite and Austenite (wt %) In d-Ferrite In Austenite Sulfure 0.18 0.05 Phosphorus 2.8 0.25 Source: Borland and Younger (52).
METALLURGICAL FACTORS 281 Figure 11.20 Iron–carbon phase diagram.when d-ferrite is the primary solidiﬁcation phase, the substantial boundaryarea between d-ferrite and austenite acts as a sink for sulfur and phosphorus.This decreases the concentration of such impurities at the austenite grainboundaries and, therefore, reduces solidiﬁcation cracking (43, 54–57). Hull(46) suggests that the propagation of solidiﬁcation cracks in cast austeniticstainless steels is halted by d-ferrite due to the fact that the ferrite–austeniteinterface energy is lower than the austenite–austenite interface energy (58,59). Solidiﬁcation cracks stopped by d-ferrite have also been observed in 309stainless steel welds by Brooks et al. (60). In addition to austenitic stainless steels, the primary solidiﬁcation phase canalso affect the solidiﬁcation cracking susceptibility of carbon steels. Accordingto the iron–carbon phase diagram shown in Figure 11.20, when the carboncontent is greater than 0.53, austenite becomes the primary solidiﬁcation phaseand solidiﬁcation cracking becomes more likely. In fact, the wider solidiﬁca-tion temperature range at a higher carbon content further increases the poten-tial for solidiﬁcation cracking.11.2.5 Surface Tension of Grain Boundary LiquidThe effect of the amount and distribution of the grain boundary liquid on thesolidiﬁcation cracking of weld metals has been described earlier in this section.The higher the surface tension of the grain boundary liquid, the larger its dihe-dral angle is. Figures 11.21a and b show the dihedral angle and distribution ofthe grain boundary liquid (61). Figure 11.21c shows the effect of the dihedralangle on the susceptibility to solidiﬁcation cracking in several aluminum alloysevaluated in autogenous spot GTAW (16). As shown, except for alloy 1100,which is essentially pure aluminum and thus not susceptible to cracking, the
282 WELD METAL SOLIDIFICATION CRACKING grain θ boundary GB (GB) (a) liquid θ = 120 o θ = 60 o θ = 0o GB liquid (b) 100 A7N01 Relative cracking ratio, % A2017 A2219 GTAW crater weld test 50 (c) A5052 A5083 A1100 0 0 20 40 60 80 Dihedral angle θ , degreeFigure 11.21 Grain boundary liquid: (a) dihedral angle; (b) distribution of liquid atgrain boundary; (c) effect of dihedral angle on solidiﬁcation cracking. (c) From Nakataand Matsuda (16). Pool (L) Weld (S) (a) grain boundary liquid GB continuous grain L S boundary liquid; (b) GB highly susceptible grain boundary liquid GB isolated grain L S boundary liquid; (c) GB less susceptibleFigure 11.22 Effect of grain boundary liquid morphology on crack susceptibility: (a)weld; (b) continuous; (c) isolated.susceptibility decreases with increasing dihedral angle of the grain boundaryliquid. The effect of the surface tension of the grain boundary liquid on solidiﬁca-tion cracking is further depicted in Figure 11.22. If the surface tension betweenthe solid grains and the grain boundary liquid is very low, a liquid ﬁlm will
METALLURGICAL FACTORS 283 (a) (b)Figure 11.23 Effect of grain structure on solidiﬁcation cracking: (a) aluminum alloys;(b) centerline cracking in a coarse-grain 310 stainless steel weld. (a) From Nakata andMatsuda (16). (b) From Kou and Le (65).form between the grains and the solidiﬁcation cracking susceptibility is high.On the other hand, if the surface tension is high, the liquid phase will be glob-ular and will not wet the grain boundaries. Such discontinuous liquid globulesdo not signiﬁcantly reduce the strength of the solid network and, therefore,are not as harmful. For example, FeS forms ﬁlms at the grain boundaries ofsteels while MnS forms globules. Due to its globular morphology and highermelting point, MnS has been known to be far less harmful than FeS.11.2.6 Grain Structure of Weld MetalFine equiaxed grains are often less susceptible to solidiﬁcation cracking thancoarse columnar grains (16, 62–64), as shown in Figure 11.23a (16) for several
284 WELD METAL SOLIDIFICATION CRACKINGaluminum alloys. Alloy A1070 is not susceptible to solidiﬁcation crackingbecause it is essentially pure aluminum. Fine equiaxed grains can deform toaccommodate contraction strains more easily, that is, it is more ductile, thancolumnar grains. Liquid feeding and healing of incipient cracks can also bemore effective in ﬁne-grained material. In addition, the grain boundary areais much greater in ﬁne-grained material and, therefore, harmful low-melting-point segregates are less concentrated at the grain boundary. It is interesting to note that, due to the steep angle of abutment betweencolumnar grains growing from opposite sides of the weld pool, welds madewith a teardrop-shaped weld pool tend to be more susceptible to centerlinesolidiﬁcation cracking than welds made with an elliptical-shaped weld pool. Asteep angle seems to favor the head-on impingement of columnar grainsgrowing from opposite sides of the weld pool and the formation of the con-tinuous liquid ﬁlm of low-melting-point segregates at the weld centerline. Asa result, centerline solidiﬁcation cracking occurs under the inﬂuence of trans-verse contraction stresses. Centerline cracking is often observed in welding.Figure 11.23b is an example in an autogenous gas–tungsten arc weld of a 310stainless steel made with a teardrop-shaped weld pool (65).11.3 MECHANICAL FACTORS11.3.1 Contraction StressesSo far, the metallurgical factors of weld solidiﬁcation cracking have beendescribed. But without the presence of stresses acting on adjacent grainsduring solidiﬁcation, no cracking can occur. Such stresses, as already men-tioned, can be due to thermal contraction or solidiﬁcation shrinkage or both.Austenitic stainless steels have relatively high thermal expansion coefﬁcients(as compared with mild steels) and, therefore, are often prone to solidiﬁcationcracking. Aluminum alloys have both high thermal expansion coefﬁcients and highsolidiﬁcation shrinkage (5). As a result, solidiﬁcation cracking can be ratherserious in some aluminum alloys, especially those with wide solidiﬁcation tem-perature ranges.11.3.2 Degree of RestraintThe degree of restraint of the workpiece is another mechanical factor ofsolidiﬁcation cracking. For the same joint design and material, the greaterthe restraint of the workpiece, the more likely solidiﬁcation cracking willoccur. Figure 11.24 illustrates the effect of workpiece restraint on solidiﬁca-tion cracking (66). As shown, solidiﬁcation cracking occurred in the second(left-hand-side) weld of the inverse “T” joint due to the fact that the degree
REDUCING SOLIDIFICATION CRACKING 285Figure 11.24 Solidiﬁcation cracking in steel weld. Reprinted from Linnert (66). Cour-tesy of American Welding Society.of restraint increased signiﬁcantly after the ﬁrst (right-hand-side) weld wasmade.11.4 REDUCING SOLIDIFICATION CRACKING11.4.1 Control of Weld Metal CompositionWeld metals of crack-susceptible compositions should be avoided. In autoge-nous welding no ﬁller metal is used, and the weld metal composition is deter-mined by the base-metal composition. To avoid or reduce solidiﬁcationcracking, base metals of susceptible compositions should be avoided. When abase metal of a crack-susceptible composition has to be welded, however, aﬁller metal of a proper composition can be selected to adjust the weld metalcomposition to a less susceptible level.A. Aluminum Alloys According to Figure 11.13, an Al–3% Cu alloy can berather crack susceptible during welding. If the Cu content of the base metal israised to above 6%, solidiﬁcation cracking can be signiﬁcantly reduced. In fact,2219 aluminum, one of the most weldable Al–Cu alloys, contains 6.3% Cu.When a ﬁller metal is used, the weld metal composition is determined bythe composition of the base metal, the composition of the ﬁller metal, and thedilution ratio. The dilution ratio, as mentioned previously, is the ratio of theamount of the base metal melted to the total amount of the weld metal. Againusing Al–3% Cu as an example, the weld metal Cu content can be increasedby using 2319 ﬁller metal, which is essentially an Al–6.3% Cu alloy. If the jointdesign and heat input are such that the dilution ratio is low, the weld metalcopper content can be kept sufﬁciently high to avoid solidiﬁcation cracking.Figure 11.25 shows the approximate dilution in three typical joint designs (40).
286 WELD METAL SOLIDIFICATION CRACKING Figure 11.25 Approximate dilution of three weld joints by base metal in aluminum welding. Reprinted from Dudas and Collins (40). Courtesy of American Welding Society.TABLE 11.2 Guid to Choice of Filler Metals for Minimizing Solidiﬁcation Cracking inWelds of High-Strength Aluminum Alloys 7000 7000 6000 5000 2000Base Metals (Al–Zn–Mg–Cu) (Al–Zn–Mg) (Al–Mg–Si) (Al–Mg) (Al–Cu)2000 (Al–Cu) NRa NR NR NR 4043 4145 23195000 (Al–Mg) 5356 5356 5356 5356 —b 5556 5556 5556 5183 5183 51836000 (Al–Mg–Si) 5356 5356 4043 — — 5556 4643 5183 53567000 (Al–Zn–Mg) 5356 5356 — — — 55567000 (Al–Zn–Mg–Cu) 5356 — — — — 5556a NR, not recommend.b Charts that recommend ﬁller choice for many applications are available from ﬁller metal suppliers.Source: Dudas and Collins (40). Table 11.2 is a guide to choice of ﬁller metals for minimizing solidiﬁcation cracking in welds of high-strength aluminum alloys (40). Experimental data such as those in Figure 11.26 from solidiﬁcation cracking testing by ring casting can also be useful (67, 68).
REDUCING SOLIDIFICATION CRACKING 287Figure 11.26 Solidiﬁcation cracking susceptibility of aluminum alloys: (a) Al–Mg–Si;(b) Al–Cu–Si (c) Al–Mg–Cu. (a, b) Modiﬁed from Jennings et al. (67). (c) Modiﬁedfrom Pumphrey and Moore (68).
288 WELD METAL SOLIDIFICATION CRACKING Minor alloying elements have also been found to affect the solidiﬁcationcracking susceptibility of aluminum alloys. For example, the Fe–Si ratio hasbeen found to signiﬁcantly affect the solidiﬁcation cracking susceptibility of3004 and other Al–Mg alloys (69, 70); therefore, proper control of the contentof minor alloying elements can be important in some materials.B. Carbon and Low-Alloy Steels The weld metal manganese content cansigniﬁcantly affect solidiﬁcation cracking. It is often kept high enough toensure the formation of MnS rather than FeS. This, as described previously, isbecause the high melting point and the globular morphology of MnS tend torender sulfur less detrimental. Figure 11.27 shows the effect of the Mn–S ratioon the solidiﬁcation cracking tendency of carbon steels (71). At relatively lowcarbon levels the solidiﬁcation cracking tendency can be reduced by increas-ing the Mn–S ratio. However, at higher carbon levels (i.e., 0.2–0.3% C),increasing the Mn–S ratio is no longer effective (72). In such cases loweringthe weld metal carbon content, if permissible, is more effective. One way of lowering the weld metal carbon content is to use low-carbonelectrodes. In fact, in welding high-carbon steels one is often required to makethe ﬁrst bead (i.e., the root bead) with a low-carbon electrode. This is because,as shown in Figure 11.28, the ﬁrst bead tends to have a higher dilution ratioand a higher carbon content than subsequent beads (73). A high carboncontent is undesirable because it promotes not only the solidiﬁcation crack-ing of the weld metal but also the formation of brittle martensite and, hence,the postsolidiﬁcation cracking of the weld metal. Therefore, in welding steelsof very high carbon contents (e.g., greater than 1.0% C), extra steps should betaken to avoid introducing excessive amounts of carbon from the base metalinto the weld metal. As shown in Figure 11.29, one way to achieve this is to 50 Ratio of manganese to sulfur 40 Intermediate Zone 30 No Cracking 20 10 Cracking 0 0 0.10 0.12 0.14 0.16 Carbon content, %Figure 11.27 Effect of Mn–S ratio and carbon content on solidiﬁcation cracking sus-ceptibility of carbon steel weld metal. Reprinted from Smith (71).
REDUCING SOLIDIFICATION CRACKING 289Figure 11.28 Schematic sketch of multipass welding. Note that the root pass has thehighest dilution ratio. From Jefferson and Woods (73).Figure 11.29 Buttering the groove faces of very high carbon steel with a 310 stainlesswire steel before welding. From Jefferson and Woods (73).“butter” the groove faces of the base metal with austenitic stainless steel (suchas 25–20 stainless) electrodes before welding (73). In welding cast irons, purenickel electrodes have also been used for buttering. In any case, the surfacelayers remain in the ductile austenitic state, and the weld can then be com-pleted either with stainless electrodes or with other cheaper electrodes.C. Nb-Bearing Stainless Steels and Superalloys The C–Nb ratio of the weldmetal can affect the susceptibility to solidiﬁcation cracking signiﬁcantly (17,31–35). A high C–Nb ratio can reduce solidiﬁcation cracking by avoiding thelow-temperature L Æ g + Laves reaction, which can widen the solidiﬁcationtemperature range.D. Austenitic Stainless Steels As mentioned previously, it is desirable tomaintain the weld ferrite content at a level of 5–10% in order to obtain soundwelds. The quantitative relationship between the weld ferrite content and theweld metal composition in austenitic stainless steels has been determined bySchaefﬂer (74), DeLong (75), Kotecki (76, 77), Balmforth and Lippold (78),and Vitek et al. (79, 80). These constitution diagrams have been shown previ-ously in Chapter 9. Alloying elements are grouped into ferrite formers (Cr,Mo, Si, and Cb) and austenite formers (Ni, C, and Mn) in order to determinethe corresponding chromium and nickel equivalents for a given alloy.Example: Consider the welding of a 1010 steel to a 304 stainless steel. Forconvenience, let us assume the dilution ratio is 30%, half from 304 stainlesssteel and half from 1010 steel, as shown in Figure 11.30. Estimate the ferritecontent and the solidiﬁcation cracking susceptibility of a weld made with atype 310 electrode that contains 0.12% carbon and a weld made with a type309 ELC (extra low carbon) electrode that contains 0.03% carbon. For the weld made with the 310 stainless steel electrode, the weld metalcomposition can be calculated as follows:
290 WELD METAL SOLIDIFICATION CRACKING Figure 11.30 Welding 304 stainless steel to 1010 carbon steel.Element Electrode ¥70% Type 304 ¥15% 1010 Steel ¥15% Weld MetalCr 26.0 18.2 18.0 2.7 0 0 20.9Ni 21.0 14.7 8.0 1.2 0 0 15.9C 0.12 0.084 0.05 0.0075 0.10 0.015 0.1065Mn 1.75 1.23 2.0 0.30 0.4 0.06 1.59Si 0.4 0.28 — — 0.2 0.03 0.31According to the WRC-1992 diagram shown in Figure 9.11, the chromium andnickel equivalents of the weld metal are as follows: Chromium equivalent = 20.9 Nickel equivalent = 15.9 + 35 ¥ 0.1065 = 19.6Based on the diagram, the weld metal is fully austenitic and, therefore, is sus-ceptible to solidiﬁcation cracking. If the 309 ELC electrode is used, the weldmetal composition can be calculated as follows:Element Electrode ¥70% Type 304 ¥15% 1010 Steel ¥15% Weld MetalCr 24 16.8 18.0 2.7 0 0 19.5Ni 13 9.1 8.0 1.2 0 0 10.3C 0.03 0.021 0.05 0.0075 0.10 0.015 0.0435Mn 1.98 1.39 2.0 0.30 0.4 0.06 1.75Si 0.4 0.28 0 0 0.2 0.03 0.31Therefore, the chromium and nickel equivalents of the weld metal are Chromium equivalent = 19.5 Nickel equivalent = 10.3 + 35 ¥ 0.0435 = 11.8According to the WRC-1992 diagram, the weld metal now is austenitic with aferrite number of about 8 and, therefore, should be much more resistant tosolidiﬁcation cracking.
REDUCING SOLIDIFICATION CRACKING 291 It should be emphasized that neither the constitution diagrams nor themagnetic measurements of the weld metal ferrite content (such as thosedetermined by Magne–Gage readings) reveal anything about the weld metalsolidiﬁcation. In fact, the primary solidiﬁcation phase and the quantity of d-ferrite at high temperatures (i.e., during solidiﬁcation) are more importantthan the amount of ferrite retained in the room temperature microstructurein determining the sensitivity to solidiﬁcation cracking (81). Also, the amountof harmful impurities such as sulfur and phosphorus should be consideredin determining the weldability of a material; a material with a higher ferritecontent can be more susceptible to solidiﬁcation cracking than another mate-rial with a lower ferrite content if the impurity level of the former is alsohigher. The cooling rate during solidiﬁcation is another factor that the consti-tution diagrams fail to recognize (Chapter 9).11.4.2 Control of Solidiﬁcation StructureA. Grain Reﬁning As mentioned previously, welds with coarse columnargrains are often more susceptible to solidiﬁcation cracking than those with ﬁneequiaxed grains. It is, therefore, desirable to grain reﬁne the weld metal. Infact, both 2219 aluminum and 2319 ﬁller metal are designed in such a way thatthey not only have a non-crack-sensitive copper content but also have smallamounts of grain reﬁning agents such as Ti and Zr to minimize solidiﬁcationcracking. Dudas and Collins (40) produced grain reﬁning and eliminated solid-iﬁcation cracking in a weld made with an Al–Zn–Mg ﬁller metal by addingsmall amounts of Zr to the ﬁller metal. Garland (82) has grain reﬁned weldsof aluminum–magnesium alloys by vibrating the arc during welding, therebyreducing solidiﬁcation cracking.B. Magnetic Arc Oscillation Magnetic arc oscillation has been reportedto reduce solidiﬁcation cracking in aluminum alloys, HY-80 steel, and iridiumalloys (83–88). Kou and Le (86–88) studied the effect of magnetic arc oscilla-tion on the grain structure and solidiﬁcation cracking of aluminum alloy welds.As already shown in Figure 7.30, transverse arc oscillation at low frequenciescan produce alternating columnar grains. Figure 11.31 demonstrates that thistype of grain structure can be effective in reducing solidiﬁcation cracking (86).As illustrated in Figure 11.32, columnar grains that reverse their orientationat regular intervals force the crack to change its direction periodically, thusmaking crack propagation difﬁcult (87). Figure 11.33 shows the effect of theoscillation frequency on the crack susceptibility of 2014 aluminum welds (86).As shown, a minimum crack susceptibility exists at a rather low frequency,where alternating grain orientation is most pronounced. This frequency canvary with the welding speed. As shown in Figure 11.34, arc oscillation at much higher frequencies than1 Hz, though ineffective in 2014 aluminum, is effective in 5052 aluminum (87).
292 WELD METAL SOLIDIFICATION CRACKINGFigure 11.31 Effect of transverse arc oscillation (1 Hz) on solidiﬁcation cracking ingas–tungsten arc welds of 2014 aluminum. Reprinted from Kou and Le (86).Figure 11.32 Schematic sketches showing effect of arc oscillation on solidiﬁcationcracking. From Kou and Le (87).As shown in Figure 11.35, this is because grain reﬁning occurs in alloy 5052welds at high oscillation frequencies (88). Heterogeneous nucleation isbelieved to be mainly responsible for the grain reﬁning, since a 0.043 wt % Tiwas found in the 5052 aluminum used.
REDUCING SOLIDIFICATION CRACKING 293 150 Crack length, mm 100 2014 aluminum transverse oscillation 50 0 0 5 10 35 Frequency, HzFigure 11.33 Effect of oscillation frequency on solidiﬁcation cracking in gas–tungstenarc welds of 2014 aluminum. From Kou and Le (86). 5052 aluminum 150 transverse oscillation Crack length, mm 100 amplitude 1.1 mm 50 1.9 mm 0 0 10 20 Frequency, HzFigure 11.34 Effect of arc oscillation frequency on the solidiﬁcation cracking ingas–tungsten arc welds of 5052 aluminum. From Kou and Le (87).Figure 11.35 Grain structure of gas–tungsten arc welds of 5052 aluminum: (a) no arcoscillation; (b) 20 Hz transverse arc oscillation. Reprinted from Kou and Le (87).
294 WELD METAL SOLIDIFICATION CRACKING11.4.3 Use of Favorable Welding ConditionsA. Reducing Strains As mentioned previously in Chapter 1, the use ofhigh-intensity heat sources (electron or laser beams) signiﬁcantly reduces thedistortion of the workpiece and hence the thermally induced strains. Lessrestraint and proper preheating of the workpiece can also help reduce strains. Dyatlov and Sidoruk (89) and Nikov (90) found that preheating the work-piece decreased the magnitude of strains induced by welding. Sekiguchi andMiyake (91) reduced solidiﬁcation cracking in steel plates by preheating.Hernandez and North (92) positioned additional torches behind and along theside of the welding head and inhibited solidiﬁcation cracking in aluminumalloy sheets. It was suggested that the local heating decreased the amount ofplastic straining resulting from the welding operation and produced a lessstressful situation behind the weld pool.B. Improving Weld Geometry The weld bead shape can also affect solidiﬁ-cation cracking (93). When a concave single-pass ﬁllet weld cools and shrinks,the outer surface is stressed in tension, as show in Figure 11.36a. The outersurface can be considered as being pulled toward the toes and the root.However, by making the outer surface convex, as shown in Figure 11.36b,pulling toward the root actually compresses the outer surface and offsets thetension caused by pulling toward the toes. Consequently, the tensile stressesalong the outer surface are reduced, and the tendency for solidiﬁcation crack-ing to initiate from the outer surface is lowered. It should be pointed out,however, that excessive convexity can produce stress concentrations andinduce fatigue cracking (Section 5.3) or hydrogen cracking (Section 17.4) atthe toes. In multiple-pass welding, as illustrated in Figure 11.37, solidiﬁcationcracking can also initiate from the weld surface if the weld passes are too wideand concave (93). The weld width-to-depth ratio can also affect solidiﬁcation cracking. Asdepicted in Figure 11.38, deep narrow welds with a low width-to-depth ratiocan be susceptible to weld centerline cracking (93) This is because of the steepangle of the abutment between columnar grains growing from opposite sides toe surface in surface less tension in tension (a) (b) root toe Concave fillet weld Convex fillet weldFigure 11.36 Effect of weld bead shape on state of stress at center of outer surface:(a) concave ﬁllet weld; (b) convex ﬁllet weld. Modiﬁed from Blodgett (93).
CASE STUDY: FAILURE OF A LARGE EXHAUST FAN 295 Crack No Crack Crack (a) (b) (c) too wide and concave washed up too flat or slightly convex (also poor slag high and not quite full width removal) concave (also good slag removal)Figure 11.37 Effect of weld bead shape on solidiﬁcation in multipass weld: (a)concave; (b) concave; (c) convex. Modiﬁed from Blodgett (93). Crack No Crack (a) (b)Figure 11.38 Effect of weld depth–width ratio on centerline cracking: (a) ratio toohigh; (b) ratio correct. Modiﬁed from Blodgett (93).of the weld pool. This type of cracking is often observed in deep and narrowwelds produced by EBW or SAW.11.5 CASE STUDY: FAILURE OF A LARGE EXHAUST FANFigure 11.39a shows a schematic sketch of a large six-bladed exhaust fan fordrawing chemical mist from a chemical processing chamber (94). The hub ofthe fan had a diameter of about 178 mm (7 in.) and a washer-shaped verticalﬁn. Two ﬂat-bar spokes were welded to the ﬁn at each 60° interval and pro-vided the support for the fan blades. The fan acted only as the drawing forceto pull the mist from the process area; it did not come into direct contact withthe mist. A “scrubber” was positioned between the fan and the process unit toremove the chemical from the exhausted air mass. The spokes and blades werefabricated from type 316 austenitic stainless steel bars and plates, and the elec-trodes used for welding were type E316 covered electrodes. The fan measuredabout 1.5 m (5 ft) between blade tips, weighed about 320 kg (700 lb), androtated at 1200 rpm in service. It failed after 12 weeks service time. Figure 11.39b shows the fractured ﬁllet weld joining the underside ofthe blade to the supporting spoke. The weld metal was nonmagnetic, thatis, containing little d-ferrite, and was therefore susceptible to solidiﬁcationcracking. Note the jagged nature of the microﬁssures following the columnargrain structure above the arrowhead, as compared with the smooth cracktypical of fatigue failure below the arrowhead. In fact, the fracture surface of
296 WELD METAL SOLIDIFICATION CRACKINGFigure 11.39 Failure of a large welded exhaust fan (94): (a) location of failure; (b)failed component.the failed spoke member exhibited the “clam shell” markings typical of fatiguefailure. In summary, the fully austenitic weld metal produced by type E316 elec-trodes suffered from solidiﬁcation cracking, which in turn initiated fatiguecracking and led to ﬁnal failure. Type 309 or 308 electrodes, which containmore d-ferrite to resist solidiﬁcation cracking, could have been used to avoidsolidiﬁcation cracking in the weld metal (94).REFERENCES 1. Kou, S., and Kanevsky, Y., unpublished research, Carnegie-Mellon University, Pittsburgh, PA, 1980. 2. Davies, G. J., and Garland, J. G., Int. Metal Rev., 20: 83, 1975. 3. Lees, D. C. G., J. Inst. Metals, 72: 343, 1946. 4. Singer, A. R. E., and Jennings, P. H., J. Inst. Metals, 73: 273, 1947. 5. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974. 6. Bishop, H. F., Ackerlind, C. G., and Pellini, W. S., Trans. AFS, 65: 247, 1957. 7. Borland, J. C., Br. Weld. J., 7: 508, 1960. 8. Li, L., and Messler, Jr., R. W., Weld. J., 78: 387s, 1999. 9. Matsuda, F., Nakagawa, H., and Sorada, K., Trans. JWS1, 11: 67, 1982.10. Matsuda, F., Nakagawa, H., Kohomoto, H., Honda, Y., and Matsubara, Y., Trans. JWSI, 12: 73, 1983.11. Houldcroft, P. T., Br. Weld. J., 2: 471, 1955.12. Liptax, J. A., and Baysinger, F. R., Weld. J., 47: 173s, 1968.
REFERENCES 29713. Garland, J. G., and Davies, G. J., Metals Const. Br. Weld. J., vol. 1, p. 565, December 1969.14. Rogerson, J. H., Cotterell, B., and Borland, J. C., Weld. J., 42: 264s, 1963.15. Savage, W. F., and Lundin, C. D., Weld. J., 44: 433s, 1965.16. Nakata, K., and Matsuda, F., Trans. JWRI, 24: 83, 1995.17. Krysiak, K. F., Grubb, J. F., Pollard, B., and Campbell, R. D., in Welding, Brazing, and Soldering, Vol. 6, ASM International, Materials Park, OH, December 1993, p. 443.18. DuPont, J. N., Michael, J. R., and Newbury, B. D., Weld. J., 78: 408s, 1999.19. Stout, R. D., in Weldability of Steels, 3rd ed., Eds. R. D. Stout and W. D. Doty, Welding Research Council, New York, 1978, p. 252.20. Messler, R. W., Jr., Principles of Welding, Processes, Physics, Chemistry and Metal- lurgy, Wiley, New York, 1999, pp. 557–589.21. Cieslak, M. J., Weld. J., 66: 57s, 1987.22. David, S. A., and Woodhouse, J. J., Weld. J., 66: 129s, 1987.23. Nelson, T. W., Lippold, J. C., Lin, W., and Baeslack III, Weld. J., 76: 110s, 1997.24. Goodwin, G. M., Weld. J., 66: 33s, 1987.25. Hondros, E. D., and Seah, M. P., Int. Metals Rev., 222: 12, 1977.26. Pease, G. R., Weld. J., 36: 330s, 1957.27. Canonico, D. A., Savage, W. F., Werner, W. J., and Goodwin, G. M., paper presented at Effects of Minor Elements on the Weldability of High-Nickel Alloys, Welding Research Council, NY, 1969, p. 68.28. Savage, W. F., Nippes, E. F., and Goodwin, G. M., Weld. J., 56: 245s, 1977.29. Kah, D. H., and Dickinson, D. W., Weld. J., 60: 135s, 1981.30. Principles and Technology of the Fusion Welding of Metals, Vol. 1, Mechanical Engi- neering Publishing Co., Peking, China, 1979 (in Chinese).31. DuPont, J. N., Robino, C. V., and Marder, A. R., Weld. J., 77: 417s, 1998.32. DuPont, J. N., Robino, C. V., Marder, A. R., Notis, M. R., and Michael, J. R., Metall. Mater. Trans. A., 29A: 2785, 1998.33. DuPont, J. N., Robino, C. V., and Marder, A. R., Acta Mater., 46: 4781, 1998.34. DuPont, J. N., Robino, C. V., and Marder, A. R., Sci. Technol. Weld. Join., 4: 1, 1999.35. DuPont, J. N., Weld. J., 78: 253s, 1999.36. Singer, A. R. E., and Jennings, P. H., J. Inst. Metals, 73: 197, 1947.37. Pumphrey, W. I., and Lyons, J. V., J. Inst. Metals, 74: 439, 1948.38. Dowd, J. D., Weld. J., 31: 448s, 1952.39. Jennings, P. H., Singer, A. R. E., and Pumphrey, W. L., J. Inst. Metals, 74: 227, 1948.40. Dudas, J. H., and Collins, F. R., Weld. J., 45: 241s, 1966.41. Michaud, E. J., Kerr, H. W., and Weckman, D. C., in Trends in Welding Research, Eds. H. B. Smartt, J. A. Johnson, and S. A. David, ASM International, Materials Park OH, June 1995, p. 154.42. Yang, Y. P., Dong, P., Zhang, J., and Tian, X., Weld. J., 79: 9s, 2000.43. Gueussier, A., and Castro, R., Rev. Metall., 57: 117, 1960.44. Takalo, T., Suutala, N., and Moisio, T., Metall. Trans., 10A: 1173, 1979.
298 WELD METAL SOLIDIFICATION CRACKING45. Lienert, T. J., in Trends in Welding Research, Eds. J. M. Vitek, S. A. David, J. A. Johnson, H. B. Smartt, and T. DebRoy, ASM International, Materials Park, OH, June 1998, p. 726.46. Hull, F. C., Weld. J., 46: 399s, 1967.47. Baeslack, W. A., Duquette, D. J., and Savage, W. F., Corrosion, 35: 45, 1979.48. Baeslack, W. A., Duquette, D. J., and Savage, W. F., Weld. J., 57: 175s, 1978.49. Baeslack, W. A., Duquette, D. J., and Savage, W. F., Weld. J., 58: 83s, 1979.50. Manning, P. G., Duquette, D. J., and Savage, W. F., Weld. J., 59: 260s, 1980.51. Thomas, R. G., Weld. J., 57: 81s, 1978.52. Borland, J. C., and Younger, R. N., Br. Weld. J., 7: 22, 1960.53. Thomas, R. D. Jr., Metals Prog., 70: 73, 1956.54. Medovar, B. I., Avtomatischeskaya Svarka, 6: 3, 1953.55. Curran, R. M., and Rankin, A. W., Weld. J., 34: 205, 1955.56. Borland, J. C., Br. Weld. J., 7: 558, 1960.57. Rollason, E. C., and Bystram, M. C. T., J. Iron Steel Inst., 169: 347, 1951.58. Smith, C. S., Interphase Imperfections in Nearly Perfect Crystals, Wiley, New York, 1952, pp. 377–401.59. Taylor, J. W., J. Inst. Metals, 86: 456, 1958.60. Brooks, J. A., Thompson, A. W., and Williams, J. C., in Physical Metallurgy of Metal Joining, Eds. R. Kossowsky and M. E. Glickstein, Metallurgical Society of AIME, Warrendale, PA, 1980, p. 117.61. Smith, C. R., Trans. AIME, 175: 15, 1948.62. Matsuda, F., Nakata, K., Tsukamoto, K., and Arai, K., Trans. JWRI, 12: 93, 1983.63. Matsuda, F., Nakata, K.,Tsukamoto, K., and Uchiyama,T., Trans. JWRI, 13: 57, 1984.64. Dvornak, M. J., Frost, R. H., and Olson, D. L., Weld. J., 68: 327s, 1989.65. Kou, S., and Le, Y., unpublished research, Carnegie-Mellon University, Pittsburgh, PA, 1981.66. Linnert, G. E., Welding Metallurgy, Vol. 2, 3rd ed., American Welding Society, New York, 1967.67. Jennings, P. H., Singer, A. R. E., and Pumphrey, W. I., J. Inst. Metals, 74: 227, 1948.68. Pumphrey, W. I., and Moore, D. C., J. Inst. Metals, 73: 425, 1948.69. Savage, W. F., Nippes, E. F., and Varsik, J. D., Weld. J., 58: 45s, 1979.70. Evancho, J. W., and Baker, C. L., Weld Crack Susceptibility of Al-Mg Alloys, ALCOA Report, ALCOA Technology Center, ALCOA Center, PA, March 1980.71. Smith, R. B., in Welding, Brazing, and Soldering, Vol. 6, ASM International, Materials Park, OH, December 1993, p. 642.72. Borland, J. C., Br. Weld. J., 8: 526, 1961.73. Jefferson, T. B., and Woods, G., Metals and How to Weld Them, James Lincoln Arc Welding Foundation, Cleveland, OH, 1961.74. Schaefﬂer, A. L., Metal. Prog., 56: 680, 1949.75. DeLong, W. T., Weld. J., 53: 273s, 1974.76. Kotecki, D. J., Weld. J., 78: 180s, 1999.77. Kotecki, D. J., Weld. J., 79: 346s, 2000.
PROBLEMS 29978. Balmforth, M. C., and Lippold, J. C., Weld. J., 79: 339s, 2000.79. Vitek, J. M., Iskander, Y. S., and Oblow, E. M., Weld. J., 79: 33s, 2000.80. Vitek, J. M., Iskander, Y. S., and Oblow, E. M., Weld. J., 79: 41s, 2000.81. Cieslak, M. J., and Savage, W. F., Weld. J., 60: 131s, 1981.82. Garland, J. G., Metal Const. Br. Weld. J., 21: 121, 1974.83. Tseng, C., and Savage, W. F., Weld. J., 50: 777, 1971.84. David, S. A., and Liu, C. T., in Grain Reﬁnement in Castings and Welds, Eds. G. J. Abbaschian and S. A. David, Metals Society of AIME, Warrendale, PA, 1983, p. 249.85. Scarbrough, J. D., and Burgan, C. E., Weld. J., 63: 54, 1984.86. Kou, S., and Le, Y., Metall. Trans., 16A: 1887, 1985.87. Kou, S., and Le, Y., Metall. Trans., 16A: 1345, 1985.88. Kou, S., and Le, Y., Weld. J., 64: 51, 1985.89. Dyatlov, V. I., and Sidoruk, V. S., Autom. Weld., 3: 21, 1966.90. Nikov, N. Y., Weld. Production, 4: 25, 1975.91. Sekiguchi, H., and Miyake, H., J. Jpn. Weld. Soc., 6(1): 59, 1975.92. Hernandez, I. E., and North, T. H., Weld. J., 63: 84s, 1984.93. Blodgett, O. W., Weld. Innovation Q., 2(3): 4, 1985.94. Fatigue Fractures in Welded Constructions, Vol. 11, International Institute of Welding, London, 1979.FURTHER READING1. Davies, G. J., and Garland, J. G., Int. Metall. Rev., 20: 83, 1975.2. Flemings, M. C., Solidiﬁcation Processing, McGraw-Hill, New York, 1974.PROBLEMS11.1 Compare the solidiﬁcation temperature range and fraction eutectic of Al–3.0Cu with those of Al–6.0Cu. For simplicity, assume Scheil’s equa- tion is a valid approximation and both the solidus and liquidus lines are straight in the Al–Cu system. CSM = 5.65, CE = 33, TE = 548°C, and Tm = 660°C (pure Al).11.2 Centerline cracking is often observed in deep-penetration electron or laser beam welds. Explain why.11.3 Fillet welds of 5052 Al (essentially Al–2.5Mg) are made with 5556 ﬁller (essentially Al–5.1Mg). What are the approximate dilution ratio and weld metal composition? Is the weld metal susceptible to solidiﬁcation cracking?11.4 Solidiﬁcation cracking in 2014 aluminum sheets can be reduced signiﬁcantly by using low-frequency transverse arc oscillation. Low-
300 WELD METAL SOLIDIFICATION CRACKING frequency circular and longitudinal arc oscillations, however, are less effective. Explain why.11.5 Low-frequency arc pulsation during autogenous GTAW of aluminum alloys, such as 6061 and 2014, is often found detrimental rather than beneﬁcial in controlling solidiﬁcation cracking. Explain why.11.6 A structural steel has a nominal composition of 0.16 C, 1.4 Mn, 0.4 Si, 0.022 S, and 0.016 P. Because of macrosegregation of carbon during ingot casting, some of the steel plates produced contained as much as 0.245% C. Severe solidiﬁcation cracking was reported in welds of these steel plates. Explain why. The problem was solved by using a different ﬁller wire. Comment on the carbon content of the new ﬁller wire.11.7 Consider welding 1018 steel to 304 stainless steel by GMAW (dilution normally between 30 and 40%). Assume approximately equal contri- bution to weld metal dilution from each side of the joint. Will the weld metal be susceptible to solidiﬁcation cracking if ER308L Si is used as the electrode? Will the weld metal be dangerously close to the marten- site boundary? 1018 steel: 0.18C–0.02Cr–0.03Ni–0.01Mo–0.07Cu– 0.01N; 304 stainless steel: 0.05C–18.30Cr–8.80Ni–0.05Mo–0.08Cu– 0.04N; ER308L Si: 0.03C–19.90Cr–10.20Ni–0.21Mo–0.19Cu–0.06N.11.8 Repeat the previous problem but with ER309L Si as the electrode. ER309L Si: 0.02C–24.10Cr–12.70Ni–0.13Mo–0.16Cu–0.05N.11.9 Stainless steels normally considered resistant to solidiﬁcation cracking in arc welding based on the constitution diagram (such as Schaefﬂer or WRC 1992), for instance, 304L, 316L, and 321Mo, can become rather susceptible in laser or electron beam welding. Explain why.11.10 It has been observed in 1100 aluminum alloy that the Ti or Zr content of the alloy, up to about 0.5 wt %, can signiﬁcantly affect its suscepti- bility to solidiﬁcation cracking. Explain how Ti or Zr affects weld metal solidiﬁcation cracking of the alloy and why.11.11 It has been reported that autogenous gas–tungsten arc welds of Invar (Fe–36 wt % Ni) are rather susceptible to solidiﬁcation cracking. Explain why based on a constitution diagram. The addition of Ti (e.g., 0.5–1.0%) has been found to change the Mn sulﬁde ﬁlms along the grain boundaries to tiny Ti sulﬁde particles entrapped between dendrite arms. What is the effect of the Ti addition on solidiﬁcation cracking?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-4PART IIIThe Partially Melted Zone
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-412 Formation of the PartiallyMelted ZoneSevere liquation can occur in the partially melted zone during welding. Severalfundamental liquation-related phenomena are discussed in this chapter,including liquation mechanisms, solidiﬁcation of the grain boundary (GB)liquid, and the resultant GB segregation.12.1 EVIDENCE OF LIQUATIONThe partially melted zone (PMZ) is the area immediately outside the weldmetal where liquation can occur during welding. Figure 12.1a shows a portionof the PMZ in a gas–metal arc weld of a 6061 aluminum made with a 4145ﬁller metal. The presence of dark-etching GBs along the fusion boundary inthis micrograph is an indication of GB liquation. The microstructure inside thewhite rectangle is enlarged in Figure 12.1b. The liquated and resolidiﬁed mate-rial along the GB consists of a dark-etching eutectic GB and a lighter etchinga (Al-rich) band along the GB. Figure 12.2 shows the PMZ microstructure in alloy 2219, which is essen-tially Al–6.3Cu (1). The liquated and resolidiﬁed material along the GB con-sists of a dark-etching eutectic GB and a light-etching a band along the GB.The a bands here appear lighter than those in Figure 12.1b because of the useof a different etching solution. As shown, the large dark-etching eutectic par-ticles within grains are surrounded by a light-etching a phase, thus indicatingthat liquation also occurs within grains. The formation of the PMZ in 2219 aluminum is explained in Figure 12.3.As shown in the phase diagram (Figure 12.3a), the composition of alloy 2219is C0 = 6.3% Cu. As shown by the thermal cycles (Figure 12.3b), the materialat position b is heated up to between the eutectic temperature TE and the liq-uidus temperature TL during welding. Therefore, the material becomes a solid-plus-liquid mixture (a + L), that is, it is partially melted. The material atposition a is completely melted while that at position c is not melted at all. Asimilar explanation for the formation of the PMZ, in fact, has been given pre-viously in Figure 7.12. 303
304 FORMATION OF THE PARTIALLY MELTED ZONEFigure 12.1 PMZ microstructure of gas–metal arc weld in 6061 aluminum made with4145 aluminum ﬁller wire. Rectangular area in (a) enlarged in (b).12.2 LIQUATION MECHANISMSHuang et al. (1–5) have conducted a series of studies on liquation and solidi-ﬁcation in the PMZ of aluminum welds. Figure 12.4 shows ﬁve different PMZliquation mechanisms. The phase diagram shown in Figure 12.4a is similar tothe Al-rich side of the Al–Cu phase diagram. Here, AxBy is an intermetalliccompound, such as Al2Cu in the case of Al–Cu alloys. Alloy C1 is within thesolubility limit of the a phase, CSM, and alloy C2 is beyond it. In the as-castcondition both alloys C1 and C2 usually consist of an a matrix and the eutec-tic a + AxBy along GBs and in between dendrite arms.12.2.1 Mechanism 1: AxBy Reacting with MatrixThis mechanism is shown in Figure 12.4b. Here alloy C2, for instance, alloy2219, consists of an a matrix and AxBy particles at any temperature up to the
LIQUATION MECHANISMS 305Figure 12.2 PMZ microstructure of gas–metal arc weld in 2219 aluminum made with2319 aluminum ﬁller wire: (a) left of weld; (b) right of weld. Reprinted from Huangand Kou (1). Courtesy of American Welding Society.eutectic temperature TE, regardless of the heating rate to TE during welding.At TE liquation is initiated by the eutectic reaction AxBy + a Æ L. The liquation mechanism for alloy 2219 can be explained with the helpof Figure 12.5. The base metal contains large and small q (Al2Cu) particlesboth within grains and along GBs (Figure 12.5a), as shown by the SEMimage at the top. At the border line between the PMZ and the basemetal (Figure 12.5b), the material is heated to the eutectic temperature TE.Regardless of the heating rate q (Al2Cu) particles are always present whenTE is reached. Consequently, liquation occurs by the eutectic reaction a +q Æ LE, where LE is the liquid of the eutectic composition CE. Upon cool-ing, the eutectic liquid solidiﬁes into the eutectic solid without composi-tion changes and results in eutectic particles and some GB eutectic (Figure12.5e). Above TE, that is, inside the PMZ, liquation intensiﬁes. The a matrix sur-rounding the eutectic liquid dissolves and the liquid increases in volume
306 FORMATION OF THE PARTIALLY MELTED ZONE Solidus Liquidus T a a o T (643 C) WM 660 L Temperature T, o C b L PMZ α+L L+ θ b 548 α c TE (548 oC) eutectic BM c α+θ θ (Al Cu) C =6.3 2 o Al C =5.65 C =33.2 55.4 (b) Time, t SM E (a) wt % Cu Weld Metal (WM) Partially Melted Zone (PMZ) a (c) T b L T c E Base Metal (BM)Figure 12.3 Formation of PMZ in 2219 aluminum weld: (a) Al-rich side of Al–Cuphase diagram; (b) thermal cycles; (c) transverse cross section.(Figure 12.5c). This causes the liquid composition to change from eutectic tohypoeutectic (<CE), as dictated by the phase diagram (Figure 12.4a). Uponcooling, the hypoeutectic liquid solidiﬁes ﬁrst as Cu-depleted a and last as Cu-rich eutectic when its composition increases to CE, as also dictated by the phasediagram. This results in a band of Cu-depleted a along the GB eutectic and aring of Cu-depleted a surrounding each large eutectic particle (Figure 12.5f ),as shown in the optical micrograph at the bottom.12.2.2 Mechanism 2: Melting of EutecticThis mechanism is also shown in Figure 12.4b. Here alloy C2, for instance, alloy2219 in the as-cast condition, consists of an a matrix and the eutectic a + AxByalong GBs and in between dendrite arms. Regardless of the heating rate to TEduring welding, the eutectic is always present before TE is reached.At TE liqua-tion is initiated by the melting of the eutectic.12.2.3 Mechanism 3: Residual AxBy Reacting with MatrixThis mechanism is shown in Figure 12.4c. This is the well-known constitutionalliquation mechanism proposed by Pepe and Savage (6, 7). Here alloy C1 stillcontains residual AxBy particles just before reaching the eutectic temperature
LIQUATION MECHANISMS 307 TL2 liquidus Tm TL1 solidus Temperature, T eutectic L L + AxBy TS1 α+ L (a) α TV TE α + AxBy solvus A C2 CE AxBy C1 < CSM C1 Concentration of B, C C2 > CSM TL1 CSM TL2 Weld Weld Metal Metal PMZ (3 or 4) PMZ (1 or 2) TE PMZ (5) TE TS1 BM Base Metal (BM) 3. Residual AxBy reacting with matrix: 1. AxBy reacting with matrix: (constitutional liquation) AxBy+ α L at T E AxBy+ α L at T E AxBy always present at T E if AxBy still present at T E regardless of heating rate 4. Melting of residual eutectic: 2. Melting of eutectic: eutetic(S) eutectic(L) at T E eutectic(S) eutectic(L) at T E if eutectic still present at T E eutectic always present 5. Melting of matrix: at T E regardless of heating rate α L at T S1 (b) if no AxBy or eutectic present at T E (c)Figure 12.4 Five mechanisms for liquation in PMZ of aluminum alloys: (a) phasediagram; (b) two mechanisms for an alloy beyond the solid solubility limit (CSM); (c)three mechanisms for an alloy within the solid solubility limit.TE. Examples of such AxBy include the titanium sulﬁde inclusion in 18% Nimaraging steel, Ni2Nb Laves phase in Inconel 718, carbides in Ni-base super-alloys, and several intermetallic compounds in aluminum alloys. When alloy C1 is heated very slowly to above the solvus temperature TV,AxBy dissolves completely in the a matrix by solid-state diffusion, and thealloy becomes a homogeneous a solid solution of composition C1. However,when alloy C1 is heated rapidly to above TV, as often the case in welding, AxBydoes not have enough time to dissolve completely in the a matrix becausesolid-state diffusion is slow. That is, AxBy remains in the a matrix above TV.Consequently, upon heating to the eutectic temperature TE, the residual AxByreacts with the surrounding a matrix and forms the liquid eutectic CE at the
308 FORMATION OF THE PARTIALLY MELTED ZONEFigure 12.5 Microstructure evolution in PMZ of 2219 aluminum with SEM image ofthe base metal on the top and optical micrograph of the PMZ at the bottom. Reprintedfrom Huang and Kou (1). Courtesy of American Welding Society.
LIQUATION MECHANISMS 309interface. Further heating to above TE would allow additional time for furtherdissolution of AxBy and further formation of the liquid phase. Therefore, it isclear that localized melting should be possible with rapid heating rates at tem-peratures signiﬁcantly below the equilibrium solidus temperature TS1. Figure 12.6 shows the microstructure of the PMZ of a resistance spot weldof 18-Ni maraging steel (6). This micrograph reveals the four stages leading toGB liquation.The ﬁrst stage, visible at point A, shows a rodlike titanium sulﬁdeinclusion beginning to form a thin liquid ﬁlm surrounding the inclusion. Thesecond stage is visible at point B, which is closer to the fusion boundary andhence experiences a higher peak temperature than at point A.As shown, liqua-tion is more extensive and an elliptical liquid pool surrounds the remainingsmall gray inclusion. Still closer to the fusion boundary, at point C, no moresolid inclusion remains in the liquid pool, and penetration of GBs by the liquidphase is evident along the GBs intersecting with the liquid phase. Finally, atposition D, GB penetration by the liquid phase is so extensive that the GBsare liquated. Constitutional liquation has also been observed in several nickel-basealloys (8–11), such as Udimet 700, Waspaloy, Hastelloy X, and Inconel 718, andin 347 stainless steel (12). Constitutional liquation can be initiated by the inter-action between the matrix and particles of carbide or other intermetallic com-pounds. Examples include M6C in Hastelloy X, MC carbide in Udimet 700,Waspaloy and Inconel 718, and Ni2Nb Laves phase in Inconel 718. Figure 12.7shows the PMZ of an Inconel 718 weld (13). Constitutional liquation occursby the eutectic reaction between the Ni2Nb Laves phase and the nickel matrix.Figure 12.6 PMZ of an electric resistance spot weld of 18-Ni maraging steel showingconstitutional liquation. The fusion zone is at the top. Magniﬁcation 385¥. Reprintedfrom Pepe and Savage (6). Courtesy of American Welding Society.
310 FORMATION OF THE PARTIALLY MELTED ZONEFigure 12.7 PMZ of Inconel 718 weld showing constitutional liquation due to Laveseutectic reaction. Reprinted from Kelly (13). Constitutional liquation alone, however, is not enough to cause the liquidto penetrate most GBs in the PMZ. For this to occur in Ni-base alloys, GBmigration is also needed. Figure 12.8 shows schematically the formation of GBﬁlms in the PMZ due to the simultaneous occurrence of constitutional liqua-tion and GB migration (6). The microstructure at location d0 is representativeof the as-received plate. At location d1, signiﬁcant grain growth occurs abovethe effective grain coarsening temperature. Meanwhile, some of the movingGBs intersect with the solute-rich pools formed by constitutional liquation,thus allowing the solute-rich liquid to penetrate these GBs.At location d2 moregrain growth occurs and sufﬁcient solute-rich liquid penetrates the GBs andforms GB ﬁlms. These GBs are pinned due to the wetting action of the ﬁlms.No further grain growth is expected until either the solute-rich liquid phase isdissipated by homogenization or the local temperature decreases to below theeffective solidus of the solute-rich liquid to cause it to solidify. If insufﬁcienttime is available to dissipate the solute-rich liquid GB ﬁlms before the localtemperature decreases to below the effective solidus of the liquid, the liquidGB ﬁlms will solidify as a solute-rich GB network. A “ghost” GB network willthus remain ﬁxed when grain growth resumes, as shown by the dashed linesat location d3. Grain growth will continue until either an equilibrium GBnetwork is formed or the temperature decreases to below the effective graincoarsening temperature. Figure 12.9 shows the ghost GB network near thefusion boundaries of gas–tungsten arc welds of 18-Ni maraging steel (6) anda Ni-base superalloy 690 (14).
Figure 12.8 Schematic representation of constitutional liquation and formation of ghost GB network. Reprinted from Pepe and Savage (6). Courtesy of American Welding Society. (a)(b) Figure 12.9 Ghost GBs near fusion boundary of gas–tungsten arc welds: (a) 18-Ni maraging steel; magniﬁcation 125¥. Reprinted from Pepe and Savage (6). Courtesy of American Welding Society. (b) Ni-base superalloy 690. Reprinted from Lee and Kuo (14).
312 FORMATION OF THE PARTIALLY MELTED ZONEFigure 12.10 PMZ microstructure of gas–metal arc weld in as-cast Al–4.5Cu.Reprinted from Huang et al. (4).12.2.4 Mechanism 4: Melting of Residual EutecticThis mechanism is also shown in Figure 12.4c. Here alloy C1, for instance, anas-cast Al–4.5Cu alloy, still contains the residual eutectic a + AxBy along GBsand in between dendrite arms when the eutectic temperature TE is reached.If the alloy is heated very slowly to above the solvus temperature TV, the eutec-tic can dissolve completely in the a matrix by solid-state diffusion. However,if it is heated rapidly to above TV, as in welding, the eutectic does not haveenough time to dissolve completely in the a matrix because solid-state diffu-sion takes time. Consequently, upon further heating to the eutectic tempera-ture TE, the residual eutectic melts and becomes liquid eutectic. Above TE thesurrounding a phase dissolves in the liquid and the liquid becomes hypoeu-tectic. Upon cooling, the hypoeutectic liquid solidiﬁes ﬁrst as solute-depleteda and last as solute-rich eutectic when its composition increases to CE. Figure12.10 shows the PMZ of a gas–metal arc weld of an as-cast Al–4.5% Cu alloy(4). Liquation is evident at the prior eutectic sites along the GB and in betweendendrite arms. A light-etching a band is present along the eutectic GB. Like-wise, light-etching a rings surround the eutectic particles near the fusionboundary.12.2.5 Mechanism 5: Melting of MatrixThis mechanism is also shown in Figure 12.4c. Here alloy C1 contains neitherAxBy particles nor the a + AxBy eutectic when the eutectic temperature TE isreached. An alloy Al–4.5Cu solution heat treated before welding is anexample. Slow heating to TE can also cause complete dissolution of AxBy oreutectic in the a matrix before TE, but this usually is not likely in welding. The
LIQUATION MECHANISMS 313Figure 12.11 PMZ microstructure of gas–metal arc weld in cast Al–4.5Cu homoge-nized before welding (a) and magniﬁed (b). Reprinted from Huang et al. (4).PMZ ranges from the solidus temperature (TS1) to the liquidus temperature(TL1), instead of from the eutectic temperature to the liquidus temperature,as in all previous cases. Figure 12.11 shows the PMZ microstructure in anAl–4.5% Cu alloy solution heat treated and quenched before GMAW (4).Eutectic is present both along GBs and within grains in the PMZ even thoughthe base metal is free of eutectic. Another example is a 6061-T6 aluminumcontaining submicrometer-size Mg2Si precipitate, which is reverted in the amatrix before reaching TE during GMAW (5).12.2.6 Mechanism 6: Segregation-Induced LiquationLippold et al. (15) proposed a segregation-induced liquation mechanism foraustenitic and duplex stainless steels. In such a mechanism the alloy and/orimpurity elements that depress the melting point segregate to GBs, lowerthe melting point, and cause GB liquation. In other words, GB segregationtakes place ﬁrst and GB liquation next. This is opposite to all the other mecha-nisms described in this chapter, where liquation takes place ﬁrst and segrega-tion occurs during the solidiﬁcation of the liquated material, as will bediscussed subsequently. They suggested that such GB segregation can be
314 FORMATION OF THE PARTIALLY MELTED ZONE Weld Metal Partially Melted Rolling Zone direction Base Metal eutectic : direction of solute- solidification depleted α Figure 12.12 Directional solidiﬁcation of GB liquid in PMZ.caused by (i) equilibrium diffusion of atoms of the elements to GBs, (ii) GBsweeping of such atoms into migrating GBs during grain growth, and (iii)“pipeline” diffusion of such atoms along GBs in the fusion zone that are con-tinuous across the fusion boundary into the PMZ. More details are availableelsewhere (15, 16).12.3 DIRECTIONAL SOLIDIFICATION OF LIQUATED MATERIALHuang et al. (1, 4) observed that the GB liquid has a tendency to solidify essen-tially upward and toward the weld regardless of its location with respect to theweld, as shown schematically in Figure 12.12. This directional solidiﬁcation iscaused by the high-temperature gradients toward the weld during welding. Ithas been generally accepted that the GB liquid between two neighboringgrains solidiﬁes from both grains to the middle between them. However, themicrographs in Figure 12.2 show that it solidiﬁes from one grain to the other—in the direction upward and toward the weld. This, in fact, suggests GB migra-tion in the same direction. However, if the grains in the PMZ are very thin or very long, there may notbe much GB area facing the weld. Consequently, solidiﬁcation of the GB liquidis still directional but just upward (5).12.4 GRAIN BOUNDARY SEGREGATIONAs the GB liquid solidiﬁes, solute atoms are rejected by the solid into theliquid if the equilibrium partition coefﬁcient k < 1, such as in the phase diagram
GRAIN BOUNDARY SEGREGATION 315shown in Figure 12.3a. The GB liquid solidiﬁes ﬁrst as a solute-depleted a butﬁnally as eutectic when the liquid composition reaches CE. Figure 12.13 depicts the GB segregation that develops during solidiﬁcationof the GB liquid in the PMZ (5). Take alloy 2219 as an example. Let C0 be theconcentration of Cu in the base metal (6.3%). Theoretically, the measured con-centration of the GB eutectic, Ce, is the eutectic composition CE (33%) if theGB eutectic is normal and q or Al2Cu (55%) if it is divorced. A normal eutec-tic refers to a eutectic with a composite-like structure of a + q. A divorcedeutectic, on the other hand, refers to a eutectic that nucleates upon an exist-ing a matrix and thus looks like q alone. In practice, with EPMA (electronprobe microanalysis) the value of Ce can be less than CE if the GB is thinnerthan the volume of material excited by the electrons, that is, the surroundinga of low-Cu is included in the composition analysis. This volume depends onthe voltage used in EPMA and the material being analyzed. In the absence of back diffusion, the concentration of the element at thestarting edge of the a strip should be kC0, where k is the equilibrium partitionratio of the element. The dashed line shows the resultant GB segregation ofthe element. However, if back diffusion of the solute from the growth frontinto the solute-depleted a strip is signiﬁcant, the concentration of the elementat the starting edge of the a strip will be greater than kC0, as the solid lineindicates. Severe GB segregation of alloying elements has been observed in the PMZof gas–metal arc welds of alloys 2219, 2024, 6061, and 7075 (2, 5). Figure 12.14shows that in alloy 2219 the composition varies from about 2% Cu at the start-ing edge of the a strip to 30% Cu at the GB eutectic (2). The 2–3% Cu contentof the a strip is signiﬁcantly lower than that of the base metal (C0 = 6.3% Cu), Weld Metal Partially Melted Zone Base Metal (a) b k<1 a Ce Concentration, C GB eutectic back diffusion solute-depleted α Solute α Co kC o a b (b) Distance, z no back diffusion (c) Figure 12.13 Grain boundary segregation in PMZ. From Huang and Kou (5).
316 FORMATION OF THE PARTIALLY MELTED ZONEFigure 12.14 Grain boundary segregation in PMZ of 2219 aluminum weld: (a) elec-tron micrograph; (b) composition proﬁle. Reprinted from Huang and Kou (2). Cour-tesy of American Welding Society. Weld Metal Partially Melted a Zone b Base Metal (a) thinner Planar Cellular thicker Solidification Solidification eutectic eutectic planar solute- cellular solute- α depleted α depleted α α (b) (c) Grain Figure 12.15 Solidiﬁcation modes of GB liquid in PMZ.thus conﬁrming that the a strip is Cu depleted. The 2% Cu content at the start-ing edge of the a strip is higher than kC0 (1.07% = 0.17 ¥ 6.3%), thus implyingback diffusion of Cu into the a strip during GB solidiﬁcation.The 30% Cu con-centration at the GB is close to the 33% Cu composition of a normal eutectic.12.5 GRAIN BOUNDARY SOLIDIFICATION MODESAs shown in Figures 12.1, 12.2, and 12.11, the a band along the eutectic GB isplanar, namely, without cells or dendrites. This suggests that the solidiﬁcationmode of the GB liquid is planar. The vertical temperature gradient G and the
GRAIN BOUNDARY SOLIDIFICATION MODES 317vertical growth rate R were determined in the PMZ of alloy 2219 and theupward solidiﬁcation of the GB liquid was analyzed (3). The ratio G/R forplanar GB solidiﬁcation was found to be on the order of 105 °Cs/cm2, which isclose to that required for planar solidiﬁcation of Al–6.3% Cu.Figure 12.16 Solidiﬁcation modes of GB liquid in PMZ of 2219 aluminum weld: (a)planar; (b) cellular. Reprinted from Huang and Kou (3). Courtesy of American WeldingSociety.
318 FORMATION OF THE PARTIALLY MELTED ZONE 1600 L fusion zone Temperature, oC L +γ partially melted zone 1200 γ heat-affected zone γ + C base metal 800 α + C Fe 1 2 3 4 Cast iron Carbon, wt% (b) (a) Figure 12.17 PMZ in a cast iron. Although planar solidiﬁcation of the GB liquid predominates in the PMZ,cellular solidiﬁcation can also occur (3, 5). These cellular a bands share twocommon characteristics. First, they are often located near the weld bottom.Second, on average, they appear signiﬁcantly thicker than the planar a bandsnearby. These characteristics, depicted in Figure 12.15, can be because of thelower vertical temperature gradient G in the area or backﬁlling of liquid fromthe weld pool (3, 5). Since a thicker GB liquid has to solidify faster, the verti-cally upward solidiﬁcation rate R is higher. The lower G/R in the area suggestsa greater chance for constitutional supercooling and hence cellular insteadof planar solidiﬁcation. Figure 12.16 shows the PMZ microstructure in agas–metal arc weld of alloy 2219 (3). However, it should be pointed out thatplanar solidiﬁcation changes to cellular solidiﬁcation gradually, and a thinnerGB liquid may not have enough room for the transition to take place. There-fore, planar GB solidiﬁcation may not necessarily mean that G/R is highenough to avoid cellular solidiﬁcation.12.6 PARTIALLY MELTED ZONE IN CAST IRONSFigure 12.17 shows the PMZ in a cast iron weld, where g, a, and C representaustenite, ferrite, and graphite, respectively. This area tends to freeze as whiteiron due to the high cooling rates and becomes very hard (17).REFERENCES 1. Huang, C., and Kou, S., Weld. J., 79: 113s, 2000. 2. Huang, C., and Kou, S., Weld. J., 80: 9s, 2001.
PROBLEMS 319 3. Huang, C., and Kou, S., Weld. J., 80: 46s, 2001. 4. Huang, C., Kou, S., and Purins, J. R., in Proceedings of Merton C. Flemings Sym- posium on Solidiﬁcation and Materials Processing, Eds. R. Abbaschian, H. Brody, and A. Mortensen, Minerals, Metals and Materials Society, Warrendale, PA, 2001, p. 229. 5. Huang, C., and Kou, S., Weld. J., in press. 6. Pepe, J. J., and Savage, W. F., Weld. J., 46: 411s, 1967. 7. Pepe, J. J., and Savage, W. F., Weld. J., 49: 545s, 1970. 8. Owczarski, W. A., Duvall, D. S., and Sullivan, C. P., Weld. J., 45: 145s, 1966. 9. Duvall, D. S., and Owczarski, W. A., Weld. J., 46: 423s, 1967.10. Savage, W. F., and Krantz, B. M., Weld. J., 45: 13s, 1966.11. Thompson, R. G., and Genculu, S., Weld. J., 62: 337s, 1983.12. Dudley, R., Ph.D. Thesis, Rensselaer Polytechnic Institute, Troy, NY, 1962.13. Kelly, T. J., in Weldability of Materials, Eds. R. A. Patterson and K. W. Mahin, ASM International, Materials Park, OH, 1990, p. 151.14. Lee, H. T., and Kuo, T. Y., Sci. Technol. Weld. Join., 4: 94, 1999.15. Lippold, J. C., Baselack III, W. A., and Varol, I., Weld. J., 71: 1s, 1992.16. Lippold, J. C., in Technology and Advancements and New Industrial Applications in Welding, Proceedings of the Taiwan International Welding Conference ’98, Eds. C. Tsai and H. Tsai, Tjing Ling Industrial Research Institute, National University, Taipei, Taiwan, 1998.17. Bushey, R. A., in ASM Handbook, Vol. 6: Welding, Brazing and Soldering, ASM International, Materials Park, OH, 1993, p. 708.PROBLEMS12.1 Sheets of alloy 2219 (Al–6.3Cu) 1.6 mm thick are welded with the GTAW process using the following welding conditions: I = 60 A, E = 10 V, U = 3 mm/s. Suppose the arc efﬁciency is 70%. Estimate the PMZ width using the Adams two-dimensional equation (Chapter 2). Assume TL = 645°C and TE = 548°C.12.2 The heating rate in resistance spot welding can be much faster than that in GTAW. Is constitutional liquation expected to be more severe in the PMZ of 18-Ni-250 maraging steel in resistance spot welding or GTAW? Explain why.12.3 It has been pointed out that Fe3C tends to dissociate upon heating more easily than most other alloy carbides. Also, the diffusion rate of the interstitial solute, carbon, is much faster than substitutional solutes, for example, sulfur in the case of titanium sulﬁde inclusion. Do you expect a plain carbon eutectoid steel containing ﬁne Fe3C particles to be susceptible to constitutional liquation when heated to the eutectic temperature under normal heating rates during welding (say less than 500 °C/s)? Why or why not?
320 FORMATION OF THE PARTIALLY MELTED ZONE12.4 It has been reported that by replacing Cb with Ta in Ni-base superalloy 718, the Laves eutectic reaction temperature increases from 1185 to 1225°C. Does the width of the PMZ induced by constitutional liquation (and liquation-induced cracking) increase or decrease in the alloy and why?12.5 It has been suggested that in welding cast irons reducing the peak tem- peratures and the duration at the high temperatures is the most effec- tive way to reduce PMZ problems. Is the use of a low-melting-point ﬁller metal desirable in this respect? Is the use of high preheat temperature (to prevent the formation of martensite) desirable in this respect?12.6 Based on the PMZ microstructure of the as-cast alloy Al–4.5Cu shown in Figure 12.10, what can be said about the solidiﬁcation direction and mode of the grain boundary liquid and why?12.7 Based on the PMZ microstructure of the homogenized alloy Al–4.5Cu shown in Figure 12.11, what can be said about the solidiﬁcation direc- tion and mode of the grain boundary liquid and why?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-413 Difﬁculties Associated with thePartially Melted ZoneThe partially melted zone (PMZ) can suffer from liquation cracking, loss ofductility, and hydrogen cracking. Liquation cracking, that is, cracking inducedby grain boundary liquation in the PMZ during welding, is also called PMZcracking or hot cracking. The causes of these problems and the remedies,especially for liquation cracking, will be discussed in this chapter. Liquationcracking and ductility loss are particularly severe in aluminum alloys. Forconvenience of discussion, the nominal compositions of several commercialaluminum alloys and ﬁller wires are listed in Table 13.1 (1).13.1 LIQUATION CRACKINGFigure 13.1 shows the longitudinal cross section at the bottom of a gas–metalarc weld of 2219 aluminum made with a ﬁller wire of 1100 aluminum. Therolling direction of the workpiece is perpendicular to the plane of the micro-graph. Liquation cracking in the PMZ is intergranular (2–6). Liquation crack-ing can also occur along the fusion boundary (3). The presence of a liquidphase at the intergranular fracture surface can be either evident (4) or unclear(5, 6).13.1.1 Crack Susceptibility TestsThe susceptibility of the PMZ to liquation cracking can be evaluated usingseveral different methods, such as Varestraint testing, circular-patch testingand hot-ductility testing, etc.A. Varestraint Testing This is usually used for partially penetrating welds inplates (Chapter 11). In brief, the workpiece is subjected to augmented strainsduring welding, and the extent of cracking in the PMZ is used as the index forthe susceptibility to liquation cracking (7–12).B. Circular-Patch Testing This is usually used for fully penetrating welds inthin sheets. A relatively high restraint is imposed on the weld zone transverseto the weld (5). The ﬁxture design shown in Figure 13.2 was used for liquation 321
322 DIFFICULTIES ASSOCIATED WITH THE PARTIALLY MELTED ZONETABLE 13.1 Nominal Compositions of Some Commercial Aluminum Alloys Si Cu Mn Mg Cr Ni Zn Ti Zr Fe1100 — 0.122014 0.8 4.4 0.8 0.52024 — 4.4 0.6 1.52219 — 6.3 0.3 — — — — 0.06 0.182319 — 6.3 0.3 — — — — 0.15 0.184043 5.25083 — — 0.7 4.4 0.155356 — — 0.12 5.0 0.12 — — 0.136061 0.6 0.28 — 1.0 0.26063 0.4 — — 0.76082 0.9 — 0.5 0.7 — — — — — 0.37002 — 0.75 — 2.5 — — 3.57075 — 1.6 — 2.5 0.23 — 5.6Source: Aluminum Association (1). Figure 13.1 PMZ cracking in 2219 aluminum welded with ﬁller metal 1100.cracking test of aluminum welds (13). The specimen is sandwiched betweentwo copper plates (the upper one having a big round opening for welding) andtightened by tightening the bolts against the stainless steel base plate.A similardesign was used by Nelson et al. (14) for assessing solidiﬁcation cracking insteel welds. Cracking is at the outer edge of the weld, not the inner. This isbecause contraction of the weld during cooling is hindered by the restraint,thus rendering the outer edge in tension and the inner edge in compression.Figure 13.3a shows a circular weld made in 6061 aluminum with a 1100 alu-minum ﬁller. The three cracks in the photo all initiate from the PMZ near theouter edge of the weld and propagate into the fusion zone along the welding
LIQUATION CRACKING 323 specimen we hole ld 2.5 cm 10 cm 10 cm washer bolt copper specimen plate with weld a hole copper plate threads stainless steel base plate Figure 13.2 Schematic sketch of a circular-patch test.direction (clockwise). Figure 13.3b shows a circular weld between 2219 alu-minum and 1100 aluminum made with a 1100 aluminum ﬁller (13). A longPMZ crack runs along the outer edge of the weld.C. Hot Ductility Testing This has been used extensively for evaluating thehot-cracking susceptibility of nickel-base alloys (15, 16). It is most often per-formed on a Gleeble weld simulator (Chapter 2), which is also a tensile testinginstrument. The specimen is resistance heated according to a predeterminedthermal cycle resembling that in the PMZ. It is tensile tested, for instance, ata stroke rate of 5 cm/s, at predetermined temperatures along the thermal cycle,either during heating to the peak temperature of the thermal cycle or duringcooling from it. Several different criteria have been used for interpreting hotductility curves (17). For instance, one of the criteria is based on the ability ofthe material to reestablish ductility, that is, how fast ductility recovers duringcooling from the peak temperature. If ductility recovers right below the peaktemperature, the alloy is considered crack resistant, such as that shown inFigure 13.4a for a low-B Cabot alloy 214 (6). On the other hand, if ductilityrecovers well below the peak temperature, the alloy is considered crack sen-sitive, such as that shown in Figure 13.4b for a high-B Cabot 214. The mecha-nism that boron affects liquation cracking in Ni-base superalloys is not clear(18).
324 DIFFICULTIES ASSOCIATED WITH THE PARTIALLY MELTED ZONEFigure 13.3 Cracking in circular-patch welds: (a) 6061 aluminum made with a 1100ﬁller wire; (b) 2219 aluminum (outside) welded to 1100 aluminum (inside) with a 1100ﬁller wire. From Huang and Kou (13). Temperature, oF Temperature, oF 1650 1830 2010 2019 2370 2550 1650 1830 2010 2019 2370 2550 Reduction of area, % Reduction of area, % 100 100 OH OH 80 80 60 60 OC OC 40 40 Peak Peak temperature 20 temperature 20 (1345 oC) (1345 oC) 0 0 900 1000 1100 1200 1300 1400 900 1000 1100 1200 1300 1400 Temperature, oC Temperature, oC (a) (b)Figure 13.4 Hot ductility response of Cabot alloy 214 with two different boron levels:(a) 0.0002 wt% B; (b) 0.003 wt% B. OH, testing done on heating to 1345°C; OC, oncooling from 1345°C. From Cieslak (6). Reprinted from ASM Handbook, vol. 6, ASMInternational.
LIQUATION CRACKING 32513.1.2 Mechanisms of Liquation CrackingFigure 13.5a is a schematic showing the formation of liquation cracking in thePMZ of a full-penetration aluminum weld (13). Since the PMZ is weakenedby grain boundary liquation, it cracks when the solidifying weld metal con-tracts and pulls it. Most aluminum alloys are susceptible to liquation cracking.This is because of their wide PMZ (due to wide freezing temperature rangeand high thermal conductivity), large solidiﬁcation shrinkage (solid densitysigniﬁcantly greater than liquid density), and large thermal contraction (largethermal expansion coefﬁcient). The solidiﬁcation shrinkage of aluminum is ashigh as 6.6%, and the thermal expansion coefﬁcient of aluminum is roughlytwice that of iron base alloys. Figure 13.5b shows liquation cracking in an alloy6061 circular weld (Figure 13.3a). The light etching a band along the grainboundary is a clear evidence of the grain boundary liquid that weakened thePMZ during welding. weld base metal PMZ pool magnified fusion boundary grain crack pulling weld pool (a) PMZ weakened by grain solidifying weld boundary (GB) liquation metal pulling PMZFigure 13.5 Forma